To the past and present staff members, support staff and students in
Textile Studies at Bolton Institute, for their friendship and support over
Technical textiles are reported to be the fastest growing sector of the textile indus-
trial sector and account for almost 19% (10 million tonnes) of the total world ﬁbre
consumption for all textile uses, totalling 53 tonnes in 1997. This ﬁgure is likely to
increase to 14 million tonnes by the year 2005. Technical textiles are estimated to
account for well over 40% of the total textile production in many developed coun-
tries and, at the year 2000, account for almost 20% of all textile manufacturing in
China (Byrne 1997).
The current volume of the market worldwide for technical textiles is more than
$60 billion. The average annual growth rate of technical textiles worldwide is
expected to be around 3.8% for the period 2000 to 2005.
The uniqueness and challenge of technical textiles lies in the need to understand
and apply the principles of textile science and technology to provide solutions,
in the main to technological problems but also often to engineering problems as
well. With the emphasis on measurable textile performance in a particular ﬁeld of
application, this requires the technologist to have not only an intricate knowledge
of ﬁbres and textile science and technology but also an understanding of the
application and the scientists, technologists and engineers who service it. Thus the
producer of geotextiles requires an intricate knowledge of the world of civil
engineering, and the medical textile producer, the requirements of consultant,
medical practitioner and nurse. This series attempts to provide a bridge between
producer and end-user.
The main principles involved in the selection of raw materials and their conver-
sion into yarns and fabrics followed by dyeing, ﬁnishing and coating of technical
textiles are explored, followed by the raw materials, processing techniques, ﬁnish-
ing, speciﬁcations, properties and special technical and commercial features of a
wide range of speciﬁc areas of application.
Each of the chapters has been specially prepared and edited to cover current
developments as well as future trends in both the principles of manufacture and the
state-of-the-art constructional speciﬁcations, properties, test methods and standards
of the major product areas and applications of technical textiles.
A team of internationally famous authors has contributed a great deal of time,
effort and above all special and signiﬁcant expertise and experience to the prepa-
ration of this handbook. The editors wish to extend their most sincere thanks to all
the authors for their important contribution, patience and cooperation. This book
once again conﬁrms that enthusiasm and love of the subject are more important
than the ﬁnancial gains.
Special thanks are also given to Patricia Morrison of Woodhead Publishing Ltd,
Cambridge for her consistent interest and effort in keeping this project warm for
so long and her continued faith in the editors.
Professor Richard Horrocks
Professor Subhash Anand
Faculty of Technology
List of contributors
Professor S C Anand
Faculty of Technology, Bolton Institute, Deane Road, Bolton BL3 5AB, UK
Professor P Bajaj
Department of Textile Technology, Indian Institute of Technology, Hauz Khas,
New Delhi, India
Mr C Byrne
David Rigby Associates, Peter House, St Peter’s Square, Manchester M1 5AQ,
Dr X Chen
Department of Textiles, UMIST, P O Box 88, Sackville Street, Manchester M60
Mr W Fung
Collins and Aikman, P O Box 29, Warley Mills, Walkden, Manchester M28 3WG,
Dr R H Gong
Department of Textiles, UMIST, P O Box 88, Sackville Street, Manchester M60
Dr M Hall
Department of Textiles, Faculty of Technology, Bolton Institute, Deane Road,
Bolton BL3 5AB, UK
Mr E Hardman
Madison Filters (formerly Scapa Filtration), Haslingden, Rossendale, Lancashire,
xvi List of contributors
Dr I Holme
Department of Textiles, University of Leeds, Leeds LS2 1JT, UK
Dr D Holmes
Department of Textiles, Faculty of Technology, Bolton Institute, Deane Road,
Bolton BL3 5AB, UK
Dr M Miraftab
Department of Textiles, Faculty of Technology, Bolton Institute, Deane Road,
Bolton BL3 5AB, UK
Dr S Ogin
School of Mechanical and Materials Engineering, University of Surrey, Guildford,
Surrey GU2 7HX, UK
Dr M Pritchard
Department of the Built Environment, Faculty of Technology, Bolton Institute,
Deane Road, Bolton BL3 5AB, UK
Professor P R Rankilor
9 Blairgowrie Drive, West Tytherington, Macclesﬁeld, Cheshire SK10 2UJ, UK
Mr A J Rigby
Department of Textiles, Faculty of Technology, Bolton Institute, Deane Road,
Bolton BL3 5AB, UK
Professor S W Sarsby
Department of the Built Environment, Faculty of Technology, Bolton Institute,
Deane Road, Bolton BL3 5AB, UK
Dr R A Scott
MOD, Defence Clothing and Textiles Agency Science and Technology Division,
Flagstaff Road, Colchester, Essex CO2 7SS, UK
Professor K Slater
Department of Textiles, University of Guelph, Guelph, Ontario N1G 2W1, Canada
Dr P Smith
26 Newhall Park, Otley, Leeds LS21 2RD, UK
Mr W Sondhelm
10 Bowlacre Road, Hyde, Cheshire SK14 5ES, UK
Technical textiles market – an overview
Chris Byrne, Principal Consultant
David Rigby Associates, Peter House, St Peter’s Square, Manchester M1 5AQ, UK
Although ‘technical’ textiles have attracted considerable attention, the use of ﬁbres,
yarns and fabrics for applications other than clothing and furnishing is not a new
phenomenon. Nor is it exclusively linked to the emergence of modern artiﬁcial ﬁbres
and textiles. Natural ﬁbres such as cotton, ﬂax, jute and sisal have been used for
centuries (and still are used) in applications ranging from tents and tarpaulins to
ropes, sailcloth and sacking. There is evidence of woven fabrics and meshes being
used in Roman times and before to stabilise marshy ground for road building – early
examples of what would now be termed geotextiles and geogrids.
What is relatively new is a growing recognition of the economic and strategic
potential of such textiles to the ﬁbre and fabric manufacturing and processing indus-
tries of industrial and industrialising countries alike. In some of the most developed
markets, technical products (broadly deﬁned) already account for as much as 50%
of all textile manufacturing activity and output. The technical textiles supply chain
is a long and complex one, stretching from the manufacturers of polymers for tech-
nical ﬁbres, coating and speciality membranes through to the converters and fabri-
cators who incorporate technical textiles into ﬁnished products or use them as an
essential part of their industrial operations. The economic scope and importance of
technical textiles extends far beyond the textile industry itself and has an impact
upon just about every sphere of human economic and social activity.
And yet this dynamic sector of the textile industry has not proved entirely
immune to the effects of economic recession, of product and market maturity, and
of growing global competition which are all too well known in the more traditional
sectors of clothing and furnishings. There are no easy paths to success and manu-
facturers and converters still face the challenge of making economic returns com-
mensurate with the risks involved in operating in new and complex markets. If
anything, the constant need to develop fresh products and applications, invest in
new processes and equipment, and market to an increasingly diverse range of
customers, is more demanding and costly than ever.
2 Handbook of technical textiles
Technical textiles has never been a single coherent industry sector and market
segment. It is developing in many different directions with varying speeds and levels
of success. There is continual erosion of the barriers between traditional deﬁnitions
of textiles and other ‘ﬂexible engineering’ materials such as paper and plastics, ﬁlms
and membranes, metals, glass and ceramics. What most participants have in common
are many of the basic textile skills of manipulating ﬁbres, fabrics and ﬁnishing
techniques as well as an understanding of how all these interact and perform in
different combinations and environments. Beyond that, much of the technology and
expertise associated with the industry resides in an understanding of the needs and
dynamics of many very different end-use and market sectors. It is here that the new
dividing lines within the industry are emerging.
An appreciation of the development and potential of technical textile markets
therefore starts with some clariﬁcation of the evolving terminology and deﬁnitions
of scope of the industry and its markets. This chapter goes on to consider some of
the factors – technical, commercial and global – which are driving the industry
It also considers how the emergence of new geographical markets in China and
other rapidly industrialising regions of the world looks set to be one of the major
inﬂuences on the growth and location of technical textiles manufacturing in the ﬁrst
10 years of the 21st century.
1.2 Deﬁnition and scope of technical textiles
The deﬁnition of technical textiles adopted by the authoritative Textile Terms and
Deﬁnitions, published by the Textile Institute1, is ‘textile materials and products
manufactured primarily for their technical and performance properties rather than
their aesthetic or decorative characteristics’.
Such a brief description clearly leaves considerable scope for interpretation,
especially when an increasing number of textile products are combining both per-
formance and decorative properties and functions in equal measure. Examples are
ﬂame retardant furnishings and ‘breathable’ leisurewear. Indeed, no two published
sources, industry bodies or statistical organisations ever seem to adopt precisely the
same approach when it comes to describing and categorising speciﬁc products and
applications as technical textiles.
It is perhaps not surprising that any attempt to deﬁne too closely and too rigidly
the scope and content of technical textiles and their markets is doomed to failure.
In what is one of the most dynamic and broad ranging areas of modern textiles,
materials, processes, products and applications are all changing too rapidly to deﬁne
and document. There are even important linguistic and cultural perceptions of what
constitutes a technical textile from geographical region to region in what is now a
global industry and marketplace.
1.2.1 Technical or industrial textiles: what’s in a name?
For many years, the term ‘industrial textiles’ was widely used to encompass all textile
products other than those intended for apparel, household and furnishing end-uses.
It is a description still more widely favoured in the USA than in Europe and
elsewhere (see, for example, the Wellington Sears Handbook of Industrial Textiles).2
Technical textiles market – an overview 3
This usage has seemed increasingly inappropriate in the face of developing appli-
cations of textiles for medical, hygiene, sporting, transportation, construction, agri-
cultural and many other clearly non-industrial purposes. Industrial textiles are now
more often viewed as a subgroup of a wider category of technical textiles, referring
speciﬁcally to those textile products used in the course of manufacturing operations
(such as ﬁlters, machine clothing, conveyor belts, abrasive substrates etc.) or which
are incorporated into other industrial products (such as electrical components and
cables, ﬂexible seals and diaphragms, or acoustic and thermal insulation for domes-
tic and industrial appliances).
If this revised deﬁnition of industrial textiles is still far from satisfactory, then the
problems of ﬁnding a coherent and universally acceptable description and classiﬁ-
cation of the scope of technical textiles are even greater. Several schemes have been
proposed. For example, the leading international trade exhibition for technical
textiles, Techtextil (organised biennially since the late 1980s by Messe Frankfurt
in Germany and also in Osaka, Japan), deﬁnes 12 main application areas (of which
textiles for industrial applications represent only one group):
• agrotech: agriculture, aquaculture, horticulture and forestry
• buildtech: building and construction
• clothtech: technical components of footwear and clothing
• geotech: geotextiles and civil engineering
• hometech: technical components of furniture, household textiles and
• indutech: ﬁltration, conveying, cleaning and other industrial uses
• medtech: hygiene and medical
• mobiltech: automobiles, shipping, railways and aerospace
• oekotech: environmental protection
• packtech: packaging
• protech: personal and property protection
• sporttech: sport and leisure.
The search for an all embracing term to describe these textiles is not conﬁned to
the words ‘technical’ and ‘industrial’. Terms such as performance textiles, functional
textiles, engineered textiles and high-tech textiles are also all used in various
contexts, sometimes with a relatively speciﬁc meaning (performance textiles are
frequently used to describe the fabrics used in activity clothing), but more often
with little or no precise signiﬁcance.
1.2.2 Operating at the boundaries of textiles
If the adjective ‘technical’ is difﬁcult to deﬁne with any precision, then so too is the
scope of the term textiles. Figure 1.1 summarises the principal materials, processes
and products which are commonly regarded as falling within the scope of technical
However, there remain many grey areas. For example, the manufacture and pro-
cessing of metallic wires into products such as cables, woven or knitted screens and
meshes, and reinforcing carcasses for tyres are not generally regarded as lying within
the scope of the textile industry. This is despite the fact that many of the techniques
employed and the ﬁnal products obtained are closely related to conventional textile
4 Handbook of technical textiles
Glass Natural Fibres
Metals Ceramics Synthetic Polymers Regenerated Fibres Wood Cotton, wool,
MATERIALS Asbestos Rayon, Acetate jute, sisal etc
Steel PES, PA, PAN, PP etc
Silk (ﬁl.) silk (staple)
Wire Monoﬁlament Tape, Multiﬁlament Tow Cutting Opening
Fibrillation Spunbond Meltblown Carding, Sliver
air laying Roving
Nonwoven bonding Spinning
PROCESSES Wet laying Ring
Laying Knotting Braiding Weaving Knitting
Plaiting Narrow Broad Warp Weft
Technical Fabrics Waddings
PRODUCTS Rope, Cord Net Thread Fibreﬁll
1.1 Technical textile materials, processes and products. PES = polyester, PA = polyamide,
PAN = polyacrylonitrile.
Within the composites industry, woven, knitted, braided, nonwoven and wound
yarn reinforcements made from glass, carbon ﬁbre and organic polymer materials
such as aramids are all now widely accepted as being technical textile products. On
the other hand, more loosely structured reinforcing materials such as chopped
strand mat, milled glass and pulped organic ﬁbres are often excluded.
The nonwovens industry has developed from several different technology
directions, including paper manufacturing. The current deﬁnition of a nonwoven
promulgated, for example, under the International Standards Organization standard
ISO 90923 acknowledges a number of borderline areas, including wet-laid products
and extruded meshes and nets. Likewise, distinctions between textile ﬁbres and ﬁl-
aments, slit or ﬁbrillated ﬁlms, monoﬁlaments and extruded plastics inevitably boil
down to some fairly arbitrary and artiﬁcial criteria. Diameter or width is often used
as the deﬁning characteristic, irrespective of the technologies used or the end-uses
served. Many of the deﬁnitions and categories embodied within existing industry
statistics reﬂect historical divisions of the main manufacturing sectors rather than a
functional or market-based view of the products involved.
Polymer membranes, composite materials and extruded grids and nets are other
products which challenge traditional notions of the scope of technical textile ma-
terials, processes and products. Increasingly, technical textiles are likely to ﬁnd their
place within a broader industry and market for ‘ﬂexible engineering materials’
(Fig. 1.2). A number of companies and groups have already adopted this outlook
and operate across the boundaries of traditional industry sectors, focusing a range
Technical textiles market – an overview 5
Paper, Technical Plastics,
pulp textiles foams, rubbers
1.2 Scope of ﬂexible engineering materials.
of materials, process technologies and product capabilities upon speciﬁc functions
and markets such as ﬁltration and health care.
1.2.3 Inconsistent statistical reporting
To add to this complexity, different geographical regions and countries tend to
adopt rather different viewpoints and deﬁnitions with regard to all of the above. A
widely quoted misconception that technical textiles in Japan account for over 40%
of all textile output or nearly twice the level in Western Europe can largely be put
down to the different statistical bases employed. In Europe, the most authoritative
source of ﬁbre consumption (and therefore textile output) data is CIRFS (Comité
International de la Rayonne et des Fibres Synthétiques), the European artiﬁcial
ﬁbre producers association. However, CIRFS’ reported statistics (at least until
recently) have speciﬁcally excluded tape and ﬁlm yarns (a signiﬁcant proportion
of all polyoleﬁn textiles), coarser monoﬁlaments and all glass products (as well
as natural ﬁbres such as jute, ﬂax, sisal, etc.). The merger of CIRFS and EATP, the
European Polyoleﬁn Textiles Association, should go some way towards resolving
The Japanese ‘Chemical’ Fibres Manufacturers Association, JCFA, at the other
extreme, includes all these products, including natural ﬁbres, within its deﬁnition of
technical/industrial textiles while the Fiber Statistics Bureau in the USA includes
polyoleﬁn tape and monoﬁlament yarns but excludes glass. Table 1.1 attempts to
restate the relative usage of the main technical ﬁbres and yarns on a more consis-
In this new light, Japan still retains a leading position worldwide in terms of
the proportion of its total textile manufacturing output devoted to technical
textiles. However, this is largely a reﬂection of the importance of its automotive
manufacturing industry (a key user of technical textiles) combined with the rela-
tively smaller size of its apparel and furnishing textile sectors (especially ﬂoor
coverings). The USA apparently accounts for the lowest proportion of technical
6 Handbook of technical textiles
Table 1.1 Comparative levels of technical ﬁbre mill consumption, 1995
% Total ﬁbre consumption + kg per capita
Textile ﬁbre, PP tape and Textile ﬁbre, PP tape,
Textile ﬁbres only
monoﬁlaments monoﬁlaments and glass
W Europe 21% 28% 34%
2.8 kg 4.2 kg 5.6 kg
USA 18% 22% 30%
4.9 kg 6.4 kg 9.7 kg
Japan 30% 35% 41%
3.3 kg 4.3 kg 5.5 kg
Source: CIRFS, Fiber Organon, JCFA and David Rigby Associates estimates.
PP = polypropylene.
textile output of the three major industrial regions but still produces and consumes
the largest quantity per capita, especially when all glass textile and technical ﬁbre
uses are included.
1.3 Milestones in the development of technical textiles
Although the development of technical and industrial applications for textiles can
be traced back many years, a number of more recent milestones have marked the
emergence of technical textiles as we know them today. Very largely, these have
centred upon new materials, new processes and new applications.
1.3.1 Developments in ﬁbre materials – natural ﬁbres
Until early in the 20th century, the major ﬁbres available for technical and indus-
trial use were cotton and various coarser vegetable ﬁbres such as ﬂax, jute and sisal.
They were typically used to manufacture heavy canvas-type products, ropes and
twines, and were characterised by relatively heavy weight, limited resistance to
water and microbial/fungal attack as well as poor ﬂame retardancy.
Some of the present day regional patterns of technical textiles manufacturing
were established even then, for example Dundee, on the east coast of Scotland
and located at the centre (then) of an important ﬂax growing area as well as being
a whaling port. Following the discovery that whale oil could be used to lubricate
the spinning of the relatively coarse jute ﬁbres then becoming available from the
Indian subcontinent, jute fabrics were widely used for sacking, furniture and carpet
manufacturing, rooﬁng felts, linoleum ﬂooring, twine and a host of other applications.
Although its jute industry was to decline dramatically from a peak at around 1900
owing to competition from other materials as well as from cheaper imports, Dundee
and the surrounding industry subsequently become a nucleus for development of
the UK polypropylene industry in the 1960s. The then newly available polymer
proved not only to be an ideal technical substitute for the natural product but was
also much more consistent in terms of its supply and price.
Traditional end-uses for sisal were similarly rapidly substituted throughout the
established rope, twine and net making centres of Europe and America.
Technical textiles market – an overview 7
Wool proved far less versatile and economic for most industrial applications
although it is still valued for its insulating and ﬂame retardency properties and ﬁnds
use in several high temperature and protective clothing applications. Silk is an
even more exotic ﬁbre, rarely used in technical applications other than for highly
specialised uses such as surgical suture thread. However, the traces of the early
silk industry are still to be seen in the present day location of centres for technical
ﬁlament weaving such as the Lyons area of France. The traditional silk industry
has also contributed to the development of technical textiles in Asia, especially in
1.3.2 Viscose rayon
The ﬁrst commercially available synthetic ﬁbre, viscose rayon, was developed
around 1910 and by the 1920s had made its mark as reinforcement material for tyres
and, subsequently, other mechanical rubber goods such as drive belts, conveyors and
hoses. Its relatively high uniformity, tenacity and modulus (at least when kept dry
within a rubber casing), combined with good temperature resistance, proved ideal
for the fast emerging automotive and industrial equipment markets.
At a much later stage of its lifecycle, other properties of viscose such as its
good absorbency and suitability for processing by paper industry-type wet lay-
ing techniques contributed to its role as one of the earliest and most successful
ﬁbres used for nonwoven processing, especially in disposable cleaning and hygiene
1.3.3 Polyamide and polyester
Polyamide (nylon) ﬁbre, ﬁrst introduced in 1939, provided high strength and abra-
sion resistance, good elasticity and uniformity as well as resistance to moisture. Its
excellent energy absorbing properties proved invaluable in a range of end-uses from
climbing ropes to parachute fabrics and spinnaker sails. Polyamide-reinforced tyres
are still used much more extensively in developing countries where the quality of
road surfaces has traditionally been poor as well as in the emerging market for off-
road vehicles worldwide. This contrasts to Western Europe where average road
speeds are much greater and the heat-resistant properties of viscose are still valued.
From the 1950s onwards, the huge growth in world production of polyester,
initially for apparel and household textile applications, provided the incentive
and economies of scale needed to develop and engineer this ﬁbre as a lower cost
alternative to both viscose and polyamide in an increasing range of technical
Nowhere is this more true than Japan and the developing industrial economies
of Asia, including China, where production capacities for both polyester staple and
ﬁlament yarn are extremely high and there is an urgent search for new applications.
Some high volume applications for technical textiles which would typically use poly-
oleﬁns in western Europe and North America such as geotextiles, carpet backing
and coverstock are more likely to use polyester in Asia largely because of the
greater availability and better economics of ﬁbre supplies in those regions.
At a slightly less obvious level, differences in the polyamide supply situation –
Western Europe and North America are more strongly oriented towards nylon 66
while Asia and Eastern Europe produce predominantly nylon 6 – are reﬂected in
8 Handbook of technical textiles
different manufacturing practices, product types and technical applications for this
Yet another example is the production and use of Vinylon (PVA, polyvinyl
alcohol) ﬁbres in Japan, where they were developed for a variety of industrial and
technical applications at a time when that country lacked other raw materials and
ﬁbre production capabilities. Use of this ﬁbre for technical textiles is almost non-
existent in the West.
The development of polyoleﬁn (mostly polypropylene but also some polyethylene)
ﬁbres as well as tape and ﬁlm yarns in the 1960s was another milestone in the
development of technical textiles. The low cost and easy processability of this ﬁbre,
combined with its low density and good abrasion and moisture-resistant properties,
have allowed its rapid introduction into a range of applications such as sacks, bags
and packaging, carpet backings and furniture linings as well as ropes and netting.
Many of these markets were directly taken over from jute and similar ﬁbres but
newer end-uses have also been developed, including artiﬁcial sports surfaces.
Properties of the polyoleﬁns such as their poor temperature resistance and com-
plete hydrophobicity have been turned to advantage in nonwovens. Initially used in
conjunction with viscose to permit thermal bonding, polypropylene has now bene-
ﬁted from a growing appreciation of the important role that moisture wicking
(as opposed to absorption) can play in hygiene applications such as coverstock
for diapers (nappies). Finally, the relatively low extrusion temperatures of the poly-
oleﬁns have proved ideally suited to the fast developing technologies of spin laying
(spun bonding and melt blowing).
As noted above, the development of the polypropylene industry was initially
focused on European and North American markets. However, it is undergoing a
major expansion worldwide as new investment in polymer capacity offers more
favourable economics to new geographical markets.
1.3.5 High performance ﬁbres
The above ‘conventional’ ﬁbre types, both chemical and natural, still account for
over 95% of all organic ﬁbre technical textiles in use (i.e. excluding glass, mineral
and metal ﬁbres). Many of them have been modiﬁed and tailored to highly speciﬁc
end-uses by adjustment of their tenacity, length, decitex, surface proﬁle, ﬁnish and
even by their combination into hybrid and bicomponent products. However, it is the
emergence of the so-called high performance ﬁbres since the early 1980s that has
provided some of the most signiﬁcant and dramatic impulses to the evolution of
First and foremost of these are the aramids, both the highly temperature-
resistant meta-aramids (widely used in protective clothing and similar applications)
and the high strength and modulus para-aramids (used in a host of applications
ranging from bulletproof vests to reinforcement of tyres, hoses, friction materials,
ropes and advanced composites). From their commercial introduction in the 1970s,
world demand for p-aramids is expected to reach almost 40 000 tonnes per annum
by 2000 while for m-aramids, consumption will be around 17–18 000 tonnes.
While not huge in overall terms (representing less than 0.5% of total world tech-
Technical textiles market – an overview 9
nical ﬁbre and yarn usage in volume terms but closer to 3–4% in value), the aramids
represent a particularly important milestone in the development of the technical
textiles industry. Partly practical and partly symbolic, the introduction of the aramids
not only led to the injection of large amounts of technical and market support into
the industry and for users by leading ﬁbre manufacturers such as DuPont and Akzo,
but also concentrated the minds of many developers of new products upon the
possibilities (and practicalities) of using similar new generation materials.
The early success of the aramids was a welcome contrast to the development of
carbon ﬁbres, which have been commercially available since the 1960s but largely
constrained by their high material and processing costs to selected high value
markets, particularly aerospace applications. Total world demand for carbon ﬁbres
was still only some 8–9000 tonnes per annum as recently as 1995. In fact, their
market actually shrank in the early 1990s owing to cutbacks in military spending.
At long last, carbon ﬁbres appear to be emerging from the doldrums, with the
appearance not only of important new civil aerospace markets but also of high
technology sporting goods and industrial applications such as wind generator turbine
blades and reinforced fuel tanks. As new manufacturing methods and greater
economies of scale start to bring prices down, the feasibility of even larger scale
applications such as the reinforcement of buildings and structures in earthquake
zones becomes more attractive. Currently, (2000), consumption is considered to be
over 13 000 tonnes per annum, rising to almost 19 000 tonnes by the year 2005.
The introduction of other high performance ﬁbres proliferated, particularly
during the late 1980s, and in the wake of the aramids. These included a range of heat
and ﬂameproof materials suitable for protective clothing and similar applications
(such as phenolic ﬁbres and PBI, polybenzimidazole), ultra-strong high modulus
polyethylene (HMPE) for ballistic protection and rope manufacture, and chemically
stable polymers such as polytetraﬂuoroethylene (PTFE), polyphenylene sulphide
(PPS) and polyethyletherketone (PEEK) for use in ﬁltration and other chemically
Individually, none of these other ﬁbres has yet achieved volume sales anywhere
near those of the aramids (or even carbon ﬁbres). Indeed, the output of some spe-
ciality ﬁbres can still be measured in tens of tonnes per year rather than hundreds
or thousands. The widespread industrial recession of the early 1990s caused many
ﬁbre manufacturers to review their development strategies and to focus upon
narrower ranges of products and markets.
1.3.6 Glass and ceramics
Glass has, for many years, been one of the most underrated technical ﬁbres. Used
for many years as a cheap insulating material as well as a reinforcement for rela-
tively low performance plastics (ﬁbre glass) and (especially in the USA) rooﬁng
materials, glass is increasingly being recognised as a sophisticated engineering ma-
terial with excellent ﬁre and heat-resistant properties. It is now widely used in a
variety of higher performance composite applications, including sealing materials
and rubber reinforcement, as well as ﬁltration, protective clothing and packaging.
The potential adoption of high volume glass-reinforced composite manufactur-
ing techniques by the automotive industry as a replacement for metal body parts
and components, as well as by manufacturing industry in general for all sorts of
industrial and domestic equipment, promises major new markets. Total world con-
10 Handbook of technical textiles
sumption of ‘textile’ glass in technical applications was some 2.3 million tonnes
per annum in 1995 and is considered likely to be over 2.9 million tonnes at 2000,
representing over 20% of all technical ﬁbre consumption.
Various higher performance ceramic ﬁbres have been developed but are
restricted to relatively specialised applications by their high cost and limited
1.4 Textile processes
Figure 1.1 summarises the wide range of processes employed in the manufacture of
technical textiles. Apart from the use of plaiting and knotting for the manufacture
of ropes and nets, weaving was, for many years, the pre-eminent technology em-
ployed in the manufacture of ‘industrial’ textiles. In terms of the total weight of
textiles produced, weaving still plays a leading role and developments such as three-
dimensional and crimpless weaving have opened up many new product and end-
However, the historical progress of technical textiles has seen the advance of
alternative textile forming technologies, most prominently the broad family of non-
woven techniques but also warp and weft knitting, stitchbonding and modern braid-
ing methods. The use of loose ﬁbres with sophisticated cross-sectional proﬁles for
insulation, protection and ﬁbreﬁll applications is another important growth area.
Fibres, yarns and textiles of all types also provide the starting point for a diverse
and fast expanding range of composite reinforcement and forming technologies.
According to a major study of the world technical textiles industry and its
markets projected to 2005 (see Table 1.2), nonwovens are set to overtake weaving
(in terms of the total weight of textiles produced) by around 2002/2003. In area
terms, nonwovens already far exceed woven and other fabric forming methods
because of their lower average weight per unit area. On the other hand, woven and
other yarn-based fabrics will remain in the lead in value terms, at least for the fore-
There is, therefore, something for every section of the textile industry in the
future of technical textiles. Most product areas will see more rapid growth in value
Table 1.2 Worldwide consumption of technical textiles by product type, 2000–2005
103 tonnes $ million
2000 2005 2000 2005
(% pa) (% pa)
Fabrics 3 760 4 100 1.7% 26 710 29 870 2.2%
Nonwovens 3 300 4 300 5.4% 14 640 19 250 5.6%
Composites 1 970 2 580 5.5% 6 960 9 160 5.6%
Other textilesa 2 290 2 710 3.4% 11 950 14 060 3.3%
All textile products 11 320 13 690 3.9% 60 260 72 340 3.7%
Source: David Rigby Associates/Techtextil.
Includes ropes, twines, thread, ﬁbreﬁll etc.
Technical textiles market – an overview 11
Table 1.3 Worldwide consumption of technical textiles by application, 2000–2005
103 tonnes $ million
2000 2005 2000 2005
(% pa) (% pa)
Transport textiles (auto, train, 2 220 2 480 2.2 13 080 14 370 1.9
Industrial products and 1 880 2 340 4.5 9 290 11 560 4.5
Medical and hygiene textiles 1 380 1 650 3.6 7 820 9 530 4.0
Home textiles, domestic 1 800 2 260 4.7 7 780 9 680 4.5
Clothing components (thread, 730 820 2.3 6 800 7 640 2.4
Agriculture, horticulture and 900 1 020 2.5 4 260 4 940 3.0
Construction – building and 1 030 1 270 4.3 3 390 4 320 5.0
Packaging and containment 530 660 4.5 2 320 2 920 4.7
Sport and leisure (excluding 310 390 4.7 2 030 2 510 4.3
Geotextiles, civil engineering 400 570 7.3 1 860 2 660 7.4
Protective and safety clothing 160 220 6.6 1 640 2 230 6.3
Total above 11 340 13 680 3.9 60 270 72 360 3.7
Ecological protection textilesa 230 310 6.2 1 270 1 610 4.9
Source: David Rigby Associates/Techtextil.
Already counted in several categories above.
than in volume as technical textiles become increasingly sophisticated and employ
more specialised and higher value raw materials. On the other hand, the total value
of yarns and ﬁbres and of all technical textile products will grow slightly less fast
than their volume because of a changing mix of materials and technologies, espe-
cially reﬂecting the growth of nonwovens.
The same study identiﬁed size and growth trends in each major application area for
technical textiles, as deﬁned by the organisers of Techtextil.The results are presented
in Table 1.3.
Ecological textiles were identiﬁed as a separate and potentially important growth
segment but are not consolidated in the total consumption ﬁgure because they have
already been counted under headings such as industrial textiles (ﬁltration media,
oil spill protection and absorption) and geotextiles (geomembrane liners for toxic
waste pits, erosion protection textiles, etc.).
Some selected examples of these broad trends which illustrate key aspects of the
development and use of technical textiles are discussed in further detail below.
12 Handbook of technical textiles
1.5.1 Transport textiles
Transport applications (cars, lorries, buses, trains, ships and aerospace) represent the
largest single end-use area for technical textiles, accounting for some 20% of the
total. Products range from carpeting and seating (regarded as technical rather than
furnishing textiles because of the very stringent performance characteristics which
they must fulﬁl), through tyre, belt and hose reinforcement, safety belts and air
bags, to composite reinforcements for automotive bodies, civil and military aircraft
bodies, wings and engine components, and many other uses.
The fact that volume and value growth rates in these applications appear to be
amongst the lowest of any application area needs to be interpreted with caution.
The automotive industry (which accounts for a high proportion of all transport
textiles) is certainly one of the most mature in market terms. Growth rates in new
end-uses such as air bags and composite materials will continue to outstrip the
above averages by a considerable margin for many years to come. However, total
technical textile usage is, in many ways, a victim of its own success. Increasing
sophistication in the speciﬁcations and uses of textile materials has led to the
adoption of lighter, stronger, more precisely engineered yarns, woven and knitted
fabrics and nonwovens in place of established materials. The decreasing weight per
tyre of textile reinforcing cord in modern radial constructions is one example of
this. Interior textiles in cars are also making use of lighter weight and lower cost
Modern textiles also last longer. Hoses and belts which used to use substantial
quantities of textile reinforcements are now capable of lasting the lifetime of a vehi-
cle, removing much of the large and continuing ‘after-market’ for textile products.
The automotive industry has led the world in the introduction of tightly organ-
ised supply chain structures and textiles are no exception. Technical textile produc-
ers have had to learn the language and practice of precision engineering, just-in-time
supply relationships and total quality management. The ideas and systems devel-
oped to serve the automotive industry have gradually ﬁltered through to other
markets and have had a profound effect in many different areas. Meanwhile, the
major automotive companies have become increasingly global players in a highly
competitive market and have demanded of their suppliers that they follow suit. The
supply of textiles to this market is already dominated by a relatively few large com-
panies in each product area. Worldwide manufacturing capabilities and strategic
relationships are essential to survival and many smaller players without these
resources have already exited from the market. Recessionary cycles in automotive
markets as well as in military and civil aerospace applications have dealt some
severe blows and only those companies with the long term commitment and
strength to survive are likely to beneﬁt from the better times that the market also
1.5.2 Industrial products and components
Set to rival transport textiles for ﬁrst place by the year 2005 or shortly thereafter
(in volume terms, although not yet in value) is the diverse ﬁeld of ‘industrial’ tex-
tiles. As now more precisely deﬁned, this includes textiles used directly in industrial
processes or incorporated into industrial products such as ﬁlters, conveyor belts and
abrasive belts, as well as reinforcements for printed circuit boards, seals and gaskets,
and other industrial equipment.
Technical textiles market – an overview 13
Use of nonwovens already considerably outweighs that of woven and other
fabric types here; consumption in 2000 is estimated at 700 000 tonnes and a little
over 400 000 tonnes, respectively. However, both are surpassed by the use of
technical ﬁbres and textiles for composite reinforcement, over 740 000 tonnes in
Growth rates are generally well above average in most areas. Because of the uni-
versal nature of many industrial requirements, some large companies have emerged
with worldwide manufacturing and distribution to dominate markets for industrial
textile products. They include companies such as Scapa (UK) and Albany (US),
leaders in papermaking felts and related product areas, Milliken (USA) in textiles
for rubber reinforcement and other industrial applications and BWF (Germany) in
1.5.3 Medical and hygiene textiles
The fact that medical and hygiene textiles are expected to show below average
growth in volume but above average growth in value reﬂects the contrasting
prospects of at least two main areas of the market.
The largest use of textiles is for hygiene applications such as wipes, babies’
diapers (nappies) and adult sanitary and incontinence products. With the possible
exception of the last of these, all are relatively mature markets whose volume
growth has peaked. Manufacturers and converters now seek to develop them
further by adding value to increasingly sophisticated products. Nonwovens domi-
nate these applications which account for over 23% of all nonwoven use, the largest
proportion of any of the 12 major markets for technical textiles.
Concern has been expressed at the growth of disposable products and the burden
which they place upon landﬁll and other waste disposal methods. Attempts have
been made to develop and introduce more efﬁcient biodegradable ﬁbres for such
end-uses but costs remain high. Meanwhile, the fastest areas of growth are in devel-
oping and newly industrialised markets where product penetration is still relatively
low; Asia is a particular target for many of the big name brand manufacturers who
operate in this area.
The other side of the medical and hygiene market is a rather smaller but higher
value market for medical and surgical products such as operating gowns and drapes,
sterilisation packs, dressings, sutures and orthopaedic pads. At the highest value end
of this segment are relatively tiny volumes of extremely sophisticated textiles for
uses such as artiﬁcial ligaments, veins and arteries, skin replacement, hollow ﬁbres
for dialysis machines and so on. Growth prospects in these areas are potentially
considerable although the proving and widespread introduction of new life-critical
products takes time.
1.5.4 Home textiles
By far the largest area of use for other textiles as deﬁned above, that is other than
fabrics, nonwovens and composite reinforcements, over 35% of the total weight
of ﬁbres and textiles in that category, lies in the ﬁeld of household textiles and
furnishing and especially in the use of loose ﬁbres in wadding and ﬁbreﬁll applica-
tions. Hollow ﬁbres with excellent insulating properties are widely used in bedding
and sleeping bags. Other types of ﬁbre are increasingly being used to replace foams
14 Handbook of technical textiles
in furniture because of concern over the ﬁre and health hazards posed by such
Woven fabrics are still used to a signiﬁcant extent as carpet and furniture back-
ings and in some smaller, more specialised areas such as curtain header tapes.
However, nonwovens such as spunbondeds have made signiﬁcant inroads into these
larger markets while various drylaid and hydroentangled products are now widely
used in household cleaning applications in place of traditional mops and dusters.
1.5.5 Clothing components
This category includes ﬁbres, yarns and textiles used as technical components in the
manufacture of clothing such as sewing threads, interlinings, waddings and insula-
tion; it does not include the main outer and lining fabrics of garments, nor does it
cover protective clothing which is discussed later.
Although the world’s consumption of clothing and therefore of these types of
technical textile continues to increase steadily, the major problem faced by estab-
lished manufacturers is the relocation of garment manufacturing to lower cost
countries and therefore the need to develop extended supply lines and marketing
channels to these areas, usually in the face of growing local competition.
As for home textile applications, this is a major market for ﬁbreﬁll products. Some
of the latest and most sophisticated developments have seen the incorporation of
temperature phase change materials into such insulation products to provide an
additional degree of control and resistance to sudden extremes of temperature, be
they hot or cold.
1.5.6 Agriculture, horticulture and ﬁshing
Textiles have always been used extensively in the course of food production, most
notably by the ﬁshing industry in the form of nets, ropes and lines but also by agri-
culture and horticulture for a variety of covering, protection and containment appli-
cations. Although future volume growth rates appear to be relatively modest, this
is partly due to the replacement of heavier weight traditional textiles, including jute
and sisal sacking and twine, by lighter, longer lasting synthetic substitutes, especially
However, modern materials are also opening up new applications. Lightweight
spunbonded ﬂeeces are now used for shading, thermal insulation and weed sup-
pression. Heavier nonwoven, knitted and woven constructions are employed for
wind and hail protection. Fibrillated and extruded nets are replacing traditional
baler twine for wrapping modern circular bales. Capillary nonwoven matting is used
in horticulture to distribute moisture to growing plants. Seeds themselves can be
incorporated into such matting along with any necessary nutrients and pesticides.
The bulk storage and transport of fertiliser and agricultural products is increasingly
undertaken using woven polypropylene FIBCs (ﬂexible intermediate bulk contain-
ers – big bags) in place of jute, paper or plastic sacks.
Agriculture is also an important user of products from other end-use sectors such
as geotextiles for drainage and land reclamation, protective clothing for employees
who have to handle sprays and hazardous equipment, transport textiles for tractors
and lorries, conveyor belts, hoses, ﬁlters and composite reinforcements in the con-
struction of silos, tanks and piping.
Technical textiles market – an overview 15
At sea, ﬁsh farming is a growing industry which uses specialised netting and other
textile products. High performance ﬁbres such as HMPE (e.g. Dyneema and
Spectra) are ﬁnding their way into the ﬁshing industry for the manufacture of
lightweight, ultra-strong lines and nets.
1.5.7 Construction – building and rooﬁng
Textiles are employed in many ways in the construction of buildings, both perma-
nent and temporary, dams, bridges, tunnels and roads. A closely related but distinct
area of use is in geotextiles by the civil engineering sector.
Temporary structures such as tents, marquees and awnings are some of the most
obvious and visible applications of textiles. Where these used to be exclusively made
from proofed heavy cotton, a variety of lighter, stronger, rot-, sunlight- and weath-
erproof (also often ﬁreproof) synthetic materials are now increasingly required. A
relatively new category of ‘architectural membrane’ is coming to prominence in the
construction of semipermanent structures such as sports stadia, exhibition centres
(e.g. the Greenwich Millenium Dome) and other modern buildings.
Nonwoven glass and polyester fabrics are already widely used in rooﬁng appli-
cations while other textiles are used as breathable membranes to prevent moisture
penetration of walls. Fibres and textiles also have a major role to play in building
and equipment insulation. Glass ﬁbres are almost universally used in place of
asbestos now. Modern metal-clad roofs and buildings can be lined with special
nonwovens to prevent moisture condensation and dripping.
Double wall spacer fabrics can be ﬁlled with suitable materials to provide sound
and thermal insulation or serve as lightweight cores for composite materials.
Composites generally have a bright future in building and construction. Existing
applications of glass-reinforced materials include wall panels, septic tanks and
sanitary ﬁttings. Glass, polypropylene and acrylic ﬁbres and textiles are all used to
prevent cracking of concrete, plaster and other building materials. More innovative
use is now being made of glass in bridge construction. In Japan, carbon ﬁbre is
attracting a lot of interest as a possible reinforcement for earthquake-prone build-
ings although price is still an important constraint upon its more widespread use.
Textiles are also widely employed in the course of construction operations them-
selves, in uses as diverse as safety netting, lifting and tensioning ropes and ﬂexible
shuttering for curing concrete.
The potential uses for textiles in construction are almost limitless. The difﬁculties
for textile manufacturers operating in this market include the strongly cyclical nature
of the construction industry and the unevenness of major projects, the long testing
and acceptance procedures and, perhaps above all, the task of communicating these
developments to a diverse and highly fragmented group of key speciﬁers, including
architects, construction engineers and regulatory bodies. The construction require-
ments, practices and standards of just about every country and region are different
and it has, so far, proved very difﬁcult for any acknowledged global leaders to emerge
in this market as they have, for example, in industrial and automotive textiles.
1.5.8 Packaging and containment
Important uses of textiles include the manufacturing of bags and sacks, tradition-
ally from cotton, ﬂax and jute but increasingly from polypropylene. The strength
16 Handbook of technical textiles
and regularity of this synthetic material, combined with modern materials handling
techniques, has allowed the introduction of FIBCs for the more efﬁcient handling,
storage and distribution of a variety of powdered and granular materials ranging
from fertiliser, sand, cement, sugar and ﬂour to dyestuffs. ‘Big bags’ with typical car-
rying capacities from one half to 2 tonnes can be ﬁtted with special liners, carrying
straps and ﬁlling/discharge arrangements. The ability to re-use these containers in
many applications in place of disposable ‘one-trip’ bags and sacks is another pow-
erful argument for their wider use.
An even faster growing segment of the packaging market uses lighter weight
nonwovens and knitted structures for a variety of wrapping and protection
applications, especially in the food industry. Tea and coffee bags use wet-laid non-
wovens. Meats, vegetables and fruits are now frequently packed with a nonwoven
insert to absorb liquids. Other fruits and vegetable products are supplied in knitted
Strong, lightweight spunbonded and equivalent nonwoven paper-like materials
are particularly useful for courier envelopes while adhesive tapes, often reinforced
with ﬁbres, yarns and fabrics, are increasingly used in place of traditional twine.
Woven strappings are less dangerous to cut than the metal bands and wires tradi-
tionally used with densely packed bales.
A powerful driver of the development and use of textiles in this area is increas-
ing environmental concern over the disposability and recycling of packaging
materials. Legislation across the European Union, implemented especially vigor-
ously in countries such as Germany, is now forcing many manufacturers and
distributors of products to rethink their packaging practices fundamentally.
1.5.9 Sport and leisure
Even excluding the very considerable use of textiles in performance clothing and
footwear, there are plenty of opportunities for the use of technical textiles through-
out the sports and leisure market. Applications are diverse and range from artiﬁcial
turf used in sports surfaces through to advanced carbon ﬁbre composites for racquet
frames, ﬁshing rods, golf clubs and cycle frames. Other highly visible uses are balloon
fabrics, parachute and paraglider fabrics and sailcloth.
Growth rates are well above average and unit values are often very high. The
sports sector is receptive to innovation and developers of new ﬁbres, fabrics and
coatings often aim them at this market, at least initially. Many of the products and
ideas introduced here eventually diffuse through to the volume leisure market and
even the street fashion market.
1.5.10 Geotextiles in civil engineering
Although still a surprisingly small market in volume and value terms, considering
the amount of interest and attention it has generated, the geosynthetics market
(comprising geotextiles, geogrids and geomembranes) is nevertheless expected to
show some of the highest growth rates of any sector over the foreseeable future.
The economic and environmental advantages of using textiles to reinforce, sta-
bilise, separate, drain and ﬁlter are already well proven. Geotextiles allow the build-
ing of railway and road cuttings and embankments with steeper sides, reducing
the land required and disturbance to the local environment. Revegetation of these
Technical textiles market – an overview 17
embankments or of the banks of rivers and waterways can also be promoted using
appropriate materials. There has been renewed interest in ﬁbres such as woven jute
as a biodegradable temporary stabilising material in such applications.
As in the case of construction textiles, one of the problems faced by manu-
facturers and suppliers of these materials is the sheer diversity of performance
requirements. No two installations are the same in hydrological or geological terms
or in the use to which they will subsequently be put. Suppliers to this market need
to develop considerable expertise and to work closely with engineers and consul-
tants in order to design and specify suitable products.
Because of the considerable areas (quantities) of fabric that can be required in
a single project, cost is always a consideration and it is as essential not to overspecify
a product as not to underspecify it. Much of the research and development work
undertaken has been to understand better the long term performance characteris-
tics of textiles which may have to remain buried in unpredictable environments
(such as landﬁll and toxic waste sites) for many years and continue to perform to
an adequate standard.
Nonwovens already account for up to 80% of geotextile applications. This is
partly a question of economics but also of the suitability of such textile structures
for many of the ﬁltration and separation duties that they are called upon to perform.
Current interest is in ‘composite’ fabrics which combine the advantages of different
textile constructions such as woven, knitted, nonwoven and membrane materials. To
supply the diversity of fabrics needed for the many different applications of geot-
extiles, leading specialist manufacturers are beginning to assemble a wide range of
complementary capabilities by acquisition and other means.
1.5.11 Protective and safety clothing and textiles
Textiles for protective clothing and other related applications are another impor-
tant growth area which has attracted attention and interest somewhat out of pro-
portion to the size and value of the existing market. As in the case of sports textiles,
a number of relatively high value and performance critical product areas have
proved to be an ideal launch pad for a new generation of high performance ﬁbres,
most notably the aramids, but including many other speciality materials.
The variety of protective functions that needs to be provided by different textile
products is considerable and diverse. It includes protection against cuts, abrasion,
ballistic and other types of severe impact including stab wounds and explosions, ﬁre
and extreme heat, hazardous dust and particles, nuclear, biological and chemical
hazards, high voltages and static electricity, foul weather, extreme cold and poor
As well as people, sensitive instruments and processes also need to be protected.
Thus, clean room clothing is an important requirement for many industries includ-
ing electronics and pharmaceuticals.
In Europe and other advanced industrial regions, strict regulations have been
placed upon employers through the introduction of legislation such as the Personal
Protective Equipment (PPE) at Work Regulations (European Union). Under such
legislation, it is not only necessary to ensure that the equipment and clothing pro-
vided is adequate to meet the anticipated hazards but also that it is also used effec-
tively, that is that the garments are well designed and comfortable to wear. This
has opened up a need for continuing research not only into improved ﬁbres and
18 Handbook of technical textiles
materials but also into increasingly realistic testing and assessment of how garments
perform in practice, including the physiology of protective clothing.
In many developing countries, there has not been the same legislative framework
in the past. However, this is rapidly changing and future market growth is likely to
concentrate less on the mature industrial markets than upon the newly industrial-
ising countries of Asia and elsewhere. The protective clothing industry is still highly
fragmented with much of the innovation and market development being provided
by the major ﬁbre and other materials producers. This could change as some global
suppliers emerge, perhaps without their own direct manufacturing but relying on
contract producers around the world, very much as the mainstream clothing indus-
try does at present.
1.5.12 Ecological protection textiles
The ﬁnal category of technical textile markets, as deﬁned by Techtextil, is technical
textiles for protection of the environment and ecology. This is not a well deﬁned
segment yet, although it overlaps with several other areas, including industrial tex-
tiles (ﬁltration media), geotextiles (erosion protection and sealing of toxic waste)
and agricultural textiles (e.g. minimising water loss from the land and reducing the
need for use of herbicides by providing mulch to plants).
Apart from these direct applications, technical textiles can contribute towards
the environment in almost every sphere of their use, for example by reducing weight
in transport and construction and thereby saving materials and energy. Improved
recycleability is becoming an important issue not only for packaging but also for
products such as cars.
Composites is an area which potentially presents problems for the recycleability
of textile reinforcing materials encased within a thermosetting resin matrix.
However, there is considerable interest in and development work being done on
thermoplastic composites which should be far simpler to recycle, for example by
melting and recasting into lower performance products.
1.6 Globalisation of technical textiles
If North America and Western Europe have the highest levels of per capita con-
sumption of technical textiles at present (see Table 1.1), then they are also relatively
mature markets. The emerging countries of Asia, Eastern Europe and the rest of
the world are becoming important markets in almost every sphere, from automo-
tive manufacture through to sporting and leisure goods. Technical textiles for food
production, construction and geotextiles are likely to be particularly important. In
the case of the last of these, geotextiles, consumption up to the year 2005 is expected
to grow at over 12% per annum across the whole of Asia compared with less than
6% in Western Europe and the USA. In the case of Eastern Europe and South
America, annual growth rates could be as high as 18% and 16% per annum respec-
tively, although from relatively small base levels at present.
In 2000, the major existing users, North America, Western Europe and Japan, are
expected to account for less than 65% of total technical textile consumption; by the
year 2005, this could be down to 60% and perhaps below 50% by 2010. Consump-
tion of technical textiles in China already exceeds that of Japan, in weight terms at
Technical textiles market – an overview 19
Table 1.4 Worldwide consumption of technical textiles by geographical region, 2000–2005
103 tonnes $ million
2000 2005 2000 2005
(% pa) (% pa)
Western Europe 2 690 3 110 2.9 13 770 15 730 2.7
Eastern Europe 420 560 5.9 2 500 3 260 5.5
North America 3 450 3 890 2.4 16 980 18 920 2.2
South America 350 430 4.2 1 870 2 270 3.9
Asia 3 560 4 510 4.8 20 560 25 870 4.7
Rest of the world 870 1 190 6.5 4 590 6 280 6.5
Total 11 340 13 690 3.9 60 270 72 330 3.7
Source: David Rigby Associates/Techtextil.
least. In 2000, Chinese technical textiles are expected to account for almost 20% of
all textile manufacturing in that country and over 12% of total world consumption
(see Table 1.4).
But globalisation is not just about increasing internationalisation of markets. It
is also about the emergence of companies and supply chains which operate across
national and continental boundaries. Such globalisation has already proceeded fur-
thest in the automotive and transport industry, the largest of the 12 market segments
deﬁned above. It is a path already being followed within the other major segments,
most notably industrial textiles and medical/hygiene textiles and will become
increasingly evident in the remainder.
Characteristics of globalisation include higher levels of international trade and
increased specialisation of manufacture within individual districts, countries and
regions, according to availability of materials, local industry strengths and regional
Relatively low unit value products requiring a signiﬁcant amount of making-up
or other fabrication such as bags and sacks have already seen a signiﬁcant shift of
manufacturing towards the Far East and Eastern Europe. Textiles for tents, luggage
and the technical components of footwear and clothing are now increasingly
sourced close to where many of these products are manufactured for export, for
example China and Indonesia.
Manufacturers in the newly industrialising world are rapidly adopting the latest
materials and processing technologies. Taiwan already has an important composites
manufacturing sector specialising in sports equipment.
1.7 Future of the technical textiles industry
The future of technical textiles embraces a much wider economic sphere of activity
than just the direct manufacturing and processing of textiles. The industry’s sup-
pliers include raw materials producers (both natural and artiﬁcial), machinery
and equipment manufacturers, information and management technology providers,
R&D services, testing and certiﬁcation bodies, consultants, education and training
organisations. Its customers and key speciﬁers include almost every conceivable
able 1.5 Technical textile functions, markets and end-uses
Protection Insulation Reinforcement Containment Filtration Absorption Miscellaneous
ndustry Engineering High Acoustic barriers Composites – Bags & sacks Dust Oil spillages Thermal
Food, temperature Thermal FRP and FIBCs ﬁltration Wicks stencil
pharmaceuticals textiles insulation advanced Balewrap Air paper
Chemicals, plastics Welders anti- Seals, joints Printed circuit Tape conditioning
spatter sheets Packings boards Curing tape Process
Other Fire blankets Pressed felt Optical ﬁbre/ Hosepipes liquid
manufacturing Dustproof components electrical Nets Efﬂuent
Power, oil, gas fabric Electrical cables Webbing treatment
Mining, quarrying Electrostatic insulation tape Electrical Diaphragms Papermakers
shielding Heating elements cables Envelopes felts
Debris, safety Electromagnetic Jacquard Floppy disc Battery
nets shields harness liners separators
Solar Electroconductive Pressure hoses Tea/coffee
protection fabrics Drive belts bags
Dielectric fabrics Conveyor belts Cigarette
Aerials Bearing ﬁlters
materials Food casing
Abrasive discs Machine
ransport Road Seat belts Sound barriers Tyre cord Containers Air ﬁlters Oil booms Decorative/
Aviation Air bags for roofs, Hoses, pipes, Tarpaulins (engine) functional
Marine Flotation bonnets etc. drive belts & Covers Air ﬁlters interior
(Military) devices Tank insulation other MRG Cordage (passenger) textiles
Inﬂatable Brake/clutch Twine Oil ﬁlters (UV, FR)
boats lining Cargo nets, Fuel ﬁlters
Parachutes Gaskets, seals straps
Ropes, cables Composites – Balloons
Barriers, nets FRP & Sailcloth
Camouﬂage, advanced Gliders
decoy Tow ropes Hovercraft
FR textiles skirts
Technical textiles market – an overview 23
downstream industry and ﬁeld of economic activity, including the architects, en-
gineers, designers and other advisors employed by those industries. In between lie
many other interested parties, including environmental, health, safety, business and
free trade regulators, patent and intellectual property agents and lawyers, investors,
bankers, regional investment agencies and providers of development aid.
The task of disseminating and communicating information to all these organisa-
tions and individuals is undertaken by a growing number of specialist and general-
ist publications as well as by international and local trade exhibitions, fairs, seminars
The economic importance of technical textiles worldwide therefore undoubtedly
far exceeds the $60 billion estimated in Tables 1.2–1.4 just for basic ﬁbres, yarns and
1.7.1 A changing strategic environment
If the 1980s was a period when the technical textiles industry enjoyed a rapid and
increasing awareness of its existence by the outside world (as well as within the
mainstream textile industry), then the 1990s was an era of more mature commer-
cial development and consolidation as ﬁbre producers and textile manufacturers
alike concentrated on overhauling and refocusing their businesses in the wake of
The new millennium promises even ﬁercer international competition which
will see manufacturers striving to engineer costs downwards and develop global
economies of scale in production and product development. Technical textiles will
become better ‘value for money’ than ever before and this should open the way
towards further applications as existing end-uses mature.
Individual companies will become less deﬁned by the technologies and ma-
terials they use than by the markets and applications they serve. Table 1.5 sum-
marises some of the key market areas and the functions which technical textiles
perform, with examples of individual products in each category. It does not pretend
to be an exhaustive list which would run into many thousands of products and would
constantly be changing.
1. The Textile Institute, Textile Terms and Deﬁnitions, Tenth Edition, Textile Institute, Manchester, 1994.
2. sabit adanur, Wellington Sears Handbook of Industrial Textiles, Technomic, Lancaster PA (USA),
3. ISO 9092:1988 Deﬁnition of nonwovens.
Department of Textiles, Faculty of Technology, Bolton Institute, Deane Road,
Bolton BL3 5AB, UK
A number of deﬁnitions1–3 have been used to describe the term ‘technical textiles’
with respect to their intended use, functional ability and their non-aesthetic or dec-
orative requirements. However, none of these carefully chosen words include the
fundamental ﬁbre elements, technical or otherwise, which make up the technical
textile structures. The omission of the word ‘ﬁbre’ may indeed be deliberate as most
technical textile products are made from conventional ﬁbres that are already well
established. In fact over 90% of all ﬁbres used in the technical sector are of the con-
ventional type.4 Specially developed ﬁbres for use in technical textiles are often
expensive to produce and have limited applications.
Historically, utilisation of ﬁbres in technical capacities dates back to the early
Egyptians and Chinese who used papyrus mats to reinforce and consolidate the
foundations respectively of the pyramids and the Buddhist temples.5,6 However,
their serious use in modern civil engineering projects only began after the ﬂoods of
1953 in The Netherlands in which many people lost their lives. The event initiated
the famous Delta works project in which for the ﬁrst time synthetic ﬁbres were
written into the vast construction programme.7 Since then, geotextiles in particular
have matured into important and indispensable multifunctional materials.
Use of silk in semitechnical applications also goes back a long way to the light-
weight warriors of the Mongolian armies, who did not only wear silk next to
their skin for comfort but also to reduce penetration of incoming arrows and enable
their subsequent removal with minimal injury. Use of silk in wound dressing
and open cuts in web and fabric form also dates back to the early Chinese and
In light of extensive utilization of conventional ﬁbres in the technical sector, this
chapter initially attempts to discuss ﬁbres under this category highlighting their
importance and the scope of their versatility. The discussion covers concisely an
outline of ﬁbre backgrounds, chemical compositions and their salient characteris-
tics. It then introduces other ﬁbres which have been specially developed to perform
Technical ﬁbres 25
under extreme stress and/or temperature; ultraﬁne and novel ﬁbres are also dis-
cussed. Finally, the chapter concludes by identifying areas of application and the
roles that selected ﬁbres play in fulﬁlling their intended purpose.
Table 2.1 presents the complete range of ﬁbres available to the end-user and
some of their mechanical properties.
2.2 Conventional ﬁbres
2.2.1 Natural ﬁbres
Cotton accounts for half of the world’s consumption of ﬁbres and is likely to remain
so owing to many of its innate properties and for economical reasons8 that will not
be discussed here. Cotton is made of long chains of natural cellulose containing
carbon, hydrogen and oxygen otherwise known as polysaccharides. The length of
the chains determines the ultimate strength of the ﬁbre. An average of 10 000 cel-
lulosic repeat or monomeric units make up the individual cellulose chains which are
about 2 mm in length. The linear molecules combine into microﬁbrils and are held
together by strong intermolecular forces to form the cotton ﬁbre. The unique physi-
cal and aesthetic properties of the ﬁbre, combined with its natural generation and
biodegradability, are reasons for its universal appeal and popularity. Chemical treat-
ments such as Proban9 and Pyrovatex10 are two examples of the type of durable ﬁn-
ishes that can be applied to make cotton ﬁre retardant. High moisture absorbency,
high wet modulus and good handle are some of the more important properties of
Wool, despite its limited availability and high cost, is the second most important
natural ﬁbre. It is made of protein: a mixture of chemically linked amino acids which
are also the natural constituents of all living organisms. Keratin or the protein in
the wool ﬁbre has a helical rather than folded chain structure with strong inter- and
intrachain hydrogen bonding which are believed to be responsible for many of its
unique characteristics. Geographical location, the breeding habits of the animals,
and climatic conditions are some of the additional variables responsible for its prop-
erties. The overall high extensibility of wool, its natural waviness and ability to trap
air has a coordinated effect of comfort and warmth, which also make it an ideal
insulating material. The sophisticated dual morphology of wool produces the char-
acteristic crimp which has also been an inspiration for the development of some
highly technical synthetic ﬁbres. Wool is inherently ﬁre retardant, but further
improvements can be achieved by a number of ﬁre-retardant treatments. Zirco-
nium- and titanium-treated wool is one such example which is now universally
referred to as Zirpro (IWS) wool.11
Flax, jute, hemp and ramie, to name but a few of the best ﬁbres, have tradition-
ally taken a secondary role in terms of consumption and functional requirements.
They are relatively coarse and durable, and ﬂax has traditionally been used for linen
making. Jute, ramie and to a lesser extent other ﬁbres have received attention within
the geotextile sector of the ﬁbre markets which seeks to combine the need for tem-
porary to short-term usage with biodegradability, taking into account the regional
availability of the ﬁbres.
Silk is another protein-based ﬁbre produced naturally by the silkworm, Bombyx
Mori or other varieties of moth. Silk is structurally similar to wool with a slightly
able 2.1 Fibres available to the end-user and associated mechanical properties
High chemical and
High strength high modulus High performance
onventional ﬁbres combustion-resistant Ultraﬁne and novelty ﬁbres
organic ﬁbres inorganic ﬁbres
atural Para-aramids Meta-aramids Carbon Microﬁbres; (linear density
g. cotton, wool, silk, jute, e.g. Kevlar (Du Pont) and e.g. Nomex (Du Pont) Ceramics <0.5 dtex)
etc. Twaron (Acordis) and Conex (Teijin) Boron Solar energy absorbing ﬁbres
egenerated Polybenzobisthiazole Kermel (Rhodia) Tungsten (solar alpha)
g. viscose, acetates tencel, (PBT) Kynol (Kynol) Alumina (e.g. Safﬁl) Heat-sensitive ﬁbres
etc. Ultra-high molecular Oxidised acrylic High modulus silicon (thermochromics)
ynthetics weight polyethylene ﬁbres, e.g. Panox (SGL) Carbide & silicon Scented ﬁbres
g. polyamide, polyester, e.g. Dyneema (DSM) and Others: Aromatic nitride etc. Antibacterial ﬁbres
polyacrylics, polyurethanes, Spectra (Allied Signal) polymers; (aseptic chloroﬁbres)
polyoleﬁns, etc. Polyether ether Hollow ﬁbres
ketone, PEEK Antistatic ﬁre-retardant
(Victrex and Zyex) ﬁbres; etc.
sulphide, PPS, e.g.
PTFE, e.g. Teﬂon (Du Pont)
(Inspec formerly Lenzing) P84
enacity: Tenacity: Tenacity: Tenacity: Tenacity:
1–0.5 N tex-1 1.5–3 N tex-1 1–2 N tex-1 0.5–2 N tex-1 0.1–0.4 N tex-1
Modulus: Modulus: Modulus: Modulus: Modulus:
–18 N tex-1 25–150 N tex-1 15–25 N tex-1 70–220 N tex-1 2–15 N tex-1
% Elongation: 2–7 % Elongation: 1–8 % Elongation: 1–4 % Elongation: 0–1.5 % Elongation: 2–17
LOIa: 0.20–0.40 LOI: 0.23–0.55
LOI: limiting oxygen index = minimum fraction of oxygen in nitrogen necessary to sustain burning.
Technical ﬁbres 27
different combination of amino acids which make up the protein or the ﬁbroin, as
it is more appropriately known. Silk is the only naturally and commercially pro-
duced continuous ﬁlament ﬁbre which has high tenacity, high lustre and good dimen-
sional stability. Silk has been and will remain a luxury quality ﬁbre with a special
place in the ﬁbre market. However, its properties of biocompatibility and gradual
disintegration, as in sutures, have long been recognised in medical textiles.
2.2.2 Regenerated ﬁbres
Viscose rayon was the result of the human race’s ﬁrst attempts to mimic nature in
producing silk-like continuous ﬁbres through an oriﬁce. Cellulose from wood pulp is
the main constituent of this novel system, started commercially in the early 1920s.
Thin sheets of cellulose are treated with sodium hydroxide and aged to allow molec-
ular chain breakage. Further treatment with carbon disulphide, dissolution in dilute
sodium hydroxide and ageing produces a viscous liquid, the viscose dope, which is
then extruded into an acid bath. The continuous ﬁlaments that ﬁnally emerge are
washed, dried and can be cut to staple lengths. The shorter cellulose molecules in
viscose and their partial crystallisation accounts for its rather inferior physical prop-
erties relative to cotton. Further development and reﬁnement of the manufacturing
technique have created a whole range of ﬁbres with improved properties. High tenac-
ity and high wet modulus viscose compare in all but appearance to cotton in both dry
and wet conditions. Chemically altered regenerated cellulose di- and triacetates do
not burn like cotton and viscose to leave a ﬂuffy black ash, but melt and drip instead.
This characteristic enables them to be shaped or textured to enhance their visual and
aesthetic appeal. Hollow viscose modiﬁcations give enhanced bulk and moisture
absorbency and have an improved cotton-like feel.
Fire-retardant (FR) viscose was ﬁrst introduced in the 1960s. A major example
is produced by Lenzing in Austria by incorporating organophosphorous compounds
into the spinning dope prior to extrusion. The additive is reasonably stable and has
no chemical interaction with the cellulose molecules. It is also unaffected by bleach-
ing, washing, dry cleaning, dyeing and ﬁnishing processes.10 Early in the 1990s
Kemira (now Sateri Fibres) of Finland introduced an alternative version of FR
viscose known as Visil in which polysilicic acid is present. The ﬁbre chars upon
heating leaving a silica residue.
Lyocell,12 is the latest addition to this series of ﬁbres, commercially known as
Tencel (Acordis), has all the conventional properties of viscose in addition to its
much praised environmentally friendly production method. The solvent used is
based on non-toxic N-methyl morpholine oxide used in a recyclable closed loop
system, which unlike the viscose process avoids discharge of waste. Highly absorbent
derivatives of Tencel, known as Hydrocell are establishing a foothold in wound
dressing and other medical-related areas of textiles.
2.2.3 Synthetic ﬁbres
All synthetic ﬁbres originate from coal or oil. The ﬁrst synthetic ﬁbre that appeared
on the world market in 1939 was nylon 6.6. It was produced by DuPont and gained
rapid public approval. A series of nylons commonly referred to as polyamides now
exists in which the amide linkage is the common factor. Nylon 6.6 and nylon 6 are
most popular in ﬁbre form. They are melt extruded in a variety of cross-sectional
shapes and drawn to achieve the desired tenacity. They are well known for their high
28 Handbook of technical textiles
extensibility, good recovery, dimensional stability and relatively low moisture
absorbency. Nylon 6.6 in particular soon became a popular household carpet ﬁbre
and was developed into ﬁbres commonly known as Antron13 manufactured by
DuPont. Antron ﬁbres of various generations use additives, varied cross-sectional
shapes and modiﬁed surface characteristics to enhance the aesthetic and visual
appeal of carpets as well as improving their resilience and dissipating static charges.
Nylon was later surpassed by the even more popular ﬁbre known as polyester,
ﬁrst introduced as Dacron by DuPont in 1951. Polyester is today the second most
used ﬁbre after cotton and far ahead of other synthetics both in terms of produc-
tion and consumption. Polyethylene terephthalate or polyester is made by conden-
sation polymerisation of ethylene glycol and terephthalic acid followed by melt
extrusion and drawing. It can be used in either continuous form or as short staple
of varying lengths. The popularity of polyester largely stems from its easycare char-
acteristics, durability and compatibility with cotton in blends. Its very low moisture
absorbency, resilience and good dimensional stability are additional qualities. Many
manufacturers across the world produce polyester under different commercial
names with almost tailor-made properties. A high glass transition temperature of
around 70 °C with good resistance to heat and chemical degradation also qualiﬁes
this polymer for most technical textile applications. These will be discussed in
greater detail later. Flame-retardant Trevira CS and Trevira high tenacity, both poly-
esters developed and marketed by Trevira GmbH in Germany, are examples of the
many varieties available today.
Wool-like properties are shown by polyacrylic ﬁbres which are produced by the
polymerisation of acrylonitrile using the addition route into polyacrylonitrile. They
can then be spun into ﬁbres by dry or wet spinning methods. Orlon14 was produced
by DuPont. It had a distinctive dumbbell shaped cross-section and was extruded by
the dry process in which the solvent is evaporated off. Acrilan15 produced by Mon-
santo and Courtelle produced by Acordis are spun by the wet extrusion technique
and have near circular cross-sections. Acrylic ﬁbres now also appear in bicompo-
nent form with wool-like characteristics. Chemically modiﬁed acrylics, principally
the modacrylics, include chlorine atoms in their molecular structure which are
responsible for their low burning behaviour and, unlike acrylics, have the ability to
self-extinguish once the source of ignition has been removed. A selected ﬁbre in
terms of ﬁbre chemistry is Oasis,16 a superabsorbent ﬁbre made by the collabora-
tive efforts of Acordis and Allied Colloids, based on crosslinking copolymers of
acrylic acid. This ﬁbre is claimed to absorb moisture many times its own weight and
holds it even under pressure. Its application in hygiene and medical care in differ-
ent forms is being pursued.
Polyoleﬁn ﬁbres include both polyethylene and polypropylene made by addition
polymerisation of ethylene and propylene and subsequent melt extrusion, respec-
tively. Polyethylene has moderate physical properties with a low melting tempera-
ture of about 110 °C for its low density form and about 140 °C for its high density
form which severely restricts its application in low temperature applications.
Polypropylene has better mechanical properties and can withstand temperatures of
up to 140 °C before melting at about 170 °C. Both polymers have a density less than
that of water which allows them to ﬂoat as ropes, nets and other similar applica-
tions. The availability, low cost and good resistance to acid and alkaline environ-
ments of polypropylene has greatly inﬂuenced its growth and substantial use in
Technical ﬁbres 29
glass ose polyester
0 10 20 30 40
2.1 Stress/strain behaviour of some common ﬁbres.
Finally, elastane ﬁbres17 are synthetic-based elastomeric polymers with at least
85% segmented polyurethane in their structure. They have rubber-like properties,
which means they can be extended up to six or more times their original length.
They are used in combination with most natural and synthetic ﬁbres in knitted and
woven materials. They were initially produced by DuPont in 1959 under the now
well-known trademark of Lycra.
Figure 2.1 presents typical stress/strain behaviour for most conventional ﬁbres.
Tenacity, modulus and percentage elongation ranges for most conventional ﬁbres
are also given at the bottom of Table 2.1.
2.3 High strength and high modulus organic ﬁbres
Keller’s much-published18 contribution to the understanding of crystal growth in
1957 and conﬁrmation of the tendency of polymers to form folded-chain crystals,
provided the insight and inspiration for development of high strength, high modulus
organic ﬁbres that would surpass conventional ﬁbres. During crystallisation, long
chains of molecules fold back on themselves to form folded-chain crystals which
only partly unfold during normal drawing. In the Netherlands in the 1970s DSM
developed a super drawing technique known as gel spinning, which uses dilute solu-
tions of ultra-high molecular weight polymers such as polyethylene to unfold the
chains further and thus increase both tensile strength and ﬁbre modulus. Ultra-high
molecular weight polyethylene (UHMWPE) ﬁbres, Dyneema or Spectra, are today
the strongest ﬁbres known, with tensile moduli in excess of 70 GN m-2. Weight for
weight this ﬁbre genus is claimed to be 15 times stronger than steel and twice as
strong as aromatic polyamides such as Kevlar.19 It is also low in density, chemically
inert and abrasion resistant. It, however, melts at around 150 °C and thermally
degrades at 350 °C which restrict its use to low temperature applications.
To achieve even better performance characteristics at higher temperatures, other
means of ﬁbre production were explored in the 1960s. One successful approach
eventually led to the advent of liquid crystalline polymers. These are based on poly-
merisation of long stiff molecules such as para-phenylene terephthalamide achiev-
ing molecular weights averaging to around 20 000. The inﬂuence of the stiff aromatic
rings, together with hydrogen-bonding crosslinks, combines the best features of both
the polyamides and the polyesters in an extended-chain conﬁguration.18–20 Molecu-
lar orientation of these ﬁbres is brought about by capillary shear along the ﬂow of
30 Handbook of technical textiles
the polymer as it exits from the spinneret thus overriding the need for subsequent
drawing. Kevlar by DuPont and Twaron by Akzo (now Acordis) were the ﬁrst of
such ﬁbres to appear in the early 1970s. There now exists a series of ﬁrst, second
and third generations of para-aramids. Kevlar HT for instance, which has 20%
higher tenacity and Kevlar HM which has 40% higher modulus than the original
Kevlar 29 are largely utilised in the composite and the aerospace industries. Para-
aramids generally have high glass transition temperatures nearing 370 °C and do not
melt or burn easily, but carbonise at and above 425 °C. All aramid ﬁbres are however
prone to photodegradation and need protection against the sun when used out of
doors. These will be discussed later.
Other high tenacity and high modulus ﬁbres include the isotropically spun Tech-
nora (Teijin) and Supara, based upon para-aramid copolymers, with slightly lower
maximum strength and modulus values than Kevlar. Several other melt-spinnable
liquid crystalline polymers are also available.21
2.4 High chemical- and combustion-resistant organic ﬁbres
The ﬁbres discussed in the previous section were developed following earlier obser-
vations that aromatic polymer backbones yielded improved tensile and heat resis-
tance compared with conventional ﬁbres. However, if the polymer chains have lower
symmetry and order, then polymer tractability and textile ﬁbre characteristics are
improved. Solvent-spun Nomex and Conex were the ﬁrst so-called meta-aramids
made from poly(meta-phenylene isophthalamide) and were produced by DuPont
in 1962 and by Teijin in 1972, respectively. The meta-phenylene isophthalamide mol-
ecule is identical in all but the position of its —NH— and —CO— groups to para-
phenylene terephthalamide (or Kevlar) molecules. The different positioning of
these groups in meta-aramids creates a zig-zag molecular structure that prevents it
from full crystallisation thus accounting for its relatively poorer tensile properties.
However, Nomex is particularly well known for its resistance to combustion, high
decomposition temperature prior to melting and high limited oxygen index (LOI),
the minimum amount of oxygen required to induce ignition.
Melt-spinnable aromatic ﬁbres with chains containing paraphenylene rings, like
polyether ether ketone (PEEK),23 polyether ketone (PEK) and poly(p-phenylene
sulphide) (PPS),22 also have high melting points but, since their melting points occur
prior to their decomposition temperature, they are unsuitable for ﬁre-retardant
applications. However, their good chemical resistance renders them suitable for low
temperature ﬁltration and other corrosive environments.
The polyheterocyclic ﬁbre, polybenzimidazole or PBI, produced by Hoechst-
Celanese has an even higher LOI than the aramids. It has excellent resistance to
both heat and chemical agents but remains rather expensive. P84, initially produced
by Lenzing and now produced by Inspec Fibres, USA, comprises polyimide groups
that yield reasonably high resistance to ﬁre and chemical attack. The acrylic
copolymer-based ﬁbre produced by Acordis known as Inidex (although now no
longer produced) unlike many aramid ﬁbres has high resistance to UV (ultraviolet)
radiation and a fairly high LOI at the expense of much reduced tenacity and rather
low long-term exposure resistance to heat.
Oxidised acrylic ﬁbre, best known as Panox (SGL, UK) is another crosslinked,
high combustion-resistant material produced by combined oxidation and pyrolysis
Technical ﬁbres 31
Table 2.2 LOI and tenacity range of some high chemical-
and combustion-resistant organic ﬁbres
Fibres brand LOI Tenacity
name (%) (GPa)
Nomex Du Pont 29 0.67
Conex Conex 29 0.61
Kermel Rhone-Poulenc 31 0.53
Inidex Courtaulds 43 0.12
PBI Hoechst-Celanese 41 0.39
PAN-OX RK Textiles 55 0.25
PPS Phillips 34 0.54
of acrylic ﬁbres at around 300 °C. Although black in appearance, it is not classed as
carbon ﬁbre and preserves much of its original non-carbonaceous structure. In addi-
tion, it does not have the graphitic or turbostratic structure of carbon ﬁbres. It
retains a sufﬁciently high extension-at-break to be subjected to quite normal textile
processes for yarn and fabric formation.24 Panox has a very high LOI of 0.55. Fully
carbonised, or carbon ﬁbres with even higher tensile properties, are achieved by full
carbonisation of these oxidised precursor ﬁbres or by the melt spinning of liquid
crystalline mesophase pitch followed by their oxidation and pyrolysis. These are dis-
cussed again in the section on inorganic ﬁbres.
Table 2.2 shows the LOI and tenacity range of some of the better known high
chemical- and combustion-resistant organic ﬁbres.
2.5 High performance inorganic ﬁbres
Any ﬁbre that consists of organic chemical units, where carbon is linked to hydro-
gen and possibly also to other elements, will decompose below about 500 °C and
cease to have long-term stability at considerably lower temperatures. For use at high
temperatures it is therefore necessary to turn to inorganic ﬁbres and ﬁbres that
consist essentially of carbon.25
Glass, asbestos and more recently carbon are three well-known inorganic ﬁbres
that have been extensively used for many of their unique characteristics. Use of glass
as a ﬁbre apparently dates back to the ancient Syrian and Egyptian civilisations26
which used them for making clothes and dresses. However, the very high modulus
or stiffness displayed by these ﬁbres means that they are quite brittle and can easily
be damaged by surface marks and defects. They are, therefore, best utilised by
embedding in matrix forms where the ﬁbres are fully protected. Epoxy resins, poly-
ester and other polymers, as well as cement, have commonly been used both to
protect and to make use of their contributory strength. Glass-reinforced boat hulls
and car bodies, to name but two application areas of such composites, reduce overall
weight and cost of fabrication as well as eliminating the traditional problems of
rotting wood and rusting metals associated with traditional materials. Their good
resistance to heat and very high melting points have also enabled them to be used
as effective insulating materials.
32 Handbook of technical textiles
Asbestos27 is a generic name for a variety of crystalline silicates that occur natu-
rally in some rocks. The ﬁbres that are extracted have all the textile-like properties
of ﬁneness, strength, ﬂexibility and more importantly, unlike conventional ﬁbres,
good resistance to heat with high decomposition temperatures of around 550 °C.
Their use as a reinforcement material has been found in clay-rich prehistoric
cooking pots discovered in Finland.28 In more recent times they have been exten-
sively used to reinforce brittle matrices such as cement sheeting, pipes, plastics29 and
also as heat insulators. However, with the discovery of their carcinogenic hazards,
their use has gradually declined and alternative ﬁbres have been developed to
replace them totally.
High purity, pyrolysed acrylic-based ﬁbres are classiﬁed as carbon ﬁbres. The
removal of impurities enhances carbon content and prevents the nucleation and
growth of graphite crystals which are responsible for loss of strength in these ﬁbres.
Carbon ﬁbres with different structures are also made from mesophase pitch. The
graphite planes in PAN-based ﬁbres are arranged parallel to the ﬁbre axis
rather than perpendicular as is the case with pitch-based carbon ﬁbres.28 Their high
strength and modulus combined with relatively low extensibility means that they
are best utilised in association with epoxy or melt-spinnable aromatic resins as
Increasing demand in the defence and aerospace industries for even better per-
formance under extreme conditions led, within the last quarter of the 20th century,
to yet another range of new and rather expensive metal oxides, boron and silicon-
based ﬁbres. These are often referred to as ceramic ﬁbres and will now be brieﬂy
Aluminosilicate compounds are mixtures of aluminium oxide (Al2O) and silicon
oxide (SiO2); their resistance to temperature depends on the mixing ratio of the two
oxides. High aluminium oxide content increases their temperature tolerance from
a low of 1250 °C to a maximum of 1400 °C. However, despite their high tempera-
ture resistance, these ﬁbres are not used in high stress applications owing to their
tendency to creep at high temperatures.29 Their prime applications are in insulation
of furnaces and replacement of asbestos ﬁbres in friction materials, gaskets and
packings.30 Both aluminium oxide or alumina ﬁbres and silicon oxide or silica ﬁbres
are also produced. Pure boron ﬁbres are too brittle to handle but they can be coated
on tungsten or carbon cores. Their complex manufacturing process makes them
rather expensive. Their prime application is in lightweight, high strength and high
modulus composites such as racket frames and aircraft parts. Boron ﬁbre use is
limited by their thickness (about 16 mm), their relatively poor stability in metal
matrices and their gradual loss of strength with increasing temperature.31 Boron
nitrides (BN) are primarily used in the electronic industry where they perform both
as electrical insulators and thermal conductors.
The most outstanding property of silicon carbide (SiC) is the ability to function
in oxidizing conditions up to 1800 °C with little loss of mechanical properties. Silicon
carbide exceeds carbon ﬁbre in its greater resistance to oxidation at high tempera-
tures, its higher compressive strength and better electrical resistance. SiC ﬁbres
containing carbon, however, lose some tensile properties at the expense of gaining
better electrical conductivity.
Finally, many of the inorganic ﬁbres so far referred to are now also produced
in microcrystalline or whisker form and not in the more normal textile-ﬁbre form.
Whiskers have extremely good mechanical properties and their tensile strength is
Technical ﬁbres 33
usually three to four times those of most reinforcing ﬁbres. They are, however, costly
to produce and their inclusion into composite structures is both difﬁcult and
2.6 Ultra-ﬁne and novelty ﬁbres
Ultra-ﬁne or microﬁbres were developed partly because of improved precision in
engineering techniques and better production controls, and partly because of the
need for lightweight, soft waterproof fabrics that eliminate the more conventional
coating or lamination processes.32 As yet there are no universal deﬁnitions of
microﬁbres. Textile Terms and Deﬁnitions2 simply describes them as ﬁbres or ﬁla-
ments with linear densities of approximately 1.0 dtex or less. Others33,34 have used
such terms as ﬁne, extra-ﬁne and micro-ﬁne corresponding to linear densities
ranging from 3.0 dtex to less than 0.1 dtex. They are usually made from polyester
and nylon polymers, but other polymers are now being made into microﬁbres. The
Japanese ﬁrst introduced microﬁbres in an attempt to reproduce silk-like proper-
ties with the addition of enhanced durability. They are produced by at least
three established methods including island-in-sea, split process and melt spinning
techniques and appear under brand names such as Mitrelle, Setila, Micrell, Tactel
and so on. Once in woven fabric form their ﬁne diameter and tight weave allows
up to 30 000 ﬁlaments cm-2, making them impermeable to water droplets whilst
allowing air and moisture vapour circulation. They can be further processed to
enhance other characteristics such as peach-skin and leather-like appearances. The
split technique of production imparts sharp-angled edges within the ﬁbre surface,
which act as gentle abraders when made into wiping cloths that are used in the
optical and precision microelectronic industries. Microﬁbres are also used to
make bacteria barrier fabrics in the medical industries. Their combined effect of low
diameter and compact packing also allows efﬁcient and more economical dyeing
Finally, constant pressure to achieve and develop even more novel applications
of ﬁbres has led to a number of other and, as yet, niche ﬁbrous products. In princi-
ple, the new ideas usually strive to combine basic functional properties of a textile
material with special needs or attractive effects.
For example, Solar-Aloha, developed by Descente and Unitika in Japan,35
absorbs light of less than 2 mm wavelength and converts it to heat owing to its zir-
conium carbide content. Winter sports equipment made from these materials use
the cold winter sun to capture more than 90% of this incident energy to keep the
wearer warm. Another interesting material gives rise to thermochromic fabrics
made by Toray which have a uniform coating of microcapsules containing heat-
sensitive dyes that change colour at 5 °C intervals over a temperature range of -40
°C to 80 °C creating ‘fun’ and special effects.
Cripy 65 is a scented ﬁbre produced by Mitsubishi Rayon (R) who have enclosed
a fragrant essence in isolated cavities along the length of hollow polyester ﬁbres.
The scent is gradually released to give a consistent and pleasant aroma. Pillows and
bed linen made from these materials are claimed32 to improve sleep and sleeping
disorders. The effect can also be achieved by printing or padding microcapsules con-
taining perfumes into fabrics which subsequently burst and release the perfume.
With careful handling, garments made from these materials are said to maintain this
34 Handbook of technical textiles
0 6 12 18
2.2 Stress/strain curves of range of available ﬁbres.
property for up to two years. Infrared-emitting and bacteria-repelling ﬁbres are
some of the other emerging novel ﬁbres.
Figure 2.2 shows stress/strain values for a selected range of the ﬁbres discussed.
The remainder of this chapter focuses on the vast application areas of ﬁbres
giving examples in each category with respect to their functional requirements, limi-
tations and means of optimising their effectiveness.
Table 2.3 summarises applications into ﬁve major areas.
2.7 Civil and agricultural engineering
Natural ﬁbres such as ﬂax, jute and ramie can be used for most temporary applica-
tions where, for instance, soil erosion is the problem. The geotextiles made from
these natural polymers help to prevent the erosion of soils by allowing vegetative
growth and their subsequent root establishment. Once the purpose is served, the
geotextile material gradually disintegrates into the soil.
In most medium to long term applications however, where physical and chemi-
cal durability and dimensional stabilities are of prime concern, synthetic ﬁbres are
preferred. There are currently at least six synthetic polymers considered suitable for
this purpose; they include:
• polyvinyl chloride
Polypropylene is by far the most utilised geotextile, followed by polyester, the other
three trailing behind with polyamide as the least used synthetic polymer. Para-
aramids are only used where very high creep resistance and tolerance to prolonged
heating are required.36
Generally, geosynthetics must have lifetimes which are deﬁned and relate to their
function. Durability, therefore, is mainly determined by the resistance offered by the
component ﬁbre and its assembled structure to the degrading species that causes a
reduction in the tensile and mechanical properties.37 At least three main degrading
mechanisms have been identiﬁed that ultimately determine the durability and life
of the contending polymer; they include:
able 2.3 Applications of technical textiles
ivil & agricultural Engineering Automotive & aeronautics Medical & hygiene Protection & defence Miscellaneous
Geotextiles, geomembranes and Tyre reinforcement Wound care Barriers to: chemical Marine engineering
geocomposites Seat belting Bandages compounds, heat, Electronics
g. Air bags Barriers to bacteria moisture, ﬂame and Filtration industry
oil reinforcement Carriage interiors Sterile wraps acoustics. Food processing
eparation Bumpers Disposable blood Insulation Sports & leisure
iltration Wings ﬁltration (dialysis) Workwear e.g.
Drainage Engine reinforcement valves Body armour Ropes,
rosion control Flexible container carriers Replacement e.g. Vests, Helmets, Belts,
Waterprooﬁng Balloons ligaments Gloves, etc. Boat Building
oil stabilization for vegetative Parachutes, etc. Artiﬁcial arteries Sails
growth Synthetic sutures, etc. Cables
Underground hoses (used for Clean room suits
irrigation & addition of Gas & liquid ﬁlters
fertilisers and pesticides) Puriﬁers
orm of application
onwoven, woven, warp Nonwoven, woven, knitted Nonwoven, woven, Nonwoven, woven, Nonwoven, woven,
knitted, grids, composites, (warp/weft), composites knitted (warp/weft), knitted (warp/weft), knitted (warp/weft),
three-dimensional network (plastic or metal resins), braided, etc. composites, network braided, composites, etc.
structures, etc. etc. structures, etc.
36 Handbook of technical textiles
• physical degradation
• chemical degradation
• biological degradation.
Physical degradation is usually sustained during transport or installation in one form
or another. Initiation of cracks is normally followed by their subsequent propaga-
tion under environmental or normal stress. In the ﬁrst instance, polymer suscepti-
bility to physical degradation depends on such factors as the weight of the
geotextile; generally lightweight or thin geotextiles suffer larger strength losses than
thick and heavy materials. Secondly, woven geotextiles suffer slightly larger strength
losses than nonwovens, owing to their greater stiffness and, ﬁnally, the generic
nature of the polymer itself plays an important role. Polyester, for instance, suffers
greater strength losses than polyoleﬁn ﬁbres owing to its high glass transition tem-
perature of around 70 °C. Under normal soil conditions, the polymer is relatively
brittle and therefore susceptible to physical damage.38 Polypropylene with its glass
transition averaging at about -10 °C is much more pliable under these conditions
but suffers from the rather critical phenomenon of extension with time or creep.
Chemical degradation is the next mechanism by which chemical agencies, often
in combination with ultraviolet light or/and heat, attack the polymer whilst in use
or being stored. The presence of energy starts off a self-destructing chain of events
that ultimately renders the polymer ineffective. Ultraviolet radiation normally
attacks the surface of the polymer and initiates chain breakage or scission which
leads to embrittlement and eventual failure of the polymer. Generally, chemical
degradation is a function of polymer type, thickness and availability of stabilizers.
The type, quantity, and distribution of stabilizers39 also controls the degree of resis-
tance to degradation. Polyoleﬁns are particularly susceptible to ultraviolet degra-
dation and need protection using light-stabilising additives. Oxidation due to heat
operates similarly by weakening the polymer thus causing rapid degradation. A
range of antioxidants are often included in the polymer during manufacture and
processing to minimise this harmful effect.
Biological degradation can result from at least three types of microbiological
attack: direct enzymatic attack, chemical production by microorganisms which may
react destructively with the polymer, and attack on the additives within the
polymer.40,41 High molecular weight polymers are much more immune to biological
attack than low molecular weight polymers because microorganisms cannot easily
locate the molecular chain endings. However, some microorganisms can permeate
less digestible polymers in order to gain access to food.
2.8 Automotive and aeronautics
Mechanical functionality has increasingly become an almost secondary requirement
for travel safety, weight efﬁciency, comfort and material durability of the transport-
ing medium. From bicycles to spacecraft, ﬁbres in one form or another fulﬁl these
important requirements. Carbon ﬁbre reinforcement of the frame of a bicycle ridden
in the 1992 Olympics was the ﬁrst of its kind to allow a comfortable win ahead of
its competitors.41 The one-piece, light, ﬁbre-reinforced composite structure and
design of the bike have since become an earmark of this industry. In the simplest
terms, composites utilise unique ﬁbre properties such as strength, stiffness and
Technical ﬁbres 37
elasticity whilst incorporating the compression resistance, and torsion and bending
characteristics of the matrix used.42 Glass ﬁbres have been traditionally used for the
manufacture of boat hulls and car bodies. UHMWPE, aramids and carbon-
reinforced composites in a variety of matrix materials are now routinely produced
and utilised in low to very high temperature applications.
Reinforcement of tyres is another area where the transport industry has bene-
ﬁted from ﬁbres and where rapid temperature change and changing weather con-
ditions demand effective response and durability. High tenacity viscose and
polyester yarns built into the internal structure of tyres now address these needs
adequately. In addition to all the obvious upholstery materials used in the interior
of cars, trains and aeroplanes, ﬁbres are now used in one form or another in such
parts as the engine components, fan belts, brake pads, door panels, seat skeletons,
seat belts and air bags. Fire-retardant additives or inherently ﬁre-retardant ﬁbres
are today standard requirements in the public sector use of all transport in order to
2.9 Medical and hygiene applications
Fibres used in relation to health care and surgery may be classiﬁed depending on
whether they are natural or synthetic, biodegradable or non-biodegradable. All
ﬁbres used, however, must be non-toxic, non-allergenic, non-carcinogenic and must
be able to be sterilised without imparting any change in their physical or chemical
Traditionally, natural ﬁbres such as cotton, silk and later viscose have been exten-
sively used in all areas of medical and surgical care. One such area of application is
on the wound, where moisture and liquid that exude from the wound are absorbed
by the ﬁbrous structure to promote healing in relatively dry conditions. However,
upon healing, small ﬁbrous elements protruding from the wound dressing are
usually trapped in the pores of the newly formed tissues which make their removal
distressing to the patients.
Research work44 in the early 1960s showed that wounds under ‘moist conditions’
would in fact heal better and faster, which would also remove the problem of ﬁbres
being trapped in the healing wound. The concept of moist healing has since been
responsible for the development of many ﬁbres which have vastly improved wound
management techniques and patient care. Alginate ﬁbres45 are one such example
where naturally occurring, high molecular weight carbohydrates or polysaccharides
obtained from seaweeds have found use in the medical textiles. Chemically, alginate
is a copolymer made from a-l-guluronic acid and b-d-mannuronic acid. It is made
into ﬁbres by extruding sodium alginate into a calcium chloride bath where calcium
alginate ﬁlaments precipitate.The ﬁlaments are then drawn, washed and dried. Upon
contact with wound ﬂuid, these ﬁbres are partially converted to a water-soluble
sodium alginate that swells to form a gel around the wound, thus keeping the wound
moist during the healing period.They can then be easily removed once the treatment
is complete. Artiﬁcial polymers based on a crosslinking copolymer of acrylic acid
have been developed which are claimed16 to have superior absorption properties to
alginates particularly when used under pressure. Hydrocel, a derivative of Acordis’s
environmentally friendly Lyocell, is also claimed to be more absorbent than calcium
alginate, taking up to 35 times its own weight of water whilst remaining intact.
38 Handbook of technical textiles
Chitin46,47 is another polysaccharide which, after cellulose, is the most abundantly
available natural polymer. It is found in the outer shells of shrimps and crabs in
combination with protein and minerals. Medicinal and medical use of this polymer
has been realised seriously since the early 1970s. High purity chitin, from which
protein, heavy metals and pyrogens have been removed, can be used for a range of
applications from food additives for controlling cholesterol levels in blood to arti-
ﬁcial skins into which tissues can safely grow. A derivative of chitin, chitosan has
better processability and is now extensively available in ﬁbre form. The particular
appeal of both chitin and chitosan within biomedical applications is due to their
• natural and biodegradable
• compatible with most living systems
• versatile in their physical form, i.e. powder, aqueous solutions, ﬁlms, shaped
objects, ﬁbres and sponges, and
• vehicles for transporting and delivering drugs.
Finally, collagen, a protein-based polymer that is collected from bovine skin and
has traditionally been used in hydrogel or gelatine form for making jellies and
sausage casings, is now available in ﬁbre form. It is very strong and completely
Besides wound care, ﬁbre-based structures in synthetic or natural form are used
in extracorporeal devices that may be used to purify blood in kidneys, create artiﬁ-
cial livers and function as mechanical lungs,47 as well as ﬁnding use in suture mate-
rials, artiﬁcial ligaments and cartilages and cardiovascular implants. In general,
healthcare and hygiene products, have applications that cover a wide spectrum from
disposable items to surgeons uniforms and hospital bedding and all are becoming
increasingly important across the world as the need to produce efﬁcient and effec-
tive medical care increases.
2.10 Protection and defence
In textile terms, protection and defence can be a passive response in which the textile
product receives and absorbs the impending impact or energy in order to protect the
underlying structure. Ballistic garments are obvious examples, where the assembled
ﬁbrous material is deliberately designed to slow down and reduce the penetration
of an incoming projectile. But they may also have a more active role, where the
ﬁbres show positive response by generating char or protective gases, shrinking or
expanding to prevent penetration of moisture or vapour and so on. In each scenario,
the protection of the underlying structure is the common objective.
In the early days, leather and metal mesh garments were used to protect the body
against sword and spear attacks, but with the passage of time development of new
materials occurred and, for example, early in the 1940s, nylon-based ﬂack jackets48
were introduced. They were a considerable improvement on the leather and metal
garments but were still rather heavy and uncomfortable to wear. With the advent
of para-aramids in the early 1970s, advanced ﬁbres were for the ﬁrst time used to
make much more acceptable protective gear. In these garments, Kevlar or Twaron
continuous ﬁlament yarns are woven into tight structures and assembled in a mul-
tilayer form to provide maximum protection. Their high tenacity and good energy
Technical ﬁbres 39
absorption combined with high thermal stability enables these garments to receive
and neutralise a range of projectiles from low calibre handguns, that is 0.22 to 0.44
inch (5.6–11.2 mm) to military bullets within the 5.56–7.62 mm range.49 In the latter
case, the fabric will require facing with ceramic tiles or other hard materials to blunt
the tips of metal-jacket spitzer-pointed bullets.
To strike a better balance between garment weight, comfort and protection an
even stronger and lighter ﬁbre based on ultra-high molecular weight polyethylene
(see Section 2.3) was developed and used in the early 1990s, which immediately
reduced average garment weight by 15%.50,51 UHMWPE, commercially known as
Dyneema (DSM) and in composite form as Spectra Shield by Allied Signal, is
now used to make cut-resistant gloves and helmets, as well as a wide range of
protective garments. However, unlike Kevlar, with a fairly low melting temperature
of 150 °C, it is best suited to low temperature applications.
Fire is another means by which fatal and non-fatal injuries can be sustained. No
textile-based material can withstand the power and ferocity of a ﬁre for sustained
periods of greater than 10 min or so. However, if the ﬁre ignition point could be
increased or the organic structure converted to a carbonaceous char replica and
its spreading rate delayed, then there may just be enough time gained to save an
otherwise lost life. This is in essence the nature and objective of all ﬁre-retardant
compounds. Such treatments give ﬁbres the positive role of forming char, reducing
the emission of combustible volatile gases and effectively starving the ﬁre of oxygen
or providing a barrier to underlying surfaces.
In contrast, water-repellent fabrics may shed water by preventing water droplets
from physically passing through them owing to their ﬁne ﬁbre dimensions and tight
weaves, as is the case with ventile fabrics52 or perforated barrier inlays such as
Goretex,53 whose tiny holes allow water vapour to pass through them but not water
droplets. Wax and chemically treated fabrics reduce water/fabric surface tension
by allowing water to roll off but do not allow permeation of moisture and air, so
It is not possible to categorise fully all disciplines within which textile-based mate-
rials are increasingly being applied. The spectrum of ﬁbre utilisation has already
grown to include anything from conventional ropes and industrial belts to sophisti-
cated two- and three-dimensional composite structures. The industries they cover,
other than those already discussed, include wet/dry ﬁltration, sports and leisure gear,
inland water and marine applications, food processing, puriﬁers, electronic kit, clean
room suits and many more. It will not be long before each area develops into its
own major category.
Conventional ﬁbres dominate the technical ﬁbre market and are likely to do so for
a long time to come. The rate of growth in consumption of ﬁbres destined for tech-
nical applications, however, is now faster than those going to the traditional cloth-
ing and furnishing sectors. It was estimated that the world’s technical ﬁbres share
40 Handbook of technical textiles
of the market would have reached the 40% mark by the year 2000.1 Much of this
growth will depend on greater realisation of the technological and ﬁnancial bene-
ﬁts that ﬁbre-based structures could bring to the traditional and as yet unyielding
sectors of engineering. Issues such as environment, recycling and biodegradability,
which are increasingly subjects of concern for the public, will further encourage and
beneﬁt the growth and use of technical textiles.
1. t nobolt, Keeping a competitive edge in technical textiles, Textile Month, Union des Industries,
February p16, 1992.
2. m c tubbs (ed.), Textile Terms and Deﬁnitions, 9th edition, The Textile Institute, Manchester, 1991.
3. c byrne, ‘Technical textiles’, Textiles Mag., issue 2.95, pp. 12–16, 1995.
4. j e mcintyre, Speciality Fibres for Technical Textiles, Department of Textile Industries, University of
5. a r horrocks, The Durability of Geotextiles, Comet Eurotex, UK 1992.
6. p r rankilor, Membranes in Ground Engineering, Wiley Interscience, London, 1981.
7. v van zanten, Geotextiles and Geomembranes in Civil Engineering, Balkema, Rotterdam, 1986.
8. p w harrison (ed.), Cotton in a Competitive World, The Textile Institute, 1979.
9. b k kandola and a r horrocks, ‘Complex char formation in ﬂame-retarded ﬁbre-intumescent com-
binations-II. Thermal analytical studies’, Polymer Degradation and Stability, 54, 289–303, 1996.
10. a r horrocks, ‘Flame-retardant ﬁnishing of textiles’, Rev. Prog. Coloration, 16, 62–101, 1986.
11. l benisek and w a phillips, Textile Res. J., 51, 1981.
12. d j cole, ‘A new cellulosic ﬁbre – Tencel’, Advances in Fibre Science, The Textile Institute, 1992.
13. c m legault, ‘Antron – a special nylon carpet ﬁbre’, Can. Textile J., April, 1982.
14. c b chapman, Fibres, Butterworths, 1974.
15. c z porczynski, Manual of Man-made Fibres, Astex, 1960.
16. p akers and r heath, Superabsorbent Fibres, The Key to the Next Generation of Medical Products,
Technical Absorbents Ltd., UK, 1996.
17. d h morton-jones, Polymer Processing, Chapman and Hall, London, 1989.
18. j w s hearle, ‘Understanding and control of ﬁbre structure, parts 1 to 3’, Textile Horizon, 1997.
19. f happey, Appl. Fibre Sci., 3.
20. a sharples, Introduction to Polymer Crystallisation, Arnold, 1966.
21. d s varma, ‘High performance organic ﬁbres for industrial applications’, Man-made Textiles in India,
380–386, August, 1986.
22. l miles (ed.), ‘Flame-resistant fabrics – Some like it hot’, Textile Month, 37–41, April, 1996.
23. p heidel, a g hoechst, Frankfurt, Germany, ‘New opportunities with aromatics’, Textile Month, 43–44,
24. l baker, ‘Polyphenylene sulphide ﬁbres for high temperature ﬁltration’, Tech. Textiles Int., 11–16,
25. e mcintyre, ‘High-performance ﬁbres for industrial textiles’, Textile Horizon, 43– 45, October,
26. f o anderegg, ‘Strength of glass ﬁbres’, Ind. Eng. Cem., 31, 290–298, 1939.
27. l michaels and s s chissick (eds.), Asbestos Properties, Applications and Hazards, Vol. 1, Wiley, New
28. i n ermolenko et al, Chemically Modiﬁed Fibres, VCH, 1990.
29. t f cooke, ‘Inorganic ﬁbres, A literature review’, J. Am. Ceramics Soc., p. 2959.
30. f d birchall, ‘Oxide inorganic ﬁbres’, Concise Encyclopedia of Composite Materials, Oxford, UK,
31. a k dhingra, ‘Advances in inorganic ﬁbre development’, Contemporary Topics in Polymer Science,
New York, 1982.
32. k nosse, ‘New developments in Japanese ﬁbres’, Textile Month, 44– 46, June, 1990.
33. d and k consulting, ‘The European potential of microﬁbres’, Textile Month, 23–25, January, 1992.
34. m golding, ‘The microﬁbre business in Japan’, Tech. Textiles Int., 18–23, May, 1992.
35. t hongu and g o phillips, New Fibres, Ellis Horwood, UK, 1990.
36. a r horrocks and j a d’souza, ‘Degradation of polymers in geomembranes and geotextiles’, Hand-
book of Polymer Degradation, S H Hamid, M B Amin and A G Maadhah (eds), Marcel Dekker,
New York, 1992, 433–501.
37. t m allen, ‘Determination of long-term tensile strength of geosynthetics: A state of the art review’,
Geosynthetics’91 Conference, Atlanta, USA, 351–379.
Technical ﬁbres 41
38. t m allen, j r bell and t s vinson, ‘Properties of geotextiles in cold region applications’,
Transportation Research Report, Oregon State University, 1983.
39. r m koerner et al, ‘Long-term durability and aging of geotextiles,’ Geotextiles Geomembranes, 1988.
40. g r koerner et al, ‘Biological clogging in leachate collection systems’, Durability Aging Geosynthet-
41. s k mukhopadhyay, ‘High performance ﬁbres’, Textile Prog., 25(3/4), 1993.
42. p bracke et al, Inorganic Fibres and Composite Materials, Pergamon Press, Oxford 1984.
43. a j rigby, s c anand and m miraftab, ‘Textile materials in medicine and surgery’, Textile Horizons,
December, 1993 and Knitting Int. February, 1994, vol. 101.
44. g d winter, Nature, 1962, 193, 293.
45. y qin, c agboh, x wang and d k gilding, ‘Novel polysaccharide ﬁbres for advanced wound dressing’,
Medical Textiles 96, conference proceedings, Woodhead, 15–20, 1997.
46. p a sandford and a steinnes, ‘Biomedical applications of high purity chitosan’, American Chemical
Society, chapter 28, 1991.
47. a s hoffman, ‘Medical applications of polymeric ﬁbres’, Appl Polym Symp 31, 313–334 J. Wiley and
Sons, New York, 1977.
48. a eldib and r walther, ‘Advanced ﬁbres for personal protective clothing’, Tech. Textiles Int., June,
49. s a young, ‘The use of Kevlar para-aramid ﬁbre in ballistic protection garments’, Tech. Textiles Int.,
26–27, July/August, 1992.
50. s a young, ‘Dyneema – the strongest ﬁbre in the world’, Tech. Textiles Int., May, 1992.
51. The use of Kevlar para-aramid ﬁbre in ballistic protection garments, Tech. Textiles Int., 24–27,
52. Ventile fabrics commercial publications, Courtaulds, Chorley, Lancashire.
53. w l gore and associates, Inc, ‘Porous materials derived from tetraﬂuoroethylene and processes for
their production’, US Patent no. 1355373, USA, 1974.
R H Gong and X Chen
Department of Textiles, UMIST, PO Box 88, Sackville Street, Manchester M60 1QD, UK
Technical yarns are produced for the manufacture of technical textiles. They
have to meet the speciﬁc functional requirements of the intended end-use. This
may be achieved through special yarn production techniques or through the selec-
tion of special ﬁbre blends or a combination of both. This chapter describes the
yarn production technologies that are applicable to technical yarns and discusses
the structures and properties of the yarns that may be produced using these
3.2 Staple ﬁbre yarns
3.2.1 Ring spinning
Ring spinning is currently the most widely used yarn production method. Initially
developed in America in the 1830s, its popularity has survived the emergence of
much faster spinning technologies. In addition to the superior yarn quality, ring spin-
ning is extremely versatile. It is capable of producing yarns with wide ranges of
linear density and twist from a great variety of ﬁbre materials. It is also used for
doubling and twisting multifold and cabled yarns.
Fibre materials must be properly prepared before they can be used on the ring
spinning machine. The preparation processes are dependent on the ﬁbre material.
Figures 3.1 and 3.2 illustrate the typical process routes for cotton and wool. The ulti-
mate objectives of the many preparation processes are to produce a feed material
for the ﬁnal spinning process that is clean, even, homogeneous and free from ﬁbre
entanglement. The ﬁbres must also be in the preferred orientation.
On the ring spinning machine, the feed material is attenuated to the required
linear density by a drafting system, typically a roller drafting system with three lines
of rollers. The drafted ﬁbre strand is then twisted by the ring spindle illustrated in
Technical yarns 43
Cotton bale cleaning Carding
Lap forming For combed yarn Drawing
Combing Spinning For carded yarn
3.1 Production of ring-spun cotton yarn.
3.2 Production of wool yarn.
The yarn leaving the front rollers is threaded through a yarn guide (the lappet),
which is located directly above the spindle axis. The yarn then passes under the C-
shaped traveller onto the bobbin. The bobbin is mounted on the spindle and rotates
with the spindle. When the bobbin rotates, the tension of the yarn pulls the traveller
around the ring. The traveller rotational speed, the spindle rotational speed and the
yarn delivery speed follow Equation 3.1:
Nt = N s - (3.1)
44 Handbook of technical textiles
ave Ring rail
3.3 Ring spindle.
where Nt is the traveller rotational speed (rpm), Ns is the spindle rotational
speed (rpm), Vd is the yarn delivery speed (m min-1) and Db is the bobbin diameter
During production, the bobbin rail moves up and down to spread the yarn along
the length of the bobbin so that a proper package can be built. The movement of the
ring rail is quite complicated, but the aim is to build a package that is stable, easy to
unwind and contains the maximum amount of yarn. As the yarn is wound on the
Technical yarns 45
bobbin, the bobbin diameter increases steadily during production.The spindle speed
and the yarn delivery speed are normally kept constant, it is therefore obvious from
Equation 3.1 that the traveller speed increases during production.
Each rotation of the traveller inserts one full turn in the yarn, so the twist inserted
in a unit length of yarn can be calculated by Equation 3.2:
where t is the yarn twist (turns m-1).
Because the traveller speed is not constant, the twist in the yarn also varies.
However, because this variation is usually very small, it is commonly ignored and
the twist is simply calculated from the spindle speed, Equation 3.3:
As can be seen from Equation 3.3, for a given yarn twist, the higher the spindle
speed the higher the yarn delivery speed. A spindle speed of up to 25 000 rpm is
possible, although speeds of between 15 000 and 20 000 rpm are more usually used.
The spindle speed is restricted by the traveller speed, which has an upper limit of
around 40 m s-1. When the traveller speed is too high, the friction between the trav-
eller and the ring will generate too much heat, which accelerates the wear on the
traveller and the ring and may also cause yarn damage. The yarn between the
yarn guide and the traveller rotates with the traveller and balloons out owing to
centrifugal force. The tension in the yarn increases with the rotational speed of the
yarn balloon. When the spindle speed is too high, the high yarn tension will increase
the yarn breakage. The traveller speed and the yarn tension are the two most criti-
cal factors that restrict the productivity of the ring spinning system. The increasing
power cost incurred by rotating the yarn package at higher speeds can also limit the
economic viability of high spindle speeds. For the same traveller linear speed, using
a smaller ring allows a higher traveller rotational speed and increases delivery
speed. A smaller ring also reduces yarn tension, as the yarn balloon is also smaller.
However, a smaller ring leads to a smaller bobbin which results in more frequent
Ring-spun yarns have a regular twist structure and, because of the good ﬁbre
control during roller drafting, the ﬁbres in the yarn are well straightened and
aligned. Ring spun yarns therefore have excellent tensile properties, which are often
important for technical applications.
The ring spinning system can be used for spinning cover yarns where a core
yarn, spun or ﬁlament, is covered by staple ﬁbres. This can provide yarns with a
combination of technical properties. For example, a high strength yarn with
good comfort characteristics may be spun from a high strength ﬁlament core with
natural ﬁbre covering. Other technical yarns, such as ﬂame-retardant and antistatic
yarns can also be made by incorporating ﬂame-retardant and electricity conductive
The main limitation of the ring spinning system is the low productivity. The other
limitations are the high drafting and spinning tensions involved. These high tensions
can become a serious problem for spinning from ﬁbres such as alginate ﬁbres that
have low strength.
46 Handbook of technical textiles
navel and tube Rotor
3.4 Rotor spinning principle.
3.2.2 Rotor spinning
The productivity limitation of the ring spinning system was recognised long before
the commercial introduction of rotor spinning in 1967. In ring spinning, the twist
insertion rate is dependent on the rotational speed of the yarn package. This is so
because of the continuity of the ﬁbre ﬂow during spinning. Numerous attempts have
been made since before the end of the 19th century, particularly since the 1950s, to
introduce a break into the ﬁbre ﬂow so that only the yarn end needs to be rotated
to insert twist. Very high twisting speeds can thus be achieved. In addition, by
separating twisting from package winding, there will be much more ﬂexibility in the
form and size of the yarn package built on the spinning machine. This increases the
efﬁciency of both the spinning machine and of subsequent processes. Rotor spin-
ning was the ﬁrst such new technology to become commercially successful and it is
the second most widely used yarn production method after ring spinning.
The principles of rotor spinning are illustrated in Fig. 3.4. The ﬁbre material is
fed into an opening unit by a feed roller in conjunction with a feed shoe. The feed
material is usually a drawn sliver. An opening roller is located inside the opening
unit and is covered with carding wire, usually saw-tooth type metallic wire. The
surface speed of the opening roller is in the region of 25–30 m s-1, approximately
2000 times the feed roller surface speed. This high speed-ratio enables the ﬁbres to
Technical yarns 47
be opened up into a very thin and open ﬁbre ﬂow. The ﬁbres are taken off the
opening roller by an air stream with a speed about twice that of the opening
roller. The ﬁbres are carried by the air stream, through the ﬁbre transportation tube,
into the spinning rotor. The air speed in the transportation tube increases, owing to
the narrowing cross-section of the tube, as the air reaches the exit point inside the
rotor. This ensures that the ﬁbres are kept aligned along the airﬂow direction
and as straight as possible. The exit angle of the ﬁbres from the transportation
tube is at a tangent to the rotor wall and the surface speed of the rotor is faster
than the exit air speed, so the ﬁbres emerging from the transportation tube are
pulled into the rotor, keeping the ﬁbres aligned in the direction of the ﬁbre ﬂow.
The centrifugal force generated by the rotor forces the ﬁbres into the rotor groove.
Because of the high surface speed of the rotor, only a very thin layer of ﬁbres, usually
one or two ﬁbres in the cross-section, is deposited in the rotor when the rotor passes
the ﬁbre exit point of the transportation tube. Many such layers of ﬁbres are needed
to make up the yarn. This doubling up of the ﬁbres in the rotor is called back
The tail of the yarn arm inside the rotor is thrown against the rotor groove
because of the centrifugal force. The yarn arm rotates with the rotor and each rota-
tion of the yarn arm inserts one full turn in the yarn. As the yarn is withdrawn con-
tinuously through the navel and tube, the contact point of the yarn arm with the
rotor groove must move around the rotor. Because the yarn arm is rotating axially,
the ﬁbres in the rotor groove are twisted into the yarn. The machine twist of the
yarn can be calculated by Equation 3.4:
where t is the yarn twist (turns m-1), Ny is the rotational speed of the yarn arm (rpm)
and Vd is the yarn delivery speed (m min-1).
The following relationship exists between the yarn arm speed, the rotor speed
and the yarn delivery speed, Equation 3.5:
(N y - N r )pD = Vd (3.5)
where D is the diameter of rotor groove.
The relative speed between the yarn arm and the rotor is normally very small in
comparison with the rotor speed and the machine twist of the yarn is commonly
calculated by Equation 3.6:
The back-doubling ratio b is equal to the ratio of the rotor speed to the relative
speed between the yarn arm and the rotor, Equation 3.7:
b= = pD = tpD (3.7)
Ny - Nr Vd
Because there is no need to rotate the yarn package for the insertion of twist,
rotor spinning can attain much higher twisting speeds than ring spinning. The rotor
speed can reach 150 000 rpm. The roving process needed in ring spinning is eli-
minated in rotor spinning, further reducing the production cost. The package can
48 Handbook of technical textiles
be much larger, with fewer knots in the product and with a more suitable form for
Because the yarn is formed in an enclosed space inside the rotor, trash particles
remaining in the ﬁbres can accumulate in the rotor groove. This leads to a gradual
deterioration of yarn quality and in severe cases yarn breakage. The cleanliness of
ﬁbres is more critical for rotor spinning than for ring spinning. In order to improve
the cleanliness of the ﬁbres, a trash extraction device is used at the opening roller.
As the twist in the yarn runs into the ﬁbre band in the rotor groove, inner layers
of the yarn tend to have higher levels of twist than outer layers. Fibres landing on
the rotating ﬁbre band close to the yarn tail, or directly on the rotating yarn arm
when the yarn arm passes the exit of the transportation tube, tend to wrap around
the yarn instead of being twisted into the yarn. These wrapping ﬁbres are charac-
teristic of rotor-spun yarns.
Rotor-spun yarns usually have lower strength than corresponding ring-spun
yarns because of the poorer ﬁbre disposition in the yarn. This is the result of using
an opening roller to open up the ﬁbres, of transporting the ﬁbres by airﬂow, and
of the low yarn tension during yarn formation. The wrapping ﬁbres also lead to a
rougher yarn surface. Rotor yarns have better short term evenness than ring-spun
yarns because of the back-doubling action.
The main advantage of rotor spinning is the high production rate. However,
because of the lower yarn strength, rotor spinning is limited to medium to course
yarn linear densities. It is also limited to the spinning of short staple ﬁbre yarns.
3.2.3 Friction spinning
Friction spinning is an open end spinning technique. Instead of using a rotor, two
friction rollers are used to collect the opened-up ﬁbres and twist them into the yarn.
The principle is shown in Fig. 3.5.
The ﬁbres are fed in sliver form and opened by a carding roller. The opened ﬁbres
are blown off the carding roller by an air current and transported to the nip area
of two perforated friction drums. The ﬁbres are drawn onto the surfaces of the fric-
tion drums by air suction. The two friction drums rotate in the same direction and
because of the friction between the ﬁbre strand and the two drum surfaces, twist is
inserted into the ﬁbre strand. The yarn is withdrawn in the direction parallel to the
friction drum axis and delivered to a package forming unit. The friction drum diam-
eter is much larger than the yarn diameter. The diameter ratio can be as high as 200.
A high twisting speed can thus be achieved by using a relatively low speed for the
friction drums. Owing to the slippage between the drum surface and the yarn end,
the yarn takes up only 15–40% of the drum rotation. Nevertheless, a high produc-
tion speed, up to 300 m min-1, can be achieved. For a ﬁner yarn the twist insertion
rate is higher with the same drum speed so the delivery speed can be practically
independent of yarn linear density.
Because the yarn is withdrawn from the side of the machine, ﬁbres fed from the
machine end away from the yarn delivery tend to form the yarn core while ﬁbres
fed from the machine end closer to the yarn delivery tend to form the sheath. This
characteristic can be conveniently exploited to produce core–sheath yarn structures.
Extra core components, ﬁlaments or drafted staple ﬁbres, can be fed from the side
of the machine while the ﬁbres fed from the top of the machine, the normal input,
form the sheath.
Technical yarns 49
Friction drum Dust extraction
3.5 DREF 2 friction spinner.
Unlike ring or rotor spinning machines that are produced by many manufactur-
ers around the world, friction spinning machines are only currently made by Dr.
Ernst Fehrer AG of Austria. The diagram shown in Fig. 3.5 is the DREF 2 machine
that has recently been upgraded to DREF 2000. The company also produces the
DREF 3 machine that has an extra drafting unit on the side of the machine for
feeding drafted staple ﬁbres as a core component.
The ﬁbre conﬁguration in friction-spun yarns is very poor. When the ﬁbres come
to the friction drum surface, they have to decelerate sharply from a high velocity to
almost stationary. This causes ﬁbre bending and disorientation. Because of the very
low tension in the yarn formation zone, ﬁbre binding in the yarn is also poor. As a
result, the yarn has a very low tensile strength and only coarse yarns, 100 tex and
above, are usually produced.
The main application of friction spinning is for the production of industrial yarns
and for spinning from recycled ﬁbres. It can be used to produce yarns from aramid
and glass ﬁbres and with various core components including wires. The yarns can
be used for tents, protective fabrics, backing material, belts, insulation and ﬁlter
3.2.4 Wrap spinning
Wrap spinning is a yarn formation process in which a twistless staple ﬁbre strand
is wrapped by a continuous binder. The process is carried out on a hollow
spindle machine as illustrated in Fig. 3.6. The hollow spindle was invented by DSO
‘Textil’ in Bulgaria. The ﬁrst wrap spinning machine was introduced in the 1979
The staple roving is drafted on a roller drafting system similar to those used on
ring frames and is passed through a rotating hollow spindle that carries a binder
bobbin. The rotation of the hollow spindle and the bobbin wraps the binder around
the staple strand.
50 Handbook of technical textiles
3.6 Wrap spinning principle.
To prevent the drafted staple strand falling apart before it is wrapped by the
binder, false twist is usually generated in the staple strand by the spindle. To intro-
duce the false twist, the staple strand is not threaded through the hollow spindle
directly. It is wrapped around either a twist regulator at the bottom of the spindle
or part of the spindle top. The false twist also allows the staple strand to be com-
pacted before the binder is wrapped around it. This improves the yarn strength.
Two hollow spindles can be arranged one above the other to wrap the staple
strand with two binders in opposite directions. This is used to produce special effect
yarns with a more stable structure. Real twist may also be added to the yarn by
passing the wrapped yarn onto a ring spindle, usually arranged directly underneath
the hollow spindle.
Core yarns, mostly ﬁlaments, can be added to the feed.This can be used to provide
extra yarn strength or other special yarn features. An example is to use this method
to spin alginate yarns. Alginate ﬁbres are very weak and cause excessive breakages
during spinning without the extra support of core ﬁlaments.
A variety of binders can be used to complement the staple core or to introduce
special yarn features. For example, a carbon-coated nylon ﬁlament yarn can be used
to produce yarns for antistatic fabrics. Soluble binders can be used for making yarns
for medical applications.
Wrap spinning is highly productive and suitable for a wide range of yarn linear
densities. Yarn delivery speeds of up to 300 m min-1 are possible. Because the binder
is normally very ﬁne, each binder bobbin can last many hours, enabling the pro-
Technical yarns 51
Ba ler Fro er
rol rol1st Nozzle N1
ro 2nd Nozzle N2
Fro er N1
3.7 Murata jet spinner.
duction of large yarn packages without piecing. Because the staple core is composed
of parallel ﬁbres with no twist, the yarn has a high bulk, good cover and very low
hairiness. The main limitation of wrap spinning is that it is only suitable for the
production of multicomponent yarns. The binder can be expensive, increasing the
3.2.5 Air-jet spinning
Air-jet spinning technology was ﬁrst introduced by Du Pont in 1963, but it has only
been made commercially successful by Murata since 1980. Du Pont used only one
jet, which produced a low strength yarn. The Murata system has two opposing air
jets, which improves the yarn strength. The twin-jet Murata Jet Spinner is illustrated
in Fig. 3.7. Staple ﬁbres are drafted using a roller drafting system with three or four
pairs of rollers. The ﬁbres are then threaded through the twin-jet assembly. The
second jet N2 has a higher twisting torque than the ﬁrst jet N1. Immediately after
leaving the front drafting rollers, the ﬁbres in the core of the yarn are twisted in the
twist direction of N2. The ﬁbres on the edges of the drafted ribbon are twisted by
the weaker N1 and wrap around the core ﬁbres in the opposite direction. Because
the jet system is located between the front drafting rollers and the yarn delivery
rollers, neither of which rotates around the axis of the yarn, the twist inserted by
the jets is not real twist and after the yarn passes through the jet system, the core
ﬁbres become twistless. The yarn strength is imparted by the wrapping of the edge
ﬁbres. Because of the small jet dimensions, very high rotational jet speeds are pos-
sible. Although twist efﬁciency is only 6–12% because of the twist resistance of the
yarn, delivery speeds of up to 300 m min-1 are possible. In a further development by
Murata the second jet is replaced with a pair of roller twisters. The principle of yarn
formation is similar to the twin-jet system. The new machine, the roller-jet spinner,
is capable of delivery speeds of up to 400 m min-1. However, the yarn has a harsher
Air-jet spinning is used mainly for spinning from short staple ﬁbres, especially
cotton and polyester blends. The vortex spinner, the latest addition to the Murata
jet spinner range, was shown in ITMA 99 for spinning from 100% cotton.
52 Handbook of technical textiles
The air-jet system can be used to produce core–sheath yarn structures by feeding
the core and sheath ﬁbres at different stages of the drafting system. Fibres fed in
from the back of the drafting system tend to spread wider under the roller pressure
and form the sheath of the yarn while ﬁbres fed in nearer to the front tend to form
the yarn core. Filament core can also be introduced at the front drafting roller. Two
spinning positions can be combined to produce a two-strand yarn that is then twisted
using the usual twisting machinery.
Air-jet yarns have no real twist, therefore they tend to have higher bulk than ring
and rotor yarns and better absorbency. They are more resistant to pilling and have
little untwisting tendency. Because the yarn strength is imparted by the wrapping
ﬁbres, not the twisting of the complete ﬁbre strand, air-jet yarns have lower tensile
strength than ring and rotor yarns.The system is only suitable for medium to ﬁne yarn
linear densities as the effectiveness of wrapping decreases with the yarn thickness.
The rigid yarn core of parallel ﬁbres makes the yarn stiffer than the ring and rotor
3.2.6 Twistless spinning
Numerous techniques have been developed to produce staple yarns without twist-
ing so that the limitations imposed by twisting devices, notably the ring traveller
system, can be avoided and production speed can be increased. Because of the
unconventional yarn characteristics, these techniques have not gained widespread
acceptance commercially, but they do offer an alternative and could be exploited to
produce special products economically.
Most of these twistless methods use adhesives to hold the drafted staple ﬁbre
strand together. They can produce low linear density yarns at a high speed. The
adhesives may later be removed after the fabric is made and the ﬁbres are then
bound by the interﬁbre forces imposed by fabric constraints. This type of yarn has
high covering power due to the untwisted yarn structure. However, these processes
mostly involve additional chemicals and require high power consumption. The yarns
can only be used for fabrics that offer good interﬁbre forces.
As an example, the TNO twistless spinning method is shown in Fig. 3.8. In the
system shown here, the roving is drafted under wet conditions, which gives better
ﬁbre control. An inactive starch is then applied to the drafted roving, which is also
false twisted to give it temporary strength. The starch is activated by steaming the
package that is then dried. The later version of TNO twistless system replaces the
starch with PVA (polyvinyl alcohol) ﬁbres (5–11%), which melt at above 80 °C to
bind the staple ﬁbres. This is also known as the Twilo system.
Another twistless spinning method is the Bobtex process, which can produce
high strength yarns for industrial/leisure fabrics, such as tents, workwear and
sacks. In this process, staple ﬁbres (30–60%) are bonded to a ﬁlament core (10–50%)
by a layer of molten polymer (20–50%). Production speeds of up to 1000 m min-1
can be achieved. The process can use all types of staple ﬁbres including waste
3.2.7 Ply yarn
Single yarns are used in the majority of fabrics for normal textile and clothing
applications, but in order to obtain special yarn features, particularly high strength
Technical yarns 53
Thread guide Paddle Inactive starch
package Drafting rollers
3.8 TNO twistless yarn production method.
and modulus for technical and industrial applications, ply yarns are often needed.
A folded yarn is produced by twisting two or more single yarns together in one
operation, and a cabled yarn is formed by twisting together two or more folded
yarns or a combination of folded and single yarns.
The twisting together of several single yarns increases the tenacity of the yarn by
improving the binding-in of the ﬁbres on the outer layers of the component single
yarns. This extra binding-in increases the contribution of these surface ﬁbres to the
yarn strength. Ply yarns are also more regular, smoother and more hard wearing.
By using the appropriate single yarn and folding twists, a perfectly balanced ply yarn
can be produced for applications that require high strength and low stretch, for
example, for tyre cords.
A typical process route of a ply yarn involves the following production
1. single yarn production
2. single yarn winding and clearing
3. assembly winding: to wind the required number of single yarns as one
(doubling) on a package suitable for folding twisting
Twisting can be carried out in a two-stage process or with a two-for-one twister. In
the two-stage process, the ring frame is used to insert a low folding twist in
the ﬁrst stage and an up-twister to insert the ﬁnal folding twist in the second
54 Handbook of technical textiles
3.9 The up-twister.
stage. The ring frame uses a low twist to enable higher delivery speeds. A suitable
package is formed on the ring frame for the over-end withdrawal of yarn on the
up-twister. Figure 3.9 shows the principle of the up-twister. The supply package
rotates with the spindle while the yarn is withdrawn over the package end from
the top. The free-rotating ﬂyer is pulled around by the yarn and inserts twist in the
The two-for-one twister is illustrated in Fig. 3.10. The supply yarn package is sta-
tionery. After withdrawal from the package, the yarn is threaded through the centre
of the spindle and rotates with the spindle. Each rotation of the spindle inserts one
full turn in the yarn section inside the spindle centre and also one turn in the yarn
section outside the yarn package (the main yarn balloon). The yarn therefore gets
two turns for each spindle rotation. If the supply package is rotated in the opposite
direction of the spindle, then the twisting rate will increase by the package rota-
tional speed. The Saurer Tritec Twister is based on this principle. In the Tritec
Twister, the package rotates at the same speed as the spindle, but in the opposite
direction, so each spindle rotation inserts three twists in the yarn. The package is
The production of a ply yarn is much more expensive than the production of
a single yarn of equivalent linear density. Not only does the ply yarn production
require the extra assembly winding and twisting processes, but the production of
the ﬁner component single yarn is also much more expensive.
Technical yarns 55
3.10 The two-for-one twister.
3.3 Filament yarns
A ﬁlament yarn is made from one or more continuous strands called ﬁlaments where
each component ﬁlament runs the whole length of the yarn. Those yarns composed
of one ﬁlament are called monoﬁlament yarns, and those containing more ﬁlaments
are known as multiﬁlament yarns. For apparel applications, a multiﬁlament yarn may
contain as few as two or three ﬁlaments or as many as 50 ﬁlaments. In carpeting, for
example, a ﬁlament yarn could consist of hundreds of ﬁlaments. Most manufactured
ﬁbres have been produced in the form of a ﬁlament yarn. Silk is the only major
natural ﬁlament yarn.
According to the shape of the ﬁlaments in the yarn, ﬁlament yarns are classiﬁed
into two types, ﬂat and bulk. The ﬁlaments in a ﬂat yarn lie straight and neat, and
are parallel to the yarn axis. Thus, ﬂat ﬁlament yarns are usually closely packed and
have a smooth surface. The bulked yarns, in which the ﬁlaments are either crimped
or entangled with each other, have a greater volume than the ﬂat yarns of the same
Texturing is the main method used to produce the bulked ﬁlament yarns. A tex-
tured yarn is made by introducing durable crimps, coils, and loops along the length
of the ﬁlaments. As textured yarns have an increased volume, the air and vapour
permeability of fabrics made from them is greater than that from ﬂat yarns.
56 Handbook of technical textiles
pump Feed rolls
Air Draw zone
cooled Draw rolls
3.11 (a) Melt spinning process, (b) drawing process.
However, for applications where low air permeability is required, such as the fabrics
for air bags, ﬂat yarns may be a better choice.
3.3.2 Manufacture of ﬁlament yarns
Most manufactured ﬁbres are extruded using either melt spinning, dry spinning, or
wet spinning, although reaction spinning, gel spinning and dispersion spinning are
used in particular situations. After extrusion, the molecular chains in the ﬁlaments
are basically unoriented and therefore provide no practical strength. The next step
is to draw the extruded ﬁlaments in order to orient the molecular chains. This is con-
ventionally carried out by using two pairs of rollers, the second of which forwards
the ﬁlaments at approximately four times the speed of the ﬁrst. The drawn ﬁlaments
are then wound with or without twist onto a package. The tow of ﬁlaments at this
stage becomes the ﬂat ﬁlament yarn. Figure 3.11 shows the melt spinning process
and the subsequent drawing process.
For many applications, ﬂat ﬁlament yarns are textured in order to gain increased
bulkiness, porosity, softness and elasticity in some situations. Thermoplastic ﬁlament
yarns are used in most texturing processes. The interﬁbre bonds break and reform
during the texturing process. A ﬁlament yarn is generally textured through three
steps. The ﬁrst step is to distort the ﬁlament in the yarn so that the interﬁbre bond
is broken. Twisting or other means are used to distort the ﬁlaments within a yarn.
The second step is to heat the yarn, which breaks bonds between polymers, allow-
ing the ﬁlaments to stay crimped. The last step is to cool the yarn in the distorted
state to enable new bonds to form between the polymers.When the yarn is untwisted
Technical yarns 57
3.12 Principles of main texturing methods: (a) false twist, (b) stuffer box, (c) air-jet,
or otherwise released from its distorted state, the ﬁlaments remain in a coiled or
There are many methods for yarn texturing, including false-twist, air-texturing,
knit-de-knit, stuffer box and gear crimp. Among these, the false-twist is the most po-
pular method. Figure 3.12 shows the principles of the main methods of yarn texturing.
3.3.3 Filament technical yarns
There have been many types of ﬁlament yarns developed for technical applications,
such as reinforcing and protecting. The reinforcing technical yarns have either high
modulus, high strength, or both. Yarns for protecting applications can be resistant
to safety hazards such as heat and ﬁre, chemical and mechanical damage. There
are many types of technical ﬁlament yarns used in various applications, it is only
possible, therefore, to list just a few yarns here that are popularly used in the
development of some technical textile products.
18.104.22.168 Aramid ﬁlament yarns
Aramid ﬁbre is a chemical ﬁbre in which the ﬁbre-forming substance is a long chain
synthetic polyamide where at least 85% of the amide linkages are attached directly
58 Handbook of technical textiles
to two aromatic rings. Nomex and Kevlar are two well-known trade names of the
aramid ﬁbre, owned by Du Pont. Aramid ﬁbres have high tenacity and high resis-
tance to stretch, to most chemicals and to high temperature. The Kevlar aramid is
well known for its relatively light weight and for its fatigue and damage resistance.
Because of these properties, Kevlar 29 is widely used and accepted for making body
armour. Kevlar 49, on the other hand, has high tenacity and is used as reinforcing
material for many composite uses, including materials for making boat and aircraft
parts. The Nomex aramid, on the other hand, is heat resistant and is used in making
ﬁre ﬁghters’ apparel and similar applications.
Aramid yarns are more ﬂexible than their other high performance counterparts
such as glass and Kevlar, and thus are easier to use in subsequent fabric making
processes, be it weaving, knitting, or braiding. Care should be taken, though, as
aramid yarns are much stronger and much more extensible than the conventional
textile yarns, which could make the fabric formation process more difﬁcult.
22.214.171.124 Glass ﬁlament yarns
Glass is an incombustible textile ﬁbre and has high tenacity too. It has been used
for ﬁre-retardant applications and also is commonly used in insulation of buildings.
Because of its properties and low cost, glass ﬁbre is widely used in the manufacture
of reinforcement for composites. There are different types of glass ﬁbres, such as E-
glass, C-glass, and S-glass. E-glass has very high resistance to attack by moisture and
has high electrical and heat resistance. It is commonly used in glass-reinforced plas-
tics in the form of woven fabrics. C-glass is known for its chemical resistance to both
acids and alkalis. It is widely used for applications where such resistance is required,
such as in chemical ﬁltration. The S-glass is a high strength glass ﬁbre and is used
in composite manufacturing.
Glass ﬁlament yarns are brittle compared with the conventional textile yarns. It
has been shown that the speciﬁc ﬂexural rigidity of glass ﬁbre is 0.89 mN mm2 tex-2,
about 4.5 times more rigid than wool. As a result, glass yarns are easy to break in
textile processing. Therefore, it is important to apply suitable size to the glass yarn
to minimise the interﬁbre friction and to hold the individual ﬁbres together in
the strand. Dextrinised starch gum, gelatine, polyvinyl alcohol, hydrogenerated
vegetable oils and non-ionic detergents are commonly used sizes.
When handling glass ﬁbres, protective clothing and a mask should be worn to
prevent skin irritation and inhalation of glass ﬁbres.
126.96.36.199 Carbon ﬁlament yarns
Carbon ﬁbres are commonly made from precursor ﬁbres such as rayon and acrylic.
When converting acrylic ﬁbre to carbon, a three-stage heating process is used. The
initial stage is oxidative stabilisation, which heats the acrylic ﬁbre at 200–300 °C
under oxidising conditions. This is followed by the carbonisation stage, when the
oxidised ﬁbre is heated in an inert atmosphere to temperatures around 1000 °C.
Consequently, hydrogen and nitrogen atoms are expelled from the oxidised ﬁbre,
leaving the carbon atoms in the form of hexagonal rings that are arranged in
oriented ﬁbrils. The ﬁnal stage of the process is graphitisation, when the carbonised
ﬁlaments are heated to a temperature up to 3000 °C, again in an inert atmos-
phere. Graphitisation increases the orderly arrangement of the carbon atoms, which
Technical yarns 59
are organised into a crystalline structure of layers. These layers are well oriented in
the direction of ﬁbre axis, which is an important factor in producing high modulus
Like the glass yarns, most carbon ﬁbres are brittle. Sizes are used to adhere the
ﬁlaments together to improve the processability. In addition to protecting opera-
tives against skin irritation and short ﬁbre inhalation, protecting the processing
machinery and auxiliary electric and electronic devices needs to be considered too,
as carbon ﬁbre is conductive.
188.8.131.52 HDPE ﬁlament yarns
HDPE refers to high density polyethylene. Although the basic theory for making
super strong polyethylene ﬁbres was available in the 1930s, commercial high
performance polyethylene ﬁbre was not manufactured until recently. Spectra,
Dyneema, and Tekmilon are among the most well-known HDPE ﬁbres. The gel
spinning process is used to produce the HDPE ﬁbre. Polyethylene with an extra
high molecular weight is used as the starting material. In the gel spinning process,
the molecules are dissolved in a solvent and spun through a spinneret. In solution,
the molecules which form clusters in the solid state become disentangled and
remain in this state after the solution is cooled to give ﬁlaments.The drawing process
after spinning results in a very high level of macromolecular orientation in the
ﬁlaments, leading to a ﬁbre with very high tenacity and modulus. Dyneema, for
example, is characterised by a parallel orientation of greater than 95% and a high
level of crystallinity of up to 85%. This gives unique properties to the HDPE ﬁbres.
The most attractive properties of this type of ﬁbre are: (1) very high tenacity, (2)
very high speciﬁc modulus, (3) low elongation and (4) low ﬁbre density, that is lighter
HDPE ﬁbres are made into different grades for different applications. Dyneema,
for example, is made into SK60, SK65 and SK66. Dyneema SK60 is the multi-
purpose grade. It is used, for example, for ropes and cordage, for protective cloth-
ing and for reinforcement of impact-resistant composites. Dyneema SK65 has a
higher tenacity and modulus than SK60. This ﬁbre is used where high performance
is needed and maximum weight savings are to be attained. Dyneema SK66 is spe-
cially designed for ballistic protection. This ﬁbre provides the highest energy absorp-
tion at ultrasonic speeds.
Table 3.1 compares the properties of the above mentioned ﬁlament yarns to steel.
184.108.40.206 Other technical yarns
There have been many other high performance ﬁbres developed for technical appli-
cations, among which are PTFE, PBI, and PBO ﬁbres.
PTFE (polytetraﬂuoroethylene) ﬁbres offer a unique blend of chemical and tem-
perature resistance, coupled with a low fraction coefﬁcient. Since PTFE is virtually
chemically inert, it can withstand exposure to extremely harsh temperature and
chemical environments. The friction coefﬁcient, claimed to be the lowest of all ﬁbres,
makes it suitable for applications such as heavy-duty bearings where low relative
speeds are involved.
PBI (polybenzimidazole) is a manufactured ﬁbre in which the ﬁbre-forming
substance is a long chain aromatic polymer. It has excellent thermal resistance and
a good hand, coupled with a very high moisture regain. Because of these, the PBI
60 Handbook of technical textiles
Table 3.1 Comparison of ﬁlament yarn properties
Density Strength Modulus Elongation
(g cm-3) (GPa) (GPa) (%)
Aramid – regular 1.44 2.9 60 3.6
Aramid – composite 1.45 2.9 120 1.9
Aramid – ballistic 1.44 3.3 75 3.6
E Glass 2.60 3.5 72 4.8
S Glass 2.50 4.6 86 5.2
Carbon HS 1.78 3.4 240 1.4
Carbon HM 1.85 2.3 390 0.5
Dyneema SK60 0.97 2.7 89 3.5
Dyneema SK65 0.97 3.0 95 3.6
Dyneema SK66 0.97 3.2 99 3.7
Steel 7.86 1.77 200 1.1
Table 3.2 High performance ﬁbres
Fibre Density (g cm-3) Tenacity (mN tex-1) Elongation (%) Regain (%)
PTFE 2.1 0.9–2.0 19–140 0
PBI 1.43 2.6–3.0 25–30 15
PBO 1.54 42 2.5–3.5 0.6–2.0
ﬁbre is ideal for use in heat-resistant apparel for ﬁre ﬁghters, fuel handlers, welders,
astronauts, and racing car drivers.
PBO (polyphenylenebenzobisoxazole) is another new entrant in the high per-
formance organic ﬁbres market. Zylon, made by Toyobo, is the only PBO ﬁbre
in production. PBO ﬁbre has outstanding thermal properties and almost twice the
strength of conventional para-aramid ﬁbres. Its high modulus makes it an excellent
material for composite reinforcement. Its low LOI gives PBO more than twice the
ﬂame-retardant properties of meta-aramid ﬁbres. It can also be used for ballistic
vests and helmets.
Table 3.2 lists some properties of these ﬁbres.
a brearley and j iredale, The Worsted Industry, 2nd edition, WIRA, Leeds, 1980.
j g cook, Handbook of Textile Fibres, Manmade Fibres, 5th edition, Merrow, 1984.
Dyneema – the Top in High Performance Fibres, Properties and Applications, DSM High Performance
Fibres B.V., Eisterweg 3, 6422 PN Heerlen, Netherlands.
e t grifﬁths, ‘Wrap Spun Plain and Fancy Yarns’, Tomorrow’s Yarns, Conference Proceedings, UMIST,
s j kadolph and a l langford, Textiles, 8th edition, Prentice-Hall, 1998.
h kato, ‘Development of MJS Yarns’, J. Text. Machinery Soc. Jpn, 32(4) 1986.
w klein, New Spinning Systems, The Textile Institute, Manchester, 1993.
w klein, Man-made Fibres and Their Processing, The Textile Institute, Manchester, 1994.
w klein, The Technology of Short Staple Spinning, 2nd edition, The Textile Institute, Manchester, 1998.
w e morton and g r wray, An Introduction to the Study of Spinning, 3rd edition, Longmans, London,
Technical yarns 61
w e morton and j w s hearle, Physical Properties of Textile Fibres, 3rd edition, Textile Institute, Heine-
mann, London, 1993.
e oxtoby, Spun Yarn Technology, Butterworth, London, 1987.
h j selling, Twistless Yarns, Merrow, 1971.
w c smith, High Performance Fibres Protect, Improve Lives, http://www.textileworld.com/
Textile Terms and Deﬁnitions, 10th edition, Textile Institute, Manchester, 1995.
Technical fabric structures – 1. Woven fabrics
Walter S Sondhelm
10 Bowlacre Road, Hyde, Cheshire SK14 5ES, UK
Technical textiles1 are textile materials and products manufactured primarily for
their technical performance and functional properties rather than their aesthetic or
decorative characteristics. Most technical textiles consist of a manufactured assem-
bly of ﬁbres, yarns and/or strips of material which have a substantial surface area in
relation to their thickness and have sufﬁcient cohesion to give the assembly useful
Textile fabrics are most commonly woven but may also be produced by knitting,
felting, lace making, net making, nonwoven processes and tufting or a combination
of these processes. Most fabrics are two-dimensional but an increasing number
of three-dimensional woven technical textile structures are being developed and
Woven fabrics generally consist of two sets of yarns that are interlaced and lie at
right angles to each other. The threads that run along the length of the fabric are
known as warp ends whilst the threads that run from selvedge to selvedge, that is
from one side to the other side of the fabric, are weft picks. Frequently they are
simply referred to as ends and picks. In triaxial and in three-dimensional fabrics
yarns are arranged differently.
Woven technical textiles are designed to meet the requirements of their end use.
Their strength, thickness, extensibility, porosity and durability can be varied and
depend on the weave used, the thread spacing, that is the number of threads per
centimetre, and the raw materials, structure (ﬁlament or staple), linear density (or
count) and twist factors of the warp and weft yarns. From woven fabrics higher
strengths and greater stability can be obtained than from any other fabric structure
using interlaced yarns. Structures can also be varied to produce fabrics with widely
different properties in the warp and weft directions.
Technical fabric structures – 1. Woven fabrics 63
4.2 Weave structures
The number of weave structures that can be produced is practically unlimited. In
this section basic structures, from which all other weave structures are developed,
are discussed. Also brieﬂy referred to are lenos, because of their importance in
selvedge constructions, and triaxial fabrics, because they show simple structural
changes which can affect the physical properties of fabrics. Most two-dimensional
woven technical fabrics are constructed from simple weaves and of these at least
90% use plain weave. Simple cloth constructions are discussed in greater detail by
Robinson and Marks2 whilst Watson3,4 describes a large variety of simple and com-
plicated structures in great detail.
4.2.1 Plain weave
220.127.116.11 Construction of a plain weave
Plain weave is the simplest interlacing pattern which can be produced. It is formed
by alternatively lifting and lowering one warp thread across one weft thread. Figure
4.1 shows 16 repeats (four in the warp and four in the weft direction) of a plain
4.1 Fabric woven with plain weave – plan view (4 ¥ 4 repeats) and warp and
64 Handbook of technical textiles
weave fabric in plan view and warp way and weft way cross-sections through the
same fabric. The diagrams are idealized because yarns are seldom perfectly regular
and the pressure between the ends and picks tends to distort the shape of the yarn
cross-sections unless the fabrics are woven from monoﬁlament yarns or strips of
ﬁlm. The yarns also do not lie straight in the fabric because the warp and weft have
to bend round each other when they are interlaced. The wave form assumed by the
yarn is called crimp and is referred to in greater detail in Section 4.4.3.
18.104.22.168 Constructing a point paper diagram
To illustrate a weave either in plan view and/or in cross-section, as in Fig. 4.1, takes
a lot of time, especially for more complicated weaves.A type of shorthand for depict-
ing weave structures has therefore been evolved and the paper used for producing
designs is referred to as squared paper, design paper or point paper. Generally
the spaces between two vertical lines represent one warp end and the spaces
between two horizontal lines one pick. If a square is ﬁlled in it represents an end
passing over a pick whilst a blank square represents a pick passing over an end. If
ends and picks have to be numbered to make it easier to describe the weave, ends
are counted from left to right and picks from the bottom of the point paper design
to the top. The point paper design shown in Fig. 4.2(a) is the design for a plain weave
fabric. To get a better impression of how a number of repeats would look, four
repeats of a design (two vertically and two horizontally) are sometimes shown.
When four repeats are shown the ﬁrst repeat is drawn in the standard way but for
the remaining three repeats crossing diagonal lines may be placed into the squares,
which in the ﬁrsts repeat, are ﬁlled in. This method is shown for a plain weave in
22.214.171.124 Diversity of plain weave fabrics
The characteristics of the cloths woven will depend on the type of ﬁbre used for
producing the yarn and whether it is a monoﬁlament yarn, a ﬂat, twisted or textured
(multi-)ﬁlament yarn or whether it has been spun from natural or manufactured
staple ﬁbres. The stiffness of the fabrics and its weavability will also be affected by
the stiffness of the raw materials used and by the twist factor of the yarn, that is the
number of turns inserted in relation to its linear density. Very highly twisted yarns
are sometimes used to produce special features in plain weave yarns. The resulting
fabrics may have high extensibility or can be semiopaque.
4.2 Point paper diagram of a plain weave fabric. (a) One repeat, (b) four repeats.
Technical fabric structures – 1. Woven fabrics 65
The area density of the fabric can be varied by changing the linear density or
count of the yarns used and by altering the thread spacing, which affects the area
covered by the yarns in relation to the total area. The relation between the thread
spacing and the yarn linear density is called the cover factor and is discussed in
Section 4.4. Changing the area density and/or the cover factors may affect the
strength, thickness, stiffness, stability, porosity, ﬁltering quality and abrasion resist-
ance of fabrics.
Square sett plain fabrics, that is fabrics with roughly the same number of ends
and picks per unit area and warp and weft yarns of the same linear densities are
produced in the whole range of cloth area densities and cloth cover factors. Low
area density fabrics of open construction include bandages and cheese cloths, light
area density high cover factor fabrics include typewriter ribbons and medical ﬁlter
fabrics, heavy open cloths include geotextile stabilization fabrics and heavy closely
woven fabrics include cotton awnings.
Warp-faced plain fabrics generally have a much higher warp cover factor than
weft cover factor. If warp and weft yarns of similar linear density are used, a typical
warp faced plain may have twice as many warp ends as picks. In such fabrics the
warp crimp will be high and the weft crimp extremely low. The plan view and cross-
sections of such a fabric are shown in Fig. 4.3. By the use of suitable cover factors
and choice of yarns most of the abrasion on such a fabric can be concentrated on
the warp yarns and the weft will be protected.
Weft-faced plains are produced by using much higher weft cover factors than
warp cover factors and will have higher weft than warp crimp. Because of the dif-
ference in weaving tension the crimp difference will be slightly lower than in warp-
faced plain fabrics. Weft-faced plains are little used because they are more difﬁcult
and expensive to weave.
4.3 Plan view and cross-sections of warp-faced plain weave fabric with a substantially
higher warp than weft cover factor.
66 Handbook of technical textiles
4.2.2 Rib fabrics and matt weave fabrics
These are the simplest modiﬁcations of plain weave fabrics. They are produced by
lifting two or more adjoining warp threads and/or two or more adjoining picks at
the same time. It results in larger warp and/or weft covered surface areas than in a
plain weave fabric. As there are fewer yarn intersections it is possible to insert more
threads into a given space, that is to obtain a higher cover factor, without jamming
126.96.36.199 Rib fabrics
In warp rib fabrics there are generally more ends than picks per unit length with a
high warp crimp and a low weft crimp and vice versa for weft rib fabrics. The sim-
plest rib fabrics are the 2/2 warp rib and the 2/2 weft rib shown respectively in Fig.
4.4(a) and (b). In the 2/2 warp rib one warp end passes over two picks whilst in the
2/2 weft rib one pick passes over two adjoining ends. The length of the ﬂoats can be
extended to create 4/4, 6/6, 3/1 or any similar combination in either the warp or weft
direction. 3/1 and 4/4 warp ribs are shown in Fig. 4.4(c) and (d).
In rib weaves with long ﬂoats it is often difﬁcult to prevent adjoining yarns from
overlapping. Weft ribs also tend to be expensive to weave because of their relatively
high picks per unit length which reduces the production of the weaving machine
unless two picks can be inserted at the same time.
188.8.131.52 Matt fabrics (or hopsack)
Simple matt (or hopsack) fabrics have a similar appearance to plain weave. The sim-
plest of the matt weaves is a 2/2 matt shown in Fig. 4.5(a), where two warp ends are
lifted over two picks, in other words it is like a plain weave fabric with two ends and
two picks weaving in parallel. The number of threads lifting alike can be increased
to obtain 3/3 or 4/4 matt structures. Special matt weaves, like a 4/2 matt, shown in
Fig. 4.5(b), are produced to obtain special technical effects. Larger matt structures
give the appearance of squares but are little used because they tend to become
unstable, with long ﬂoats and threads in either direction riding over each other. If
large matt weaves are wanted to obtain a special effect or appearance they can be
stabilized by using fancy matt weaves containing a binding or stitching lift securing
a proportion of the ﬂoats.
Matt weave fabrics can be woven with higher cover factors and have fewer
intersections. In close constructions they may have better abrasion and better ﬁltra-
tion properties and greater resistance to water penetration. In more open construc-
tions matt fabrics have a greater tear resistance and bursting strength. Weaving costs
may also be reduced if two or more picks can be inserted at the same time.
4.2.3 Twill fabrics
A twill is a weave that repeats on three or more ends and picks and produces diago-
nal lines on the face of a fabric. Such lines generally run from selvedge to selvedge.
The direction of the diagonal lines on the surface of the cloth are generally described
as a fabric is viewed along the warp direction. When the diagonal lines are running
upwards to the right they are ‘Z twill’ or ‘twill right’ and when they run in the oppo-
site direction they are ‘S twill’ or ‘twill left’. Their angle and deﬁnition can be varied
68 Handbook of technical textiles
4.5 Matt fabrics. (a) 2/2 Matt, (b) 4/2 matt.
by changing the thread spacing and/or the linear density of the warp and weft yarns.
For any construction twills will have longer ﬂoats, fewer intersections and a more
open construction than a plain weave fabric with the same cloth particulars.
Industrial uses of twill fabrics are mainly restricted to simple twills and only
simple twills are discussed here. Broken twills, waved twills, herringbone twills and
elongated twills are extensively used for suiting and dress fabrics. For details of such
twills see Robinson and Marks2 or Watson.3,4
The smallest repeat of a twill weave consists of 3 ends ¥ 3 picks. There is no theo-
retical upper limit to the size of twill weaves but the need to produce stable fabrics
with ﬂoats of reasonable length imposes practical limits.
The twill is produced by commencing the lift sequence of adjacent ends on
one pick higher or one pick lower. The lift is the number of picks which an end
passes over and under. In a 2/1 twill, an end will pass over two picks and under one,
whilst in a 1/2 twill the end will pass over one pick and then under two picks. Either
weave can be produced as a Z or S twill. There are, therefore, four combinations of
this simplest of all twills and they are illustrated in Fig. 4.6(a) to (d). To show
how pronounced the twill line is even in a 3 ¥ 3 twill, four repeats (2 ¥ 2) of
Fig. 4.6(a) are shown in Fig. 4.6(e) with all lifted ends shown in solid on the point
paper. 2/1 twills are warp faced twills, that is fabrics where most of the warp yarn
is on the surface, whilst 1/2 twills have a weft face. Weft-faced twills impose less
strain on the weaving machine than warp-faced twills because fewer ends have to
be lifted to allow picks to pass under them. For this reason, warp-faced twills are
sometimes woven upside down, that is as weft-faced twills. The disadvantage of
weaving twills upside down is that it is more difﬁcult to inspect the warp yarns
Twills repeating on 4 ends ¥ 4 picks may be of 3/1, 2/2 or 1/3 construction and
may have ‘Z’ or ‘S’ directions of twill. Weaves showing 4 ¥ 4 twills with a Z twill
line are shown in Fig. 4.7(a) to (c). As the size of the twill repeat is increased further,
the number of possible variations also increases. In the case of a 5 ¥ 5 the possible
combinations are 4/1, 3/2, 2/3 and 1/4 and each of these can be woven with the twill
Technical fabric structures – 1. Woven fabrics 69
4.6 3 ¥ 3 Twill weaves. (a) 2/1 Twill with Z twill line, (b) 2/1 twill with S twill line, (c) 1/2
twill with Z twill line, (d) 1/2 twill with S twill line, (e) four repeats of (a) (2/1 twill with
a Z twist line).
(a) (b) (c)
4.7 4 ¥ 4 Twill weaves. (a) 3/1 Twill with Z twill line, (b) 2/2 twill with Z twill line,
(c) 1/3 twill with Z twill line.
70 Handbook of technical textiles
4.8 5 ¥ 5 Twill weaves. (a) 4/1 Twill with Z twill line, (b) 1/4 twill with Z twill line.
line in either direction. In Fig. 4.8(a) and (b) 4/1 and 1/4 twills with a Z twill line
4.2.4 Satins and sateens
In Britain a satin is a warp-faced weave in which the binding places are arranged
to produce a smooth fabric surface free from twill lines. Satins normally have a much
greater number of ends than picks per centimetre. To avoid confusion a satin is
frequently described as a ‘warp satin’. A sateen, frequently referred to as a ‘weft
sateen’, is a weft-faced weave similar to a satin with binding places arranged to
produce a smooth fabric free of twill lines. Sateens are generally woven with a much
higher number of picks than ends. Satins tend to be more popular than sateens
because it is cheaper to weave a cloth with a lower number of picks than ends.
Warp satins may be woven upside down, that is as a sateen but with a satin
construction, to reduce the tension on the harness mechanism that has to lift the
To avoid twill lines, satins and sateens have to be constructed in a systematic
manner. To construct a regular satin or sateen weave (for irregular or special ones
see Robinson and Marks2 or Watson3) without a twill effect a number of rules have
to be observed. The distribution of interlacing must be as random as possible and
there has only to be one interlacing of each warp and weft thread per repeat, that
is per weave number. The intersections must be arranged in an orderly manner, uni-
formly separated from each other and never adjacent. The weaves are developed
from a 1/¥ twill and the twill intersections are displaced by a ﬁxed number of steps.
The steps that must be avoided are:
(i) one or one less than the repeat (because this is a twill),
(ii) the same number as the repeat or having a common factor with the repeat
(because some of the yarns would fail to interlace).
The smallest weave number for either weave is 5 and regular satins or sateens also
cannot be constructed with weave numbers of 6, 9, 11, 13, 14 or 15. The most popular
weave numbers are 5 and 8 and weave numbers above 16 are impracticable because
of the length of ﬂoats. Weave numbers of 2 or 3 are possible for ﬁve-end weaves
and 3 or 5 for 8-end weaves.
Technical fabric structures – 1. Woven fabrics 71
4.9 5-End weft sateen. (a) 5-end and two step sateen, (b) 5-end three step sateen.
4.10 5-End warp satin. (a) 5-end two step satin, (b) 5-end three step satin.
Figure 4.9(a) and (b) shows 5-end weft sateens with two and three steps, respec-
tively. They have been developed from the 1/4 twill shown in Fig. 4.8(b). Mirror
images of these two weaves can be produced. Five-end warp satins with two
and three steps are shown in Fig. 4.10(a) and (b). It is the cloth particulars, rather
than the weave pattern, which generally decides on which fabric is commercially
described as a sateen or a satin woven upside down. Five-end satins and sateens are
most frequently used because with moderate cover factors they give ﬁrm fabrics.
Figure 4.11(a) and (b) shows 8-end weft sateens with three and ﬁve step repeats and
Fig. 4.12 shows an 8-end warp satin with a 5 step repeat.
Satins and sateens are widely used in uniforms, industrial and protective cloth-
ing. They are also used for special fabrics such as downproofs.
In North America a satin is a smooth, generally lustrous, fabric with a thick close
texture made in silk or other ﬁbres in a satin weave for a warp-face fabric or sateen
weave for a ﬁlling (weft) face effect. A sateen is a strong lustrous cotton fabric gen-
erally made with a ﬁve-harness satin weave in either warp or ﬁlling-face effect.
In lenos adjoining warp ends do not remain parallel when they are interlaced with
the weft but are crossed over each other. In the simplest leno one standard end and
72 Handbook of technical textiles
4.11 8-End weft sateen. (a) 8-end three step sateen, (b) 8-end ﬁve step sateen.
4.12 8-End ﬁve step warp satin.
one crossing end are passed across each other during consecutive picks. Two vari-
ations of this structure are shown in plan view and cross-section in Fig. 4.13(a) and
(b).4 Whenever the warp threads cross over each other, with the weft passing
between them, they lock the weft into position and prevent weft movement. Leno
weaves are therefore used in very open structures, such as gauzes, to prevent thread
movement and fabric distortion. When the selvedge construction of a fabric does
not bind its edge threads into position, leno ends are used to prevent the warp
threads at each side of a length of cloth from slipping out of the body of the
fabric. They are also used in the body of fabrics when empty dents are left in weav-
ing because the fabrics are to be slit into narrower widths at a later stage of
Leno and gauze fabrics may consist of standard and crossing ends only or pairs
or multiples of such threads may be introduced according to pattern to obtain the
required design. For larger effects standard and crossing ends may also be in pairs
or groups of three. Two or more weft threads may be introduced into one shed and
Technical fabric structures – 1. Woven fabrics 73
Plan View Cross-
4.13 (a) Leno with standard and crossing ends of same length (woven from one beam),
(b) leno with standard and crossing ends of different length (woven from two beams).
areas of plain fabric may be woven in the weft direction between picks where warp
ends are crossed over to give the leno effect. Gauze fabrics used for ﬁltration gen-
erally use simple leno weaves.
Standard and crossing ends frequently come from separate warp beams. If both
the standard and crossing ends are warped on to one beam the same length of
warp is available for both and they will have to do the same amount of bending,
that is they will have the same crimp. Such a leno fabric is shown in plan view
and cross-section in Fig. 4.13(a). If the two series of ends are brought from
separate beams the standard ends and the crossing ends can be tensioned differ-
ently and their crimp can be adjusted separately. In such a case it is possible for
the standard ends to lie straight and the crossing ends to do all the bending. Such
a fabric is shown in Fig. 4.13(b). This ﬁgure also shows that crossing threads can be
moved either from the right to the left or from the left to the right on the same pick
and adjoining leno pairs may either cross in the same or opposite directions. The
direction of crossing can affect locking, especially with smooth monoﬁlament yarns.
When using two beams it is also possible to use different types or counts of yarn
for standard and crossing ends for design or technical applications. The actual
method of weaving the leno with doups or similar mechanisms is not discussed in
74 Handbook of technical textiles
When lenos are used for selvedge construction only one to four pairs of threads
are generally used at each side and the leno selvedge is produced by a special leno
mechanism that is independent of the shedding mechanism of the loom. The leno
threads required for the selvedge then come from cones in a small separate creel
rather than from the warp beam. The choice of selvedge yarns and tensions is par-
ticularly important to prevent tight or curly selvedges. The crimps selected have to
take into account the cloth shrinkage in ﬁnishing.
4.2.6 Triaxial weaves
Nearly all two-dimensional woven structures have been developed from plain
weave fabrics and warp and weft yarns are interlaced at right angles or at nearly
right angles. This also applies in principle to leno fabrics (see Section 4.2.5 above)
and to lappet fabrics where a proportion of the warp yarns, that is the yarns forming
the design, are moved across a number of ground warp yarns by the lappet mecha-
nism. The only exceptions are triaxial fabrics, where two sets of warp yarns are gen-
erally inserted at 60° to the weft, and tetra-axial fabrics where four sets of yarns are
inclined at 45° to each other. So far only weaving machines for triaxial fabrics are
in commercial production. Triaxial weaving machines were ﬁrst built by the Barber-
Colman Co. under licence from Dow Weave and have been further developed by
Howa Machinery Ltd., Japan.
Triaxial fabrics are deﬁned as cloths where the three sets of threads form a
multitude of equilateral triangles. Two sets of warp yarn are interlaced at 60°
with each other and with the weft. In the basic triaxial fabric, shown in Fig. 4.14(a),
the warp travels from selvedge to selvedge at an angle of 30° from the vertical.
When a warp yarn reaches the selvedge it is turned through an angle of 120°
and then travels to the opposite selvedge thus forming a ﬁrm selvedge. Weft
yarn is inserted at right angles (90°) to the selvedge. The basic triaxial fabric is
fairly open with a diamond-shaped centre. The standard weaves can be modiﬁed
by having biplane, stuffed or basic basket weaves, the latter being shown in
Fig. 4.14(b). These modiﬁed weaves form closer structures with different character-
istics. Interlacing angles of 75° to the selvedge can be produced. At present
thread spacing in the basic weave fabric is limited to 3.6 or 7.4 threads per
The tear resistance and bursting resistance of triaxial fabrics is greatly superior
to that of standard fabrics because strain is always taken in two directions. Their
shear resistance is also excellent because intersections are locked. They have a wide
range of technical applications including sailcloths, tyre fabrics, balloon fabrics,
pressure receptacles and laminated structures.
The selvedges form the longitudinal edges of a fabric and are generally formed
during weaving. The weave used to construct the selvedge may be the same, or may
differ from, the weave used in the body of the cloth. Most selvedges are fairly narrow
but they can be up to 20-mm wide. Descriptions may be woven into the selvedge,
using special selvedge jacquards, or coloured or fancy threads may be incorporated
for identiﬁcation purposes. For some end-uses selvedges have to be discarded but,
Technical fabric structures – 1. Woven fabrics 75
4.14 Triaxial fabrics (weaving machine: Howa TRI-AX Model TWM). (a) Basic weave,
(b) basic basket weave.
4.15 (a) Hairpin selvedge – shuttle loom, (b) leno selvedge with dummy selvedge,
(c) helical selvedge, (d) tucked-in or tuck selvedge.
whenever possible, selvedges should be constructed so that they can be incorpo-
rated into the ﬁnal product so as to reduce the cost of waste.
In cloths woven on weaving machines with shuttles selvedges are formed by the
weft turning at the edges after the insertion of each pick. The weft passes continu-
ously across the width of the fabric from side to side. In cloths woven on shuttleless
weaving machines the weft is cut at the end of each pick or after every second pick.
To prevent the outside ends from fraying, various selvedge motions are used to bind
the warp into the body of the cloth or edges may be sealed. The essential require-
ments are that the selvedges should protect the edge of the fabric during weaving
and subsequent processing, that they should not detract from the appearance of the
cloth and that they should not interfere with ﬁnishing or cause waviness, contrac-
tion or creasing. Four types of woven selvedges are shown in Fig. 4.15.
76 Handbook of technical textiles
4.3.1 Hairpin selvedge – shuttle weaving machine
Figure 4.15(a) shows a typical hairpin selvedge which is formed when the weft
package is carried in a reciprocating media, for example a shuttle. With most weaves
it gives a good edge and requires no special mechanism. Frequently strong two-ply
yarns are incorporated into the selvedge whilst single yarns are used in the body of
the cloth because the edge threads are subjected to special strains during beat-up.
To ensure a ﬂat edge a different weave may be used in the selvedge from the body
of the cloth. For twills, satins and fancy weaves this may also be necessary to ensure
that all warp threads are properly bound into the edge. If special selvedge yarns are
used it is important to ensure that they are not, by mistake, woven into the body of
the fabric because they are likely to show up after ﬁnishing or cause a reduction in
the tear and/or bursting resistance of industrial fabrics.
When two or more different weft yarns are used in a fabric only one weft yarn
is being inserted at a time and the other yarn(s) are inactive until the weft is
changed. In shuttle looms the weft being inserted at any one time will form a normal
selvedge whilst the weft yarn(s) not in use will ﬂoat along the selvedge. If long ﬂoats
are formed in weaving, because one weft is not required for a considerable period,
the ﬂoats may have to be trimmed off after weaving to prevent them from causing
problems during subsequent processing. Whenever a pirn is changed, or a broken
pick is repaired, a short length of yarn will also protrude from the selvedge and this
has to be trimmed off after weaving.
Industrial fabrics with coarse weft yarn are sometimes woven with loop selvedges
to ensure that the thread spacing and cloth thickness remains the same right to the
edge of the cloth. To produce a loop selvedge a wire or coarse monoﬁlament yarn
is placed 3 or 4 mm outside the edge warp end and the pick reverses round the wire
to form a loop. As the wire is considerably stiffer than a yarn it will prevent the weft
pulling the end threads together during beat-up. The wire extends to the fell of the
cloth and is automatically withdrawn during weaving. Great care is required to
ensure that no broken-off ends of wire or monoﬁlament remain in the fabric because
they can cause serious damage to equipment and to the cloth during subsequent
4.3.2 Leno and helical selvedges
In most shuttleless weaving machines a length of weft has to be cut for every pick.
For looms not ﬁtted with tucking motions the warp threads at the edges of the fabric
have to be locked into position to prevent fraying. With some weft insertion systems
the weft has to be cut only after every second pick and it is possible to have a hairpin
selvedge on one side of the fabric and a locked selvedge on the second side. Leno
and helical selvedges are widely used to lock warp yarns into position and these are
shown in Fig. 4.15(b) and (c), respectively. When shuttleless weaving machines were
ﬁrst introduced there was considerable customer resistance to fringe selvedges but,
in the meantime, it has been found that they meet most requirements.
With leno selvedges (see also Section 4.2.5) a set of threads at the edge of the
fabric is interlaced with a gauze weave which locks round the weft thread and pre-
vents ravelling of the warp. As the precut length of the picks always varies slightly,
a dummy selvedge is sometimes used at the edge of the cloth as shown in Fig.
4.15(b). This makes it possible to cut the weft close to the body of the cloth result-
ing in a narrow fringe which has a better appearance than the selvedge from which
Technical fabric structures – 1. Woven fabrics 77
weft threads of varying lengths protrude. It also has the advantage in ﬁnishing and
coating that there are no long lengths of loose weft that can untwist and shed
ﬂy. Because of the tails of weft and because of the warp in dummy selvedges,
more waste is generally made in narrow shuttleless woven fabrics than in fabrics
woven on shuttle looms. For wide cloth the reverse frequently applies because there
is no shuttle waste. Leno selvedges, sometimes referred to as ‘centre selvedges’, may
be introduced into the body of the cloth if it is intended to slit the width of
cloth produced on the loom into two or more widths either on the loom or after
Helical selvedges consist of a set of threads which make a half or complete
revolution around one another between picks. They can be used instead of leno
selvedges and tend to have a neater appearance.
4.3.3 Tucked-in selvedges
A tuck or tucked-in selvedge is shown in Fig. 4.15(d). It gives a very neat and strong
selvedge and was ﬁrst developed by Sulzer5 Brothers (now Sulzer-Textil), Win-
terthur, Switzerland, for use on their projectile weaving machines. Its appearance is
close to that of a hairpin selvedge and it is particularly useful when cloths with fringe
selvedges would have to be hemmed. High-speed tucking motions are now avail-
able and it is possible to produce tucked-in selvedges even on the fastest weaving
Tucked-in selvedges, even when produced with a reduced number of warp
threads, are generally slightly thicker than the body of the cloth. When large batches
of cloth with such selvedges are produced it may be necessary to traverse the cloth
on the cloth roller to build a level roll. The extra thickness will also have to be
allowed for when fabrics are coated. When tucked-in selvedges can be incorporated
into the ﬁnished product no yarn waste is made because no dummy selvedges are
produced but the reduced cost of waste may be counterbalanced by the relatively
high cost of the tucking units.
4.3.4 Sealed selvedges
When fabrics are produced from yarns with thermoplastic properties the edge of a
fabric may be cut and sealed by heat. The edge ends of fringe selvedges are fre-
quently cut off in the loom and the edge threads with the fringe are drawn away
into a waste container. Heat cutting may also be used to slit a cloth, in or off the
loom, into a number of narrower fabrics or tapes.
For special purposes ultrasonic sealing devices are available. These devices are
fairly expensive and can cut more cloth than can be woven on one loom. Whilst they
can be mounted on the loom they are, because of their cost, more frequently
mounted on a separate cutting or inspection table.
4.4 Fabric speciﬁcations and fabric geometry
Fabric speciﬁcations6 describe a cloth but frequently need experience for correct
interpretation. The most important elements are cloth width, threads per centime-
tre in the warp and weft directions, linear density (count) and type of warp and weft
78 Handbook of technical textiles
yarns (raw material, ﬁlament or staple, construction, direction of twist and twist
factors), weave structure (see Section 4.2 above) and ﬁnish. From these, if the
weaving machine particulars and ﬁnishing instructions are known, the cloth area
density can be calculated.
It has been assumed that other cloth particulars, such as warp and weft cover
factors, crimp, cloth thickness, porosity and drape, have either to be estimated or
measured by various test methods. Peirce7 showed that standard physical and engi-
neering principles can be applied to textiles and cloth speciﬁcations can be forecast
if the effect of interlacing the warp and weft threads and the distortion of the yarns
caused thereby is allowed for.
4.4.1 Fabric width
The width of fabrics is generally expressed in centimetres and has to be measured
under standard conditions to allow for variations which are caused by moisture and
tension. It is necessary to know whether the cloth width required is from edge to
edge or whether it excludes the selvedges. Before deciding on the weaving speciﬁ-
cations of a fabric, allowance has to be made not only for shrinkage from reed width
to grey width during weaving but also for contraction (if any) during ﬁnishing. If
the cloth width changes, other parameters such as cloth area density and threads
per centimetre, will be effected.
4.4.2 Fabric area density
The fabric area density is generally expressed in grams per square metre although
sometimes it is reported as grams per linear metre. It is essential to specify whether
the area density required is loomstate or ﬁnished. The loomstate area density
depends on the weaving speciﬁcation, that is, yarns, thread spacing and weave, and
on any additives, such as size, which are used to improve the weaving process. During
ﬁnishing the cloth area density is frequently altered by tension and chemical treat-
ments or compressive shrinkage which affect cloth width and length, by the removal
of additives needed in weaving and by substances added during ﬁnishing.
The waviness or crimp1 of a yarn in a fabric, shown in the cross-sections of Fig. 4.1,
is caused during weaving and may be modiﬁed in ﬁnishing. It is due to the yarns
being forced to bend around each other during beat-up. It depends on the warp and
weft cover factors, which are described in Section 4.4.4, the characteristics of the
yarns and the weaving and ﬁnishing tensions.
The crimp is measured by the relation between the length of the fabric sample
and the corresponding length of yarn when it has been straightened after being
removed from the cloth, as shown in Fig. 4.16, which, as drawn, is idealized and
only applies to monoﬁlament yarns. Multiﬁlament and staple yarn will be deformed
to some extent at intersections by the pressure exerted by the warp on the weft
or vice versa depending on yarn particulars and cloth construction. It is most
convenient to express crimp as a percentage, which is 100 divided by the fabric
length and multiplied by the difference between the yarn length and the fabric
Technical fabric structures – 1. Woven fabrics 79
4.16 Crimp – relation of length of yarn in cloth to length of cloth. x is the width of sample,
y is the length of yarn extracted from sample and percentage crimp = (y - x)/x ¥ 100.
Warp crimp is used to decide the length of yarn which has to be placed on to a
warper’s beam to weave a speciﬁed length of fabric. Allowance has to be made for
stretching of the yarns during weaving which is generally low for heavily sized
yarns but can be of importance when unsized or lightly sized warps are used. For
fabrics woven on shuttleless weaving machines, the estimated weft crimp has to be
adjusted for the length of yarn used to produce a selvedge and, sometimes, a dummy
4.4.4 Cover factors
The cover factor1 indicates the extent to which the area of a fabric is covered by
one set of threads. For any fabric there are two cover factors: the warp cover factor
and the weft cover factor. The cloth cover factor is obtained by adding the weft
cover factor to the warp cover factor. The cover factors can be adjusted to allow for
yarns of different relative densities – either because of the yarn structure or because
of the raw material used.
The cover factors in SI units8 are calculated by multiplying the threads per cen-
timetre by the square root of the linear density of the yarn (in tex) and dividing by
10. The resultant cover factor differs by less than 5% from the cotton cover factor
pioneered by Peirce7 and expressed as the number of threads per inch divided by
the square root of the cotton yarn count.
For any given thread spacing plain weave has the largest number of intersections
per unit area. All other weaves have fewer intersections than plain weave. The likely
weavability of all fabrics woven with the same weave and from similar yarns can be
forecast from their cover factors. Plain weave fabrics with warp and weft cover
factors of 12 in each direction are easy to weave. Thereafter weaving becomes more
difﬁcult and for cover factors of 14 + 14 fairly strong weaving machines are required.
At a cover factor of 16 + 16 the plain structure jams and a very strong loom with
heavy beat-up is needed to deform the yarns sufﬁciently to obtain a satisfactory beat-
up of the weft. Some duck and canvas fabrics woven on special looms achieve much
greater cover factors.Three cloths with cover factors of 12 + 12 are shown in Table 4.1.
It shows how thread spacing and linear density have to be adjusted to maintain the
required cover factor and how cloth area density and thickness are affected.
When widely varying cover factors are used for warp and weft, a high cover factor
in one direction can generally be compensated by a low cover factor in the other
direction. In Fig. 4.3, which shows a poplin-type weave, the warp does all the bending
and the weft lies straight. With this construction warp yarns can touch because they
bend around the weft and cloth cover factors of well above 32 can be woven fairly
easily. Peirce calculated the original adjustment factors for a number of weave
80 Handbook of technical textiles
Table 4.1 Comparison of fabrics with identical warp and weft cover factors woven with
yarns of different linear densities (in SI units)
per cm density Cloth weighta Thicknessb
n1 n2 N1 N2
A 24 24 25 25 12.0 12.0 130 0.28
B 12 12 100 100 12.0 12.0 260 0.56
C 6 6 400 400 12.0 12.0 520 1.12
n1 are warp threads, n2 are weft threads, N1 is the linear density of warp, N2 is the linear density of weft,
K1 is the warp cover factor, K2 is the weft cover factor.
Allowing for 9% of crimp.
Allowing 25% for ﬂattening and displacement of yarns.
Table 4.2 Cover factor adjustment factors for weave
Weave Adjustment factora
Plain weave 1.0
2/2 weft rib 0.92
1/2 and 2/1 twills 0.87
2/2 matt 0.82
1/3, 3/1 and 2/2 twills 0.77
5 end satin and 5 end sateen 0.69
Multiply actual cover factor by adjustment factor to obtain equiva-
lent plain weave cover factor.
structures. Rüti9 published an adjustment factor that they found useful to establish
whether fabrics with various weave structures can be woven in their machines and
these are shown in Table 4.2. Sulzer have prepared graphs showing how easy or dif-
ﬁcult it is to weave fabrics with different weave structures, thread spacings and linear
densities in various types of weaving machines.
Yarn properties are as important as cloth particulars when forecasting cloth thick-
ness. It is difﬁcult to calculate the cloth thickness because it is greatly inﬂuenced by
yarn distortion during weaving and by pressures exerted on the cloth during ﬁnish-
ing. It is also difﬁcult to measure thickness because the results are inﬂuenced by the
size of the presser feet used in the test instrument, the pressure applied and the time
that has elapsed before the reading is taken. It is therefore essential to specify the
method of measurement of thickness carefully for many industrial fabrics.
4.5 Weaving – machines (looms) and operations
Whilst the principle of weft interlacing in weaving has not changed for thousands
of years, the methods used and the way that weaving machines are activated and
controlled has been modiﬁed. During the last few decades of the 20th century the
Technical fabric structures – 1. Woven fabrics 81
rate of change increased continuously and weft insertion rates, which control
machine productivity, increased ten-fold from around 1950–2000 and they are likely
to double again during the ﬁrst ﬁve to ten years of the 21st century. The productiv-
ity of the weaver has increased even more and is likely soon to have increased a
hundred-fold. Weaving, which used to be a labour-intensive industry, is now capital
intensive using the most modern technology.
The essential operations in the weaving of a cloth are:
1. Shedding, i.e. the separation of the warp threads into two (or more) sheets
according to a pattern to allow for weft insertion
2. Weft insertion (picking) and
3. Beating-up, i.e. forcing the pick, which has been inserted into the shed, up to
the fell of the cloth (line where the cloth terminates after the previous pick has
Provision has also to be made for the supply of warp and weft warp yarns and for
the cloth, after weaving, to be collected. The warp yarn is usually supplied on warp
beam(s) and the weft on pirn (shuttle looms only) or cones. A typical cross-section
through a shuttle weaving machine10 showing the main motions, together with the
arrangement of some ancillary motions, is shown schematically in Fig. 4.17. Most
single phase machines, irrespective of their weft insertion system, use similar
motions and a nearly horizontal warp sheet between the back rest(2) and the front
rest(9).Although this is the most common layout, other successful layouts have been
developed. One of these, for an air jet,11 is shown in Fig. 4.18 and an interesting
double-sided air jet with two vertical warp lines back to back is being developed
2 3 4 7 8 9
4.17 Schematic section through Rüti shuttle weaving machine (machine motions and
parts shown in italics). 1, Weaver’s beam holding warp yarn (controlled by let-off ); 2, back
rest guiding yarn and controlling warp tension; 3, drop wires of warp stop motion; 4, shed
formed by top and bottom warp sheet; 5, healds controlled by shedding motion (crank, cam
or dobby) (Jacquard shedding motions do not use healds); 6, sley carrying reed and shuttle.
It reciprocates for beat-up. (In many shuttleless machines the weft insertion system and the
reed have been separated); 7, shuttle carrying the pirn; 8, fell where cloth is formed; 9, front
rest for guiding cloth; 10, take-up motion controlling the pick spacing and cloth wind-up;
11, cloth being wound on to cloth roller.
82 Handbook of technical textiles
4.18 Schematic section through Elitex air jet weaving machine (machine motions and
parts shown in italics). 1, Weaver’s beam holding warp yarn (controlled by let-off ); 2, back
rest guiding warp yarn; 3, drop wires of warp stop motion; 4, shed formed by top and
bottom warp sheet; 5, healds controlled by cam shedding motion; 6, weft insertion area (the
reed for beating-up located in this area is not shown); 7, fell where cloth is formed; 8, front
rest for guiding cloth; 9, take-up motion controlling the pick spacing and cloth wind-up;
10, cloth being wound on to cloth roller.
Weaving machines can be subdivided into single phase machines, where one weft
thread is laid across the full width of the warp sheet followed by the beat-up
and the formation of the next shed in preparation for the insertion of the next pick,
and multiphase machines, in which several phases of the working cycle take place
at any instant so that several picks are being inserted simultaneously. Single phase
machines are further subdivided according to their weft insertion system, whilst
multiphase machines are classiﬁed according to their method of shed formation. The
classiﬁcation of weaving machines is summarized in Table 4.3.
In this chapter the details of the different types of weaving machines and their
functions can only be outlined and the most important points highlighted. Weaving
machines and their operation are described and discussed by Ormerod and
For the successful operation of a weaving machine good warps are essential.Warp
preparation is, therefore, discussed in Section 4.5.1. This is followed by shedding in
Section 4.5.2, weft insertion and beating-up in Section 4.5.3 and other motions used
on machines in Section 4.5.4. The importance of machine width is considered in
4.5.1 Warp preparation
The success of the weaving operation depends on the quality of the weaver’s beam
presented to the weaving machine because each fault in the warp will either stop
the machine and require rectiﬁcation, or cause a fault in the cloth, which is woven
Before most fabrics can be woven a weaver’s beam (or beams) holding the warp
yarn has to be prepared. For very coarse warp yarns or when very long lengths of
Technical fabric structures – 1. Woven fabrics 83
Table 4.3 Classiﬁcation of weaving machines
Single-phase weaving machines
Machines with shuttles (looms):
Hand operated (hand looms)
Non-automatic power looms (weft supply in shuttle changed by hand)
Automatic weaving machines
• shuttle changing
rotary batteries, stack batteries, box loaders or
pirn winder mounted on machine (Uniﬁl)
• pirn changing
Shuttleless weaving machines:
• rigid rapier(s)
single rapier, single rapier working bilaterally
or two rapiers operating from opposite sides of machine
• air (with or without relay nozzles)
• liquid (generally water)
Multiphase weaving machines
Wave shed machines:
Weft carriers move in straight path
Circular weaving machines (weft carriers travel in circular path)
Parallel shed machines (rapier or air jet)
ﬁlament can be woven without modiﬁcation of the warping particulars, a separate
cone creel placed behind each weaving machine can be used economically. It
improves the weaving efﬁciency by avoiding frequent beam changes but requires a
large amount of space. For most yarns, especially sized yarns, it is more economical
to prepare a weaver’s beam and use it in the weaving machine.
The object of most warp preparation systems is to assemble all ends needed in
the weaving machine on one beam and to present the warp with all ends continu-
ously present and the integrity and elasticity of the yarns as wound fully preserved.
Before this can be done the yarns have ﬁrst to be wound on to a cone, then rewound
on to a warper’s beam and ﬁnally sized before the weaver’s beam is made. The
purpose of warp sizing is to apply a protective coating to the yarn to enable it to
withstand the complex stresses to which it is subjected in the weaving machine.
Some coarse ply yarns and some strong ﬁlament yarns can be woven without
Details of the various warp preparation processes are described by Ormerod and
Irrespective of whether cloth is woven on an ancient handloom or produced on the
most modern high speed multiphase weaving machine a shed has to be formed
before a pick can be inserted prior to beat-up and cloth formation. The shed must
be clean, that is slack warp threads or hairy or taped ends must not obstruct the
84 Handbook of technical textiles
passage of the weft or of the weft carrier. If the weft cannot pass without obstruc-
tion either the machine will stop for rectiﬁcation, a warp end may be cut or damaged
or a faulty weave pattern may be produced.
184.108.40.206 Shedding in single phase machines
In most single phase weaving machines, before pick insertion commences, an upper
and a lower warp sheet is formed and the lifting pattern is not changed until the
weft thread has been inserted across the full width of the warp. The shedding
mechanism is used to move individual ends up or down in a prearranged order gov-
erned by the weave pattern. To maintain a good separation of the ends during
weaving and avoid adjoining ends from interfering with each other the ends in each
warp sheet can be staggered but in the area of weft insertion an unobstructed gap
through which the weft can pass has to be maintained. The shedding mechanism
chosen for a given weaving machine depends on the patterns that it is intended to
weave on it. Most shedding mechanisms are expensive and the more versatile the
mechanism the greater its cost. On some weaving machines there are also techni-
cal limitations governing the shedding mechanisms that can be ﬁtted.
When crank, cam (or tappet) or dobby shedding is used, ends are threaded
through eyes in healds that are placed into and lifted and lowered by heald frames.
All healds in one heald frame are lifted together and all ends controlled by it will
therefore lift alike. The weave pattern therefore controls the minimum number of
healds required. To prevent overcrowding of healds in a heald frame or to even out
the number of ends on a heald frame, more than one frame may lift to the same
pattern. To weave a plain fabric, for example, 2, 4, 6, or 8 heald frames may be used
with equal numbers of frames lifting and lowering the warp on each pick. Crank
motions are generally limited to 8 shafts, cams to 10 or 12 and dobbies to 18 or 24.
When the necessary lifting pattern cannot be obtained by the use of 24 shafts a
Jacquard shedding mechanism, in which individual ends can be controlled sepa-
rately, has to be used.
The crank shedding mechanism is the simplest and most positive available. It can
only be used to weave plain weave. It is cheap, simple to maintain and in many high
speed machines increases weft insertion rates by up to 10%. This mechanism has
not been used as much as would be expected because of its lack of versatility. It is
however particularly useful for many industrial fabrics that, like the majority of all
fabrics, are woven with plain weave.
Cam or tappet shedding motions on modern high speed machines use grooved
or conjugate cams because they give a positive control of the heald shafts. Negative
proﬁle cams are, however, still widely used especially for the weaving of fairly open
fabrics of light and medium area density. The cam proﬁle is designed to give the
necessary lifting pattern to healds in the sequence required by the lifting plan which
is constructed from the weave structure.
The third method of controlling heald shafts is by dobby and its main advantage
is that there is practically no limit to the size of pattern repeat that can be woven,
whilst with cam motions it is difﬁcult and expensive to construct a repeat of more
than eight or ten picks. It is also easier to build dobbies for a large number of heald
shafts. Dobbies were controlled by pattern chains containing rollers or pegs which
accentuated the lifting mechanism of the heald shafts. Punched rolls of paper or
plastic were used instead of the heavier wooden pegs or metal chains for long
repeats. During the 1990s electronic dobbies have replaced mechanical ones
Technical fabric structures – 1. Woven fabrics 85
enabling weaving machines to operate at much greater speeds, reducing the cost of
preparing a pattern and the time required for changing to a new design. Following
the development of electronic dobbies, cam machines are becoming less popular
because cams for high speed machines are expensive. If large numbers are required,
because of the weave structure or because of frequent pattern changes, it may be
cheaper to buy machines ﬁtted with dobbies.
Shedding mechanisms are still undergoing intensive development and electronic
control of individual shafts may soon reduce the difference in cost between crank,
cam and dobby machines. Developments are likely to simplify the shedding units,
reduce the cost of shedding mechanisms and their maintenance and make weaving
machines more versatile.
When the patterning capacity of dobbies is insufﬁcient to weave the required
designs, Jacquards have to be used. Modern electronic Jacquards can operate at very
high speeds and impose practically no limitation on the design. Every end across
the full width of the weaving machine can be controlled individually and the weft
repeat can be of any desired length. Jacquards are expensive and, if a very large
number of ends have to be controlled individually, rather than in groups, the
Jacquard may cost as much as the basic weaving machine above which it is mounted.
220.127.116.11 Shedding in multiphase weaving machines
In all multiphase weaving machines1 several phases of the working cycle take place
at any instant so that several picks are being inserted simultaneously. In wave
shed machines different parts of the of the warp sheet are in different parts of the
weaving cycle at any one moment. This makes it possible for a series of shuttles or
weft carriers to move along in successive sheds in the same plane. In parallel shed
machines several sheds are formed simultaneously with each shed extending across
the full width of the warp and with the shed moving in the warp direction. The
difference between the methods of shed formation are shown schematically in
Weaving machines in which shuttles travel a circular path through the wave shed
are generally referred to as ‘circular weaving machines’. They have been widely used
for producing circular woven polypropylene fabrics for large bags for heavy loads.
4.19 Weft insertion on multiphase weaving machines (plain weave). (a) Wave shed
principle, (b) multiphase parallel shed principle. Reproduced by kind permission of
86 Handbook of technical textiles
1830 800 3210 800 1830
4.20 Schematic drawing of Starlinger circular loom SL4. Reproduced by kind permission
of Starlinger & Co. G.m.b.H. (all dimensions in mm).
Combined shed-forming reed/insertion channel
4.21 Shed formation of Sulzer Textil multiphase parallel shed M8300. Shed-forming reed
with weft insertion channel and beat-up reed mounted on drum. Reproduced by kind
permission of Sulzer Textil.
The layout of a Starlinger circular weaving machine16 is shown in Fig. 4.20. The creels
containing cheeses of polypropylene tape are located on either side of the weaving
unit that is in the centre. The warp yarns are fed into the weaving elements from
the bottom, interlaced with weft carried in either four or six shuttles through the
wave shed in the weaving area, and the cloth is drawn off from the middle top and
wound on to a large cloth roll by the batching motion located on the right.
No wave shed machine using weft carriers moving in a straight path has proved
commercially successful because the shedding elements have no upper constraint,
making it impossible to guarantee a correct cloth structure, and because maintain-
ing a clean shed has proved very difﬁcult. Their attraction was a weft insertion rate
of up to 2200 m min-1 but they became obsolescent when simpler single phase air jet
machines begun to exceed this speed.
The ﬁrst parallel shed machine to win limited commercial acceptance was the
Orbit 112,13 which on a two head machine weaving used rigid rapiers for weft inser-
tion and reached weft insertion rates of up to 3600 m min-1 when weaving bandage
fabrics. Sulzer Textil released their new multiphase linear air jet machine, which is
already operating at up to 5000 m min-1 and is only at the beginning of its opera-
tional development. This machine, which needs no healds, has a rotating drum on
which the shed-forming reed and beat-up reed are mounted (Fig. 4.21).17 On this
machine shedding is gentle and individual picks are transported across the warp
sheet at relatively low speeds. Weft yarns do not have to be accelerated and decel-
erated continuously thus reducing the stresses imposed on the yarns. This reduces
demands on yarn and, for the ﬁrst time, we have a machine with a high insertion
Technical fabric structures – 1. Woven fabrics 87
rate which should be able to weave relatively weak yarns at low stop rate and high
4.5.3 Weft insertion and beat-up (single phase machines)
All single phase weaving machines are classiﬁed in accordance with their weft in-
sertion system. The different types have been summarised in Table 4.3. The main
methods of single phase weft insertion are by shuttle (Fig. 4.22), projectile (Fig. 4.23),
rapier and air or water jet (Fig. 4.24).
18.104.22.168 Weft insertion by shuttle
Looms using shuttles for carrying the weft through the warp sheet dominated cloth
production until the 1980s even in high wage countries like the USA. They are now
obsolete, except for use in weaving a few highly specialised fabrics. In spite of this,
large numbers of automatic bobbin changing looms are still in use but they are being
rapidly replaced by shuttleless weaving machines. Shuttleless machines produce
more regular fabrics with fewer faults and need less labour for weaving and main-
tenance. Millions of handlooms are still in operation in south east Asia being pro-
tected by legislation.
Figure 4.22 shows schematically the production of cloth on a shuttle loom. The
shuttle carrying the pirn, on which the weft is wound, is reciprocated through the
warp by a picking motion (not shown) on each side of the machine. For each pick
the shuttle has to be accelerated very rapidly and propelled along the race board.
Whilst crossing through the shed, one pick of weft is released and when the shuttle
reaches the second shuttle box, the shuttle has to be stopped very rapidly. After each
pick has been inserted it has to be beaten-up, that is moved to the fell of the cloth.
The reed and the race board are mounted on the sley and during the weaving cycle
are reciprocated backward and forward. Whilst the shuttle passes through the shed
the sley is close to the healds to enable the shuttle to pass without damaging the
warp yarns. The sley is then moved forward for beat-up. The need to have an open
shed for weft insertion during a considerable part of the picking cycle, and the
weight of the sley carrying the race board and the reed, impose restrictions on the
picking speed, i.e. the number of revolutions at which the loom can operate.
The basic weakness of ﬂy shuttle weaving machines is the unsatisfactory ratio
existing between the large projected mass of the shuttle and the weft bobbin in rela-
tion to the small variable mass of the weft yarn carried in the shuttle.13 Only about
4.22 Weft insertion by shuttle (schematic). 1, Warp yarns; 2, reed; 3, shuttle carrying pirn
(entering shed); 4, fell of cloth. Picking motions and race board not shown. Reproduced by
kind permission of Sulzer Textil.
88 Handbook of technical textiles
3% of the energy imparted to the shuttle is used for the actual weft insertion.
Further limitations on machine speed are imposed by the need to reciprocate the
heavy sley. Whilst theoretically it is possible to attain weft insertion rates of up to
450 m min-1 for wide machines, few shuttle machines in commercial use exceed 250
In a non-automatic power loom each time a pirn is nearly empty the weaver has
to stop the loom and replace it. Pirns should be replaced when there is still a little
weft left on them to prevent the weft running out in the middle of the shed and cre-
ating a broken pick which has to be repaired. In industrialized countries most power
looms have been replaced by automatic pirn changing weaving machines that, in
turn, are now being replaced by shuttleless weaving machines. In automatic weaving
machines the pirns are changed without attention from the weaver and without the
loom stopping. The replacement pirns are periodically placed into a magazine by an
operative so that the machine can activate the pirn replacement whenever neces-
sary. The magazine ﬁllers can be replaced by a ‘box loader’ attachment when the
pirns are brought to the loom in special boxes from where they are transferred auto-
matically to the change mechanism. Shuttle change looms, where the shuttle rather
than the pirn is changed whenever the pirn empties, are available for very weak
yarns. All these methods require pirns to be wound prior to being supplied to the
loom. Alternatively a Uniﬁl attachment can be ﬁtted to wind the pirns on the
weaving machine and feed them into the change mechanism.
There are practically no restrictions on the widths or area density of fabrics which
can be woven on shuttle machines. Automatic looms can be ﬁtted with extra shuttle
boxes and special magazines so that more than one weft yarn can be inserted in
accordance with a prearranged pattern. Compared with similar equipment for shut-
tleless machines this equipment is clumsy and labour intensive.
22.214.171.124 Projectile machines
Projectile machines can use either a single projectile, which is ﬁred from each side
of the machine alternately and requires a bilateral weft supply, or use a unilateral
weft supply and a number of projectiles which are always ﬁred from the same
side and are returned to the picking position on a conveyor belt. Since Sulzer
commenced series production of their unilateral picking multiple projectile
machines in the 1950s they have dominated the market and have sold more shut-
tleless machines than any other manufacturer. Sulzer Textil have continuously
developed their machines, improved weft insertion rates and machine efﬁciency
and extended the range of fabrics that can be woven on them. They are now used
not only for weaving a vast range of standard fabrics but also for heavy industrial
fabrics of up to 8 m wide, for sailcloth, conveyor belts, tyre cord fabrics, awnings,
geotextiles, airbags and a wide range of ﬁlter fabrics of varying area density and
One of the major advantages of all shuttleless machines is that weft on cone does
not have to be rewound before it is used. This eliminates one process and reduces
the danger from mixed yarn and ensures that weft is used in the order in which it
is spun. On shuttle looms weft is split into relatively short lengths, each one of which
is reversed during weaving which can show up long periodic faults in a yarn.
The standard projectile is 90 mm long and weighs only 40 g, a fraction of the mass
of a shuttle. For pick insertion on a Sulzer machine (see Fig. 4.23) weft is withdrawn
from the package through a weft brake and a weft tensioner to the shuttle feeder,
Technical fabric structures – 1. Woven fabrics 89
4.23 Weft insertion by projectile (Sulzer system) (schematic). 1, Weft (on cone); 2, yarn
brake (adjustable); 3, weft tensioner; 4, weft presenter; 5, torsion rod; 6, weft cutter
(scissors); 7, gripper (to hold cut end); 8, guide teeth; 9, projectile; 10, projectile brake
(receiving side). Reproduced with kind permission of Sulzer Textil.
which places it into the gripper of the projectile. A torsion bar system is used for
picking which transfers the maximum possible strain-energy to the projectile before
it separates from the picker shoe. The torsion bar can be adjusted to deliver the
energy required to propel the projectile through the guide teeth to the shuttle brake.
Sulzer redesigned the reed and the beat-up mechanism so as to obtain a stronger
and more rapid beat-up thus making a higher proportion of the picking cycle avail-
able for weft insertion.
Narrow machines can operate at weft insertion rates of up to 1000 m min-1 whilst
3600 mm wide machines can insert weft at up to 1300 m min-1. Models are available
for weaving heavy fabrics, for weaving coarse and fancy yarns and for up to six weft
colours. The machines can be ﬁtted with a variety of shedding motions and are
equipped with microprocessors to monitor and adjust machine performance.
Because of the increase in weft insertion rates with increases in reed width and
because of the decrease in capital cost per unit width for wider projectile machines,
it is often attractive to weave a number of widths of fabric side by side in one pro-
For even wider and heavier fabrics Jürgens18 build a machine using the Sulzer
Rüti system of pick insertion. They can propel a heavier projectile carrying a weft
yarn of up to 0.7 mm diameter across a reed width of up to 12 m. Their machines
take warp from one, two or three sets of warp beams and maintain weaving ten-
sions of up to 30 000 N m-1, accommodate up to 24 shafts controlled by an extra
heavy dobby, and deliver the cloth on to a large batching motion. Jäger have devel-
oped a projectile weaving machine for fabrics of medium area density and up to
12 m wide using a hydraulically propelled projectile.
126.96.36.199 Rapier machines
At ITMA Paris 1999, out of 26 machinery manufacturers showing weaving machines
no fewer than 17 offered rapier machines and some offered machines of more than
one type. Rapier machines were the ﬁrst shuttleless machines to become available
90 Handbook of technical textiles
but, at ﬁrst, they were not commercially successful because of their slow speed. With
the introduction of precision engineering and microprocessor controls, the separa-
tion of the weft insertion from the beat-up and improved rapier drives and heads,
their weft insertion rates have increased rapidly. For machines of up to 2500 mm
reed space they equal those of projectile machines with which they are now in direct
Machines may operate with single or double rapiers. Single rapier machines gen-
erally use rigid rapiers and resemble reﬁned versions of ancient stick looms. They
have proved attractive for weaving fairly narrow cloths from coarse yarns. Wide
single rapier machines are too slow for most applications. In single rapier machines
the rapier traverses the full width of the shed and generally picks up the weft and
draws it through the shed on its return. A variation of the single rigid rapier is the
single rapier working bilaterally, sometimes referred to as a two-phase rapier. As it
has not been used to any extent for industrial fabrics it is not considered here but
details can be found in the book by Ormerod and Sondhelm.13
Most rapier machines use double rapiers, one rapier entering the shed from each
side. They meet in the middle and transfer the yarn. With the Gabler system weft is
inserted alternately from both sides of the machine and yarn is cut every second
pick with hairpin selvedges being formed alternately on both selvedges. The Gabler
system has now been largely superseded by the Dewas system where weft is inserted
from one side only and is cut after every pick.
Double rapiers machines use either rigid or ﬂexible rapiers. Rigid rapier
machines need more space than machines ﬁtted with any other weft insertion
system. Rigid rapier machines, of which the Dornier HTV and P19 series are prime
examples, are capable of weaving most types of industrial fabrics with weft linear
densities of up to 3000 tex, in widths of up to 4000 mm and at weft insertion rates
of up to 1000 m min-1. Typical fabrics being produced on them range from open-
coated geotextile mesh to heavy conveyor belting. A variation of the rigid rapier is
the telescopic rapier.
By far the largest number of rapier machines use double ﬂexible rapiers which
are available in widths up to 4600 mm with even wider machines being custom built
for industrial applications. Standard machines have a relatively low capital cost and
can be used to weave a wide range of low and medium area density fabrics. They
are ideal for weaving short runs and for fabrics woven with more than one weft
because their weft change mechanism for up to eight colours is simple and cheap.
They are widely used for furnishing and fashion fabrics, often with Jacquards. They
are also used for some industrial cloths.
188.8.131.52 Fluid jet weaving machines
Fluid jet machines use either air or water to propel the yarn through the shed. They
do not need a weft carrier or a rapier for weft insertion and therefore have fewer
moving parts and less mass to move. Water jets are only suitable for hydrophobic
yarns whilst most yarns can be woven on air jets. Water jets generally use a single
nozzle at the picking side to propel the yarn through the full width of the shed and
this limits their width to about 2 m. As the ﬂow of air is more difﬁcult to control
than the ﬂow of water under pressure, air jets with single nozzles have only been
commercially successful in widths of up to 1700 mm. For wider machines, booster or
relay nozzles are placed along the reed to ensure the smooth movement of the weft
across the full reed width. Although theoretically wide air jets can be built, com-
Technical fabric structures – 1. Woven fabrics 91
4.24 Weft insertion by airjet (Sulzer Rüti L5000). 1, Supply package; 2, measuring disc;
3, rollers; 4, storage tube; 5, clamp; 6, main nozzle; 7, relay nozzles; 8, reed with tunnel.
Reproduced by kind permission of Sulzer Textil.
mercially single width machines are most attractive and machinery makers limit
their ranges to 3600 or 4000 mm reed width.
Compressed air is expensive to produce and its ﬂow is difﬁcult to control. The
air ﬂow in the shed has, therefore, to be restricted either by special air guides or
‘confusers’ or by passing the weft through a channel in a special ‘proﬁle’ reed. The
former method was pioneered by Elitex and is used in most of their ‘P’ type weaving
machines (Fig. 4.18) of which a large number are in use for weaving light and
medium weight fabrics up to 150 cm wide. Sulzer Rüti developed the ‘te strake’
proﬁle reeds with relay nozzles and this system is shown schematically in Fig. 4.24.
There is one main nozzle per colour and one set of relay nozzles spaced at regular
intervals along the reed. The weft is measured to length in the weft feeder and then
carried by the air stream of the main nozzle into the weft duct, accelerated and
transported further by air discharged from the relay nozzles. After insertion, a
stretch nozzle at the receiving side holds the pick under tension until it is bound
into the cloth.
Since air jets came into large scale commercial use in the 1970s they have been
developed rapidly. They can now weave the majority of fabrics and are dominant
for the mass production of fairly simple cloths. They have reached weft insertion
rates of up to 3000 m min-1, twice that of any other single phase weft insertion system
and are still under intensive development. Their capital cost per metre of weft
inserted is highly competitive. Their operating costs depend largely on the local cost
of electricity and whether low grade waste heat from the compressors can be used
for other operations in the plant.
Air jet machines ﬁtted with an automatic weft fault repair system can correct the
majority of weft faults, including part picks, which occur between the main nozzle
92 Handbook of technical textiles
and the selvedge on the receiving side. The unit removes the broken thread from
the shed without disturbing the warp ends and then restarts the machine. Only if
the machine cannot locate and repair the fault will it signal for attention. As weft
stops represent the majority of stops on an air jet, the system greatly reduces the
weaver’s work load, frequently by more than 50%. It also reduces machine inter-
ference and improves the quality of many fabrics.
4.5.4 Other motions and accessories for single phase weaving machines
184.108.40.206 Warp supply and let-off motion
Warp yarns are generally supplied to the weaving machine on one or more weaver’s
beams. In special cases, as already mentioned above, cone creels can be used. The
warp yarns assembled on the weaver’s beam should be evenly spaced and under
standard tension to ensure that all are of exactly the same length when they are
unwound for weaving. The larger the diameter of the beams the longer the length
of warp which can be wound on to it and the fewer the warp changes required but
the greater the tension variations which have to be compensated. Different weaving
machines accommodate beams of different maximum diameter but most modern
machines can take beams of up to 1000 mm diameter. If even larger diameter beams
are needed for very coarse warp yarns, for example for industrial fabrics or denims,
the beams can be placed into a separate beam creel outside the loom frame. Such
units cater for beams of up to 1600 mm diameter.
The width of yarn on the weaver’s beam has to be at least as wide as the yarn in
the reed. When the warp width required exceeds 2800 mm, more than one beam is
frequently used to simplify sizing and warp transport. If yarns from more than one
beam are used in one cloth it is essential that both beams are prepared under iden-
tical conditions to prevent variations which can cause cloth faults after ﬁnishing. The
let-off tensions of different beams have to be carefully controlled and this has
become simpler with the introduction of electronic sensors. When the cloth design
requires the use of warp yarns of widely differing linear densities or results in dif-
ferent warp yarns weaving with widely differing crimps, two or more warp beams
may have to be used in parallel. They can be placed either above each other or
behind each other in the weaving machine. Comparison of Figs. 4.17 and 4.18 shows
how the layout of machines can be modiﬁed without impairing their efﬁciency.
During weaving the let-off motion will release the required amount of yarn for
each pick cycle. It must also hold the warp yarns under even tension so that they
separate easily into two or more sheets during shedding prior to weft insertion and
so that the required tension is maintained during beat-up when the newly inserted
weft is moved by the reed to the fell of the cloth. Let-off motions used to be
mechanically controlled with tension being measured by the deﬂection of the back
rest but now electronic sensors are used for tension measurements and the let-off
is frequently controlled by separate servo motors.
220.127.116.11 Take-up motion
Take-up motions are required to withdraw the cloth at a uniform rate from the fell.
The speed of withdrawal controls the pick spacing, which has to be regular to
prevent weft bars and other faults. In most weaving machines the take-up motion
also controls the winding of the cloth on to the cloth roller. If large rolls of large
Technical fabric structures – 1. Woven fabrics 93
diameter have to be made, as is common for heavy fabrics, a separate batching
motion is placed outside the loom frame. Batching motions can be on a different
level from the weaving machine, either below or above, to reduce the area required
for the weaving shed. To prevent the weaving of long lengths of reject fabric, batch-
ing motions can incorporate cloth inspection facilities, sometimes with an interme-
diate cloth storage unit.
18.104.22.168 Automatic stop motions
The ﬁrst group, warp protector motions, are only necessary on machines which use
a free ﬂying shuttle or projectile. They are designed to prevent the forward move-
ment of the reed if the shuttle fails to reach the receiving side. This prevents
damage to the machine and the breakage of large numbers of ends if the shuttle
Warp stop motions stop the machine if an end breaks. They are activated when
a drop wire, through which an end has been threaded, drops because a broken end
will no longer support it. Drop wires can be connected to mechanical or electrical
stop motions. Yarns have to be properly sized to prevent them being damaged by
the drop wires. Electronic warp stop motions, which do not require physical contact
with the warp, are now being introduced especially for ﬁne ﬁlament yarns.
Weft stop motions are used to activate weft changes in automatic shuttle looms
and to stop weaving machines if the weft breaks during weft insertion. Electronic
motions are available that will stop the machine even if a broken end catches on
again before it reaches the receiving side. In air jet machines ﬁtted with automatic
repair facilities the weft stop motion also starts the weft repair cycle.
22.214.171.124 Quick style change
QSC (quick style change) equipment, ﬁrst shown by Picanol in 1991 and now avail-
able from most manufacturers, greatly reduces the time a weaving machine has to
be stopped for a warp change. The warp beam, back rest, warp stop motion, heald
frames and reed are located on a module which separates from the main frame of
the weaving machine and which is transferred by a special transport unit to and
from the entering and knotting department where the module becomes the prepa-
ration frame for a replacement warp.14 Thus 90% of the work load, which is nor-
mally carried out on the stopped weaving machine, is eliminated from the warp
replenishment cycle and the weaving machine efﬁciency is improved. It also results
in cleaner reeds and healds resulting in better machine performance and improved
4.5.5 Machine width
The reed width of the machine must be equal to or greater than the width in reed
of the fabric to be woven. Width in reed must allow for the width of selvedge and
dummy ends. If the machine is narrower the cloth cannot be woven in the machine.
Generally it is impossible to increase the available reed width of a machine.
Whilst the machine width cannot be exceeded, it is generally possible to weave
narrower fabrics. In Sulzer projectile machines weaving down by up to 50% is pos-
sible. Different manufacturers and models have different arrangements for weaving
down – some allow for only 200 mm which is often insufﬁcient considering likely
changes in materials and styles. It is most economic to use a high proportion of the
94 Handbook of technical textiles
reed width because weaving down is likely to reduce the weft insertion rate. Wider
machines also tend to have higher capital and running costs. On some occasions it
is economic to weave a number of fabrics side by side in one machine. Five, six or
seven roller towels, each with its own tucked selvedges, can be produced in a wide
Sulzer projectile machine.
4.6 The future
Because of rapid technological advances modern weaving machines have become
highly automated with most functions electronically controlled. Machine settings
can be adjusted and transferred and many faults can be repaired without requiring
attention by an operative. The frequency of machine stops and their duration has
been reduced. The cost of labour has been desensitized and the cost of production
has been reduced whilst product quality has improved. Because of the cost of
modern machines it becomes ever more important to use the right equipment for
the job and operate machines at high efﬁciency.
At present projectile weaving machines are the most versatile of conventional
machines and by bolting the right equipment to the machine there is hardly a fabric
they cannot weave well. Most simple fabrics can be woven at much lower capital cost
on air jets ﬁtted with simple shedding systems. Their economic range is being
extended continuously. In between there are fabrics which can be woven most
cheaply on rapiers. Multiphase machines, like Sulzer Textil’s linear air jet M8300, are
likely to become cheap producers of simple fabrics in the not too distant future.
1. The Textile Institute Terms and Deﬁnitions Committee, Textile Terms and Deﬁnitions, 10th edition,
The Textile Institute, Manchester, 1995.
2. a t robinson and r marks, Woven Cloth Construction, The Textile Institute, Manchester, 1973.
3. w watson, Textile Design and Colour–Elementary Weaves and Figured Fabrics, Longmans, London,
1912 (later editions revised by Grosicki and published by Butterworth).
4. w watson, Advanced Textile Design, Longmans, London, 1912 (later editions revised by Grosicki and
published by Butterworth).
5. Sulzer Brothers (now Sulzer-Textil), Winterthur, Switzerland.
6. r marks, An Intoduction to Textiles – Workbook: Fabric Production – Weaving, ed. W S Sondhelm,
Courtaulds Textiles plc, Manchester, 1989.
7. f t peirce, The Geometry of Cloth Structure, Manchester, Journal of the Textile Institute, T45, 1937.
8. The Textile Institute Terms and Deﬁnitions Committee, Textile Terms and Deﬁnitions, 10th edition,
Table of SI Units and Conversion Factors, The Textile Institute, Manchester, 1995.
9. Rüti Machinery Works Ltd, Verkauf, Rüti, Switzerland, 1977.
10. Rüti Machinery Works Ltd, Switzerland, ‘C’ Model shuttle weaving machine.
11. Investa, Czechoslovakia, Elitex air jet, ‘P’ type.
12. Somet, Colzate (BG), Italy, ‘Mach 3’ air jet.
13. a ormerod and w s sondhelm, Weaving–Technology and Operations, Chapter 5: ‘Weaving,’ The
Textile Institute, Manchester, 1995 (reprinted 1999).
14. a ormerod and w s sondhelm, Weaving–Technology and Operations, Chapter 2: ‘Warping’ and
Chapter 3: ‘Sizing,’ The Textile Institute, Manchester, 1995 (reprinted 1999).
15. Sulzer Rüti, Wilmslow, Fabric Structure, 3085/06.10.95/Legler/sei, 1995.
16. Maschinenfabrik Starlinger, Vienna, Austria, Circular Loom SL4, Drwg. 0304A3, 1997.
17. Sulzer Rüti, Wilmslow, Shed Formation, 3138/10.10.95/Legler/kaa, 1995.
18. Jürgens GmbH, Emsdetten, Germany, Projectile weaving machine JP-2000, 1996.
19. Lindauer Dornier GmbH, Germany, 1999.
Technical fabric structures – 2. Knitted fabrics
Subhash C Anand
Faculty of Technology, Bolton Institute, Deane Road, Bolton BL3 5AB, UK
5.1 Terms and deﬁnitions
• Warp knitting is a method of making a fabric by normal knitting means, in which
the loops made from each warp are formed substantially along the length of the
fabric. It is characterised by the fact that each warp thread is fed more or less in
line with the direction in which the fabric is produced. Each needle within the
knitting width must be fed with at least one separate and individual thread at
each course. It is the fastest method of converting yarn into fabric, when com-
pared with weaving and weft knitting (Fig. 5.1).
• Weft knitting is a method of making a fabric by normal knitting means, in which
the loops made by each weft thread are formed substantially across the width
of the fabric. It is characterised by the fact that each weft thread is fed more or
less at right angles to the direction in which the fabric is produced. It is possible
to knit with one thread only, but up to 144 threads can be used on one machine.
This method is the more versatile of the two in terms of the range of products
produced as well as the type of yarns utilised (Fig. 5.2).
• Single-jersey fabric is a weft-knitted fabric made on one set of needles.
• Double-jersey fabric is a weft-knitted fabric made on two sets of needles, usually
based on rib or interlock gaiting, in a manner that reduces the natural exten-
sibility of the knitted structure. These fabrics can be non-Jacquard or Jacquard.
• Course is a row of loops across the width of the fabric. Courses determine the
length of the fabric, and are measured as courses per centimetre.
• Wale is a column of loops along the length of the fabric. Wales determine the
width of the fabric, and are measured as wales per centimetre.
• Stitch density is the number of stitches per unit area of a knitted fabric (loops
cm-2). It determines the area of the fabric.
• Stitch length is the length of yarn in a knitted loop. It is the dominating factor
for all knitted structures. In weft knitting, it is usually determined as the average
length of yarn per needle, while in warp knitting, it is normally determined as
the average length of yarn per course.
96 Handbook of technical textiles
3 2 1 0
1 - 0 / 1 - 2
5.1 Warp knitting.
5.2 Weft knitting.
• Yarn linear density indicates the thickness of the yarn and is normally deter-
mined in tex, which is deﬁned as the mass in grams of 1 km of the material. The
higher the tex number, the thicker is the yarn and vice-versa.
• Overlap is the lateral movement of the guide bars on the beard or hook side of
the needle. This movement is normally restricted to one needle space. In the
fabric a loop or stitch is also termed the overlap.
• Underlap is the lateral movement of the guide bars on the side of the needle
remote from the hook or beard. This movement is limited only by the mechani-
Technical fabric structures – 2. Knitted fabrics 97
WEFT KNITTING MACHINES
Bearded needle Latch needle
Straight bar Circular Flat bar Circular
One Two One One Two One Two Double
needle needle needle needle needle needle needle cylinder
beds bed bed beds bed beds
Sinker Loop Vee Flat
wheel wheel bed purl
pile and jersey
KNITWEAR FABRIC KNITWEAR KNITWEAR or GARMENT GARMENT
(Shaped) GARMENT FABRIC, or or
(3-d Knitting) KNITWEAR KNITWEAR
5.3 Simpliﬁed classiﬁcation of knitting machinery.
cal considerations. It is the connection between stitches in consecutive courses
in a warp knitted fabric.
• Tightness factor K is a number that indicates the extent to which the area of a
knitted fabric is covered by the yarn. It is also an indication of the relative
looseness or tightness of the knitting. (K = tex1/2 l-1), where l is the stitch length.
• Area density is a measure of the mass per unit area of the fabric (g m-2).
5.2 Weft knitting machines
Figure 5.3 shows a simpliﬁed classiﬁcation of weft knitting equipment. It will be
noticed from Fig. 5.3 that the latch needle is the most widely used needle in weft
knitting, because it is self-acting or loop controlled. It is also regarded as more ver-
98 Handbook of technical textiles
5.5 Latch needle.
5.4 Bearded needle.
5.7 Compound needle (Kokett needle).
5.6 Compound needle (ﬂy
satile in terms of the range of materials that can be processed on latch needle
machines. Bearded needles are less expensive to manufacture, can be produced
in ﬁner gauges and supposedly knit tighter and more uniform stitches compared
with latch needles, but have limitations with regard to the types of material that
can be processed as well as the range of structures that can be knitted on them.
Bearded needle machines are faster than the equivalent latch needle machines.
The compound needle has a short, smooth and simple action, and because it requires
a very small displacement to form a stitch in both warp and weft knitting, its
production rate is the highest of the three main types of needle. Compound needles
are now the most widely used needles in warp knitting and a number of manufac-
turers also offer circular machines equipped with compound needles. The operation
speeds of these machines are up to twice those of the equivalent latch needle
The main parts of the bearded, latch, compound needle (ﬂy needle frame) and
compound needle (Kokett) are shown in Figs. 5.4, 5.5, 5.6 and 5.7, respectively.
Variations of latch needles include rib loop transfer needles and double-ended purl
Technical fabric structures – 2. Knitted fabrics 99
needles, which can slide through the old loop in order to knit from an opposing bed
and thus draw a loop from the opposite direction.
5.2.1 Loop formation with latch needles
Figure 5.8(a) illustrates the needle at tuck height, that is high enough to receive a
new yarn, but not high enough to clear the old loop below the latch. The needle is
kept at this position because the loop formed at the previous course (A) lies on the
open latch and stops the latch from closing. Note that once a latch is closed, it can
only be opened by hand, after stopping the machine.
In Fig. 5.8(b), the needle has been lifted to the clearing position and the new yarn
(B) is presented. The old loops (A) are below the latch and the new yarn (B) is fed
into the needle hook. A latch guard normally prevents the latch from closing at this
In Fig. 5.8(c), the needle has now moved to its lowest position or knitting point
and has drawn the new loop (B) through the old loop (A) which is now cast-off or
knocked over. The needle now rises and the sequence of movements is repeated for
the next course.
The loop formation on a latch needle machine is also illustrated in Fig. 5.9(a) and
a typical cam system on such a machine is shown in Fig. 5.9(b).
A A B A
5.8 Loop formation with latch needles.
100 Handbook of technical textiles
Latches New Hooks open
Feeder closing loop
Needle positions moving through the CAM
GUARD CAM STITCH CAM (ADJUSTABLE) GUARD CAM
1 4 6
RUNNING CAM CLEARING CAM 5 UPTHROW CAM
5.9 (a) Loop formation and (b) typical cam system on a latch needle machine.
5.2.2 Single-jersey latch needle machines
This type of machinery is employed throughout the world, either as a basic
machine or with certain reﬁnements and modiﬁcations, to produce fabric ranging
from stockings to single-jersey fabric for dresses and outerwear, as well as a wide
range of fabrics and products for technical applications. The machine sizes vary from
1 feeder 1 inch diameter to 144 feeds 30 inches diameter. Most single-jersey
machines are rotating cylinder type, although a few rotating cam box machines
are still used for specialised fabrics. These machines are referred to as sinker top
machines and use web holding sinkers. Comprehensive reviews of single- and
double-jersey knitting machinery and accessories exhibited at ITMA’95 and
ITMA’99 were published that illustrate the versatility and scope of modern weft
126.96.36.199 Knitting action of a sinker top machine
Figures 5.10(a) to (d) show the knitting action of a sinker top machine during the
production of a course of plain fabric.
Figure 5.10(a) illustrates the rest position. This shows the relative position of
the knitting elements in-between the feeders with the needle at tuck height and the
fabric loop held on the needle latch by the forward movement of the sinker towards
the centre of the machine.
Figure 5.10(b) illustrates the clearing position. The needle has been raised to its
Technical fabric structures – 2. Knitted fabrics 101
5.10 Knitting action of a sinker top machine.
highest position by the clearing cam acting on the needle butt; the old loop slides
down from the open latch on to the needle stem.
Figure 5.10(c) illustrates the yarn feeding position. The sinker is partially with-
drawn allowing the feeder to present its yarn to the descending needle hook, at the
same time freeing the old loop so that it can slide up the needle stem and under the
open latch spoon.
Figure 5.10(d) illustrates the knock-over position. The needle has now reached
its lowest position and has drawn the new loop through the old loop which is now
knocked over the sinker belly.
Stitch length may be controlled in a number of ways. On machines without
positive feed mechanism, it is controlled mainly by the distance the needle
descends below the sinker belly. Other factors such as input tension (Ti), yarn to
metal coefﬁcient of friction (m) and take-down tension also inﬂuence the ﬁnal
stitch length in the fabric. When a positive feed device is used, the length of
yarn fed to the needles at a particular feed is the factor that decides the stitch
length. Other factors such as input tension Ti , m, stitch cam setting and take-
down tension inﬂuence the yarn or fabric tension during knitting, and hence
determine the quality of the fabric. Stitch length is ﬁxed by the positive feed device
The sinker has two main functions and these are:
• to hold the fabric loop in a given position whenever the needles rise and
• to provide a surface over which the needles draw the loops.
Other advantages of using sinkers include:
• The control exerted by the sinker allows minimum tension on the fabric thus
producing a good quality fabric with even loops.
102 Handbook of technical textiles
Rib machine Timing Dial
L L L
L L L L
Timing Dial Interlock machine
L L S
S S L S
Cylinder L S
Eightlock timing L L S
Cylinder S S
5.11 Double-jersey machine needle layouts.
• Fine adjustments in quality and those required in the knitting of certain difﬁcult
yarns and structures are possible.
• The sinker facilitates the setting-up of the machine after a partial or full
press-off (after the latches have been opened manually).
5.2.3 Double-jersey machines
Figure 5.11 shows the needle layout of rib and interlock machines. Both types of
machine are available as circular or ﬂat machines, whereas straight bar or fully fash-
ioned machines are available in rib-type only.
Rib and interlock double-jersey machines are used either as garment length
machines or for producing rolls of fabric. They can be either plain or equipped with
a wide range of mechanical patterning mechanisms at each feed in the cylinder. Both
types can also be equipped with electronic needle mechanisms to produce large area
Jacquard patterns at high speeds.
Technical fabric structures – 2. Knitted fabrics 103
188.8.131.52 Rib machines
Rib machines use two sets of needles and can be ﬂat, circular or fully fashioned. The
needles in the two beds are staggered or have spaces between them (rib gaiting).
Most machines have revolving needle cylinders but in some cases the cams rotate
past stationary needles. Patterning is obtained by altering cam and needle set-out
or by using various needle selection mechanisms including individual needle elec-
tronic selection with computer aided design system. Machine diameters range from
71/2–20 inches for garment length and from 30–33 inches for fabric machines. An
example of a modern double-jersey machine is the Monarch V-7E20, a 30 inch di-
ameter, E20, 72 feeders 8-lock machine with RDS on dial and ACT II motorised
automatic friction take-down system. The machine has 2 ¥ 2 cam tracks and can be
converted from rib to interlock or 8-lock timing in minutes. All basic non-jacquard
double-jersey structures can be knitted at a speed factor of 900 (machine diameter
(inches) ¥ machine rpm).
184.108.40.206 Interlock machines
These are latch needle circular machines of the rib type, provided with a cylinder
and dial. Unlike rib machines where the tricks of the dial alternate with the tricks
of the cylinder (rib gaiting) the needle tricks of the cylinder are arranged exactly
opposite those of the dial (interlock gaiting). Long-and short-stemmed needles
are used that are arranged alternately, one long, one short in both cylinder and
dial as shown in Fig. 5.11. An example of a modern high-speed interlock machine
is Sulzer Morat Type 1L 144, which is a 30 inches diameter, 144 feeds, 28 or 32
gauge (npi, needles per inch), 28 rpm, producing at 100% efﬁciency 86.4 m h-1
(15.55 kg h-1) of 76 dtex polyester with 14 cpc (courses per centimetre) and with
an area density of 180 g m-1 (60 inches wide) ﬁnished fabric.
To accommodate the long- and short-stemmed needles, the cam system is
provided with a double cam track. The long dial needles knit with the long cylinder
needles at feeder 1 and the short cylinder needles knit with the short dial needles at
feeder 2. Thus two feeders are required to make one complete course of loop.
220.127.116.11 Needle timing
Two different timings can be employed on 1 ¥ 1 rib and 1 ¥ 1 interlock machines.
• Synchronised timing is the timing of a machine that has two sets of needles where
the point of knock-over of one set is aligned with the point of knock-over of the
• Delayed timing is the setting of the point of knock-over of one set of needles
on a two-bed knitting machine out of alignment with that of the other set so
as to permit the formation of a tighter stitch. Broad ribs (i.e. 2 ¥ 2, 3 ¥ 3 etc.),
and rib Jacquard fabrics cannot be produced in delayed timing because there
will not always be cylinder needles knitting either side of the dial needles from
which to draw yarn. Up to nine needles delay is possible, but 4–5 needles delay
18.104.22.168 Knitting action of V-bed ﬂat machine
Figure 5.12 illustrates the different stages of loop formation on a V-bed ﬂat knitting
machine, and Fig. 5.13 shows the cam system used on a simple single system ﬂat
104 Handbook of technical textiles
Position of needles
Brushes open any
Adjacent needles are
raised to clearing height
Yarn fed to
5.12 Loop formation on a V-bed ﬂat knitting machine.
Knit (clear) S4 S1
5.13 V-bed single-system cams. S are stitch cams, R are raising cams and C
are clearing cams.
Technical fabric structures – 2. Knitted fabrics 105
machine. Power V-bed ﬂat machines are used mainly for the production of knitwear
for children, women and men. They range from simple machines through mechani-
cal jacquard machines to fully electronic and computerised ﬂat machines, even
equipped with presser foot. The developments in the automation of fabric design-
ing, pattern preparation, and electronic needle selection, as well as in the range of
structures and effects which can be produced, have been tremendous and ﬂat
machines and their products are now regarded as extremely sophisticated. High
quality garments can now be produced at competitive prices owing to revolu-
tionary garment production systems feasible with presser foot. Two- and three-
dimensional structures as well as complete garments without any seams or joins can
be produced on the latest electronic ﬂat knitting machines and the associated design
5.3 Weft-knitted structures
The basic weft-knitted structures and stitches are illustrated in Fig. 5.14 (A to G),
and the appearance, properties and end-use applications of plain, 1 ¥ 1 rib, 1 ¥ 1
purl and interlock structures are summarised in Table 5.1. These basic stitches are
often combined together in one fabric to produce an enormous range of single- and
double-jersey fabrics or garments. Weft-knitted fabrics are produced commercially
for apparel, household and technical products and they are used for an extremely
large array of products, ranging from stockings and tights to imitation furs and rugs.
The importance and diversity of warp- and weft-knitted fabrics used for various
technical applications has been discussed by Anand,2 who highlighted the fact that
knitted fabrics are being increasingly designed and developed for technical prod-
ucts ranging from scouring pads (metallic) to fully fashioned nose cones for super-
sonic aircrafts. Warp- and weft-knitted products are becoming popular for a wide
spectrum of medical and surgical products.3
5.4 Process control in weft knitting
5.4.1 Main factors affecting the dimensional properties of knitted
fabrics or garments
• Fabric structure: different structures relax differently.
• Fibre(s) type: fabrics or garments made from different ﬁbre(s) relax differently.
• Stitch length: the length of yarn in a knitted loop is the dominating factor for all
• Relaxation/ﬁnishing route: the fabric dimensions vary according to relaxation/
• Yarn linear density: affects the dimensions slightly, but affects fabric tightness,
area density (g m-2) and other physical properties.
5.4.2 Laboratory stages of relaxation
• On machine – Strained state: this is predominantly length strain.
• Off machine – Dry relaxed state: the fabric moves to this state with time. The dry
106 Handbook of technical textiles
Plain single-jersey A Plain single-jersey B
Technical Face Technical Back
Feed 1 Feed 2
Feed 3 Feed 3
Feed 2 Feed 2
Feed 1 Feed 1
Single Tuck Stitch F Single Tuck Stitch G
Feed 3 Feed 3
Feed 2 Feed 2
Feed 1 Feed 1
5.14 Weft-knitted structures (A–G).
able 5.1 Comparison of appearance and properties
roperty Plain 1 ¥ 1 Rib 1 ¥ 1 Purl Interlock
ppearance Different on face and back; Same on both sides, like Same on both sides, like Same on both sides, like
V-shapes on face, arcs on back face of plain back of plain face of plain
Lengthwise Moderate (10–20%) Moderate Very high Moderate
Widthwise High (30–50%) Very high (50–100%) High Moderate
Area Moderate–high High Very high Moderate
hickness and warmth Thicker and warmer than Much thicker and warmer Very much thicker and Very much thicker and
plain woven made from same than plain warmer than plain woven warmer than plain woven
nroving Either end Only from end knitted last Either end Only from end knitted
urling Tendency to curl No tendency to curl No tendency to curl No tendency to curl
nd-uses Ladies’ stockings Socks Children’s clothing Underwear
Fine cardigans Cuffs Knitwear Shirts
Men’s and ladies’ shirts Waist bands Thick and heavy Suits
Dresses Collars Outerwear Trouser suits
Base fabric for coating Men’s outerwear Sportswear
108 Handbook of technical textiles
relaxed state is restricted by fabric structure and ﬁbre type. Only wool can attain
• Static soak in water and dry ﬂat – Wet relaxed state: tight structures do not always
reach a ‘true’ relaxed state. Only wool and silk can attain this state.
• Soak in water with agitation, or Agitation in steam, or Static soak at selected
temperatures (>90 °C) plus, dry ﬂat – Finished relaxed state: the agitation and/or
temperature induces a further degree of relaxation, producing a denser fabric.
Wool, silk, textured yarn fabrics, acrylics.
• Soak in water and Tumble dry at 70 °C for 1 hour – Fully relaxed state:
three-dimensional agitation during drying. All ﬁbres and structures.
5.4.3 Fabric geometry of plain single-jersey structures
1. Courses per cm (cpc) a 1 l =
2. Wales per cm (wpc) a 1 l =
3. s = (cpc ¥ wpc) a 1 l 2 =
4. ac = (shape factor)
kC, kW, kS are dimensionless constants, l is the stitch length and s is the stitch density.
5.4.4 Practical implications of fabric geometry studies
• Relationship between yarn tex and machine gauge is given by Equation (5.1):
Optimum tex = (5.1)
For single-jersey machines, the optimum tex = 1650/G2, and for double-jersey
machines, the optimum tex = 1400/G2, where G is measured in needles per
• Tightness factor is given by Equation (5.2):
where l is the stitch length, measured in millimetres. For single-jersey fabrics:
1.29 £ K £ 1.64. Mean K = 1.47. For most weft-knitted structures (including
single- and double-jersey structures and a wide range of yarns): 1 £ K £ 2. Mean
K = 1.5. The tightness factor is very useful in setting up knitting machines. At
mean tightness factor, the strain on yarn, machine, and fabric is constant for a
wide range of conditions.
• Fabric area density is given by Equation (5.3):
s ¥ l ¥T
Area density = g m -2 (5.3)
Technical fabric structures – 2. Knitted fabrics 109
Table 5.2 k-Constant values for wool plain single jerseya
kc kw ks kc /kw
Dry relaxed 50 38 1900 1.31
Wet relaxed 53 41 2160 1.29
Finished relaxed 56 42.2 2360 1.32
Fully relaxed 55 ± 2 42 ± 1 2310 ± 10 1.3 ± 0.05
Courses and wales are measured per centimetre and l is measured
For a relaxed fabric cpc/wpc = 1.3. cpc/wpc > 1.3 indicates widthwise
stretching. cpc/wpc < 1.3 indicates lengthwise stretching. ks > 2500
indicates felting or washing shrinkage. Relaxation shrinkage is the
change in loop shape. Felting/washing shrinkage is the change in loop
where s is the stitch density/cm2; l is the stitch length (mm) and T is the yarn tex,
or, Equation (5.4):
¥ g m -2 (5.4)
where ks is a constant and its value depends upon the state of relaxation, that is,
dry, wet, ﬁnished or fully relaxed. The area density can also be given by Equa-
tions (5.5) and (5.6)
n ¥ l ¥ cpc ¥ T
Area density = g m -1 (5.5)
where n is the total number of needles, l is the stitch length (mm) and T is the
yarn tex, or
n ¥ kc ¥ T
g m -1 (5.6)
where kc is a constant and its value depends upon the state of relaxation, that is
dry, wet, ﬁnished or fully relaxed.
• Fabric width is given by Equation (5.7)
Fabric width = cm (5.7)
where kw is a constant, and its value depends upon the state of relaxation, that
is, dry, wet, ﬁnished or fully relaxed. It can also be given by Equation (5.8)
n ¥ l = L (course length) Fabric width = cm (5.8)
Fabric width depends upon course length and not upon the number of needles
• Fabric thickness. In the dry and wet relaxed states, fabric thickness (t) is
dependent upon fabric tightness, but in the fully relaxed state, it is more or less
independent of the fabric tightness factor. In the fully relaxed state t ª 4d where
d is the yarn diameter.
110 Handbook of technical textiles
5.4.5 Quality control in weft knitting
The dimensions of a weft-knitted fabric are determined by the number of
stitches and their size, which in turn is determined by stitch length. Most knitting
quality control therefore reduces to the control of stitch length; differences in mean
stitch length give pieces of different size; variation of stitch length within the piece
gives appearance defects, by far the most common one being the occurrence of
widthwise bars or streaks owing to variation in stitch length between adjacent
22.214.171.124 Measurement of stitch length, l
• Off machine (in the fabric):
– HATRA course length tester
– Shirley crimp tester.
• On machine (during knitting):
– Yarn speed meter (revolving cylinder only)
– Yarn length counter (both revolving cylinder and cambox machines).
126.96.36.199 Control of stitch length, l
• Positive feed devices:
– Capstan feed: cylindrical or tapered
– Nip feed: garment length machines
– Tape feed: (Rosen feed) circular machines producing plain structures
– Ultrapositive feed: IPF or MPF
• Constant tension device: Storage feed device: ﬂat, half-hose, hose and circular
machines producing either plain or jacquard structures.
• Specialised positive feed devices:
– Positive Jacquard Feeder MPF 20 KIF
– Striper Feeder ITF
– IROSOX Unit (half-hose machines)
– Elastane Feed MER2
– Air controlled feeds for ﬂat and fully fashioned machines. Figure 5.15 shows
a tape feed. A modern ultrapositive feed and a yarn storage feed device are
illustrated in Figs. 5.16 and 5.17, respectively.
5.5 End-use applications of weft-knitted fabrics
Weft-knitted fabrics are used for apparel, household and technical products. The
main outlets for the different types of weft-knitted fabrics are as shown below.
The knitting equipment used to produce these fabrics is also given.
5.5.1 Flat bar machines
• Machine gauge: normally needles per inch, 3–18 npi
• Machine width: up to 78.7 inches
• Needle type: latch (compound needle machines are being developed)
• Needle bed type: single (hand machines), but mainly rib type
Yarn from top
Wheels may be taken out of action by lowering
the pot-eye plate; thus allowing the yarn to
run free below the level of the tape
5.15 Tape positive feed device.
5.16 Ultrapositive feed device.
112 Handbook of technical textiles
5.17 Yarn storage feed device.
• Products: jumpers, pullovers, cardigans, dresses, suits, trouser suits, trimmings,
hats, scarves, accessories, ribs for straight-bar machines (fully fashioned
machines). Cleaning clothes, three-dimensional and fashioned products for
technical applications, multiaxial machines are under development.
5.5.2 Circular machines
• Machine gauge: normally needles per inch, 5–40 npi
• Machine diameter: up to 30 inches. Up to 60 inch diameter machines are now
• Needle type: latch, (bearded on sinker wheel and loop wheel, some compound
• Needle bed type: single, rib, interlock, double cylinder
– Hose machines: seamfree hose, tights, industrial use dye bags, knit-de-knit
yarns, industrial fabrics
– Half-hose machines: men’s and boy’s half-hose, ladies’ stockings, children’s
tights, sports socks
– Garment blank machines: underwear, T-shirts, jumpers, pullovers, cardigans,
dresses, suits, trouser suits, vests, briefs, thermal wear, cleaning cloths, techni-
– Fabric machines: rolls of fabric with the following end-uses: jackets, ladies’
Technical fabric structures – 2. Knitted fabrics 113
tops, sports and T-shirts, casual wear, suits, dresses, swimwear, bath robes,
dressing gowns, track suits, jogging suits, furnishing, upholstery, automotive
and technical fabrics, household fabrics.
5.5.3 Straight-bar machines (fully fashioned machines)
• Machine gauge: normally needles per 11/2 inch, 9–33 (up to 60 gauge machines
have been produced)
• Machine width: from 2–16 section machines – each section up to 36 inches wide
(up to 40 section machines have been produced)
• Needle type: bearded or bearded and latch
• Needle bed type: single and rib
• Products: jumpers, pullovers, cardigans, dresses, suits, trouser suits, fully
fashioned hose, sports shirts, underwear, thermal wear.
5.6 Warp-knitting machines
The ﬁrst weft-knitting machine was built by William Lee in 1589. In 1775, just under
200 years later, the ﬁrst warp-knitting machine was invented by Crane, an English-
man. It was a single guide bar machine to make blue and white zig-zag striped silk
hosiery and these fabrics were named after Van Dyck, the painter. With the advent
of acetate continuous-ﬁlament yarns after World Ward I, the ﬁrst bulk production
of tricot fabrics was commenced by British Celanese on German Saupe 2-guide bar,
28 gauge machines. Locknits replaced the single guide bar atlas fabrics for lingerie,
the latter being difﬁcult to ﬁnish and laddered easily.
From 1950 to 1970, the growth of the warp-knitting industries in the UK and
other western countries was phenomenal. The main reasons for this colossal
expansion are summarised below (although developments in the various ﬁelds
mentioned here were taking place concurrently). The state of the art and current
developments in tricot and raschel machinery have been summarised below.
Anand also published a review of warp-knitting equipment exhibited by Karl
Mayer at ITMA in 19954 and ITMA’99.8
188.8.131.52 Yarn developments
• The discovery of thermoplastic yarns and their suitability, even in very low linear
densities (deniers) and in ﬂat or low-twist form, to be knitted with very low yarn
breakage rates on modern high speed tricot and raschel machines
• The extra design scope offered by differential dye yarns
• Improved cover-comfort attained through textured and producer-bulked yarns
• Elastomeric yarns, which have given a tremendous ﬁllip to the raschel power-
184.108.40.206 Machinery developments
• Higher machine speeds, (up to 3500 cpm)
• Finer gauges (up to 40 needles per inch)
114 Handbook of technical textiles
• Wider machines (up to 260 inches)
• Increased number of guide bars (up to 78 guide bars)
• Special attachments such as cut presser, fallplate, swanwarp, etc.
• Some speciality raschel machines such as Co-we-nit and Jacquard machines
and, more recently, redesigned full-width weft insertion raschel and tricot
• High speed direct-warping machines and electronic yarn inspection equipment
• Electronic stop motions for the knitting machines
• Larger knitting beams and cloth batches
• Modern heat-setting and beam-dyeing machinery
• Electronic warp let-off, electronic patterning, electronic jacquard and electronic
fabric take-up mechanisms
• Loop-raised fabrics
• Stable constructions, such as sharkskins, queenscord, etc.
• Various net constructions utilising synthetic yarns
• Mono-, bi-, tri- and multiaxial structures for technical applications
• Three-dimensional and shaped (fashioned) structures for medical and other high
It is well known that the warp-knitting sector, particularly tricot knitting has grown
in step with the expansion of manufactured ﬁbres. In 1956, 17.8 million lbs of regen-
erated cellulosic and synthetic ﬁbre yarns were warp knitted; the ﬁgure reached a
staggering 70.6 million lbs in 1968.
In the mid-1970s, the tricot industry suffered a major setback, mainly because
of a signiﬁcant drop in the sale of nylon shirts and sheets, which had been the
major products of this sector. It is also true that the boom period of textured poly-
ester double-jersey was also a contributing factor in the sudden and major decline
in the sales of tricot products. A change in fashion and the growth in the demand
for polyester/cotton woven fabrics for shirting and sheeting was another cause of
this decline. The two major manufacturers of warp-knitting equipment, Karl
Mayer and Liba, both in West Germany, have been actively engaged in redesign-
ing their machinery in order to recapture some of the lost trade. The compound
needle is the major needle used on both tricot and raschel machines, and many
specialised versions of warp-knitting machines are now available for producing
household and technical products. One of the major developments in warp
knitting has been the commercial feasibility of using staple-ﬁbre yarns for a wide
range of products. It is also signiﬁcant to note that the warp-knitting sector has
broadened its market base and has expanded into household and technical
fabric markets, such as lace, geotextiles, automotive, sportswear and a wide spec-
trum of surgical and healthcare products. The current and future potential of
warp-knitted structures in engineering composite materials has been discussed by
5.6.2 Tricot and raschel machines
The principal differences between tricot and raschel machines are listed here:
1. Latch needles are generally used in raschel machines, while bearded or com-
pound needle machines are referred to as tricot machines. Compound needle
Technical fabric structures – 2. Knitted fabrics 115
raschel machines are also now fairly common. The compound needle is the most
commonly used needle on warp knitting equipment.
2. Raschel machines are normally provided with a trick plate, whereas tricot
machines use a sinker bar.
3. In raschel machines the fabric is taken up parallel to the needle stems; in the
tricot machines, however, it is taken up at approximately right angles to the
4. Raschel machines are normally in a coarser gauge; they are also slower
compared with tricot machines, because more guide bars are frequently used
and they also require a longer and slower needle movement.
5. Raschel machines are much more versatile in terms of their ability to knit most
types of yarns such as staple yarns, and split ﬁlms, etc. Only continuous-ﬁlament
yarns can be successfully knitted on most tricot machines.
6. Generally, warp beams are on the top of the machine on raschel machines; on
tricot machines, they are generally at the back of the machine.
A simpliﬁed classiﬁcation of warp-knitting equipment is given in Fig. 5.18; it will be
noticed that apparel, household and technical fabrics are produced on modern
warp-knitting machinery. It is in fact in the technical applications that the full poten-
tial of warp knitting is being exploited. It is virtually possible to produce any product
on warp-knitting equipment, but not always most economical.
The simplest warp-knitted structures are illustrated in Fig. 5.19. It can be seen
that both closed- and open-loop structures can be produced and there is normally
very little difference in the appearance and properties between the two types of
5.6.3 Knitting action of compound needle warp-knitting machine
In Fig. 5.20(a) the sinkers move forward holding the fabric down at the correct level
in their throats. The needles and tongues rise with the needle rising faster until the
hook of the needle is at its highest position and is open. In Fig. 5.20(b) the guides
then swing through to the back of the machine and Fig. 5.20(c) shows the guides
shog for the overlap and swing back to the front of the machine.
Figure 5.20(d) shows the needles and the tongues starting to descend, with the
tongues descending more slowly thus closing the hooks. The sinkers start to with-
draw as the needles descend so that the old loop is landed onto the closed hook and
the new loops are secured inside the closed hook.
In Fig. 5.20(e) the needle descends below the sinker belly and the old loop is
knocked-over. At this point, the underlap occurs and in Fig. 5.20(f) the sinkers move
forward to hold down the fabric before the needles commence their upward rise to
form a fresh course.
5.6.4 Knitting action of standard raschel machine
In Fig. 5.21(a) the guide bars are at the front of the machine completing their
underlap shog. The web holders move forward to hold the fabric down at the
correct level, whilst the needle bar starts to rise from knock-over to form a fresh
Figure 5.21(b) shows that the needle bar has risen to its full height and the old
116 Handbook of technical textiles
Tricot machines Raschel machines
(Bearded, Compound needle) (Latch, Compound needle)
Single needle bar Double needle bar
2–5 Bars Weft insertion Cut presser Pile Pile
(lingerie, shirts, 2–3 Bars (blouses, 3–4 Bars 3–4 Bars
dresses (bed linen, curtains, (Bed linen, (car and
sportswear) curtains, lining, dresses) bath robes, domestic
Jacquard industrial) gowns) upholstery)
Single needle bar Double needle bar
Face-to-face Plush Special version
(Jacquard) [Split ﬁlm]
(High pile, technical,
car and domestic (Fruit/vegetable bags,
Standard Raschel Weft insertion Lace Jacquard Lace Special Version Directionally
(curtains, industrial 12–48 Bars up to 78 Bars up to 18 Bars orientated structures
1–12 Bars furnishing) (Fall-plate) [Fall-plate] [Fall-plate] (with or without
High speed 3–16 Bars (curtain lace, corsetry, Weft insertion Weft insertion ﬂeece)
foundation (curtains) (curtains) (Technical fabrics)
Net Power net Outerwear Elastic Industrial
5.18 Simpliﬁed classiﬁcation of knitting machinery.
loops slip down from the latches onto the stems after opening the latches. The
latches are prevented from closing by the latch guard. The web holders then start
to withdraw to allow the guide bars to form the overlap movement.
In Fig. 5.21(c) the guide bars swing to the back of the machine and then shog for
the overlap and in Fig. 5.21(d) the guide bars swing back to the front and the warp
threads are laid into the needle hooks. Note: only the front guide bar threads have
formed the overlap movement, the middle and back guide bar threads return
through the same pair of needles as when they swung towards the back of the
machine. This type of movement is called laying-in motion.
In Fig. 5.21(e) the needle bar descends so that the old loops contact and
Technical fabric structures – 2. Knitted fabrics 117
5.19 Single-guide bar warp-knitted fabrics. (a) Closed lap fabric, (b) open lap fabric.
(a) (b) (c)
(d) (e) (f)
5.20 Knitting action of compound needle warp-knitting machine.
118 Handbook of technical textiles
Back G.B. Front guide bar
(a) (b) (c)
(d) (e) (f)
5.21 Knitting action of a standard raschel machine. (a) Start of new course, (b) start of
overlap, (c) guide bar swinging motion, (d) return swing after overlap, (e) old loop closing
latch, (f) knock-over and underlap movements.
close the latches, trapping the new loops inside. The web holders now start to
Figure 5.21(f) shows the needle bar continuing to descend, its head passing below
the surface of the trick-plate, drawing the new loops through the old loops, which
are cast-off, and as the web holders advance over the trick-plate, the underlap shog
of the guide bar is commenced.
The knitting action of bearded needle warp-knitting machines has not been
given here because in the main the machines likely to be used for technical textile
products would use either latch or compound needles. Also the proportion of new
bearded needle machines sold has decreased steadily over the years. This is mainly
due to the lack of versatility of these machines in terms of the variety of yarns that
can be processed and the range of structures that can be normally knitted on them.
The displacement curves for the three main types of needle are shown in Fig. 5.22.
Technical fabric structures – 2. Knitted fabrics 119
16 Bearded Needle
12 Compound Needle
0° 30° 60° 90° 120° 150° 180° 210° 240° 270° 300° 330° 360°
Rotation of mainshaft (Degree)
5.22 Displacement curves of various needles.
It is obvious that compound needle machines would operate at faster rates,
provided all other factors are similar.
5.7 Warp-knitted structures
5.7.1 Stitch notation
Some of the more popular stitches used in the production of warp-knitted fabrics
are given in Fig. 5.23. These stitches, together with the number of guide bars used,
a comprehensive range of types and linear densities of yarns available, fancy thread-
ing, controlling individual run-ins and run-in ratios, and various ﬁnishing techniques
are combined and modiﬁed to construct an endless variety of fabrics. The lapping
movements of the individual guide bars throughout one repeat of the pattern are
normally indicated on special paper, called point paper. Each horizontal row of
equally spaced dots represents the same needles at successive courses. The spaces
between the dots, or needles, are numbered 0, 1, 2, 3, 4, and so on, and show the
number of needles transversed by each guide bar. Although three links per course
are normally employed, only two are actually required; the third (last link) is only
used to effect a smoother movement of the guide bar during the underlap. The ﬁrst
link determines the position of the guide bars at the start of the new course. The
second link determines the direction in which the overlap is made. The links, there-
fore, are grouped together in pairs and the lapping movements at each course are
separated by a comma. For instance, the lapping movements shown in Fig. 5.23(c)
are interpreted as follows:
• (1-0) is the overlap at the ﬁrst course
• (0,1) is the underlap at the same course, but made in the opposite direction to
• (1-2) is the overlap at the second course, and
120 Handbook of technical textiles
(a) (b) (c) (d) (e)
(f) (g) (h) (i) (j)
5.23 Stitch notation in tricot knitting. (a) Open pillar, (b) closed pillar, (c) tricot stitch,
(d) 2 ¥ 1 closed lap, (e) 3 ¥ 1 closed lap, (f) 4 ¥ 1 closed lap, (g) open tricot stitch,
(h) two-course atlas, (i) misslapping, ( j) laying-in.
• (2,1) is the underlap at the second course, but made in the opposite direction
to the previous underlap.
It will also be observed from Fig. 5.23 that when the underlap is made in the oppo-
site direction to the immediately preceding overlap, a closed loop is formed, but
when the underlap is made in the same direction as the immediately preceding
overlap, or no underlap is made, then an open loop will result.
It is vital to ensure when placing a pattern chain around the drum that the correct
link is placed in contact with the guide bar connecting rod, otherwise the underlap
will occur on the wrong side of the needles, or open loops may be formed instead
of the intended closed loops.
5.7.2 Single-guide bar structures
Although it is possible to knit fabrics using a single fully threaded guide bar, such
fabrics are now almost extinct owing to their poor strength, low cover, lack of
stability and pronounced loop inclination on the face of the fabric. Three examples
of single guide bar structures are shown in Fig. 5.24.
5.7.3 Two-guide bar full-set structures
The use of two guide bars gives a much wider pattern scope than is possible
when using only one, and a large proportion of the fabrics produced in industry
Technical fabric structures – 2. Knitted fabrics 121
5.24 Single-guide bar structures.
are made with two guide bars. The ﬁrst group of fabrics to consider are those
made with fully threaded guide bars, as many different effects may be obtained
by altering the lapping movements and these effects may be increased still further
by the use of colour, mixing different yarn, linear densities or using different
yarn types, such as yarns with different dyeing characteristics, textured yarns, and
220.127.116.11 Loop plating
With two fully threaded guide bars, each loop in the fabric will contain two threads,
one supplied by each bar. The underlaps made by the front guide bar are plated on
the back of the fabric and the loops from this bar are plated on the face of the fabric,
whereas the loops and the underlaps formed by the back guide bar are sandwiched
between those from the front guide bar (see Fig. 5.25). It will be observed from
Fig. 5.20(c) that when the guide bars swing through the needles to form the overlap,
the ends will be crossed on the needle hook (normally the two bars form overlaps
in opposite directions). As the guide bars return to the front of the machine, the
threads of the front guide bar are ﬁrst to strike the needles and are wrapped around
the needle hook ﬁrst, whereas the back guide bar threads are placed later and
above those from the front guide bar. If the tensions of the two warp sheets are
similar and the heights of the guide bars are correctly adjusted, the front bar loops
will always be plated on the face of the fabric. Any coloured thread in the front
guide bar will thus appear prominent on both fabric surfaces, an important
factor to be remembered in warp-knit fabric designing (see Fig. 5.25 for loop
122 Handbook of technical textiles
5.25 Full tricot.
18.104.22.168 Different structures
The two guide bars may make their underlaps in the same or opposite directions.
If made in the same direction, the fabric will show distortion similar to the single
bar fabric (see Fig. 5.29(a)) as the loops will be inclined. If, however, the underlaps
are made in opposite directions, an equal tension will be imposed in both directions,
and loops will be upright.
The structure of the simplest fabric made with two guide bars is shown in
Fig. 5.25 and is known as full tricot. The appearance of full tricot may be varied by
threading the guide bars with different coloured threads to give vertical stripes of
The most common fabric of all is locknit and its structure and the lapping move-
ments are shown in Fig. 5.26. When correctly knitted, the fabric shows even rows of
upright loops on the face of the fabric, and the two needle underlaps on the back
of the fabric give a smooth sheen. It has a soft handle and is very suitable for lin-
gerie. If the lapping movements for the bars are reversed to give reverse locknit,
the fabric properties are completely changed (Fig. 5.29(e)). The short underlaps will
now appear on the back of the fabric and will trap in the longer ones to give a more
stable and stiff structure, with far less width shrinkage from the needles than ordi-
nary locknit. The underlaps of the back guide bar may be increased to give even
greater stability and opacity with practically no width shrinkage from the needles.
An example of this is sharkskin, whose structure and lapping movements are shown
in Fig. 5.27. Another stable structure is shown in Fig. 5.28, and is know as queens
cord. The long back guide bar underlaps are locked ﬁrmly in the body of the fabric
by the chain stitches of the front guide bar. Both sharkskin and queenscord struc-
tures can be made more stable, heavier and stronger by increasing the back guide
underlaps to four or ﬁve needle spaces. The vertical chains of loops from the front
Technical fabric structures – 2. Knitted fabrics 123
5.27 Three-needle sharkskin.
guide bar may be used to give single wale vertical stripes of colour, such as pin
stripes in men’s suiting.
If the guide bars making a sharkskin are reversed, that is, if the front bar makes
the longer underlaps, the resultant fabric is known as satin which is a lustrous soft
fabric similar to the woven satin. Because of the long ﬂoats on the back of the fabric,
124 Handbook of technical textiles
5.28 Three-needle queenscord.
satin laps are used to make loop-raised fabrics. The raising machine is set so that
the underlaps are raised into loops without actually breaking any ﬁlaments. In order
to achieve the maximum raising effect, the two guide bars in a loop-raised fabric
are normally made to traverse in the same direction, and open loops may also be
used. The lapping movements of three-needle satin are shown in Fig. 5.29(b) and
those for a three-needle loop-raised fabric are shown in Fig. 5.29(a). The density
and height of pile can be increased by increasing the front guide bar underlaps to
four, ﬁve or six needle spaces.
Yarns may be introduced into the fabric without actually knitting. Figure 5.30
shows the structure lapping movements and pattern chains of a laid-in fabric. The
laid-in thread is trapped between the loop and the subsequent underlap of the guide
bar which must be situated in front of the laying-in bar. In order to lay-in a yarn,
therefore, that yarn must be threaded in a guide bar to the rear of the guide bar
(knitting bar), and it must make no overlaps. Laying-in is a useful device because a
laid-in thread never goes round the needle, and therefore very thick or fancy yarns
may be introduced into the fabric, such as heavy worsted yarn or metallic threads.
Figure 5.31 shows the laid-in thread being trapped in the fabric by the front guide
bar threads knitting an open tricot stitch (0-1, 2-1).
5.7.4 Grey speciﬁcation of a warp-knitted fabric
A complete grey speciﬁcation of a warp-knitted fabric should include the following
1. gauge of machine in needles per inch
2. number of guide bars in use
Technical fabric structures – 2. Knitted fabrics 125
5.29 Some two-guide bar full set structures. (a) Loop raised, (b) satin, (c) locknit, (d) full
tricot, (e) reverse locknit, (f) sharkskin, (g) queenscord, (h) laid-in fabric.
3. number of ends in each warp
4. types and linear densities of yarns used
5. run-in per rack for each warp
6. knitted quality of the fabric in courses per centimetre
7. order of threading in each guide bar
8. lapping movements of each guide bar during one repeat of the pattern or
details of the pattern wheels or pattern chains
9. relative lateral positions of the guide bars at a given point in the lapping
10. any special knitting instructions.
5.7.5 Fabric quality
The main parameter controlling the quality and properties of a given structure is
the run-in per rack, or the amount of yarn fed into the loop. Run-in per rack is
5.30 Laid-in structure.
5.31 Principle of laying-in.
Technical fabric structures – 2. Knitted fabrics 127
deﬁned as the length of warp fed into the fabric over 480 courses (1 rack = 480
courses). In two-guide bar fabrics, the run-in per rack for each guide bar may be the
same or different, depending upon the fabric structure. For example, in full tricot
structures (front: 1-2, 1-0 and back: 1-0, 1-2), it is normal to use the same run-in per
rack from both beams or 1 : 1, whereas in three-needle sharkskin fabrics (front: 1-2,
1-0 and back: 1-0, 3-4), the run-in per rack required from the back beam would be
more than the front beam say 1 : 1.66.
The run-in may be altered in two different ways, ﬁrst by altering the total run-in
of the bars, and second by altering the ratio or difference between the bars. Alter-
ing the total run-in will affect the ﬁnished number of courses per centimetre and
hence the area density of the fabric, the stability and the cover, but not the general
shape of the loop. Altering the difference between the guide bars will change the
balance of the fabric, affect the inclination of the loops and, because it puts more
or less strain on the individual yarns, change the strength.
Fabric take-up on the machine is adjusted to attain trouble-free knitting and also
to effect ease of ﬁnishing.
5.7.6 Tightness factor
The tightness factor K of a knitted fabric is deﬁned as the ratio of the fabric area
covered by the yarn to the total fabric area. It is regarded as a measure of loose-
ness or tightness of the structure, and inﬂuences dimensions such as the length,
width, and thickness and many other fabric characteristics such as area density,
opacity, abrasion resistance, modulus, strength and shrinkage.
If the tightness factor of a single-guide bar fabric is deﬁned as in Equation 5.2
where l is the stitch length, measured in millimetres, and tex is the yarn linear density,
then the tightness factor of a two-guide bar, full-set fabric is given by Equation (5.10)
tex f tex b
K= + (5.10)
where sufﬁxes f and b refer to front and back guide bars, and l is the stitch length
equal to (run-in/rack)/480 and is measured in millimetres. If the same tex is
employed in both bars, then
Ê 1 1ˆ
K = tex + (5.11)
Ë lf lb ¯
For most commercial two-guide bar full-set fabrics 1 £ K £ 2 with a mean tightness
factor value of 1.5.6
5.7.7 Area density
The area density of a single-guide bar fabric can be determined from Equation
Mass of the fabric = cpc ¥ wpc ¥ l ¥ T ¥ 10-2 gm-2
= s ¥ l ¥ T ¥ 10-2 gm-2 (5.12)
128 Handbook of technical textiles
where s is the stitch density (cm-2) or (cpc ¥ wpc), l is the stitch length (mm) and
T is the yarn tex.
Similarly, the area density of a two-guide bar full-set fabric would be Equation
Mass of the fabric = s[(l f ¥ Tf ) + (l b ¥ Tb )] ¥ 10 -2 gm -2 (5.13)
where sufﬁxes f and b refer to the front and back guide bars. If the same tex is
used in both guide bars, then the above equation can be written as Equation
Mass of the fabric = s ¥ T ¥ 10 -2 (l f + l b )gm -2
Ê Total run-in ˆ
or = s ¥ T ¥ 10 -2 gm -2 (5.14)
Ë 480 ¯
If the stitch density, that is, the number of loops cm-2, stitch length in mil-
limetres of the individual guide bars and tex of yarns employed in indi-
vidual beams are known, the fabric area density can be readily obtained using the
above equation in any fabric state, that is, on the machine, dry relaxed or fully
The geometry and dimensional properties of warp-knitted structures have been
studied by a number of researchers including Anand and Burnip.6
5.7.8 End-use applications of warp-knitted fabrics
Speciﬁcation for tricot machines is:
• Type of needle: compound or bearded
• Machine gauge: from 18 to 40 needles per inch (E18–E40)
• Machine width: from 213 to 533 cm (84–210 inches)
• Machine speed: from 2000 to 3500 courses per minute (HKS 2 tricot machine
operates at 3500 cpm)
• Number of needle bars: one or two
• Number of guide bars: from two to eight
• Products: lingerie, shirts, ladies’ and gents’ outerwear, leisurewear, sportswear,
swimwear, car seat covers, upholstery, technical fabrics, bed linen, towelling,
lining, nets, footwear fabrics, medical textiles.
Speciﬁcation for raschel machines is:
• Type of needle: latch or compound
• Machine gauge: from 12 to 32 needles per inch (E12–E32).
• Machine width: from 191 to 533 cm (75–210 inches)
• Machine speed: from 500 to 2000 courses per minute
• Number of needle bars: one or two
• Number of guide bars: from two to seventy-eight
• Products: marquisettes, curtains, foundation garments, nets, ﬁshing nets, sports
nets, technical fabrics, curtain lace, power nets, tablecloths, bed covers, elastic
bandages, cleaning cloths, upholstery, drapes, velvets, carpets, ladies’ underwear,
fruit and vegetable bags, geotextiles, medical textiles.
Technical fabric structures – 2. Knitted fabrics 129
1. s c anand, ‘ITMA ’95 review of circular knitting machines and accessories’, Asian Textile J.,
February 1996, 49.
2. s c anand, ‘Contributions of knitting to current and future developments in technical textiles’, Inaugural
Conference of Technical Textiles Group, The Textile Institute, Manchester, 23–24 May, 1988.
3. s c anand, ‘Knitting’s contribution to developments in medical textiles’, Textile Technol. Int., 1994,
4. s c anand, ‘Fine array of warp knitting machines from Karl Mayer’, Asian Textile J., April 1996, 51.
5. s c anand, ‘Warp knitted structures in composites’, ECCM-7 Proceedings, Volume 2, Woodhead Pub-
lishing, Cambridge, UK, 14–16 May 1996, p. 407.
6. s c anand and m s burnip, ‘Warp–knit construction’, Textile Asia, September 1981, 65.
7. s c anand, ‘Speciality knitting equipment at ITMA’99’, Asian Textile J., December 1999, 49.
8. s c anand, ‘Karl Mayer warp knitting equipment at ITMA’99’, Asian Textile J., September 1999, 49.
Technical fabric structures – 3. Nonwoven
Philip A Smith
Department of Textile Industries, University of Leeds, Leeds LS2 9JT, UK
It is an unfortunate fact that there is no internationally agreed deﬁnition of non-
wovens, in spite of the fact that the International Standards Organization published
a deﬁnition in 1988 (ISO 9092:1988). Many countries, particularly those that have
played an active part in the development of nonwovens, still prefer their own
national deﬁnition, which is generally wider in its scope than the very narrow deﬁ-
nition of ISO 9092.
As it is essential to be clear on the subject matter to be included in this chapter,
I have decided to use the deﬁnition of the American Society for Testing Materials
(ASTM D 1117-80). This deﬁnition is as follows: ‘A nonwoven is a textile struc-
ture produced by the bonding or interlocking of ﬁbres, or both, accomplished by
mechanical, chemical, thermal or solvent means and combinations thereof. The term
does not include paper or fabrics that are woven, knitted or tufted.’ It has to be ad-
mitted that this deﬁnition is not very precise, but it has been chosen because it
includes many important fabrics which most people regard as nonwovens, but which
are excluded by ISO 9092. Nonwovens are still increasing in importance; produc-
tion is increasing at the rate of 11% per annum.
One of the major advantages of nonwoven manufacture is that it is generally
done in one continuous process directly from the raw material to the ﬁnished fabric,
although there are some exceptions to this. This naturally means that the labour cost
of manufacture is low, because there is no need for material handling as there is in
older textile processes. In spite of this mass-production approach, the nonwovens
industry can produce a very wide range of fabric properties from open waddings
suitable for insulation containing only 2–3% ﬁbres by volume to stiff reinforcing
fabrics where the ﬁbre content may be over 80% by volume. How is this wide range
of properties produced? All nonwoven processes can be divided into two stages, the
preparation of the ﬁbres into a form suitable for bonding and the bonding process
itself. There are a number of different ways of ﬁbre processing, each producing its
Technical fabric structures – 3. Nonwoven fabrics 131
own particular characteristic in the ﬁnal fabric. Equally there are a number of
different bonding methods which have an even bigger effect on the ﬁnished fabric
properties. Almost all the ﬁbre processing methods can be combined with all the
bonding methods, so that the range of different possible manufacturing lines is
enormous, allowing a great range of ﬁnal properties.
However, this does raise a difﬁculty in describing the nonwoven process. We
know that the process is essentially a continuous one in which the ﬁbre processing
and bonding take place in two machines tightly linked together, but it is impossible
to describe the combined machines together owing to the wide number of machine
combinations that are possible. Instead it is necessary to explain the methods of
ﬁbre processing and the methods of bonding separately.
In ﬁbre processing it is common to make ﬁrst a thin layer of ﬁbre called a web
and then to lay several webs on top of each other to form a batt, which goes directly
to bonding. The words web and batt are explained by the previous sentence,
but there are cases where it is difﬁcult to decide if a ﬁbre layer is a web or a batt.
Nevertheless the ﬁrst stage of nonwoven processing is normally called batt
6.2 Methods of batt production using carding machines
The principles of carding and the types of carding machines have already been dis-
cussed in Chapter 3. The machines in the nonwoven industry use identical princi-
ples and are quite similar but there are some differences. In particular in the process
of yarn manufacture there are opportunities for further opening and for improving
the levelness of the product after the carding stage, but in nonwoven manufacture
there is no further opening at all and very limited improvements in levelness are
possible. It therefore follows that the opening and blending stages before carding
must be carried out more intensively in a nonwoven plant and the card should be
designed to achieve more opening, for instance by including one more cylinder,
though it must be admitted that many nonwoven manufacturers do not follow
Theoretically either short-staple revolving ﬂat cards or long-staple roller cards
could be used, the short-staple cards having the advantages of high production and
high opening power, especially if this is expressed per unit of ﬂoor space occupied.
However, the short-staple cards are very narrow, whereas long-staple cards can be
many times wider, making them much more suitable for nonwoven manufacture,
particularly since nonwoven fabrics are required to be wider and wider for many
end-uses. Hence a nonwoven installation of this type will usually consist of auto-
matic ﬁbre blending and opening feeding automatically to one or more wide long-
staple cards. The cards will usually have some form of autoleveller to control the
mass per unit area of the output web.
6.2.1 Parallel laying
The mass per unit area of card web is normally too low to be used directly in a non-
woven. Additionally the uniformity can be increased by laying several card webs
over each other to form the batt. The simplest and cheapest way of doing this is by
parallel laying. Figure 6.1 shows three cards raised slightly above the ﬂoor to allow
a long conveyor lattice to pass underneath. The webs from each card fall onto the
132 Handbook of technical textiles
6.1 Parallel laying.
Card Card Card
1 2 3
6.2 Alternative layout for parallel laying.
lattice forming a batt with three times the mass per unit area. If the cards are longer
this method becomes unwieldy and instead the cards are placed side-by-side as in
The card webs are turned through a right angle by a guide at 45°, but the batt
produced by this method is identical in all respects to the previous method. It is
important to recognise that it is not cross laid, as in Section 6.2.2, in spite of the
similarities between the layouts.
In any card web there is a marked tendency for the ﬁbres to lie along the web
rather than across it. Since in parallel laying all the card webs are parallel to each
other (and to the batt), it follows that most of the ﬁbres will lie along the batt and
very few across it. At this stage it is important to introduce two terms used widely
in nonwovens. The direction along the batt is called the ‘machine direction’ and the
direction at right angles is called the ‘cross direction’. Whatever method of bonding
is used it is found that the bonds are weaker than the ﬁbres. A tensile test on a
bonded parallel-laid material in the machine direction will depend mainly on the
ﬁbre strength, whereas in the cross direction it will depend more on the bond
strength. The effect of these facts on the relative ﬁbre frequency and on the direc-
tional strength of a typical parallel-laid fabric in various directions is shown in
The weakness of the fabric in the cross direction has a profound effect on pos-
sible uses of the fabric. Brieﬂy it can be used when strength is not required in either
Technical fabric structures – 3. Nonwoven fabrics 133
(a) direction (b) direction
6.3 Polar diagrams showing (a) the relative frequency of ﬁbres lying in various directions
and (b) the relative strength in various directions for a parallel-laid fabric.
direction, for example, a ﬁlter fabric which is completely supported or as a wiping
cloth. It is especially useful when high strength is required in one direction but
strength in the other direction is not important, but examples of this are rare; the
one usually quoted is a narrow tape cut in the machine direction and used mainly
for medical purposes.
This situation has been altered by the advent of cards designed especially for the
nonwoven industry. These cards are given a randomising doffer, which as its name
implies, makes the ﬁbre directions more random, together with ‘scrambling rollers’
that condense the card web in length, having the effect of buckling those ﬁbres lying
in the machine direction and forming segments lying in the cross direction.
By using these two techniques together it is possible to bring the strength ratio of
parallel-laid fabric down from the normal 10 or 20 : 1 to 1.5 : 1, which is about as
isotropic as any nonwoven. It may also be worth mentioning that similar carding
techniques have been expanded even further to make a card that produces a really
thick web, making laying unnecessary. However, all parallel-lay processes suffer
from a further fundamental problem; the width of the ﬁnal fabric cannot be wider
than the card web, while current trends demand wider and wider fabrics.
6.2.2 Cross laying
When cross laying, the card (or cards) are placed at right angles to the main con-
veyor just as in Fig. 6.2, but in this case the card web is traversed backwards and
forwards across the main conveyor, which itself is moving. The result is a zig-zag as
shown in Fig. 6.4.
Usually the conveyor B is moving only slowly so that many layers of card web
are built up, as shown in the diagram. The thickness of the card web is very small
in comparison with the completed batt, so that the zig-zag marks, which appear so
prominent in the ﬁgure, do not usually show much. There are two major problems
with cross layers; one is that they tend to lay the batt heavier at the edges than in
the middle. This fault can be corrected by running the traversing mechanism
rather slower in the centre and more rapidly at the edges, with a very rapid change
134 Handbook of technical textiles
6.4 Cross laying. A, card web; B, main conveyor; C, traverse mechanism; q, angle of
of direction at the edge. The other problem is trying to match the input speed of the
cross layer with the card web speed. For various reasons the input speed of the cross
layer is limited and the speed of the card web has to be reduced to match it. Because
for economic reasons the card is forced to run at maximum production, the card
web at the lower speed is thicker and the cross-laying marks discussed above will
tend to show more. In spite of these problems, cross layers are used much more
frequently than parallel layers.
The diagram in Fig. 6.4 showing webs crossing at an angle seems to imply that
the batt will be fairly isotropic. However, this is not so because the cross-laying angle
(q in Fig. 6.4) is normally less than 10°, so that the great majority of ﬁbres lie in or
near the cross direction. Cross-laid fabrics are consequently very strong in the
cross direction and weak in the machine direction. In many cases this may not
matter, because cross-laid fabrics are often quite heavy and may not require much
strength, but in many other cases a more isotropic batt is required. The obvious solu-
tion is to combine parallel laying and cross laying together; this is done very occa-
sionally but it is uncommon because it combines the limitations of both systems,
that is, the relatively narrow width of parallel laying and the slow output speed of
the cross laying. The common solution is to stretch the batt in the machine direc-
tion as it exits from the cross layer. Various machines are available for doing this;
the important criterion is that the stretching should be even, otherwise it could
create thick and thin places in the batt. Cross laying, with or without stretching, is
much more popular than parallel laying and is probably the most widely used system
6.3 Air laying
The air-laying method produces the ﬁnal batt in one stage without ﬁrst making a
lighter weight web. It is also capable of running at high production speeds but is
similar to the parallel-lay method in that the width of the ﬁnal batt is the same as
the width of the air-laying machine, usually in the range of 3–4 m.
Technical fabric structures – 3. Nonwoven fabrics 135
The degree of ﬁbre opening available in an air-lay machine varies from one
manufacturer to another, but in all cases it is very much lower than in a card. As a
consequence of this more ﬁbre opening should be used prior to air laying and the
ﬁbres used should be capable of being more easily opened, otherwise the ﬁnal batt
would show clumps of inadequately opened ﬁbre. In the past the desire for really
good ﬁbre opening (which is needed for lightweight batts) led to a process consist-
ing of carding, cross laying, then feeding the cross-laid batt to an air-laying machine.
The only purpose of the air-lay machine in this example was to obtain the desired
machine : cross-direction strength ratio, but it is a very expensive way compared to
the stretching device discussed above and such a process would not be installed
The diagram in Fig. 6.5 shows the principle of an air-lay machine, although the
actual machines may vary considerably from this outline. Opened ﬁbre from the
opening/blending section is fed into the back of hopper A, which delivers a uniform
sheet of ﬁbres to the feed rollers. The ﬁbre is then taken by the toothed roller B,
which is revolving at high speed. There may or may not be worker and stripper
rollers set to the roller B to improve the opening power. A strong air stream C dis-
lodges the ﬁbres from the surface of roller B and carries them onto the permeable
conveyor on which the batt is formed. The stripping rail E prevents ﬁbre from recir-
culating round the cylinder B. The air ﬂow at D helps the ﬁbre to stabilise in the
Figure 6.6 shows the formation zone in more detail. This shows that the ﬁbres
fall onto an inclined plane, and that the angle between this plane and the plane of
the fabric depends on the width of the formation zone, w, and the thickness of the
6.5 Principle of air-lay machine. A, Hopper/chute feed; B, opening roller; C, air ﬂow from
fan; D, suction to fan; E, stripping rail; F, batt conveyor.
6.6 Close-up of the formation zone.
136 Handbook of technical textiles
batt, t. It is possible when making thick fabrics to reduce the width, w, so that the
ﬁbres lie at a substantial angle to the plane of the batt. It is claimed that for this
reason air-laid fabrics show better recovery from compression compared with cross-
laid fabrics. It is often thought because the ﬁbres are deposited without control
from an air stream that they will be random in the plane of the batt. This belief is
so widespread that air-laid fabrics are frequently called ‘random-laid’ fabrics. The
use of this term should be strongly discouraged, because it gives a false impression.
In fact air-laid fabrics can have strength ratios as high as 2.5 : 1, which is far from
random. It is thought that the increase in the machine direction strength is caused
by the movement of the conveyor; a ﬁbre in the air-stream approaching the con-
veyor will tend to be pulled into the machine direction as it lands on the moving
The parallel-laid, cross-laid and air-laid methods discussed so far, are collec-
tively known as dry-laid processes. They are the most similar to traditional textile
processing and currently account for slightly less than half the total nonwoven
6.4 Wet laying
The wet-laid process is a development from papermaking that was undertaken
because the production speeds of papermaking are very high compared with textile
production. Textile ﬁbres are cut very short by textile standards (6–20 mm), but at
the same time these are very long in comparison with wood pulp, the usual raw
material for paper. The ﬁbres are dispersed into water; the rate of dilution has to
be great enough to prevent the ﬁbres aggregating. The required dilution rate turns
out to be roughly ten times that required for paper, which means that only spe-
cialised forms of paper machines can be used, known as inclined-wire machines. In
fact most frequently a blend of textile ﬁbres together with wood pulp is used as the
raw material, not only reducing the necessary dilution rate but also leading to a big
reduction in the cost of the raw material. It is now possible to appreciate one of the
problems of deﬁning ‘nonwoven’. It has been agreed that a material containing 50%
textile ﬁbre and 50% wood pulp is a nonwoven, but any further increase in the wood
pulp content results in a ﬁbre-reinforced paper. A great many products use exactly
50% wood pulp. Wet-laid nonwovens represent about 10% of the total market, but
this percentage is tending to decline. They are used widely in disposable products,
for example in hospitals as drapes, gowns, sometimes as sheets, as one-use ﬁlters,
and as coverstock in disposable nappies.
6.5 Dry laying wood pulp
The paper industry has attempted for many years to develop a dry paper process
because of the problems associated with the normal wet process, that is, the removal
of very large volumes of water by suction, by squeezing and ﬁnally by evaporation.
Now a dry process has been developed using wood pulp and either latex binders or
thermoplastic ﬁbres or powders to bond the wood pulp together to replace hydro-
gen bonding which is no longer possible. Owing to the similarity of both the bonding
methods and some of the properties to those of nonwovens, these products are being
Technical fabric structures – 3. Nonwoven fabrics 137
referred to as nonwovens in some areas, although it is clear from the deﬁnition
above they do not pass the percentage wood pulp criterion. Hence although the dry-
laid paper process cannot be regarded as a nonwoven process at present, it is very
likely that the process will be modiﬁed to accept textile ﬁbres and will become
very important in nonwovens in the future. It is for this reason that it has been
6.6 Spun laying
Spun laying includes extrusion of the ﬁlaments from the polymer raw material,
drawing the ﬁlaments and laying them into a batt. As laying and bonding are nor-
mally continuous, this process represents the shortest possible textile route from
polymer to fabric in one stage. In addition to this the spun-laid process has been
made more versatile. When ﬁrst introduced only large, very expensive machines
with large production capabilities were available, but much smaller and relatively
inexpensive machines have been developed, permitting the smaller nonwoven pro-
ducers to use the spun-laid route. Further developments have made it possible to
produce microﬁbres on spun-laid machines giving the advantages of better ﬁlament
distribution, smaller pores between the ﬁbres for better ﬁltration, softer feel and
also the possibility of making lighter-weight fabrics. For these reasons spun-laid pro-
duction is increasing more rapidly than any other nonwoven process.
Spun laying starts with extrusion. Virtually all commercial machines use ther-
moplastic polymers and melt extrusion. Polyester and polypropylene are by far the
most common, but polyamide and polyethylene can also be used. The polymer chips
are fed continuously to a screw extruder which delivers the liquid polymer to a
metering pump and thence to a bank of spinnerets, or alternatively to a rectangu-
lar spinneret plate, each containing a very large number of holes. The liquid polymer
pumped through each hole is cooled rapidly to the solid state but some stretching
or drawing in the liquid state will inevitably take place. Up to this stage the tech-
nology is similar to the ﬁbre or ﬁlament extrusion described in Chapter 2, except
that the speeds and throughputs are higher, but here the technologies tend to divide.
In spun laying the most common form of drawing the ﬁlaments to obtain the correct
modulus is air drawing, in which a high velocity air stream is blown past the ﬁla-
ments moving down a long tube, the conditions of air velocity and tube length being
chosen so that sufﬁcient tension is developed in the ﬁlaments to cause drawing to
take place. In some cases air drawing is not adequate and roller drawing has to be
used as in normal textile extrusion, but roller drawing is more complex and tends
to slow the process, so that air drawing is preferred.
The laying of the drawn ﬁlaments must satisfy two criteria; the batt must be as
even as possible in mass per unit area at all levels of area, and the distribution of
ﬁlament orientations must be as desired, which may not be isotropic. Taking the
regularity criterion ﬁrst, the air tubes must direct the ﬁlaments onto the conveyor
belt in such a way that an even distribution is possible. However, this in itself is not
sufﬁcient because the ﬁlaments can form agglomerations that make ‘strings’ or
‘ropes’ which can be clearly seen in the ﬁnal fabric. A number of methods have been
suggested to prevent this, for instance, charging the spinneret so that the ﬁlaments
become charged and repel one another or blowing the ﬁlaments from the air tubes
against a bafﬂe plate, which tends to break up any agglomerations. With regard to
138 Handbook of technical textiles
6.7 Diagram of a spun-laid process.
the ﬁlament orientation, in the absence of any positive traversing of the ﬁlaments
in the cross direction, only very small random movements would take place.
However, the movement of the conveyor makes a very strong machine direction
orientation; thus the fabric would have a very strong machine-direction orientation.
Cross-direction movement can most easily be applied by oscillating the air tubes
backwards and forwards. By controlling the speed and amplitude of this oscillation
it is possible to control the degree of cross-direction orientation. A simpliﬁed
diagram of a spun-laid plant is shown in Fig. 6.7.
6.7 Flash spinning
Flash spinning is a specialised technique for producing very ﬁne ﬁbres without the
need to make very ﬁne spinneret holes. It is used in making only two fabric types.
Flash spinning depends on the fact that the intramolecular bonds in polyethylene
and polypropylene are much weaker than similar bonds in polyester and polyamide.
When a thin sheet of polyoleﬁn is very highly drawn (10 or 12 to 1) the molecules
align in the direction of drawing giving high strength in that direction, but across
the drawing direction the strength is based only on the intramolecular bonds and
so is very low, so low that any mechanical action such as bending, twisting or abra-
sion causes the sheet to split. Depending on the original thickness of the sheet and
the amount of splitting, the result may be ﬁbre-like but with a rectangular cross-
section. The process is known as ﬁbrillation.
In ﬂash spinning the polymer is dissolved in a solvent and is extruded as a sheet
at a suitable temperature so that when the pressure falls on leaving the extruder the
Technical fabric structures – 3. Nonwoven fabrics 139
solvent boils suddenly. This blows the polymer sheet into a mass of bubbles with a
large surface area and consequently with very low wall thickness. Subsequent
drawing of this sheet, followed by mechanical ﬁbrillation, results in a ﬁbre network
of very ﬁne ﬁbres joined together at intervals according to the method of produc-
tion. This material is then laid to obtain the desired mass per unit area and direc-
Flash-spun material is only bonded in two ways, so that it seems sensible to
discuss both the bonding and the products at this juncture. One method (discussed
later in Section 6.10.3) involves melting the ﬁbres under high pressure so that vir-
tually all ﬁbres adhere along the whole of their length and the fabric is almost solid
with very little air space. This method of construction makes a very stiff material
with high tensile and tear strengths. It is mainly used in competition with paper for
making tough waterproof envelopes for mailing important documents and for
making banknotes. The fact that the original ﬁbres were very ﬁne means that the
material is very smooth and can be used for handwriting or printing. The alterna-
tive method of bonding is the same, that is, heat and pressure (see Section 6.10.4)
but is only applied to small areas, say 1 mm square, leaving larger areas, say 4 mm
square, completely unbonded. The bonded areas normally form a square or diago-
nal pattern. This material, known as Tyvek, has a lower tensile strength than the fully
bonded fabric, but has good strength and is ﬂexible enough to be used for clothing.
Because the ﬁne ﬁbres leave very small pores in the fabric, it is not only waterproof
but is also resistant to many other liquids with surface tensions lower than water.
The presence of the pores means that the fabric is permeable to water vapour and
so is comfortable to wear. Tyvek is used principally for protective clothing in the
chemical, nuclear and oil industries, probably as protection for the armed forces and
certainly in many industries not requiring such good protection but where it is found
to be convenient. The garments can be produced so cheaply that they are usually
regarded as disposable.
6.8 Melt blown
The process of melt blowing is another method of producing very ﬁne ﬁbres at high
production rates without the use of ﬁne spinnerets. Figure 6.8 shows that the
polymer is melted and extruded in the normal way but through relatively large
As the polymer leaves the extrusion holes it is hit by a high speed stream of hot
air at or even above its melting point, which breaks up the ﬂow and stretches the
many ﬁlaments until they are very ﬁne. At a later stage, cold air mixes with the hot
and the polymer solidiﬁes. Depending on the air velocity after this point a certain
amount of aerodynamic drawing may take place but this is by no means as satis-
factory as in spun laying and the ﬁbres do not develop much tenacity. At some point
the ﬁlaments break into staple ﬁbres, but it seems likely that this happens while the
polymer is still liquid because if it happened later this would imply that a high
tension had been applied to the solid ﬁbre, which would have caused drawing before
breaking. The ﬁne staple ﬁbres produced in this way are collected into a batt on a
permeable conveyor as in air laying (Section 6.3) and spun laying (Section 6.6). The
big difference is that in melt blowing the ﬁbres are extremely ﬁne so that there are
many more ﬁbre-to-ﬁbre contacts and the batt has greater integrity.
140 Handbook of technical textiles
Cold air Collecti
6.8 Diagram of melt-blown equipment.
For many end-uses no form of bonding is used and the material is not non-
woven, but simply a batt of loose ﬁbres. Such uses include ultraﬁne ﬁlters for air
conditioning and personal face masks, oil-spill absorbents and personal hygiene
products. In other cases the melt-blown batt may be laminated to another nonwo-
ven, especially a spun-laid one or the melt-blown batt itself may be bonded but the
method must be chosen carefully to avoid spoiling the openness of the very ﬁne
ﬁbres. In the bonded or laminated form the fabric can be used for breathable pro-
tective clothing in hospitals, agriculture and industry, as battery separators, indus-
trial wipes and clothing interlinings with good insulation properties. Melt blowing
started to develop rapidly in about 1975, although the process was known before
1950. It is continuing to grow at about 10% per annum.
6.9 Chemical bonding
Chemical bonding involves treating either the complete batt or alternatively isolated
portions of the batt with a bonding agent with the intention of sticking the ﬁbres
together. Although many different bonding agents could be used, the modern indus-
try uses only synthetic lattices, of which acrylic latex represents at least half and
styrene–butadiene latex and vinyl acetate latex roughly a quarter each. When the
bonding agent is applied it is essential that it wets the ﬁbres, otherwise poor adhesion
will be achieved. Most lattices already contain a surfactant to disperse the polymer
particles, but in some cases additional surfactant may be needed to aid wetting. The
next stage is to dry the latex by evaporating the aqueous component and leaving the
polymer particles together with any additives on and between the ﬁbres. During this
stage the surface tension of the water pulls the binder particles together forming a
ﬁlm over the ﬁbres and a rather thicker ﬁlm over the ﬁbre intersections. Smaller
binder particles will form a more effective ﬁlm than larger particles, other things
being equal. The ﬁnal stage is curing and in this phase the batt is brought up to a
higher temperature than for the drying.The purpose of curing is to develop crosslinks
both inside and between the polymer particles and so to develop good cohesive
strength in the binder ﬁlm. Typical curing conditions are 120–140 °C for 2–4 min.
6.9.1 Saturation bonding
Although the principles discussed above apply to all forms of chemical bonding
whatever the method of binder application, this latter factor has a profound
Technical fabric structures – 3. Nonwoven fabrics 141
inﬂuence on the properties of the nonwoven material. As implied by the name,
saturation bonding wets the whole batt with bonding agents, so that all ﬁbres are
covered in a ﬁlm of binder. It is clear that saturation bonding would not be suitable
for ﬂash-spun or melt-blown batts, since it would impair the ﬁne ﬁbres, but it is inher-
ently suitable for all other batts, although other methods of bonding are generally
preferred for spun-laid batts.
To saturate the batt, it is carried under the surface of the bonding agent. In most
cases the batt is very open and weak and care is needed to avoid distortion. The
action of the liquid greatly reduces the thickness of the batt and the thickness is
further reduced by the squeeze rollers which follow. Hence saturation bonded
fabrics are generally compact and relatively thin. However, as in most technologies,
there is an exception to this rule; if coarse ﬁbres containing a lot of crimp are used
they can spring back after being crushed by the squeeze rollers and produce a thick
open fabric, but this is very rare.
The drying is often done in a dryer designed basically for woven fabric, modiﬁed
by having a permeable conveyor to support and transport the nonwoven through
the machine. Hot air is blown against the top and bottom surfaces to cause drying,
the top air pressure being slightly greater than the bottom pressure to press and
control the nonwoven against the conveyor. Because the air only penetrates the
immediate surfaces of the nonwoven, drying is conﬁned to these areas and the
central layers of the nonwoven remain wet. The result is that the liquid wicks from
the wet areas to the dry ones, unfortunately carrying the suspended binder particles
with the water. This is the cause of the problem known as binder migration; under
adverse conditions virtually all the binder can be found in the surface layers and
the central layers contain no binder at all, leaving them very weak. Such a fabric
can easily split into two layers, a problem known as delamination. Fortunately a
number of ways have been found to control binder migration, several of them being
rather complicated. Only one method will be mentioned here, through-drying. In
this case only one air stream is used to blow down and through the fabric. Drying
conditions are then almost the same in all parts of the fabric and no binder migra-
tion takes place. However, the air pressure may exert a signiﬁcant force on the non-
woven, pressing it against the conveyor so hard that it may be imprinted with the
pattern of the conveyor.
In contrast the curing stage is simpler; it should be done in a separate compart-
ment in order to achieve the correct temperature. However, it is quite common for
curing to be done in the ﬁnal part of the dryer in order to keep down machinery
Many of the physical properties of saturation-bonded fabric derive from the fact
that all ﬁbres are covered with a ﬁlm of binder. First, the fabric feels like the binder
and not the ﬁbres it is made from. However, in some cases this can be an advan-
tage, because by using either a hydrophobic or a hydrophilic binder the reaction of
the fabric to water can be changed regardless of which ﬁbres are used.
The mechanical properties can be explained from a model of a network of ﬁbres
bonded together at close intervals. The fabric cannot stretch without the ﬁbres also
stretching by a similar amount. Hence the fabric modulus is of the order of the ﬁbre
modulus, that is, extremely high. A high modulus in a spatially uniform material
means that it will be stiff, which explains why saturation-bonded fabrics are very
stiff relative to conventional textiles. At the same time tensile strength is low,
because the bonds tend to break before most ﬁbres break. Efforts to make the
142 Handbook of technical textiles
fabrics more ﬂexible include using a more ﬂexible binder and using a lower per-
centage of binder, but both of these reduce the tensile strength; in fact the ratio of
fabric modulus to tensile strength remains remarkably constant.
One of the major uses of saturation bonded fabric turns this apparent disad-
vantage into an advantage. Interlining fabric for textile clothing is required to be
stiff and to have a high modulus. Other uses are as some types of ﬁlter fabric, in
some coverstock and in wiping cloths.
6.9.2 Foam bonding
It can be inferred above that one of the problems of saturation bonding is that too
much water is used. This not only increases the cost of drying but also increases the
risk of binder migration. Application of chemicals as a foam was developed not
only for nonwovens but also for the dyeing and ﬁnishing industry as a means of
using less water during application. The binder solution and a measured volume of
air are passed continuously through a driven turbine which beats the two compo-
nents into a consistent foam. The foam is then delivered to the horizontal nip of the
impregnating roller, as shown in Fig. 6.9. The foam delivery has to be traversed
because the foam does not ﬂow easily; end plates, which cannot be shown in the
cross-section diagram prevent the foam from running out of the gap at the end of
The rollers serve the dual purpose of metering the amount of foam applied and
also of squeezing the foam into the batt. If the set-up shown in Fig. 6.9 does not give
adequate foam penetration, then the batt can be entered vertically and the foam
can be applied from both sides.
Foam application should only be thought of as an alternative method of satura-
tion bonding. The properties and uses of the fabrics are identical.
6.9.3 Print bonding
Print bonding involves applying the same types of binder to the batt but the appli-
cation is to limited areas and in a set pattern. The binder does not penetrate well
into the dry batt so the batt is ﬁrst saturated with water and then printed with either
a printing roller or a rotary screen printer. The ﬁnal properties of the fabric depend
6.9 Foam impregnation.
Technical fabric structures – 3. Nonwoven fabrics 143
vitally on the printed/unprinted area ratio, which could be changed signiﬁcantly if
the binder migrated sideways from the printed area. To prevent this the binder
formulation must contain some thickener.
Print-bonded fabrics are much softer in feel and also much more ﬂexible owing
to the strong effect of the free ﬁbres in the unbonded areas. They are also signiﬁ-
cantly weaker than saturation-bonded fabrics owing to the ﬁbres slipping in un-
bonded areas, but knowing the ﬁbre length and the ﬁbre orientation distribution it
is possible to design a print pattern which will minimise the strength loss.
Print-bonded fabrics tend to be used in applications where the textile-like handle
is an advantage. Examples are disposable/protective clothing, coverstock and wiping
cloths, particularly domestic ones (washing-up and dusting).
6.9.4 Spray bonding
Similar latex binders may also be applied by spraying, using spray guns similar to
those used in painting, which may be either operated by compressed air or be airless.
On the ﬁrst passage the spray penetrates about 5 mm into the top surface, then the
batt is turned over for a spray application on the lower surface. Each spray
application reduces the thickness of the batt slightly, but it is still left substantially
lofty; the drying and curing stage also causes some small dimensional changes.
The ﬁnal product is a thick, open and lofty fabric used widely as the ﬁlling in
quilted fabrics, for duvets, for some upholstery and also for some types of ﬁlter
6.10 Thermal bonding
Thermal bonding is increasingly used at the expense of chemical bonding for a
number of reasons. Thermal bonding can be run at high speed, whereas the speed
of chemical bonding is limited by the drying and curing stage.Thermal bonding takes
up little space compared with drying and curing ovens. Also thermal bonding
requires less heat compared with the heat required to evaporate water from the
binder, so it is more energy efﬁcient.
Thermal bonding can use three types of ﬁbrous raw material, each of which
may be suitable in some applications but not in others. First, the ﬁbres may be all
of the same type, with the same melting point. This is satisfactory if the heat is
applied at localised spots, but if overall bonding is used it is possible that all the
ﬁbres will melt into a plastic sheet with little or no value. Second, a blend of
fusible ﬁbre with either a ﬁbre with a higher melting point or a non-thermoplastic
ﬁbre can be used. This is satisfactory in most conditions except where the fusible
ﬁbre melts completely, losing its ﬁbrous nature and causing the batt to collapse in
thickness. Finally, the fusible ﬁbre may be a bicomponent ﬁbre, that is, a ﬁbre
extruded with a core of high melting point polymer surrounded by a sheath of lower
melting point polymer. This is an ideal material to process because the core of the
ﬁbre does not melt but supports the sheath in its ﬁbrous state. Thermal bonding is
used with all the methods of batt production except the wet-laid method, but it is
worth pointing out that the spun-laid process and point bonding (see Section 6.10.4)
complement each other so well that they are often thought of as the standard
144 Handbook of technical textiles
6.10.1 Thermal bonding without pressure
The batt may be processed through a hot air oven with just sufﬁcient air movement
to cause the fusible portion to melt. This method is used to produce high loft fabrics;
the products are similar to spray-bonded materials except that in this case the
bonding is uniform all the way through and there is virtually no limit to the thick-
ness of fabric made. The uses of the thermal-bonded fabric are basically the same
as those of a spray-bonded fabric but they would be used in situations where a
higher speciﬁcation is required. One interesting example is in the fuel tanks of
Formula 1 cars to limit the rate of fuel loss in the event of a crash.
6.10.2 Thermal bonding with some pressure
This method is basically the same as the previous one, except that as the batt leaves
the thermobonding oven it is calendered by two heavy rollers to bring it to the
required thickness. The products could be used as insulation, as rather expensive
packaging or for ﬁltration.
6.10.3 Thermal bonding with high pressure
The batt is taken between two large heated rollers (calender rollers) that both melt
the fusible ﬁbre and compress the batt at the same time. Provided the batt is not
too heavy in mass per unit area the heating is very rapid and the process can be
carried out at high speed (300 m min-1). The design of calender rollers for this
purpose has become highly developed; they can be 4–5 m wide and can be heated
to give less than 1 °C temperature variation across the rollers. Also the rollers have
to be specially designed to produce the same pressure all the way across the rollers,
because rollers of this width can bend quite signiﬁcantly.
The products tend to be dense and heavily bonded, although of course the
amount of bonding can be adjusted by varying the percentage of fusible ﬁbre in the
blend. Typical properties are high strength, very high modulus and stiffness but good
recovery from bending. The main uses are in some geotextiles, stiffeners in some
clothing and in shoes, some ﬁltration media and in rooﬁng membranes.
6.10.4 Thermal bonding with point contact
Although it is very strong, the fabric produced with bonding all over the batt (area
bonding) is too stiff and non-textile-like for many uses. It is far more common to
use point bonding, in which one of the calender rollers is engraved with a pattern
that limits the degree of contact between the rollers to roughly 5% of the total area.
The bonding is conﬁned to those points where the rollers touch and leaves roughly
95% of the batt unbonded. The area, shape and location of the bonding points are
of great importance.
Fabrics made in this way are ﬂexible and relatively soft owing to the unbonded
areas. At the same time they maintain reasonable strength, especially in the case of
the spun-laid fabrics. These fabrics have many uses, for example, as a substrate
for tufted carpets, in geotextiles, as a ﬁltration medium, in protective/disposable
clothing, as a substrate for coating, in furniture and home furnishings and as
Technical fabric structures – 3. Nonwoven fabrics 145
6.10.5 Powder bonding
Thermoplastic powders may be used as an alternative to thermoplastic ﬁbres for
bonding in all the methods of thermobonding except for point bonding, where
powder in the unbonded areas would be wasted and would drop out in use. Prod-
ucts made by powder bonding seem to be characterised by softness and ﬂexibility
but in general they have relatively low strength. Again there is a very wide range
of uses covering particularly the high bulk applications, protective apparel and
6.11 Solvent bonding
This form of bonding is only rarely used but it is interesting from two points of view;
ﬁrst, the solvent can be recycled, so the process is ecologically sound, although
whether or not recycling is practical depends on the economics of recovering the
solvent. Second, some of the concepts in solvent bonding are both interesting and
unique. In one application of the method, a spun-laid polyamide batt is carried
through an enclosure containing the solvent gas, NO2 which softens the skin of the
ﬁlaments. On leaving the enclosure bonding is completed by cold calender rolls and
the solvent is washed from the fabric with water using traditional textile equipment.
This is a suitable method of bonding to follow a spun-laid line because the speeds
of production can be matched. The other application uses a so-called latent solvent,
by which is meant one that is not a solvent at room temperature but becomes a
solvent at higher temperatures. This latent solvent is used in conjunction with
carding and cross laying and is applied as a liquid before carding. The action of
carding spreads the solvent and at the same time the solvent lubricates the ﬁbres
during carding. The batt is passed to a hot air oven which ﬁrst activates the solvent
and later evaporates it. The product will normally be high loft, but if less loft is
required a compression roller could be used.
All the methods of bonding discussed so far have involved adhesion between the
ﬁbres; hence they can be referred to collectively as adhesive bonding. The ﬁnal three
methods, needlefelting, hydroentanglement and stitch bonding rely on frictional
forces and ﬁbre entanglements, and are known collectively as mechanical bonding.
The basic concept of needlefelting is apparently simple; the batt is led between
two stationary plates, the bed and stripper plates, as shown in Fig. 6.10. While
between the plates the batt is penetrated by a large number of needles, up to about
4000 m-1 width of the loom. The needles are usually made triangular and have barbs
cut into the three edges as shown in Fig. 6.11.
When the needles descend into the batt the barbs catch some ﬁbres and pull them
through the other ﬁbres. When the needles return upwards, the loops of ﬁbre formed
on the downstroke tend to remain in position, because they are released by the
barbs. This downward pressure repeated many times makes the batt much denser,
that is, into a needlefelt.
The above description illustrates how simple the concept seems to be. Without
going into too much detail it may be interesting to look at some of the complica-
146 Handbook of technical textiles
Batt Needles Drawing rollers
6.10 Diagram of a needleloom.
6.11 Diagram of three needle barbs on a section of a needle.
tions. First, the needles can only form vertical loops or ‘pegs’ of ﬁbre and increase
the density of the batt. This alone does not form a strong fabric unless the vertical
pegs pass through loops already present in the horizontal plane of the batt. It follows
from this that parallel-laid fabric is not very suitable for needling since there
are few ﬁbre loops present, so most needling processes are carried out with cross-
laid, air-laid and spun-laid batts. Second, the amount of needling is determined
partly by the distance the drawing rollers move between each movement of the
needleboard, the ‘advance’, and partly by the number of needles per metre across
the loom. If the chosen advance happens to be equal to, or even near the distance
between needle rows as shown in Fig. 6.10, then the next row of needles will
come down in exactly the same position as the previous row, and so on for all the
rows of needles. The result will be a severe needle patterning; to avoid this the
distance between each row of needles must be different. Computer programs
have been written to calculate the best set of row spacings. Third, if it is necessary
to obtain a higher production from a needleloom, is it better to increase the number
of needles in the board or to increase the speed of the needleboard? Finally, in
trying to decide how to make a particular felt it is necessary to choose how
many needle penetrations there will be per unit area, how deep the needles will
penetrate and what type of needles should be used from a total of roughly 5000
different types. The variations possible seem to be inﬁnite, making an optimisation
process very difﬁcult.
There are several different types of needleloom. Figure 6.10 is called a ‘down-
punch’ because it is pushing the ﬁbres downwards. Similarly an ‘up-punch’ pushes
the ﬁbres upwards. There is some advantage in combining an up-punch with a down-
punch when trying to make a dense felt, rather than to punch continually in the
same direction. For this reason some looms are made ‘double-punch’, that is, one
board punching down and one board punching up. Although this type of double
punch loom is better than unidirectional punching, it has the disadvantage that all
the down-punching is completed before the up-punching even starts. The up-punch
and the down-punch are far from symmetrical. In order to improve this situation
the modern form of double-punch loom has been developed in which both boards
penetrate through the same bed and stripper plates. The normal operation is for the
Technical fabric structures – 3. Nonwoven fabrics 147
boards to penetrate the fabric alternately, one from above and the other from below.
To all intents and purposes the two boards are now symmetrical and this appears
to give optimum needling. This type of loom can often be adjusted so that both sets
of needles enter and leave the batt simultaneously. (Alternate rows of needles have
to be taken out of both boards to prevent serious needle damage.) This is not found
to be advantageous with long ﬁbres (50 mm upwards) because there is quite a high
chance that the same ﬁbre may be pulled upwards by one needle and pushed down-
wards by another, leading to serious ﬁbre breakage. However, the very short mineral
ﬁbres used for high temperature insulation are found to consolidate better using
this form of simultaneous needling.
Needlefelts have a high breaking tenacity and also a high tear strength but the
modulus is low and the recovery from extension is poor. For these last two reasons
any needlefelt which is likely to be subjected to a load has to have some form of
reinforcement to control the extension. Needled carpets, for instance, may be
impregnated with a chemical binder that gives better dimensional stability and
increases the resistance to wear. In other cases thermal bonding may be used for
the same object. For heavy duty applications such as ﬁlter media and papermakers’
felts, yarns are used, either spun yarns or ﬁlament yarns. In some cases with a cross-
laid batt the threads may run only in the machine direction, but it is also common
to use a woven fabric as the foundation and to build up the nonwoven on one or
both sides. In both applications the presence of the woven fabric or base fabric
reduces the efﬁciency by restricting the liquid ﬂow; in a few cases ‘baseless’ fabrics,
that is nonwovens without woven supports have been made, but there are still very
many situations where a base fabric is essential.
Needlefelts are used widely in gas ﬁltration media and in some wet ﬁltration. The
principal advantage is that the nonwoven is practically homogeneous in compari-
son with a woven fabric so that the whole area of a nonwoven ﬁlter can be used for
ﬁltration, whereas in a woven fabric the yarns effectively stop the ﬂow, leaving only
the spaces between the yarns for ﬁltration. In papermakers’ felts the same consid-
erations apply, but in some cases the design of the felt has also to allow for the fact
that the felt is acting as an enormous drive belt to drive some parts of the machine.
In both gas ﬁltration and papermakers’ felts needlefelts hold virtually the whole
market. Needlefelts are used in geotextiles, but in view of the low modulus their
application is mainly in removing water rather than as reinforcement. If the water
is ﬂowing through the fabric this is termed ﬁltration. For instance a simple drain
may be formed by lining a trench with a geotextile, partly ﬁlling it with graded
gravel, drawing the edges of the geotextile together and back-ﬁlling the trench as
shown in Fig. 6.12. The geotextile will keep the drain open for many years by ﬁl-
tering out ﬁne particles. Less frequently the geotextile is required for drainage,
which means water movement in the plane of the fabric. Because of the inevitable
contamination of the surface layers, together with the compression of the geotex-
tile caused by the soil pressure, only a limited part of the fabric cross-section is
actually available for drainage and more complicated compound structures are
frequently used in preference.
Many makers of synthetic leather have taken the view that the structure should
be similar to natural leather. In these cases the backing or foundation of the
synthetic leather is a needlefelt. The method of production is to include heat-
shrinkable ﬁbres which are made to shrink after intense needling in order to make
the felt even more dense. After shrinking the felt is impregnated using a binder
148 Handbook of technical textiles
6.12 Simple drain using geotextiles.
that ﬁlls the voids in the felt but does not adhere to the ﬁbres, otherwise the felt
would become very stiff. The leather is then ﬁnished by coating the face side with
one or two layers of suitable polymer. Needlefelts are also widely used in home and
commercial carpeting; in many cases the carpet may have either a velour or a loop
pile surface to improve the appearance. Both velour and loop pile are produced in
a separate needling operation using special needles and a special bedplate in the
needleloom. Similar materials in a lighter weight are used for car carpeting, head-
liners and other decorative features on cars.
6.13 Stitch bonding
The idea of stitch bonding was developed almost exclusively in Czechoslovakia, in
the former East Germany and to some extent in Russia, though there was a brief
development in Britain. The machines have a number of variants which are best dis-
cussed separately; many possible variants have been produced but only a limited
number are discussed here for simplicity.
6.13.1 Batt bonded by threads
Stitch bonding uses mainly cross-laid and air-laid batts. The batt is taken into a
modiﬁcation of a warp knitting machine (see Chapter 5) and passes between the
needles and the guide bar(s). The needles are strengthened and are specially
designed to penetrate the batt on each cycle of the machine. The needles are of the
compound type having a tongue controlled by a separate bar. After the needles pass
through the batt the needle hooks open and the guide bar laps thread into the hooks
of the needles. As the needles withdraw again the needle hooks are closed by the
tongues, the old loops knock over the needles and new loops are formed. In this
way a form of warp knitting action is carried out with the overlaps on one side of
the batt and the underlaps on the other. Generally, as in most warp knitting, con-
tinuous ﬁlament yarns are used to avoid yarn breakages and stoppages on the
machine. Two structures are normally knitted on these machines, pillar (or chain)
stitch, or tricot. When knitting chain stitch the same guide laps round the same
needle continuously, producing a large number of isolated chains of loops. When
Technical fabric structures – 3. Nonwoven fabrics 149
knitting tricot structure, the guide bar shogs one needle space to the left, then one
to the right. Single-guide bar structure is called tricot, whereas the two-guide bar
structure is often referred to as full tricot.
The nature of this fabric is very textile-like, soft and ﬂexible. At one time it was
widely used for curtaining but is now used as a backing fabric for lamination, as cov-
ering material for mattresses and beds and as the fabric in training shoes. In decid-
ing whether to use pillar or tricot stitch, both have a similar strength in the machine
direction, but in the cross direction the tricot stitch fabric is stronger, owing to the
underlaps lying in that direction. A cross-laid web is already stronger in that direc-
tion so the advantage is relatively small. The abrasion resistance is the same on the
loop or overlap side, but on the underlap side the tricot fabric has signiﬁcantly better
resistance owing to the longer underlaps. However, continuous ﬁlament yarn is very
expensive relative to the price of the batt, so tricot fabric costs signiﬁcantly more.
The decision then becomes a purely ﬁnancial one; is it worth paying more for the
greater abrasion resistance?
6.13.2 Stitch bonding without threads
In this case the machine is basically the same as in the previous section, but the
guide bar(s) are not used. The needle bar moves backwards and forwards as before,
pushing the needles through the batt. The main difference is that the timing of the
hook closing by the tongues is somewhat delayed, so that the hook of the needle
picks up some of the ﬁbre from the batt. These ﬁbres are formed into a loop on the
ﬁrst cycle and on subsequent cycles the newly formed loops are pulled through the
previous loops, just as in normal knitting. The ﬁnal structure is felt-like on one side
and like a knitted fabric on the other. The fabric can be used for insulation and as
a decorative fabric.
6.13.3 Stitch bonding to produce a pile fabric
To form a pile fabric two guide bars are usually used, two types of warp yarns (pile
yarn and sewing yarn) and also a set of pile sinkers, which are narrow strips of metal
over which the pile yarn is passed and whose height determines the height of the pile.
The pile yarn is not fed into the needle’s hook so does not form a loop; it is held in
place between the underlap of the sewing yarn and the batt itself. It is clear that this
is the most efﬁcient way to treat the pile yarn, since any pile yarn in a loop is effec-
tively wasted. This structure has been used for making towelling with single-sided
pile and also for making loop-pile carpeting in Eastern Europe.The structure has not
been popular in the West owing to competition with double-sided terry towelling and
tufted carpets. Equally it has not been used in technical textiles, but it could be a solu-
tion in waiting for the correct problem. Strangely a suitable problem has been pro-
posed. Car seating usually has a polyester face with a foam backing, but this material
cannot be recycled, because of the laminated foam. It has been suggested that a poly-
ester nonwoven pile fabric could replace the foam and would be 100% recyclable.
6.13.4 Batt looped through a supporting structure
In this technique the needles pass through the supporting fabric and pick up as much
ﬁbre from the batt as possible. Special sinkers are used to push ﬁbre into the needle’s
150 Handbook of technical textiles
hook to increase this pick-up. The ﬁbre pulled through the fabric forms a chain of
loops, with loose ﬁbre from the batt on the other surface of the fabric. The fabric is
ﬁnished by raising, not as one might expect on the loose side of the fabric but instead
the loops are raised because this gives a thicker pile. This structure was widely used
in Eastern Europe, particularly for artiﬁcial fur, but in the West it never broke the
competition from silver knitting, which gives a fabric with similar properties. The
method could be used for making good quality insulating fabrics.
6.13.5 Laid yarns sewn together with binding threads
Two distinct types of fabric can be made using the same principle. The ﬁrst is a
simulated woven fabric in which the cross-direction yarns are laid many at a time
in a process a bit like cross laying. The machine direction yarns, if any are used, are
simply unwound into the machine. These two sets of yarns are sewn together using
chain stitch if there are only cross-direction threads and tricot stitch if machine-
direction threads are present, the underlaps holding the threads down. Although
fabric can be made rapidly by this system this turns out to be a situation in which
speed is not everything and in fact the system is not usually economically com-
petitive with normal weaving. However, it has one great technical advantage; the
machine and cross threads do not interlace but lie straight in the fabric. Conse-
quently the initial modulus of this fabric is very high compared with a woven fabric,
which can ﬁrst extend by straightening out the crimp in the yarn. These fabrics are
in demand for making ﬁbre-reinforced plastic using continuous ﬁlament glass and
similar high modulus ﬁbres or ﬁlaments.
The alternative system makes a multidirectional fabric. Again sets of yarns are
cross-laid but in this case not in the cross direction but at, say, 45° or 60° to the cross
direction. Two sets of yarns at, say, +45° and -45° to the cross direction plus another
layer of yarns in the machine direction can be sewn together in the usual way. Again
high modulus yarns are used, with the advantage that the directional properties of
the fabric can be designed to satisfy the stresses in the component being made.
The process of hydroentanglement was invented as a means of producing an entan-
glement similar to that made by a needleloom, but using a lighter weight batt. A
successful process was developed during the 1960s by Du Pont and was patented.
However, Du Pont decided in the mid-1970s to dedicate the patents to the public
domain, which resulted in a rush of new development work in the major industrial
countries, Japan, USA, France, Germany and Britain.
As the name implies the process depends on jets of water working at very high
pressures through jet oriﬁces with very small diameters. A very ﬁne jet of this sort
is liable to break up into droplets, particularly if there is any turbulence in the water
passing through the oriﬁce. If droplets are formed the energy in the jet stream will
still be roughly the same, but it will spread over a much larger area of batt so that
the energy per unit area will be much less. Consequently the design of the jet to
avoid turbulence and to produce a needle-like stream of water is critical. The jets
are arranged in banks and the batt is passed continuously under the jets held up
by a perforated screen which removes most of the water. Exactly what happens
Technical fabric structures – 3. Nonwoven fabrics 151
to the batt underneath the jets is not known, but it is clear that ﬁbre ends become
twisted together or entangled by the turbulence in the water after it has hit the batt.
It is also known that the supporting screen is vital to the process; changing the
screen with all other variables remaining constant will profoundly alter the fabric
Although the machines have higher throughputs compared with most bonding
systems, and particularly compared with a needleloom, they are still very expensive
and require a lot of power, which is also expensive. The other considerable problem
lies in supplying clean water to the jets at the correct pH and temperature. Large
quantities of water are needed, so recycling is necessary, but the water picks up air
bubbles, bits of ﬁbre and ﬁbre lubricant/ﬁbre ﬁnish in passing through the process
and it is necessary to remove everything before recycling. It is said that this ﬁltra-
tion process is more difﬁcult than running the rest of the machine.
Fabric uses include wipes, surgeons’ gowns, disposable protective clothing and
backing fabrics for coating. The wipes produced by hydroentanglement are guar-
anteed lint free, because it is argued that if a ﬁbre is loose it will be washed away
by the jetting process. It is interesting to note that the hydroentanglement process
came into being as a process for entangling batts too light for a needleloom, but
that the most recent developments are to use higher water pressures (400 bar) and
to process heavier fabrics at the lower end of the needleloom range.
p lennox-kerr (ed.), Needlefelted Fabrics, Textile Trade Press, Manchester, 1972.
g e cusick (ed.), Nonwoven Conference, Manchester, University of Manchester Institute of Science and
a newton and j e ford, ‘Production and properties of nonwoven fabrics’, Textile Progr., 1973 5(3) 1–93.
p j cotterill, ‘Production and properties of stitch-bonded fabrics’, Textile Progr., 1975 7(2) 101–135.
a t purdy, ‘Developments in non-woven fabrics’, Textile Progr., 1980 12(4) 1–97.
k pﬂiegel, ‘Nonwovens for use in the geotextile area’, Textile Institute Ind., 1981 19 178–181.
a krauter and p ehler, ‘Aspects of ﬁbre to binder adhesion in nonwovens’, Textil Praxis Int., 1980, No.
10, 1206–1212; No. 11, 1325–1328.
anon, ‘Foam padder and foam production for the nonwoven industry’, Chemiefaser/Textilindustrie
(English edition), 1981 4, E.35–36 in English (pp. 336–338 in German).
g e cusick and a newton, (eds), ‘Nonwovens Conference’, Manchester, University of Manchester Insti-
tute of Science and Technology, 1988.
g e cusick and k l ghandi, (eds), ‘Conference on nonwovens’, Huddersﬁeld, University of Huddersﬁeld,
a j rigby and s c anand, ‘Nonwovens in medical and healthcare products’, Tech. Textiles Int., 1996, Part
I, Sept. pp. 22–28 Part II, Oct. pp. 24–29.
Index 1999 Congress, Geneva, EDANA (European Disposables and Nonwovens Association), Brussels,
Finishing of technical textiles
Michael E Hall
Department of Textiles, Faculty of Technology, Bolton Institute, Deane Road,
Bolton BL3 5AB, UK
The name textile ﬁnishing covers an extremely wide range of activities, which are
performed on textiles before they reach the ﬁnal customer. They may be temporary,
for example the way bed sheets are pressed before packing, or they may be per-
manent, as in the case of a ﬂame-retardant tenting fabric. However, all ﬁnishing
processes are designed to increase the attractiveness or serviceability of the textile
product. This could involve such techniques as putting a glaze on an upholstery
fabric, which gives it a more attractive appearance, or the production of water-
repellent ﬁnishes, which improve the in-service performance of a tenting fabric.
Thus a further aim of textile ﬁnishing may be described as improvement in customer
satisfaction, which ﬁnishing can bring about. This improvement in the perceived
value of a product to the consumer forms the basis of modern ideas on product mar-
keting. Technical textiles are deﬁned as those materials with non-clothing applica-
tions. Thus the fashion aspects of textiles will be ignored, although aesthetic aspects
of say upholstery and drapes will be covered.
7.2 Finishing processes
The ﬁnishing processes that are available can be divided into four main groups,
• Mechanical processes: these involve the passage of the material through
machines whose mechanical action achieves the desired effects. A heating
process, the purpose of which is usually to enhance these desired effects, fre-
quently accompanies this.
These mechanical ﬁnishes, which will be discussed in detail later in this section,
– Calendering: compression of the fabric between two heavy rolls to give a
ﬂattened, smooth appearance to the surface of the fabric.
Finishing of technical textiles 153
– Raising: plucking the ﬁbres from a woven or knitted fabric to give a nap
effect on the surface.
– Cropping: cutting the surface hairs from the a fabric to give a smooth appear-
ance, often used on woollen goods where the removal of surface hair by a
singeing process is not possible.
– Compressive shrinkage: the mechanical shrinking of the warp ﬁbres in woven
fabrics so that shrinkage on washing is reduced to the desired level.
• Heat setting: this is a process for the stabilisation of synthetic ﬁbres so that they
do not shrink on heating.
• Chemical processes: these may be described as those processes that involve the
application of chemicals to the fabric. The chemicals may perform various func-
tions such as water repellency or ﬂame retardancy, or may be used to modify the
handle of a fabric. Chemical ﬁnishes are normally applied in the form of an
aqueous solution or emulsion and may be applied via a variety of techniques,
the main one being the pad mangle, which is illustrated in Fig. 7.1.
After the padding or the application stage of the chemical ﬁnishing the fabric
is usually dried to remove the water from the fabric and some form of ﬁxation
of the ﬁnish is then performed. This commonly takes the form of a baking
process, where the fabric is subjected to a high temperature for a short period,
which enables the applied chemicals to form a more durable ﬁnish on the fabric
than would otherwise be achieved.
Surface coating is a most important part of the ﬁnishing of technical textiles and as
such deserves a separate chapter (see Chapter 8).
7.3 Mechanical ﬁnishes
Calendering may be deﬁned as the modiﬁcation of the surface of a fabric by the
action of heat and pressure.1 The ﬁnish is obtained by passing the fabric between
heated rotating rollers (or bowls as they are frequently called), when both speed of
rotation and pressure applied are variable. The surfaces of the rollers can be either
smooth or engraved to provide the appropriate ﬁnish to the fabric, while the actual
construction of the rollers may be varied from hardened chromium-plated steel to
elastic thermoplastic rollers.
7.1 Simple pad mangle.
154 Handbook of technical textiles
7.2 Flattening effect on fabric of calendering.
22.214.171.124 Effects which may be achieved by calendering
Calendering is done for many purposes but the main effects are:
• smoothing the surface of the fabric
• increasing the fabric lustre
• closing the threads of a woven fabric
• decreasing the air permeability
• increasing the fabric opacity
• improving the handle of a fabric, i.e. softening
• ﬂattening slubs
• obtaining silk-like to high gloss ﬁnishes
• surface patterning by embossing
• consolidation of nonwovens.
The ﬂattening of the fabric is illustrated in Fig. 7.2, which shows the effect of the
ﬂattened yarn structure. This gives a greater light reﬂectance than the original
rounded yarn structure.
126.96.36.199 Types of calender
In general calenders usually have between two and seven rollers, with the most
common being the three-bowl calender. Perhaps the most important factor in
calender design is the composition of the rollers and the surface characteristics
of these.2 Textile calenders are made up from alternate hard steel and elastic bowls.
The elastic bowls are made from either compressed paper or compressed cotton,
however, a lot of modern calenders are made with a thermoplastic thick covering,
which is usually nylon 6. The latter have the advantage that they are less liable to
damage from knots, seams and creases than cotton and paper bowls, damage that
would then mark off onto the calendered fabric. In fact the development of the
‘in situ’ polymerisation technique for nylon 6 has enabled the simple production
of elastic rollers from this material. Because of this improved performance, nylon 6
covered rollers often enable the required effects to be achieved in a single nip thus
reducing the overall number of bowls.
In two-bowl calenders (Fig. 7.3), it is normal to have the steel bowl on top so that
the operator can see any ﬁnish. This type of arrangement is often used with the
nylon bottom bowl mentioned previously, especially where the calender is used for
glazing or the embossed type of ﬁnishes.
The arrangement where two steel bowls are used together only occurs in excep-
tional circumstances, for example, in the compaction of nonwovens. Here both bowls
Finishing of technical textiles 155
“Soft” paper or nylon
7.3 Two-bowl calender.
7.4 Three-bowl calender.
are usually oil heated so that some form of permanent setting occurs. Finally, the
arrangement with two elastic bowls is not common but is sometimes used on cotton
knitgoods to obtain a soft handle.
The three-bowl calender (Fig. 7.4) was developed from the two-bowl calender
and with this type of calender it is normal to use only the top nip, with the bowls
arranged steel–elastic–steel.The bottom bowl is used to keep the central elastic bowl
smooth and thus assist in the ﬁnishing. The same arrangement also serves the same
purpose on embossing calenders, where there is the possibility of permanent inden-
tation from the top roller.
Pressure used in all of the above calenders can be varied between 10 and 40
tonnes, with running speeds up to 60 m min-1. However, these are very much average
ﬁgures with ﬁgures as low as 6 tonnes for a 1 m wide calender to as high as 120
tonnes for a 3 m wide calender. In addition, running speeds of 20 m min-1 are used
on an embossing calender, while on a glazing calender speeds of over 150 m min-1
have been quoted.
The temperatures which are used in calender rollers can, of course, vary from
room temperature to 250 °C. However, it must be stressed that temperature control
is of vital importance, with a tolerance of ±2 °C being commonly quoted. Some gen-
eralisations can be made as follows:
156 Handbook of technical textiles
• Cold bowls give a soft handle without much lustre; warm bowls (40–80 °C) give
a slight lustre.
• Hot bowls (150–250 °C) give greatly improved lustre, which can be further
improved by the action of friction and waxes.
188.8.131.52 Types of ﬁnish
• Swissing or normal gloss: a cold calender produces a smooth ﬂat fabric.
However, if the steel bowl of the calender is heated then in addition to smooth-
ness the calender produces a lustrous surface. If a seven-bowl multipurpose cal-
ender is used then a smooth fabric with surface gloss on both sides is produced.
• Chintz or glazing: this gives the highly polished surface which is associated with
glazed chintz. The effect is obtained by heating the top bowl on a three-bowl
calender and rotating this at a greater speed than that of the fabric. The speed
of this top bowl can vary between 0 and 300% of the speed of the fabric. In
certain cases where a very high gloss is required, the fabric is often preimpreg-
nated with a wax emulsion, which further enhances the polished effect. This type
of calendering is often called friction calendering.
• Embossing: in this process the heated top bowl of a two-bowl calender is
engraved with an appropriate pattern which is then transferred to the fabric
passing through the bowls. The effect can be made permanent by the use of
thermoplastic ﬁbres or in the case of cellulosics by the use of an appropriate
• Schreiner or silk ﬁnishing: this is a silk-like ﬁnish on one side of the fabric. It is
produced (see Fig. 7.5) by embossing the surface of the fabric with a series of
ﬁne lines on the surface of the bowls. These lines are usually at an angle of about
30° to the warp threads. The effect can be made permanent by the use of
thermoplastic fabric or, in the case of cotton, by the use of a resin ﬁnish. This
ﬁnish is particularly popular on curtains and drapes because of the silk-like
appearance this type of ﬁnish gives to the product.
• Delustering: this is commonly achieved by passing the fabric through the bottom
two bowls of a three-bowl calender, where these are elastic. However, steel bowls
with a special matt ﬁnish have been manufactured that are very effective for this
• Chasing: the fabric is threaded through the calender in such a way as to press the
fabric against itself several times. It is common to use a ﬁve- or seven-bowl calen-
der, the fabric passing through each nip of the calender in two or three layers.
7.5 Principle of Schreiner calender.
Finishing of technical textiles 157
• Palmer ﬁnishing: in this type of ﬁnish the damp fabric is carried on the inside of
a felt blanket round a steam-heated cylinder, often called a Palmer drier. The
face of the fabric, which is run on the surface of the heated cylinder, takes a light
polish from the cylinder, while the back of the fabric, which is in contact with
the felt blanket, takes a roughened effect from the cylinder. This ﬁnish is par-
ticularly popular for cotton drill fabric.
These descriptions of calendering should not be regarded in any way as complete
and for a more complete description the reader is recommended to contact the cal-
ender manufacturers. Some of these are Küsters in Germany, Parex Mather in the
UK, Kleinewefers in Germany and Metallmeccanica in Italy.
Raising is the technique whereby a surface effect is produced on the fabric that gives
the fabric a brushed or napped appearance. It is achieved by teasing out the indi-
vidual ﬁbres from the yarns so that they stand proud of the surface.3 The way this
was done originally was to use the seedpod of the thistle, which was known as a
teasel. These teasels were nailed to a wooden board and the fabric was drawn over
them to produce a fabric with a hairy surface, which had improved insulating prop-
erties. This method has largely been superseded by the use of rotating wire brushes,
although where a very gentle raising action is required, such as in the case of mohair
shawls, teasels are still used.
184.108.40.206 Modern raising machines
All modern raising machines (see Fig. 7.6) use a hooked or bent steel wire to tease
the ﬁbres from the surface of fabric. The most important factor in the raising oper-
ation is the relationship between the point and the relative speed of the cloth. The
raising wires or ‘card’ wires are mounted on a ﬂexible base, which is then wrapped
around a series of rollers, which are themselves mounted on a large cylindrical
frame, illustrated in Fig. 7.6.
The raising action is brought about by the fabric passing over the rotating rollers
and the wire points teasing out the individual ﬁbres in the yarn. Because there are
a large number of points acting on the fabric at any one time, the individual ﬁbres
must be sufﬁciently free to be raised from the ﬁbre surface. This is a combination
of the intraﬁbre friction and the degree of twist in the raised yarns. Thus for ‘ideal’
raising, the yarns should be of low twist and be lubricated. One further point to note
is that because the fabric runs in the warp direction over the machine, only the weft
threads are at right angles to the rotating raising wires and therefore only the weft
threads take part in the raising process.
220.127.116.11 Raising action
From Fig. 7.6 it can be seen that both the card wire rollers and the cylinder to
which these are attached may be rotated; it is the relative speed of these in relation to
that of the fabric that produces the various raising effects that may be achieved.
There are two basic actions in raising and these are governed by the direction in
which the card wires point and the relative speed of rotation of these in relation to
the fabric.These actions are called the pile and the counterpile actions and are shown
in Fig. 7.7.
158 Handbook of technical textiles
7.6 The modern raising machine.
In the counterpile action, the working roller rotates in the opposite direction to
that of the cylinder with the points of the wire moving in the direction of rotation.
This action pulls the individual ﬁbres free from the surface.
In the pile action, the points of the wire are pointing away from the direction
of movement of the fabric. This results in an action where the raised ﬁbres are
subject to a combing action which tends to tuck back the ﬁbres into the body of the
Finishing of technical textiles 159
Direction of Counterpile
rotation of the main roller
7.7 The raising action.
The most common raising action uses a combination of both of these actions,
producing an even raise over the whole of the fabric surface. Control of the raising
action has been achieved by measurement of the surface roughness of the raised
fabric.4 It is therefore possible to control the exact height of the nap on the surface
This is a process by which the ﬁbres which protrude from the surface of a fabric,
are cut to an even height. The principle used in this technique is similar to a lawn
mower in that a spiral cutter rotates against a stationary blade and cuts off any mate-
rial protruding from the fabric surface.5
This principle is illustrated in Fig. 7.8, which shows the fabric passing over the
cutting bed and the protruding hairs on the surface being caught between the rotat-
ing head of the spiral cutter and the ledger blade. By raising and lowering the height
of the cutting bed, the depth of cut may be varied. Obviously the cutting action pro-
duces a great deal of cut pile and this must be removed by strong suction otherwise
a large amount of ﬂy rapidly accumulates. In order to achieve an even cut and
a smooth surface, several passes through the machine are required or a single
pass through a multiple head machine is required. Average speeds of about
15 m min-1 are commonly encountered.
One important use for this technique is the production of pile fabrics from a
looped terry fabric. When this type of fabric is sheared the top of the loops of the
terry fabric are cut off and a velvet like appearance is produced. When knitted loop
pile fabrics are sheared, knitted velour is produced that has found a great deal of
use in upholstery fabric.
7.3.4 Compressive shrinkage
The shrinkage of fabrics on washing is a well-known phenomenon. It is caused in
part by the production and processing stresses on the fabric. Production stresses are
introduced into the fabric by the yarn tension and also by the tension which is nec-
160 Handbook of technical textiles
Spiral cutting cylinder
Scroll unit Cutting table
7.8 Shearing or cropping.
7.9 Fabric relaxation.
essary for the satisfactory production of fabric. Processing stresses are introduced
during the bleaching, dyeing and ﬁnishing of fabric when the fabric is pulled in the
warp direction. This tends to remove the warp crimp from the fabric as illustrated
in Fig. 7.9.
In order to replace the warp crimp and thus minimise warp shrinkage, a process
known as compressive shrinkage is carried out on the fabric to replace the crimp
that has been pulled out in the preparation and ﬁnishing processes. This may be
illustrated in the following way. A strip of fabric is placed on a convex rubber surface
and gripped at each end of the rubber. As the rubber is allowed to straighten, the
length of the fabric exceeds that of the rubber as illustrated in Fig. 7.10. However,
if the fabric could be stuck to the surface of the rubber then the fabric would be
subjected to compression and warp crimp would be introduced.
This principle then is applied to the compressive shrinking machine, where the
cloth is fed in a plastic state onto a thick rubber belt at point A as shown in Fig.
7.11. While the belt is in the convex position for A to B the fabric merely lies on
the surface, but at point B the belt starts to wrap its way round a large heated cylin-
der and thus changes from a convex to a concave shape. Thus the surface of the
rubber belt contracts and the fabric, which is held onto the surface of the rubber, is
Finishing of technical textiles 161
7.10 (a) Fabric under tension, (b) tension relaxed.
7.11 Shrinkage belt.
7.12 Complete shrinkage range.
subject to a warp compression over the region C to D. The actual degree of shrink-
age which takes place is controlled by the amount of fabric fed onto the rubber belt
and the pressure between the heated metal cylinder and the belt, which increases
or decreases the concave shape of the rubber belt. The principles of compressive
shrinkage have also been reviewed.6
A sketch of the complete compressive shrinkage range is shown in Fig. 7.12.
7.4 Heat setting
The main aim of the heat setting process is to ensure that fabrics do not alter their
dimensions during use. This is particularly important for uses such as timing and
driving belts, where stretching of the belt could cause serious problems. It is impor-
tant to examine the causes of this loss in stability so that a full understanding can
be obtained of the effects that heat and mechanical forces have on the stability of
fabrics. All fabrics have constraints placed on them by their construction and
method of manufacture, but it is the heat-setting mechanism that occurs within the
ﬁbre that will ultimately inﬂuence fabric dimensions.
162 Handbook of technical textiles
7.4.1 Heat-setting mechanisms
The ﬁrst attempt to describe the various mechanisms of heat setting synthetic ﬁbres
was that of Hearle.7 He describes the various techniques which have been used to
set fabrics into a given conﬁguration and leaving aside the chemical methods of sta-
bilisation, these techniques may be described as inﬂuencing the following:
1. chain stiffness
2. strong dipole links
3. hydrogen bonds
all of which are inﬂuenced by temperature, moisture and stress.
Hydrogen bonding is the most important of the factors which inﬂuence setting,
and nylon has a strong hydrogen-bonded structure whereas polyester has not. Thus
relaxation of nylon can occur in the presence of water at its boiling point. In fact
one of the common tests for the nylon fabrics used in timing belts is a 5 min boil in
7.4.2 Fibre structure
All ﬁbre-forming molecules consist of long chains of molecules. In fact, a typical
nylon molecule will have a length which is some 5000 times the molecule diameter.
X-ray diffraction techniques have conﬁrmed that all synthetic ﬁbres contain crys-
talline and non-crystalline regions. In nylon and polyester these crystalline regions
occupy about 50% of the total space in the ﬁbre.
It can be shown that these ordered or crystalline regions are small compared to the
overall length of the polymer chain. To explain this phenomenon the polymer chains
cannot be perfectly aligned over the whole length of the molecule, but must pass
through alternating regions of order and disorder. The picture that thus emerges is
one of short crystalline regions connected by relative regions of disorder.This view of
molecular structure is now an accepted model and is known as the fringed micelle
model. Figure 7.13 represents this scheme for a disorientated polymer.
The short parallel areas represent regions of order where adjacent chains pack
in an ordered fashion. The non-parallel regions are where the chains do not pack
together in a regular fashion, creating the non-crystalline regions or amorphous
regions in the ﬁbre.
7.4.3 Polymer orientation
During the processing of both polyester and nylon, the ﬁbres are spun through ﬁne
holes and have a structure similar to that in Fig. 7.13. However, to develop the
7.13 Undrawn ﬁbre.
Finishing of technical textiles 163
7.14 Drawn ﬁbre.
strength in the ﬁbre these ﬁbres are then cold drawn to create an orientated struc-
ture, which is illustrated in Fig. 7.14. Once the chains have been orientated then the
ﬁbres show a much greater resistance to applied loads and a greater stiffness, hence
the reason for cold drawing.
7.4.4 Transition temperatures
In the previous section the crystalline and amorphous regions of the polymer were
discussed. These do have an effect on two important parameters:
• Glass transition temperature: this represents the temperature at which molecu-
lar movement starts in the amorphous regions of the polymer, and was given
the name because it is the temperature at which the polymer changes from
a glassy solid to a rubbery solid. This is the temperature at which segmental
loosening takes place and hence dyeing can only take place above this
• Melting point: at this point the forces holding the molecules in the crystal-
line regions of the ﬁbre are overcome by the thermal energy and the polymer
melts. In both polyester and nylon these temperatures are separated by
about 150 °C.
7.4.5 Heat shrinkage
All textile ﬁbres are subjected to a cold drawing process and hence when they are
heated above the point at which molecular motion sets in, they will progressively
shrink until they reach the point of thermodynamic equilibrium represented by
Fig. 7.13. In other words the cold drawing process is reversed by the application
7.4.6 Heat setting
If the model of the drawn ﬁbre (Fig. 7.14) is considered then it can be observed that
in the drawn ﬁbre, the molecules in the amorphous areas, while still random, are
much more parallel than in the non-drawn state. Thus if the ﬁbre is held so that
shrinkage is prevented and heated above its glass transition temperature, the
164 Handbook of technical textiles
molecules in the amorphous areas start to move, and because of their relative ori-
entation, to crystallise. In practice the ﬁbres are usually heated to about 20–40 °C
below the melting point. It now becomes apparent that the whole process of heat
setting is time dependent, because it takes time for the motion of the molecules to
line themselves up in the ﬁrst place and then to crystallise. It is possible to heat set
at much lower temperatures than are used in practice. However, if low tempera-
tures are used, the ﬁbres are only stabilised up to the heat set temperature and as
soon as this temperature is exceeded, severe shrinkage occurs. In addition the rate
of crystallisation decreases with decreasing temperature and heat setting would be
a long and tedious process.
Obviously it is the temperature the yarns in the fabric actually achieve that is
important in the setting process. This is dependent not only on the fabric construc-
tion but also on the method of heating, because it is essential that the setting tem-
perature is achieved quickly and evenly over the width of the fabric. Commonly,
stenters are used for this purpose, because temperature control to ±1% over a 2 m
width can be obtained. Where contact heating is used, special designs are available
to obtain this degree of control.
7.4.7 Essentials of heat setting
From the previous discussion it can be seen that heat setting is a temperature-
dependent process and for practical purposes the heat setting temperatures vary for
polyester between 190–200 °C and for nylon 6.6 between 210–220 °C.The ﬁbres must
not be allowed to move during the heating process and the heating must be sufﬁ-
ciently long enough to allow crystallisation to take place, after which the ﬁbre must
be cooled down to well below the heat setting temperature before being released.
There is an important difference between the behaviour of the two common
polyamides (nylon 6 and nylon 6.6) and polyester, because of their different behav-
iour towards water. Polyester is non-absorbent, so the heat setting behaviour is not
affected by water. However, nylon will absorb sufﬁcient water to obtain a tempo-
rary set that is based on hydrogen bonding and is destroyed on boiling in water. The
consequence of this is that to obtain a permanent set on nylon, the water has to be
removed from the ﬁbre so that crystallisation can take place. Therefore nylon tends
to be heat set at a higher temperature than polyester.
1. Heat the fabric to within about 20–40 °C of the ﬁbre melting point.
2. Hold at this temperature under tension for approximately 20 s.
3. Cool fabric before removing tension.
The time–temperature relationship will vary depending on the polymer, the fabric
weight and construction.10 The simple way to determine these is to look at the shrink-
age of the ﬁnished product, if the material has been correctly heat set then it should
show a residual shrinkage of less than 1% on a 5 min immersion in boiling water.
7.5 Chemical processes
It has been suggested that by the end of 2000 some 50% of all textile ﬁbre con-
sumption in industrialised countries will be in technical textiles.11 A large percent-
age of this will consist of safety equipment and protective clothing and in fact this
Finishing of technical textiles 165
comprises the most signiﬁcant portion of the technical textiles market. Protective
clothing must provide resistance to the elements in the workplace, whilst at the same
time providing comfort during wear.The customers for these products demand strict
compliance with the regulations designed to protect the wearer. One of the most
important properties of this type of clothing is its resistance to small burning
sources, thus ﬂame resistance combined with easy cleaning is a most important con-
sideration. The ﬂame retardance must be maintained throughout the lifetime of the
The main regulation governing the use of ﬂame-retardant technical textiles was
the Furniture and Furnishing Fire Safety Regulations which were introduced
into the UK in 1988.12
7.5.1 Durable ﬂame-retardant treatments13,14
Fire-retardant technical textiles have been developed from a variety of textile ﬁbres,
the choice of which is largely dependent on the cost of the ﬁbre and its end-use.
However, the main ﬁbre in this area is cotton and thus treatments of this ﬁbre will
be discussed ﬁrst. Two major ﬂame-retardant treatments are popular. These are
Proban (Rhodia, formerly Albright and Wilson) and Pyrovatex (Ciba).13
The Proban process uses a phosphorus-containing material, which is based on
tetrakis(hydroxymethyl)phosphonium chloride (THPC). This is reacted with urea
and the reaction product is padded onto cotton fabric and dried. The fabric is then
reacted with ammonia and ﬁnally oxidised with hydrogen peroxide. The full reac-
tion scheme is shown in Fig. 7.15.
The Proban process may be summarised as follows:
7.15 Chemistry of the Proban process.
166 Handbook of technical textiles
1. Pad the fabric with Proban CC.
2. Dry the fabric to a residual moisture content of 12%.
3. React the fabric with dry ammonia gas.
4. Oxidise the fabric with hydrogen peroxide.
5. Wash off and dry the fabric.
6. Soften the fabric.
The actual chemistry of the process is fairly straightforward and the Proban forms
an insoluble polymer in ﬁbre voids and the interstices of the cotton yarn. There is
no actual bonding to the surface of the cellulose, but the insoluble Proban polymer
is held by mechanical means in the cellulose ﬁbres and yarns. Because of this the
Proban treated fabric has a somewhat harsh handle and some softening is usually
required before the fabric is ﬁt for sale. The chemistry is shown in Fig. 7.15.
The next method of forming a durable treatment for cellulose is by the use of
Pyrovatex. This material is closely related to the crosslinked resins used in textile
ﬁnishing and is in fact always applied with a crosslinked resin to form a chemical
bond to the cellulose. The application scheme is given in Fig. 7.16.
The Pyrovatex process may be summarised as follows:
1. Pad the Pyrovatex mixture.
2. Dry at 120 °C.
7.16 Chemistry of the Pyrovatex process.
Finishing of technical textiles 167
3. Cure at 160 °C for 3 min.
4. Wash in dilute sodium carbonate.
5. Wash in water.
6. Dry and stenter to width.
As the reaction is with the cellulose, the ﬂame-retardant substance is chemically
bound to the ﬁbre and is therefore durable. However, because the ﬂame-retardant
substance has to be applied with a crosslink resin, then the ﬁnished fabric has good
dimensional stability and also excellent crease-recovery properties making this
ﬁnish the one preferred for curtains. Unfortunately these desirable properties are
not without disadvantages, the main one in the case of Pyrovatex being the loss in
tear strength, which occurs with this and all crosslinking systems.
7.5.2 Synthetic ﬁbres with inherent ﬂame-retardant properties
The Furniture and Furnishing (Fire) (Safety) Regulations12 made it manda-
tory that all upholstery materials should withstand the cigarette and match test
as speciﬁed in BS 5852:1979: Pt1. This produced an enormous amount of work
in the industry on possible routes which could be used to meet this legislation.
These ranged from the use of materials that would not support combustion to chem-
ical treatments and backcoating techniques. It is now clear, however, that back-
coating is the main means by which these regulations are being met. Currently, some
5000 tonnes of backcoating formulations are being used in the UK for upholstery
The majority of backcoating formulations are based on the well-known ﬂame-
retardant effect of the combination of antimony(III) oxide and a halogen, which is
usually bromine, although chlorine is also used to a lesser degree. The synergistic
mixture for this is one part of antimony(III) oxide to two parts of bromine con-
taining organic compound. A typical formulation which describes the application
level per square metre, is shown in Table 7.1.
To this basic formulation are often added softeners, which modify the fabric
handle and antifungal compounds. In addition, foaming agents are used which
enable the use of foam application techniques, so that a minimum amount of
penetration of the backcoating compound onto the face of the fabric is achieved.
The use of foam application also enables higher precision in the weights applied
and shorter drying times to be achieved.15
Thus Proban, Pyrovatex and backcoating with antimony/bromine compounds
represent the major ﬂame-retardant treatments for cellulose.
7.5.3 Water-repellent ﬁnishes
The early water-repellent ﬁnishes were all based on the application of a mixture of
waxes, which were pliable at normal temperatures, applied to tightly woven cotton
fabrics. These were, of course, well suited to sail cloth and protective clothing, but
problems were encountered when the garments were cleaned. Therefore, the search
was on for water-repellent treatments that were simple to apply but would also allow
the treated fabrics to be cleaned.
It was noted early on that the heavy metal soaps did have water-repellent prop-
erties and therefore the ﬁrst attempt at the production of a durable treatment was
168 Handbook of technical textiles
Table 7.1 Typical backcoating formulation
Application level (g m-2)
Antimony(III) oxide 40
Decabromodiphenyl oxide 80
Acrylic binder 120
Cellulose surface with hydroxyl groups
7.17 Reaction of the chromium salt of a fatty acid with cellulose.
to use the chromium salt of a fatty acid, which was applied to cotton and then baked.
This gave a certain durability to the fabric thus treated and the mechanism is illus-
trated in Fig. 7.17.
Some of the later treatments involved the use of other fatty acid derivatives and
some of these are shown in Fig. 7.18.
The most recent treatments involve the use of the ﬂuorocarbons which are
basically esters of polyacrylic acid and a perﬂuorinated hexanol, as illustrated in
Fig. 7.19. A list of ﬁnishes is given in Table 7.2.6
7.5.4 Antistatic ﬁnishes
Static electricity is formed when two dissimilar materials are rubbed together. It
cannot be formed if identical materials are rubbed together. Thus when dissimilar
materials are rubbed together a separation of charges occurs and one of the mate-
rials becomes positively charged and the other negatively charged. The actual sign
of the charge depends on the nature of the two materials that are taking part and
this may be deduced from the triboelectric series, shown in Table 7.3. The materials
at the top of the table will derive a positive charge when rubbed with any of the
materials below them.17
Cotton is a ﬁbre that has very good antistatic properties on its own and presents
few problems. This is because the natural water content of cotton is high (moisture
contents of around 8% are commonly quoted), which provides the ﬁbre with sufﬁ-
cient conductivity to dissipate any charge that might accumulate. However, with the
advent of synthetic ﬁbres, which had a low water content and were sufﬁciently non-
conductive to hold a static charge on the surface, severe static problems began to
arise. Thus some synthetics, particularly polyesters, can sustain such a high charge
density on the surface that it can actually ionise the air in the vicinity giving rise to
Finishing of technical textiles 169
7.18 Reactions of some permanent repellents.
7.19 Fluorocarbon showing polyacrylate backbone and perﬂuoro side chain.
a spark, which discharges the static that has been built up. In most cases this results
in a mild shock to the person experiencing this static discharge, but where explo-
sive gases might be present it can result in disaster.
Antistatic treatments, therefore, are based on the principle of making the ﬁbre
conductive so that high charge densities are dissipated before sparks can form. This
170 Handbook of technical textiles
Table 7.2 Common water repellent ﬁnishes
Finish Application method Trade names
Parafﬁn wax emulsion Spray Mystoline, Ramasit
Parafﬁn wax plus Al or Cr salt As above but lower Mystoline
Metal soap plus fatty acid Pad, dry, bake Persistol
Methylol stearamide Reactive resin, pad, dry, Phobotex
Pyridinium compounds Pad, dry, bake Velan (ICI), Zelan (Du Pont)
Reactive silicone resins Pad, dry, bake Silicone Finish (ICI)
Fluorocarbon emulsion Pad, dry, bake Zepel (Du Pont), Scotchgard
Table 7.3 The Triboelectric Series
Rayon and cotton
is done by the application of both anionic and cationic agents to the ﬁbre. Typical
structures of these materials are similar to the softening agents used for cotton,
which contain a long chain hydrocarbon with an ionic group at the end. One of the
most interesting advances in the ﬁeld of antistatic treatments has been the devel-
opment of the permanent antistatic ﬁnishes, one of which was the Permolose ﬁnish
developed by ICI. These are actually a series of ﬁnishes that consist of block copoly-
mers of ethylene oxide and a polyester. When polyester ﬁbres are treated with Per-
molose, the polyester block of the copolymer is adsorbed by the polyester ﬁbre but
the polyethylene oxide portion is incompatible with the polyester ﬁbre and thus
remains on the surface, where it attracts water and forms a conductive surface on
the polyester ﬁbre.
7.5.5 Antimicrobial and antifungal ﬁnishes
Problems of hygiene are coming more and more to the fore in textile ﬁnishing18 and
it is now generally realised that a microbiocidal ﬁnish is very valuable in certain
textiles for two reasons: as a prophylactic measure to avoid reinfections and as a
Perhaps at this stage it might be useful to deﬁne some of these terms:
Finishing of technical textiles 171
• Bacteriostatic: a chemical that inhibits the growth of bacteria. Fabric that has
been impregnated with a bacteriostat will stop the growth of germs, which
eventually die in time.
• Fungistatic: a chemical that inhibits the growth of fungi.
Bactericidal, fungicidal and microbicidal all mean that the chemical will kill these
three types of microorganism.
Here are just a few of the many microorganisms with the infections they cause:
• Staphylococcus aureus: found in mucus membranes, causes boils and abscesses
• Pseudomonas pyocyanea: causes spots and boils
• Trichophylon menagrophytes: fungus, which causes dermatomycosis of the feet
• Candida albicans: yeast-like mould which is the main cause of thrush and foot rot.
18.104.22.168 Areas of use
Microbicidal ﬁnishes are mainly used in textiles that are being handled continuously
by a large number of people. Locations where these are used include, hotels, hos-
pitals, asylums and student hostels, where mattress ticking, blankets and pillows,
7.20 Microbicidal ﬁnishes.
172 Handbook of technical textiles
carpets and upholstery all come into contact with a large number of different indi-
viduals. The following companies all manufacture microbiocide:
• Bayer: Movin
• Thomson Research Associates: Ultra-Fresh
• British Sanitised: Actifresh
• Sandoz: Antimucin
• Protex: Microcide
• Ciba-Geigy: Fungicide G.
Any one of the following methods can apply all these products:
• pad batch
The normal add on depends on the efﬁciency of the particular product, but add-on
weights of 1– 4% are commonly quoted. Some of these are shown in Fig. 7.20.
1. d gilbert, Nonwovens Report Int., 1998 327 21.
2. d behr, Knitting Technol., 1996 18(1) 311.
3. anon, Knitting Technol., 1999 (1) 29.
4. m a bueno et al., Textile Res. J., 1997 67(11) 779.
5. anon, Knitting Technol., 1999 (1) 29.
6. Sanfor Services, Tinctora, 1994 91(1) 37.
7. j w s hearle, in The Setting of Fibres and Fabrics, eds J W S Hearle and L W C Miles, Merrow
Publishing, Watford, Herts, 1971, 1–25.
8. s ranganathan, Colourage, 1985 32(25) 29.
9. w j morris, ‘The use of heat in the production of synthetic ﬁbre textiles’, Textiles, 1981 10(1) 1–10.
10. j s heaton, in The Setting of Fibres and Fabrics, eds J W S Hearle and L W C Miles, Merrow
Publishing, Watford, Herts, 1971, Chapter 8.
11. anon, Tessili per impieghi Tecnici, 1995 2(2) 25.
12. UK Furniture and Furnishings (Fire) (Safety) Regulations, The Home Ofﬁce 1988.
13. m e hall and a r horrocks, Trends Polym. Sci., 1993 1(2) 55.
14. m e hall and a r horrocks, Encyclopedia of Advanced Materials, ed Bloor et al., Pergamon Press,
Oxford, 1994, 231.
15. j kukula, ‘Progress in Textile Coating and Laminating’, BTTG conference, 2–3 July Manchester, 1990.
16. i holme, Wool Record, 1996 155(3618) 37.
17. v k joshi, Man made Textiles in India, 1996 39(7) 245.
18. j d payne and d w kudner, Textile Chemist and Colorist, 1996 28(5) 28.
Coating of technical textiles
Michael E Hall
Department of Textiles, Faculty of Technology, Bolton Institute, Deane Road, Bolton
BL3 5AB, UK
This chapter will deal with the chemistry of coatings and their application to various
coated technical textiles that are in use. It will leave the reader to make use of the
many excellent reviews, which are referenced in this article, for details of individ-
8.2 Chemistry of coated textiles
Coatings used in the production of technical textiles are largely limited to those
products that can be produced in the form of a viscous liquid, which can be spread
on the surface of a substrate. This process is followed by a drying or curing process,
which hardens the coating so that a non-blocking product is produced. Thus the
coatings for these products are limited to linear polymers, which can be coated as
a polymer melt or solution and on cooling form a solid ﬁlm or form a solid ﬁlm by
evaporation of the solvent. There are some types of coatings that can be applied in
the liquid form and then chemically crosslinked to form a solid ﬁlm.
The coatings used in technical textiles are all thermoplastic polymers, which
are long chain linear molecules, some of which have the ability to crosslink. The
properties of these polymeric materials directly inﬂuence the durability and
performance of the end product. Therefore, some description of these materials is
8.2.1 Polyvinyl chloride (PVC)
This polymer is manufactured from the free radical polymerisation of vinyl chlo-
ride as shown in Fig. 8.1.
The polymer is a hard rigid solid, which if it is to be used as a coating material
for technical textiles needs to be changed to a soft ﬂexible ﬁlm.1 This is possible
174 Handbook of technical textiles
8.1 Polyvinyl chloride.
because of a remarkable property of PVC, the ability of the powdered polymer to
absorb large quantities of non-volatile organic liquids. These liquids are known as
plasticisers and a typical plasticiser for PVC is cyclohexylisooctylphthalate. The
polymer can absorb its own weight of this plasticiser. However, when the powdered
polymer and plasticiser are ﬁrst mixed, a stable paste is formed which is easily
spreadable onto a textile surface. The paste of PVC and plasticiser, known as a
plastisol, consists of the partially swollen particles of PVC suspended in plasticiser.
When this mixture is heated to 120 °C complete solution of the plasticiser and
polymer occurs, which on cooling gives a tough non-blocking ﬁlm. The ﬂexibility of
this ﬁlm can be varied by the amount of plasticiser added. However, for most
uses plasticiser contents of up to 50% are most common. Plasticised PVC forms a
clear ﬁlm, which shows good abrasion resistance and low permeability. The ﬁlm may
be pigmented or ﬁlled with ﬂame-retardant chemicals to produce coloured pro-
ducts of low ﬂammability. The coatings are resistant to acids and alkalis but organic
solvents can extract the plasticiser, making the coatings more rigid and prone to
One great advantage of a polymer with an asymmetric chlorine atom is its large
dipole and high dielectric strength. This means that the coated product may be
joined together by both radiofrequency and dielectric weldings techniques. This
factor combined with its low price make it ideal for protective sheetings such as tar-
paulins, where the low permeability and good weathering properties make it a very
cost effective product.
8.2.2 Polyvinylidene chloride (PVDC)
PVDC is very similar to PVC. As in the case of PVC it is made by the
emulsion polymerisation of vinylidene chloride, as illustrated in Fig. 8.2.
The resulting polymer forms a ﬁlm of low gas permeability to gases, however,
the polymer is more expensive than PVC and therefore only tends to be used
where ﬂame resistance is required.2 As may be seen from the formula, PVDC
contains twice the amount of chlorine as PVC and this extra chlorine is used in
ﬂame-resistant coatings. When a ﬂame heats these materials the polymer produces
chlorine radicals which act as free radical traps, thus helping to snuff out the
8.2.3 Polytetraﬂuoroethylene (PTFE)
PTFE is perhaps the most exotic of the polymers which occur in coated textiles. It
is manufactured by the addition polymerisation of tetraﬂuoroethylene (Fig. 8.3).
Since its discovery by Du Pont in 1941, PTFE has found many uses in coating
particularly in the protection of fabrics from the harmful effects of sunlight.3
Coating of technical textiles 175
8.2 Polyvinylidene chloride.
One remarkable feature of the polymer is its very low surface energy, which means
that the surface cannot be wetted by either water or oil. Textile surfaces treated with
this polymer are both water repellent and oil repellent. Hence PTFE is found on
diverse substrates which range from conveyer belts used in food manufacture to
carpets where stain resistance is required. In addition the polymer shows excellent
thermal stability and may be used up to a temperature of 250 °C. It is resistant to
most solvents and chemicals, although it may be etched by the use of strong
oxidising acids; this latter fact may be used to promote adhesion. In many ways
PTFE could be regarded as an ideal polymer, the main drawback to its use being
its very high cost compared to the other coating materials.
In order to reduce the cost of ﬂuoropolymers several less expensive compounds
have been produced, such as polyvinyl ﬂuoride (PVF) and polyvinylidene ﬂuoride
(PVDF), which are analogous to the corresponding PVC and PVDC. However,
while these materials are similar to PTFE they are slightly inferior in terms of resist-
ance to weathering.
Natural rubber is a linear polymer of polyisoprene, found in the sap of many plants,
although the main source is the tree Hevea brasiliensis. Rubber occurs as an emul-
sion, which may be used directly for coating, or the polymer may be coagulated and
mixed at moderate temperatures with appropriate ﬁllers.4 The formula, see Fig. 8.4,
shows that the natural polymer contains unsaturated double bonds along the
The double bonds may be crosslinked with sulphur, a process known as vulcan-
isation, which can give tough abrasion-resistant ﬁlms or hard ebony-like structures.
The ﬂexibility of the rubber may be adjusted by the amount of crosslinking which
takes place. However, one great advantage of this process is that the rubber can
be mixed at high rates of shear with the appropriate compounding ingredients
and spread onto a textile, after which the coated textile is heated to vulcanise the
rubber compound. These principles are used in the production of tyres and belting,
where the excellent abrasion resistance of natural rubber makes it the material of
Unfortunately, the presence of a double bond makes the polymer susceptible to
176 Handbook of technical textiles
8.4 Polyisoprene (rubber).
8.5 Styrene–butadiene rubber (SBR).
oxidation. In addition, the polymer swells in organic solvents although it is unaf-
fected by water and dilute acids and alkalis. Natural rubber is far more sensitive to
both oxygen and ozone attack than the other synthetic materials which are
described in the next section.
8.2.5 Styrene–Butadiene Rubber (SBR)
SBR is made by the emulsion polymerisation of styrene and butadiene as illustrated
in Fig. 8.5.
The formula illustrated implies a regular copolymer but this is not the case and
SBR is a random copolymer. The compounding and application techniques are very
similar to those for natural rubber although the material is not as resilient as natural
rubber and also has a greater heat build-up, which make SBR inferior to natural
rubber in tyres. In the case of coated fabrics, the superior weatherability and ozone
resistance of SBR, combined with the ease of processing, make this the product of
choice. It is estimated that 50% of all rubber used is SBR.5
8.2.6 Nitrile rubber
Nitrile rubbers are copolymers of acrylonitrile and butadiene shown in Fig. 8.6.
These materials are used primarily for their excellent oil resistance, which varies
with the percentage acrylonitrile present in the copolymer and show good tensile
strength and abrasion resistance after immersion in oil or petrol. They are not suit-
able for car tyres but are extensively used in the construction of ﬂexible fuel tanks
and fuel hose.6
Coating of technical textiles 177
8.6 Nitrile rubber.
8.7 Butyl rubber.
8.2.7 Butyl rubber
Butyl rubbers are copolymers of isobutylene with a small amount of isoprene to
make the copolymer vulcanisable or crosslinked as illustrated in Fig. 8.7.
Because of the low amount of isoprene in the structure, the vulcanised structure
contains little unsaturation in the backbone and consequently the rate of oxidation
or oxygen absorption is less than that of other elastomers except for the silicones
and ﬂuorocarbons. When an elastomer contains double bonds, oxidation leads to
crosslinking and embrittlement, whereas in butyl rubbers oxidation occurs at the
tertiary carbon atom which leads to chain scission and softening. Further, the close
packing of the hydrocarbon chains leads to a structure which is impermeable to
gases and its main use is in tyre tubes and inﬂatable boats.7
8.2.8 Polychloroprene (neoprene)
Neoprene rubber was ﬁrst developed in the United States as a substitute for natural
rubber, which it can replace for most applications. It is made during the emulsion
polymerisation of 2-chlorobutadiene as illustrated in Fig. 8.8.
Neoprene rubbers can be vulcanised and show tensile properties similar to
natural rubber, however, they are perhaps most widely used for their excellent oil
resistance.8 Weathering and ozone resistance is good and the polymer ﬁnds its main
178 Handbook of technical textiles
8.8 Polychloroprene (neoprene).
8.9 Silicone rubbers. R1 and R2 are unreactive alkyl or aryl groups.
end-uses in the production of belts and hoses. The neoprene latex can also be used
in dipping and coating.
8.2.9 Chlorosulphonated polyethylene (Hypalon)
Treatment of polyethylene with a mixture of chlorine and sulphur dioxide in
solution yields a product in which some of the hydrogen atoms in the polyethylene
are replaced by chlorine and some by the sulphonyl chloride groups (—SO2Cl). The
resulting polymer can be crosslinked via the sulphonyl chloride by the use of metal
oxides. Typically the polymer will contain about one sulphur atom for every 90
carbon atoms in the polyethylene chain and about 25% by weight of chlorine.9
These products show good resistance to weathering and have excellent ozone
resistance, but they do have low elongation. Their main uses in coating are where
ﬂame resistance is required; here the synergism between sulphur and chlorine pro-
motes ﬂame retardancy.
8.2.10 Silicone rubbers
Silicone rubbers are polymers which contain the siloxane link Si—O—Si and are
formed by the condensation of the appropriate silanol which is formed from the
halide or alkoxy intermediate; the ﬁnal condensation then takes place by the elim-
ination shown in Fig. 8.9.
The groups R1 and R2 are normally inert groups such as methyl, but they may
include a vinyl group and therefore are capable of crosslinking. It is also normal to
ﬁll these polymers with ﬁnely divided silica, which acts as a reinforcing ﬁller.10
These polymers show outstanding low temperature ﬂexibility and can be used at
temperatures as low as -80 °C, while they retain their properties up to 250 °C. They
also show good resistance to weathering and oxidation. Unfortunately their price is
Polyurethanes are made by the reaction of a diisocyanate with a diol as shown in
The particular diisocyanate shown is 2,4-toluene diisocyanate and the diol is
Coating of technical textiles 179
pentane diol but any of the analogues may be used. Polyurethanes used for coating
textiles are not quite as simple as the one illustrated and the materials are frequently
supplied as an isocyanate-tipped prepolymer and a low molecular weight hydroxyl-
tipped polyester, polyether or polyamide. The two materials will react at room tem-
perature although this is often accelerated by raising the temperature. The only
drawback to this system is that once the components are mixed, crosslinking starts
immediately and so the pot life of the system is limited. Stable prepolymers which
contain a blocked diisocyanate usually as a bisulphite adduct are now available.
These blocked isocyanates will not react at room temperature, but will react at
elevated temperatures in the presence of organotin catalysts.
Polyurethane coatings show outstanding resistance to abrasion combined with
good resistance to water and solvents, in addition they offer good ﬂexibility. The
chemistry of the diol can be varied considerably so as to convey water vapour per-
meability to the coating. Coatings made from polyurethanes do have a tendency to
yellow on exposure to sunlight and they are therefore normally pigmented in use.
8.3 Coating techniques12
The original methods of coating were largely based on various impregnating tech-
niques based on an impregnating trough followed by a pair of squeeze rollers to
ensure a constant pick-up. The material was then air dried at constant width, usually
on a stenter, and rolled. However, when the coating was required on one side of the
fabric then total immersion of the fabric in the coating liquor was not possible and
other techniques had to be developed.
8.3.1 Lick roll
In this method the fabric was passed over the coating roll which was rotated in a
trough of the coating liquor as shown in Fig. 8.11.
There were several variations on this theme, which were developed to ensure a
180 Handbook of technical textiles
8.11 A lick roll.
8.12 Other lick roll methods. (a) A metering roll and (b) a knife doctor.
more even application of the coating by metering the coating onto the fabric. This
was done by two main approaches, the ﬁrst of which was to use a second roll on the
primary coating roll, which picked up a ﬁxed amount.The second was to use a doctor
blade on the primary roll, so that again only a ﬁxed amount of liquor was trans-
ferred to the fabric. These are also illustrated above in Fig. 8.12.
The main disadvantage of these systems was that the amount of coating on the
fabric was dependent on the surface tension and viscosity of the coating ﬂuid and
also the surface condition of the fabric. To overcome this problem knife coating was
developed, which functions in basically the same way that butter is spread on toast.
8.3.2 Knife coating
In this method the coating ﬂuid is applied directly to the textile fabric and spread
in a uniform manner by means of a ﬁxed knife. The thickness of the coating is
controlled by the gap between the bottom of the knife and the top of the fabric.
The way in which this gap is controlled determines the type of machinery used. The
following are the main techniques used:
• knife on air
• knife over table
• knife over roller
• knife over rubber blanket.
In the ﬁrst of these the spreading blade is placed in direct contact with the fabric
under tension and the coating compound is thus forced into the fabric. This is shown
in Fig. 8.13.
The main advantage of this technique is that any irregularities in the fabric do
not affect the running of the machine. However, this is not the case with the knife
over table or knife over roll methods (Fig. 8.14), for although the coating thickness
can be accurately controlled, any fabric faults or joints in the fabric are likely to jam
under the blade causing fabric breakage.
The problem of metering an accurate amount of coating onto the substrate was
ﬁnally solved by the use of a ﬂexible rubber blanket, which gives a controlled gap
for the coating compound and yet is sufﬁciently ﬂexible to allow cloth imperfections
or sewing to pass underneath the blade without getting trapped and causing break-
outs. This is shown in Fig. 8.15.
Coating of technical textiles 181
8.13 Knife on air.
8.14 Coating methods using (a) knife over table and (b) knife over roller.
8.15 Knife over blanket.
22.214.171.124 Knife geometry
The geometry of the coating knife and the angle of application also have an impor-
tant role to play in the effectiveness and penetration of the coating. Obviously if
uniform coatings are to be obtained over the width of the fabric then an accurately
machined ﬂat blade is mandatory. In addition the proﬁle of the knife can have a
marked inﬂuence on the coating weights and penetration of the coating. There are
three main types of knife proﬁle, illustrated in Fig. 8.16 with many variations in
between these three:
• Pointed blade: the sharper the blade the more of the coating compound is
scraped off and consequently the lower the coating weight.
• Round blade: this gives a relatively higher coating weight than a sharp point.
• Shoe blade: this gives the highest coating of all the blade proﬁles; the longer the
length of the shoe the higher the coating weight.
In general knife coating ﬁlls in any irregularities in the fabric surface giving a smooth
ﬁnish to the coated surface. The machines which use knife coating are in general
simple to operate and can be used for a wide variety of thicknesses from about
1 mm up to 30 mm.
182 Handbook of technical textiles
8.16 Three blade proﬁles.
126.96.36.199 Air knife coating
In discussing knife coating, mention must also be made of the air knife as a method
of removal of the excess coating ﬂuid. In this technique a blast of air is used to blow
off the excess coating ﬂuid. The viscosity of the ﬂuid is much lower than in the case
of conventional knife doctoring and the coating applied follows the proﬁle of the
substrate to which it is being applied. The technique is more frequently used in the
paper industry, where it is used to coat photographic paper, rather than in the textile
8.3.3 Gravure coating
The use of a gravure roller in coating was developed from the printing industry,
where it was used to print designs. The technique involves the use of a solid roller,
the surface of which has been engraved with a closely packed series of small hemi-
spherical depressions. These act as metering devices for the coating ﬂuid, which ﬁlls
the hemispheres with coating ﬂuid from reservoirs of the ﬂuid. The excess ﬂuid is
scraped from the roll with a doctor blade, leaving the depressions with an exact
amount of ﬂuid in each. This is then transferred to the substrate to be coated. The
quantity of ﬂuid transferred depends on the volume of the engraved depressions
and the packing on the surface of the roll. However this technique is perhaps the
most accurate, in terms of the applied coating weight, of all the techniques discussed.
The greatest drawback to this technique is that for a ﬁxed depth of engraving a ﬁxed
coating weight is obtained. Thus if a different coating weight is required then a new
engraved roll has to be produced. Further, unless the viscosity characteristics of the
coating ﬂuid are controlled, the pattern of the printed dot can be seen on the coated
substrate. What is required is a printing ﬂuid that will ﬂow and form a ﬂat surface
in the drying process. This formation of a ﬂat coating can be greatly improved by
the use of offset gravure printing. Here the ﬂuid is printed onto a rubber roller
before being transferred onto the substrate.
8.3.4 Rotary screen coating
This technique is similar to the rotary screen printing process that is used to apply
coloured patterns to fabric. The applicator is a cylindrical nickel screen, which has
Coating of technical textiles 183
a large number of perforated holes. The coating compound is fed into the centre of
the screen, from whence it is forced through the holes by either a doctor blade or
a circular metal rod. The coating weight can be controlled by the number of holes
per unit area and the coating weights are very precise. However, the coatings have
a dot conﬁguration and to obtain a continuous coating a wiper blade that spreads
the dots into a continuous coat must be used. The two companies associated with
this type of coating are Stork Brabant BV, whose system uses a metal doctor blade,
and Zimmer, whose system uses the circular metal rod.
8.3.5 Hot-melt coating
In this technique the coating materials must be thermoplastic, so that they melt
when heated and in this condition are capable of being spread onto a textile sub-
strate. Thus, in some respects they are similar to paste coating. However, the big
difference from paste coating is that the thermoplastic coating has no solvents to
evaporate and no water that has to be evaporated, giving the process both economic
and ecological advantages. The molten polymer is usually calendered directly onto
the textile or in some cases extruded directly from a slotted die. This is followed by
contact with a polished chill roller, if a smooth surface is required on the coating or
a patterned roll if a patterned effect is required.
One further process, the use of powdered polymers as a coating medium, needs
to be mentioned in the area of hot-melt coating. In this technique the powdered
polymer is sprinkled onto the substrate, followed by heating with radiant heaters to
melt the thermoplastic. The coating is then compacted and rendered continuous by
a compaction calender. The main materials used in this are polyethylenes and nylon
and these are now being applied in the production of carpets for car interiors, where
because of the mouldability of the thermoplastic, a complete car carpet may be
pressed out in one operation.
8.3.6 Transfer coating
The ﬁnal coating technique to be described in this section is transfer coating. In
this the coating material is preformed into a continuous sheet which is laminated
to the substrate either by the application of heat or by the use of an adhesive known
as a tie coat. The great advantage of this technique over all the others is that
the coating ﬁlm may be made completely free of holes and defects before it is
applied to the fabric. In general, transfer coating will give the softest coating
of all coating techniques in terms of fabric handle and furthermore there is
no possibility of the coating bleeding through onto the face of the coated
8.4 Fusible interlinings
Fusible interlinings13 represent an important ﬁeld in technical textiles and as such
deserve a special mention. A fusible interlining is a fabric that has been coated with
184 Handbook of technical textiles
an adhesive coating, which under the inﬂuence of heat and pressure will melt and
form a bond with any other fabric that is pressed against it.
The basic function of a fusible interlining is to control and reinforce the fabric
to which it is fused. It does this by giving a degree of stiffness to the fabric by increas-
ing the apparent thickness of the fabric, causing the ﬂexural modulus of the fabric
to increase proportionally to the cube power of that thickness. Thus a relatively
small increase in thickness will produce a relatively large increase in the stiffness of
The use of stiffening materials in clothing has been known for many thousands of
years. From the tomb drawings in Egypt, for example, we can see how these mate-
rials were used to accentuate the rank or social status of the wearer. The Eliza-
bethans used both linen and woven animal hair to reinforce and stiffen the elaborate
clothing of the court ladies and gentlemen. This material had to be laboriously sewn
into the garments by hand but as long as labour was cheap and servants in plenti-
ful supply, it did not present any problem to the upper classes of the time. The cost
of producing these ‘hand made’ garments was, of course, beyond the reach of any
but the moneyed classes and it was not until the development of mechanised
methods of garment production and the use of fusible interlinings that it became
possible for the man or woman in the street to be able to afford a suit, which carried
both elegance and style. Thus it became no longer possible to tell a gentleman by
the cut of his jacket.
8.4.3 Development of adhesives
The ﬁrst synthetic resin to be developed for clothing applications is usually attrib-
uted to Alexander Parkes, who at the Great Exhibition of 1862 introduced a nitro-
cellulose plasticised with camphor, which he called, with all due modesty, Parkesine.
This material was a thermoplastic and could thus be moulded by heat and pressure.
It was also found that the material was unaffected by water and it was used in the
Victorian era for the manufacture of cheap collars and cuffs. Eventually it was given
the name ‘celluloid’ and its use was extended into many areas. It was, for example,
the original material on which the early moving pictures were shot. Unfortunately,
celluloid had one major disadvantage, it was highly ﬂammable and burned with an
almost explosive violence. This prompted the search for a less ﬂammable alterna-
tive to celluloid.
The beginning of the 20th century saw the development of another thermoplas-
tic resin from cellulose, cellulose acetate. Benjamin Liebowitz in the USA devel-
oped the use of this material in fusible interlinings. He developed a fabric that
consisted of both cotton and cellulose acetate woven together. It could be softened
in acetone, which produced a very sticky fabric that was used to reinforce the collar
of a man’s shirt. The Trubenised Process Corporation exploited this invention pro-
ducing the Trubenised semi-stiff collar, which was washable. Because the cellulose
acetate adhesive did not form a continuous glue line in the collar, the collar
remained permeable and hence very comfortable to wear. The result was that many
millions of men’s shirts with Trubenised collars were made in the thirty years from
Coating of technical textiles 185
Table 8.1 Typical coating resins
Low density polyethylene Poor Very good
High density polyethylene Very good Very good
PVA/Novolac Fair Fair
PVC/plasticised Good Good
Polyamide Very good Good
Polyester Very good Very good
Reactive Very good Very good
8.4.4 Modern adhesive development
In the early 1950s a search began for a fusible adhesive resin which could be coated
onto the base fabric and fused by the action of heat and pressure alone, thus avoid-
ing the use of ﬂammable and toxic solvents. The ﬁrst of these was obtained by the
plasticisation of polyvinyl acetate, which was applied to the fabric in the form of a
knife coating by an emulsion of plasticised PVA. After the material was dried the
coated fabric was wrapped in a release paper for use. The fused products were stiff
and were used in the preparation of fabric belts for ladies dresses and suits; this is
still their main use.
However, the continuously coated fabrics used as fusibles produced laminates
that were rather too stiff for normal clothing use. The use of these materials
would have remained in the special belting product, had it not been for the
development of the powdered adhesive, for when this was used as a fusible inter-
lining, the resultant stiffness of the laminate could be controlled by the particle
size of the adhesive powder and by the amount of powder in the glue line of the
laminate. The powder had to be applied to the interlining in an even manner and
much thought went into development of machinery to ensure that this was so. The
main resins used for these coatings are shown in Table 8.1. However, the most recent
development has been the introduction of a reactive adhesive resin. This material
melts when heated and then undergoes crosslinking, thus producing a very stable
The initial coatings produced were known as sinter or scatter coatings. New
coating techniques were then developed and reﬁned by more precise positioning of
the adhesive dot, so that the handle of the fused product could be more accurately
controlled. This led to the printing of the adhesive in dot form which can be done
either by a paste print through a mesh screen, or by the use of a gravure roller.
All these interlinings are fused by the application of heat and pressure in an elec-
trically heated press, which has developed from the original ﬂat bed system of
heated platens to the continuous roller bed presses of the present day.
No discussion on interlinings would be complete without mention of laminating, as
this is the ultimate use of these materials. In general, textile laminates are produced
by the combination of two or more fabrics using an adhesive. The hot-melt adhe-
186 Handbook of technical textiles
sive is environmentally friendly, requires less heat and is now preferred over the
more conventional solvent-based adhesives.14 Flame bonding using a thin layer of
polyurethane foam is still being used in some applications, where the bulky appear-
ance of the ﬁnal product is required by the market. However, strict legislation con-
cerning the gaseous efﬂuent from this process has most manufacturers searching
for alternatives that are more environmentally acceptable. It seems likely that hot-
melt adhesives will replace most of the other adhesive techniques, either on energy
grounds, or environmental grounds. The other driving force behind this change is
the continued development of the hot-melt adhesives that are available to the man-
ufacturer, which produce laminates at a higher speed, or more permanently bonded
An interesting development in the improved efﬁciency of the process, for
example, was the development of Xironet.15 This is a lightweight net of fusible
adhesive, which when sandwiched between two fabrics can effectively laminate the
fabrics together by the application of heat and pressure from a heated calender.
To improve the permanence of the adhesive bond, and as mentioned above, a
hot-melt adhesive has been developed that will crosslink after the adhesive bond
has been formed.16 These materials will melt at 130 °C and form an adhesive bond
and on further heating will crosslink to give an adhesive that is relatively inert.
1. j a brydson, Plastics Materials, Iliffe Publishers, 1966.
2. t tasidim, Textile Asia, 1980 11 169.
3. anon, High Performance Textiles, 1993 February 11.
4. b g crowther, Natural Rubber Technol., 1980 11(4) 69.
5. m m hirschler and r r poletti, J. Coated Fabrics, 1984 19 94.
6. j r williams, Am. Assoc. Industrial Hygiene Quart., 1980 41 884.
7. n ellerbrok, US Patent No. 5,375,878.
8. j o stull, Industrial Fabrics Products Rev., 1996 72(12) 42–46.
9. anon, Du Pont Magazine, 1991 85(1) 1–3.
10. f bohin et al., J. Coated Fabrics, 1998 27 326.
11. k krishnan, J. Coated Fabrics, 1995 25 103.
12. f a woodruff, ‘Coating and laminating techniques’, Clemson University Presents – Industrial Textiles,
Conference at Clemson University USA, 28th January 1998.
13. anon, World Clothing Manufacturer, 1996/7 Dec–Jan 77(10) 48.
14. i holme, Textile Horizons, 1997 June/July 35–38.
15. g peltier, ‘Environmentally friendly dry thermoplastic adhesive ﬁlms and webs for industrial bonding
applications’, 2nd International Conference on Textile Coating and Laminating: Assessing Environ-
mental Concerns, Charlotte, USA, Technomic 1992.
16. d farrell, ‘Reactabond – A reactive response to industry’, 8th International Conference on Textile
Coating and Laminating, November 9–10, Frankfurt, Technomic 1998.
Coloration of technical textiles
School of Textile Industries, University of Leeds, Leeds LS2 1JT, UK
Technical textiles are used in a very wide variety of end-uses in which the functional
performance requirements are paramount. Thus, technical textiles must possess the
requisite physical and mechanical properties to maintain the structural integrity
throughout all the manufacturing and fabrication processes and during the service
life of the material. For some end-uses, therefore, coloration is not strictly necessary
because the aesthetic properties of the technical textile, for example colour and
pattern, and also lustre, texture, handle and drape, may not always be required to
appeal to the visual and tactile senses of the customer.
Coloration of technical textiles by dyeing or printing is primarily intended for
aesthetic reasons but also provides a ready means of identifying different qualities
or ﬁneness of the materials. For example, the ﬁneness of a surgical suture and its
visibility at the implant site are easily identiﬁed by colour. High visibility clothing
and camouﬂage printing clearly provide the extreme ends of the coloration spec-
trum for technical textiles.
Coloration also introduces other functional properties distinct from the aesthetic
appeal of colour. Colorants can hide ﬁbre yellowing and aid ﬁbre protection against
weathering, both factors of importance where the physical properties of the tech-
nical textile must be maintained over a long service life under adverse end-use
conditions.1 Heat absorption is also increased where black materials are exposed to
sunlight, an important factor for baling materials for agriculture.
9.2 Objectives of coloration
The objectives of coloration treatments are ﬁrst to produce the desired colour in
dyeing and colours in the coloured design image in printing on the technical textile.2
Second, coloration treatments are to ensure that the necessary colour fastness
requirements for the end-use are achieved. Third, the whole operation should be
188 Handbook of technical textiles
carried out at the lowest cost commensurate with obtaining the desired technical
performance. After dyeing, the levelness and uniformity of colour across the width
and along the length of a technical textile fabric must be within the deﬁned colour
tolerances agreed between the dyer and the customer prior to coloration. Preser-
vation of the original appearance and quality of the technical textile prior to
coloration is also essential in order to ensure that the technical textile is of mar-
9.3 Coloration of technical textiles
Coloration involves the application of colorants to the technical textile and is a
complex ﬁeld because of the variety of ﬁbres, ﬁlaments, yarns, fabrics and other
materials requiring coloration and the diverse nature of the end-use and per-
formance requirements. Coloration may be carried out by dyeing the materials to a
uniform colour, or by printing to impart a design or motif to the technical textile.
Fibres, yarns and fabrics may also be multicoloured by specialised dyeing techniques,
for example space dyeing, or by weaving or knitting different coloured yarns.3
The colorants used may be either water-soluble (or sparingly water-soluble) dyes,
or alternatively water-insoluble pigments.4 Most dyes are applied to technical tex-
tiles in an aqueous medium in dyeing and in printing, although selected disperse
dyes may also be dyed in supercritical ﬂuid carbon dioxide (above the critical point
under very high pressure) for a few specialised end-uses, for example polyester
sewing threads.5 By contrast, pigments are either physically entrapped within the
ﬁlaments during synthetic ﬁbre extrusion, for example by mass pigmentation, to give
a spun-dyed ﬁbre,6 or alternatively adhered to technical textiles in pigment printing
through the use of an adhesive binder.7
Dyeing is normally carried out on textile materials from which surface impu-
rities, for example ﬁbre lubricants, spin ﬁnishes, sizes, particulate dirt or natural
colouring matters and so on, have been removed by appropriate pretreatments
(e.g. by desizing and scouring), and to which a stable whiteness has been imparted
by chemical bleaching.8 However, many synthetic ﬁbres do not normally require
chemical bleaching prior to coloration because the ﬁbres may be whitened by
incorporation of a ﬂuorescent brightening agent during ﬁbre manufacture.
Printing may be carried out mainly on technical fabrics that may be in their
natural state, or chemically bleached, or whitened with a ﬂuorescent brightening
agent, or after tinting or dyeing. Conventional dyeing and particularly printing are
most conveniently and economically carried out on fabrics, which also allow greater
ﬂexibility through the selection of colours late in the technical textile production
sequence to meet the varying market requirements.
The dyes used commercially to dye technical textiles may be selected from the very
wide range of synthetic organic colorants, based upon aromatic compounds derived
from petroleum.4 Dyes are conjugated organic structures containing an alternating
system of single and double bonds within the molecule which impart the ability to
absorb certain wavelengths of visible light, so that the remaining light scattered by
the dyed technical textile is perceived as coloured.4,9
Coloration of technical textiles 189
The dye structure must contain a chromophore, a chemical group that confers
upon a substance the potential to becoming coloured, for example nitro, nitroso, azo
and carbonyl groups. To become a useful dye, however, the molecule should contain
other chemical groups such as amino, substituted amino, hydroxyl, sulphonic or
carboxyl groups which are called auxochromes. These generally modify or intensify
the colour, render the dye soluble in water and assist in conferring substantivity of
the dye for the ﬁbre.4,9 High substantivity aids a high degree of dye exhaustion on
to the ﬁbres during exhaust dyeing when dyes are progressively and preferentially
adsorbed by the ﬁbres from the dyebath to give coloured technical textile ma-
terials. High dye-ﬁbre substantivity also generally confers high colour fastness
during end-use, for example high colour fastness when exposed to washing and light.
Manufactured dyestuffs are formulated colorants typically containing only
30–40% active colorant. The rest of the dyestuff formulation consists of diluents to
dilute the colour strength, electrolytes to improve the dye exhaustion on the ﬁbre,
and dispersing agents to facilitate dispersing of the dye in the dyebath.10 To avoid
dusting dyestuffs into the air during weighing and dispensing, granular, grain or
pearl forms of dyestuffs are used. Antidusting agents are added to powdered
dyestuffs for the same reason. Water-soluble dyes can be produced as true liquid
dyestuffs (e.g. basic dyes), but liquid dispersions of disperse and vat dyestuffs
are also produced. The latter may contain a viscosity modiﬁer to minimise sedi-
mentation/settling of the dye particles during storage and must be stirred prior to
use. Liquid dyestuffs are preferred for continuous dyeing and for printing because
of their convenience for use on automated weighing, metering and dispensing
Commercial dyestuffs are subjected to stringent quality control procedures for
hue and colour strength, average particle size and particle size distribution, and are
dried to a uniform moisture content and packaged in drums or plastic containers
suitable for transportation, storage and dispensing.10,11 Resealable packaging may
be used to prevent the ingress of moisture from the atmosphere, and in many colour
kitchens the ambient temperature and relative humidity are controlled in order to
maintain reproducibility in weighing. Some dyestuffs are mixtures formulated for
speciﬁc shades such as black, or contain dyes from different application classes suit-
able for dyeing speciﬁc ﬁbre blends, for example 65/35 polyester/cellulosic ﬁbre
Pigments are synthetic organic or inorganic compounds that are insoluble in water,
although some are soluble in organic solvents.4,9 The pigment particles are ground
down to a ﬁne state of subdivision (0.5–2 mm) and stabilised for use by the addition
of dispersing agents and stabilisers. Both powder and liquid (i.e. dispersions of) pig-
ments are used for the coloration of technical textiles, and the pigment ﬁnish must
be compatible with the application conditions used in mass pigmentation of manu-
factured ﬁbres or in pigment printing of technical textile fabrics.13,14
9.3.3 Fluorescent brightening agents
These are organic compounds that absorb some of the ultraviolet radiation in
sunlight or other sources of illumination and re-emit in the longer wavelength
190 Handbook of technical textiles
Table 9.1 Percentage distribution of each chemical class between major application ranges
Distribution between application ranges (%)
Acid Basic Direct Disperse Mordant Pigment Reactive Solvent Vat
Unmetallised azo 20 5 30 12 12 6 10 5
Metal complex azo 65 10 12 13
Thiazole 5 95
Stilbene 98 2
Anthraquinone 15 2 25 3 4 6 9 36
Indigoid 2 17 81
Quinophthalone 30 20 40 10
Aminoketone 11 40 8 3 8 30
Phthalocyanine 14 4 8 4 9 43 15 3
Formazan 70 30
Methine 71 23 1 5
Nitro, nitroso 31 2 48 2 5 12
Triarylmethane 35 22 1 1 24 5 12
Xanthene 33 16 9 2 2 38
Acridine 92 4 4
Azine 39 39 3 19
Oxazine 22 17 2 40 9 10
Thiazine 55 10 10 25
Source: see ref 4.
blue–violet region of the visible spectrum.15–17 Such compounds can be applied to
technical textiles either by mass pigmentation (in manufactured ﬁbres) or via
machinery used for conventional dyeing of all types of materials, and add bright-
ness to the whiteness obtained from chemical bleaching of the textile.
9.3.4 Range of colorants available
The Colour Index International is the primary source of information on colorants
and lists the majority of commercial dyestuffs and pigments (both past and present)
although the situation continually changes as the manufacture of some colorants
ceases, to be replaced by new products.18 The wide variety of colorants available is
based upon many chemical types that make up the major application groups of col-
orants.The percentage distribution of each chemical class between major application
ranges is illustrated in Table 9.1, based upon all the dyes listed where the chemical
class is known, but also including products which are no longer used commercially.4
Azo colorants make up almost two-thirds of the organic colorants listed in the
Colour Index International. Anthraquinones (15%), triarylmethanes (3%) and
phthalocyanines (2%) are also of major importance. Where the structure of the col-
orant is known, it is assigned a speciﬁc CI (Colour Index) chemical constitution
number, although for many new commercial products the structure is undisclosed.
In the Colour Index International dyes are classiﬁed by application class, by colour
and by number, for example CI Acid Blue 45. The commercial name of the dyestuff
will, however, vary according to the dye maker, and dyestuffs, being formulated prod-
ucts, although nominally the same CI number, may vary in active colorant content
and in the nature of the additives incorporated within the formulation.19 Metamerism
may also be observed on the dyed textile, that is a difference in colour is observed
when two colours are viewed under different illumination conditions, even when
using dyestuffs that nominally possess the same colour index number. The Colour
Index International is available in book form and on CD–ROM.
Coloration of technical textiles 191
Table 9.2 Major classes of dyes and the ﬁbres to which they are applied
Dye class Major ﬁbre type
Acid (including 1 : 1 and 1 : 2 Wool, silk, polyamides (nylon 6, nylon 6.6)
metal complex dyes)
Mordant (chrome) Wool
Azoic Cellulosic ﬁbres (cotton)
Direct Cellulosic ﬁbres (cotton, viscose, polynosic, HWM, modal,
cuprammonium, lyocell ﬁbres), linen, ramie, jute and
other lignocellulosic ﬁbres
Reactive Cellulosic ﬁbres (cotton, viscose, polynosic, HWM, modal,
cuprammonium, lyocell, linen, ramie, jute), protein (wool,
Sulphur Cellulosic (cotton)
Vat Cellulosic ﬁbres (cotton, linen)
Basic Acrylic, modacrylic, aramid
Disperse Polyester, cellulose triacetate, secondary cellulose acetate,
polyamide, acrylic, modacrylic, polypropylene, aramid
HWM = high wet modulus.
The major classes of dyes and the ﬁbres to which they are applied are illustrated
in Table 9.2. The type of dyestuff used for dyeing technical textiles depends upon
the ﬁbre(s) present in the material, the required colour and the depth of colour, the
ease of dyeing by the intended application method and the colour fastness perfor-
mance required for the end-use. Some dyestuff classes will dye a number of differ-
ent ﬁbres, but in practice one ﬁbre will predominate. For example, disperse dyes are
mainly used to dye polyester ﬁbres, although they can also be applied to nylon 6,
nylon 6.6, acrylic, modacrylic, secondary cellulose acetate, cellulose triacetate and
polypropylene ﬁbres, but with limitations upon the depth of colour and the colour
fastness that can be attained.20
There are, however, many types of manufactured ﬁbres, particularly synthetic
ﬁbres, which are currently virtually impossible to dye with conventional dyestuffs
using normal dye application methods. This is because ﬁlaments which are designed
for high strength end-uses are often composed of polymer repeat units that do not
contain functional groups that could act as dyesites (e.g. polyethylene, polypropy-
lene, polytetraﬂuoroethylene), and/or may be highly drawn to produce a highly
oriented ﬁbre with a high crystallinity.21
Because dyes are considered to diffuse in monomolecular form into the ﬁbre only
through non-crystalline regions, or regions of low order (i.e. high disorder), it follows
that highly oriented ﬁbres such as meta-aramid, para-aramid, and high strength
polyethylene ﬁbres, are extremely difﬁcult to dye. In some cases, specialised dyeing
techniques utilising ﬁbre plasticising agents (‘carriers’) to lower the glass transition
temperature (Tg) of the ﬁbre (i.e. the temperature at which increased polymer seg-
mental motion opens up the ﬁbre structure) together with selected dyes may be
employed to speed up the diffusion of dyes into the ﬁbres, but the colour depth may
be restricted to pale-medium depths.21–23 In addition, or alternatively, resort may be
made to high temperature dyeing in pressurised dyeing machinery at temperatures
in the range 130–140 °C for the same purpose.
192 Handbook of technical textiles
However, for many high strength ﬁbres, mass pigmentation offers a more satis-
factory production route to coloured ﬁbres, provided that the introduction of the
pigments does not signiﬁcantly impair the high strength properties.6 Some ﬁbres
such as carbon ﬁbres and partially oxidised polyacrylonitrile ﬁbres cannot be dyed,
simply because they are already black as a result of the ﬁbre manufacturing process.
However, contrasting colours may be printed on such ﬁbres using pigment printing
methods, or by blending with other dyed ﬁbres.
Microﬁbres are generally deﬁned as ﬁbres or ﬁlaments of linear density less than
1 dtex.24 Such silk-like ﬁbres pose considerable difﬁculties for level dyeing of
medium to heavy depths of colour. The high surface area per unit volume of microﬁ-
bres increases the light scattering, necessitating the use of greater amounts of
dye to achieve the same colour depth as on coarser ﬁbres. The use of bright trilobal
ﬁlaments, or the incorporation of titanium dioxide delustring agents within
the microﬁbres increases the light scattering, making the difference even more
9.4 Dye classes and pigments
9.4.1 Acid dyes
Acid dyes are anionic dyes characterised by possessing substantivity for protein
ﬁbres such as wool and silk, and also polyamide (e.g. nylon 6 and nylon 6.6) ﬁbres,
or any other ﬁbres that contain basic groups. Acid dyes are normally applied from
an acid or neutral dyebath.24
As the size of the acid dye molecule generally increases from level dyeing (or
equalising) acid dyes to fast acid, half-milling or perspiration-fast dyes to acid
milling dyes and thence to supermilling acid dyes, the colour fastness to washing
increases because of the increasing strength of the non-polar forces of attraction for
the ﬁbre.26 1 : 1 Metal complex and 1 : 2 metal complex dyes also behave like acid
dyes from the viewpoint of application to the ﬁbre, and possess good colour fast-
ness to washing and light. Level dyeing acid dyes yield bright colours, while the
larger sized milling acid and supermilling acid dyes are progressively duller. 1 : 1 and
1 : 2 metal complex dyes also lack brightness, but can provide good colour fastness
Acid dyes contain acidic groups, usually sulphonate groups, either as —SO3Na or
—SO3H groups, although carboxyl groups (—COOH) can sometimes be incorpo-
rated. Wool, silk and polyamide ﬁbres contain amino groups (—NH2) which in an
acid dyebath are protonated to yield basic dyesites (—NH3+). The acid dye anion
D.SO3-, where D is the dye molecule, is thus substantive to the ﬁbre and is adsorbed,
forming an ionic linkage, a salt link, with the ﬁbre dyesite. Monosulphonated acid
dyes can be adsorbed to a greater extent than di-, tri-, and tetrasulphonated acid
dyes because the number of basic dyesites in the ﬁbres is limited by the ﬁbre struc-
ture. Thus, the colour build-up is generally greatest with monosulphonated dyes on
wool. However, the dyestuff solubility in water increases with the degree of dye
Dyed wool ﬁbre quality is improved by pretreatment before dyeing with Valsol
LTA-N(TM), an auxiliary which extracts lipids from the cell membrane complex of
wool, thereby speeding up the intercellular diffusion of dyes.28 In this Sirolan (TM)
Coloration of technical textiles 193
LTD (low temperature dyeing) process, wool may be dyed for the conventional time
at a lower temperature, or for a shorter time at the boil, decreasing ﬁbre degrada-
tion in the dyebath.
Levelling agents may be used to promote level dyeing of acid dyes on wool and
other ﬁbres.29 Anionic levelling agents enter the ﬁbre ﬁrst and interact with basic
dyesites, restricting dye uptake. Amphoteric levelling agents, which contain both a
positive and a negative charge, block the basic dyesites in the ﬁbre but also complex
with the acid dyes in the dyebath, slowing down the rate at which the dyes exhaust
on to the ﬁbres. As the dyebath temperature is increased, the anionic (or ampho-
teric) levelling agent desorbs from the ﬁbres, allowing the dye anions to diffuse and
ﬁx within the ﬁbre. In addition, as the dyebath temperature is raised, the dye/ampho-
teric levelling agent complex breaks down, releasing dye anions for diffusion inside
the ﬁbre. The dyes are thus gradually adsorbed by the wool as the dyebath tem-
perature is increased.
In the iso-ionic region (pH 4–5), the cystine (disulphide) crosslinks in the wool
are reinforced by salt links formed between charged carboxyl and amino groups in
opposing amino acid residues in adjacent protein chain molecules within the wool
ﬁbre. This temporarily strengthens the wool and the abrasion resistance of the dyed
fabric is improved. Fibre yellowing is decreased and brighter colours may be dyed.30
The build-up of acid dyes on silk and polyamide ﬁbres is limited by the fewer
number of ﬁbre dyesites compared with wool. Acid dyes are attracted to the amine
end groups (AEG) in polyamide ﬁbres such as nylon 6 and nylon 6.6. Nylon 6 has
a more open physicochemical structure and a lower glass transition temperature
(Tg) compared with nylon 6.6. Thus, acid dyes diffuse more readily into nylon 6 but
the colour fastness to washing of a similar dye on nylon 6.6 will generally be su-
perior because of the more compact ﬁbre structure.31 False twist texturing processes,
which use contact heating of the yarns, open up the ﬁbre structure and may modify
some of the ﬁbre cross-sections which were in contact with the heater, resulting in
a slightly lower colour fastness to washing.
Chemical variations due to changes in the AEG of nylon ﬁbres, can give rise to
dyeability variations with acid dyes, a problem often referred to as barré or barri-
ness.31 Physical variations caused by temperature and/or tension differences in nylon
ﬁbres can similarly lead to differences in the uptake of disperse or 1 : 2 disperse
premetallised dyes. Physical variations can be minimised by dyeing at higher tem-
peratures (e.g. up to 120 °C) with nylon 6.6, or prolonging the dyeing time. High
temperature dyeing is used with the larger 1 : 2 metal complex acid dyes in order to
achieve better ﬁbre levelling and also ﬁbre penetration, which leads to improved
colour fastness to washing. Acid dyes can also be printed on to wool (which has
been pretreated by chlorination), degummed silk, polyamide and other ﬁbres using
conventional print thickeners in a print-dry-steam ﬁxation-wash off and dry
Colour fastness to washing with acid dyes on nylon ﬁbres, especially nylon
microﬁbres, is improved by after-treatments such as syntanning, that is, the adsorp-
tion of a sulphonated synthetic tanning agent that provides a physical barrier to
desorption by blocking the ﬁbre pore structure in the ﬁbre surface regions and by
providing electrostatic (ionic) repulsion to dye desorption.31 Combining an appro-
priate syntan with a ﬂuorochemical treatment can provide, in addition, stainblock-
ing properties.33 However, syntan treatments degrade during high temperature or
steaming treatments and tend to yellow the dyed fabric, dulling the colour.
194 Handbook of technical textiles
9.4.2 Mordant dyes
Chrome dyes are the only type of mordant dye of any commercial signiﬁcance.26
These are used in exhaust dyeing to dye wool or occasionally polyamide ﬁbres to
deep dull colours of high colour fastness to wet treatments and light. The ﬁbres are
usually dyed by the afterchrome method in which a chrome dye (similar to an acid
dye) is dyed on to the ﬁbre and then the dyed ﬁbre is given a treatment at pH 3.5
in a second bath containing sodium or potassium dichromate.34 The absorption of
dichromate ions leads to the formation of a 1 : 1 and/or 1 : 2 chromium metal complex
dye inside the ﬁbre, which can lead to some problems in batch-to-batch repro-
ducibility of shade, particularly if the pH control in chroming is variable. Low
chrome dyeing procedures can promote exhaustion of the chromium on to the
ﬁbres, decreasing environmental pollution from the waste water from dyeing.26,34 A
major disadvantage of the afterchrome method is that the ﬁnal colour is not
developed until the chroming stage which can give difﬁculties in shade matching.
Ammonia aftertreatment can improve the colour fastness to washing.
9.4.3 Basic dyes
Basic dyes are cationic dyes characterised by their substantivity for standard acrylic,
modacrylic, basic-dyeable polyester and basic-dyeable nylon ﬁbres.24 Basic dyes can
be applied to protein and other ﬁbres, for example secondary cellulose acetate, but
the light fastness of basic dyes on hydrophilic ﬁbres is poor.35 The major outlets for
basic dyes are acrylic and modacrylic ﬁbres, on which basic dyes can impart bright
colours with considerable brilliance and ﬂuorescence. The ionic attraction between
the basic dye and the sulphonic acid dyesites in acrylic ﬁbres is strong, which yields
high colour fastness to washing. The close-packed physicochemical nature of acrylic
ﬁbres and the strong dye-ﬁbre bonding can result in poor migration and levelling
properties during dye application, but impart very high colour fastness to light.21,35
Acrylic ﬁbres vary widely in their dyeability because of the different amounts of
different co-monomers used with poly(acrylonitrile) that modify the ﬁbre glass tran-
sition temperature. This may range from 70–95 °C according to the source of the
acrylic ﬁbre manufacturer.36 Cationic retarders are widely used on acrylic and
modacrylic ﬁbres to promote level dyeing and the basic dyes used should prefer-
ably be selected with the same compatibility value. The compatibility value may
range from 5 (slow diffusing) down to 1 (rapid diffusing). A compatibility value of
3 has been recommended for package dyeing, but for printing, compatibility values
are of much less importance. Print ﬁxation is by the print-dry-steam-wash off and
dry process, although wet transfer printing techniques are also possible using
The acidic dyesites in acrylic ﬁbres become much more accessible over a narrow
band of temperatures in the glass transition temperature range. Therefore, even
when using cationic retarders, which initially adsorb on to the ﬁbre blocking the
dyesites, the dyebath temperature must be raised slowly through this temperature
range to allow the cationic retarder to desorb slowly and allow the basic dye to
be adsorbed uniformly.35,36 Alternatively, constant temperature dyeing methods may
be used in exhaust dyeing. Continuous pad-steam-wash off and dry methods can
also be used for dyeing acrylic fabrics.
The basic dye uptake is limited by the number of acidic dyesites in the ﬁbre, but
approximately 95% of all colours on acrylic ﬁbres are dyed using basic dyes.
Coloration of technical textiles 195
However, where very pale colours are to be dyed it is common to use disperse dyes,
which have superior migration and levelling properties, in order to attain a level
dyeing, because the strong dye-ﬁbre bonding renders this very difﬁcult to achieve
using basic dyes.35 The build-up of disperse dyes on acrylic ﬁbres is limited and
the colour fastness to washing and light are generally lower than for basic dyes. The
colour fastness of basic dyes on acrylic ﬁbres is superior to similar dyeings on
modacrylic ﬁbres. Some modacrylic ﬁbres are prone to delustring during dyeing and
may require relustring by boiling for 30 min in a high concentration of electrolyte
(e.g. 50–200 g l-1 sodium chloride) or by dry-heat or treatment in saturated steam.36
9.4.4 Azoic colouring matters
Azoic colouring matters are formed inside the ﬁbre (usually cellulosic ﬁbres)
generally by adsorption of an aromatic hydroxyl-containing compound, such as a
naphthol or naphtholate (azoic coupling component) followed by coupling with a
stabilised aromatic diazonium compound (the azoic diazo component also termed
fast base or salt) to form a coloured insoluble azo compound.2,37 The application
method has to be carried out with care and the ﬁnal colour is only obtained after
soaping off to remove any traces of the azoic dye on the ﬁbre surface that would
give inferior colour fastness to washing and rubbing (crocking). Although they are
economical for the production of red and black, the colour range is now more
limited as some diazo components based upon certain aromatic amines have been
withdrawn because of their possible carcinogenic nature. Precise colour matching
with such a complex two-bath procedure can also give problems in practice.
9.4.5 Direct dyes
Direct dyes were the ﬁrst class of synthetic dyes to dye cotton directly without
the use of a mordant. Direct dyes are sulphonated bisazo, trisazo or polyazo dyes
and are anionic dyes which are substantive to cellulosic ﬁbres when applied from
an aqueous bath containing an electrolyte.2,38 Direct dyes based on stilbene, copper-
complex azo, oxazine, thiazole and phthalocyanine structures are also used. Less
bright in colour than acid or basic dyes, the brightness diminishes with the mol-
ecular complexity of the dye. Phthalocyanine dyes are used for very bright blue and
turquoise-blue colours of good colour fastness to light, and copper-complex azo dyes
also exhibit good fastness to light, although these dyes yield relatively dull colours.
Electrolyte, in the form of sodium sulphate, is usually added into the dyebath to
overcome the negative charge on the cellulosic ﬁbre surface which otherwise would
repel the approach of the direct dye anions. The sodium cations from the electrolyte
neutralise the negative charge at the ﬁbre surface, allowing the dye anions to be
adsorbed and retained within the ﬁbre.38
Coulombic attraction, hydrogen bonding and non-polar van der Waals forces
may operate depending upon the speciﬁc direct dye and the ﬁbre structure. Direct
dyes are normally linear and planar molecules allowing multipoint attachment to
cellulose chain molecules, but the forces of attraction between dye and ﬁbre are
relatively weak when the dyed ﬁbre is immersed in water.38,39 Thus, the colour
fastness to washing is moderate to poor, but the colour fastness to light may vary
from excellent to poor depending on the molecular structure.
The colour fastness to washing can be improved by aftertreatment of the dyed
196 Handbook of technical textiles
ﬁbre, originally by the use of after-coppering (i.e. treatment with copper sulphate to
form a metal-complex direct dye) or by diazotisation and development. Both
approaches lead to a pronounced shade change and copper in the waste water from
dyeing is environmentally undesirable. Modern aftertreatments make use of
cationic ﬁxatives that may simply complex with the anionic dye, and/or form a metal
complex and/or react with the cellulose ﬁbre hydroxyl groups to form strong cova-
lent bonds. Improvement in colour fastness to washing may be accompanied by
some diminution in colour fastness to light.38,40
Direct dyes may be used on all cellulosic ﬁbres and selected dyes may also be
used to dye wool, silk and nylon ﬁbres in the manner of acid dyes. Addition of elec-
trolyte into the dyebath increases dye aggregation in the dyebath. As the dyeing
temperature is increased, the dye aggregation decreases, releasing individual direct
dye anions for diffusion and adsorption inside the ﬁbre. Direct dyes have been sep-
arated into three classes, Class A – salt-controllable, Class B – temperature-
controllable, and Class C – both salt- and temperature-controllable. It is normal to
select compatible dyes from within the same class, but selected dyes from Class A
and B, and Class B and C may be dyed together in the same dyebath in exhaust
dyeing. Direct dyes may also be applied to cellulosic fabrics by continuous pad-
steam-wash off and dry methods.2,38
The depth of colour obtained using direct dyes is deeper on viscose, lyocell and
high wet modulus ﬁbres and on mercerised cotton compared with bleached cotton,
and careful dye selection is required to produce level, solid colours when dyeing
blends of these ﬁbres.
9.4.6 Reactive dyes
Reactive dyes, sometimes termed ﬁbre-reactive dyes, are a very important class of
dyes for dyeing cellulosic ﬁbres41 and are also used to dye protein ﬁbres such as
wool42 or silk.43 Although relatively expensive they provide a wide colour gamut of
bright colours with very good colour fastness to washing. This is because during dye
ﬁxation, usually conducted under alkaline conditions, strong covalent bonds are
formed between the dye and the ﬁbre.2,44 Reactive dyes may react by substitution
(e.g. monochlorotriazinyl and dichlorotriazinyl dyes) or by addition (e.g. vinylsul-
Typical ranges of reactive dyes and their respective reactive groups are illustrated
in Table 9.3. Recent developments have led to the introduction of homobifunctional
reactive dyes (e.g. two monochlorotriazine groups) and heterobifunctional reactive
dyes (e.g. using monochlorotriazine plus vinyl sulphone) in an attempt to increase
the dye ﬁxation on the ﬁbre under alkaline conditions from 50–70% with one reac-
tive group, to 80–95% with two reactive groups. Dye application methods on fabrics
include exhaust dyeing, cold pad-batch-wash off or continuous pad-steam-wash off
and dry methods. Fixation by dry heat, saturated steam or superheated steam may
also be used according to the type of reactive dye employed.41
Reactive dyes hydrolyse in contact with water and alkali, and during dyeing some
hydrolysed reactive dye is adsorbed by the ﬁbre because it behaves like a substan-
tive direct dye, but with lower colour fastness to washing than the reactive dye that
is covalently bonded. Thus, the dyeing stage must always be followed by an extended
washing-off treatment to remove hydrolysed reactive dye.41,45 Provided that the
residual hydrolysed reactive dye left within the cellulosic ﬁbre after dyeing or print-
Coloration of technical textiles 197
Table 9.3 Important reactive dye systems
System Typical brand name
Dichlorotriazine Procion MX (BASF)
Aminochlorotriazine Procion H (BASF)
Aminoﬂuorotriazine Cibacron F (Ciba)
Trichloropyrimidine Drimarene X (Clariant)
Chlorodiﬂuoropyrimidine Drimarene K (Clariant)
Dichloroquinoxaline Levaﬁx E (DyStar)
Sulphatoethylsulphone Remazol (DyStar)
Sulphatoethylsulphonamide Remazol D (DyStar)
Bis(aminochlorotriazine) Procion H-E (BASF)
Bis(aminonicotinotriazine) Kayacelon React (Nippon Kayaku)
Aminochlorotriazine–sulphatoethylsulphone Sumiﬁx Supra (Sumitomo)
Aminoﬂuorotriazine–sulphatoethylsulphone Cibacron C (Ciba)
Source: see ref 41.
ing is at a concentration <0.1 g m-2, the best colour fastness to washing will be
obtained.46 If the concentration of hydrolysed reactive dye in the ﬁnal hot wash bath
is <0.003 g l-1, staining of white grounds in the fabric will be prevented.46
Generally reactive dyes are produced in granular form, but vinyl sulphone dyes are
also available as liquids, which are more convenient for use in continuous dyeing and
printing.Reactive dyes are sulphonated and highly water soluble and are exhausted on
to the ﬁbre using electrolyte (e.g. in the manner of direct dyes) and ﬁxed using an
appropriate alkali. The high water solubility creates an environmental problem in
waste water treatment plants because generally only 0–30% of the hydrolysed reactive
dye is removed by such treatment.47 Low salt reactive dyes have also been introduced
to decrease dyeing costs and to avoid corrosion problems in concrete waste water
pipework networks caused by high concentrations of sulphate anions.
9.4.7 Sulphur dyes
Sulphur dyes are chemically complex and are prepared by heating various aromatic
diamines, nitrophenols, and so on with sulphur and sodium sulphide. Sulphur dyes
are produced in pigment form without substantivity for cellulose.2 Treatment with
a reducing agent (e.g. sodium sulphide or sodium hydrosulphide) in an alkaline
dyebath converts the sulphur dye into an alkali-soluble reduced (leuco) form with
substantivity for cellulosic ﬁbres. Once absorbed within the ﬁbre, the dye is then
oxidised, usually with hydrogen peroxide, back to the insoluble pigment form.
Soaping off after dyeing is important to ensure the maximum colour fastness to
washing and rubbing is obtained.2,48
Sulphur black and navy are the major dyestuffs used and the colour gamut is
limited to dull colours of moderate colour fastness to washing and light. The
colour fastness to chlorine and to bleach fading is poor when using multiple
wash cycles with detergents containing low temperature bleach activators such as
TAED (tetraacetylethylenediamine, UK) or SNOBS (sodium nonanoyloxyben-
zenesulphonate, USA).49 Sulphur dyes cost less than many other dyes but the waste
198 Handbook of technical textiles
water from dyeing may require specialised treatment before release to a conven-
tional waste water treatment plant.
9.4.8 Vat dyes
Vat dyes are water-insoluble, but contain two or more keto groups (>C==O)
separated by a conjugated system of double bonds that are converted into alkali-
soluble enolate leuco compounds (>C—O-) by alkaline reduction, a process called
vatting.2,50 The dye application method involves three stages, namely, alkaline
reduction and dissolution of the vat dye (normally using sodium hydroxide and
sodium dithionite (hydrosulphite)), absorption of the substantive leuco compound
by the ﬁbre, aided by electrolyte (e.g. sodium sulphate and wetting, dispersing
and levelling agent), followed by regeneration of the vat dye inside the ﬁbre by oxi-
dation in air or hydrogen peroxide. The dyed ﬁbre is then thoroughly soaped off
(washed with soap or special detergent at a high temperature) to remove any surface
dye and to complete any dye aggregation inside the ﬁbre in order to obtain the ﬁnal
Vat dyes are based upon indanthrone, ﬂavanthrone, pyranthrone, dibenzan-
throne, acylaminoanthraquinone, carbazole, azoanthraquininone, indigoid and
thioindigoid structures.2,50 Application methods include both batch exhaust dyeing
and continuous pad-steam-wash off and dry methods, and apart from sodium
dithionite, formaldehydesulphoxylate or hydroxyacetone may be used for the reduc-
Vat dyes are relatively expensive but do offer outstanding colour fastness to light
and washing on cellulosic ﬁbres. In the unreduced form some vat dyes behave like
disperse dyes and can therefore be applied to polyester and polyester/cellulosic
blends to achieve pale-medium colour depths. For polyester/cellulosic fabrics a
pad-dry-bake-chemical pad-steam-oxidise-wash off and dry production sequence is
used. For exhaust dyeing, the novel technique of electrochemical reduction dyeing
has been claimed to provide a redox potential of up to -960 mV suitable for the
reduction of vat dyes and also sulphur dyes. Cathodic reduction of vat dyes with the
addition of a mediator (a soluble reversible redox system, e.g. an iron [II/III]–
amino complex) could potentially decrease the chemical costs for reduction and
lower the chemical load in the waste water by 50–75%.51
9.4.9 Disperse dyes
Disperse dyes are substantially water-insoluble dyes which have substantivity for
one or more hydrophobic ﬁbres (e.g. secondary cellulose acetate) and are usually
applied as a ﬁne aqueous dispersion.2,52,53 The major chemical classes used are
aminoazobenzene, anthraquinone, nitrodiphenylamine, styryl (methine), quinoph-
thalone and benzodifuranone-based dyes. Disperse dyes are milled (ground) with a
dispersing agent (e.g. polymeric forms of sodium dinaphthylmethane sulphonates)
to a ﬁne dispersion (0.5–2 mm) and may be supplied as grains, powders or liquid
Disperse dyes are essentially nonionic dyes that are attracted to hydrophobic
ﬁbres such as conventional polyester, cellulose triacetate, secondary cellulose
acetate and nylon through non-polar forces of attraction.33,52,53 In the dyebath, some
of the disperse dye particles dissolve to provide individual dye molecules that are
Coloration of technical textiles 199
Disperse dye Dyebath
Dye dispersion in the bath
Dye solubility in the bath
Dye diffusion in the bath Dye migration in the bath
Dye adsorption on the ﬁbre Dye desorption from the ﬁbre
Dye diffusion into the ﬁbre
9.1 General dyeing mechanism for disperse dyes (source: see ref 35, p. 126).
small enough to diffuse into the hydrophobic ﬁbres. The aqueous solubility of dis-
perse dyes is low, for example 0.2–100 mg l-1 at 80 °C, but increases with increase in
dyebath temperature, in turn increasing the concentration of soluble dye available
for diffusion so that the dyeing rate increases.
Dispersing agents are essential because they assist in the process of decreasing
the dye particle size and enable the dye to be prepared in powder and liquid forms.52
In addition, the dispersing agent facilitates the reverse change from powder to
dispersion during dyebath preparation and maintains the dye particles in ﬁne dis-
persion during dyeing. This prevents agglomeration of the dye particles in powder
form and aggregation in the dyebath. The dye solubility in the dyebath can be
increased by the use of levelling agents and carriers.
The general mechanism of dyeing with disperse dyes under exhaust dyeing con-
ditions is illustrated in Fig. 9.1. The diffusion and adsorption of dye molecules is
accompanied by desorption of some of the dye molecules from the dyed ﬁbre back
into the dyebath, to facilitate dye migration from ﬁbre to ﬁbre to achieve level
dyeing.35 The disperse dyes are considered to dye ﬁbres via a solid solution mecha-
nism that involves no chemical change.23 Each disperse dye dissolves in the ﬁbre
more or less independently of any other disperse dye present. Under constant
dyebath conditions the ratio of the amount of dye on the ﬁbre to the amount of dye
in the bath is a constant at equilibrium, which varies according to the particular dye,
but ultimately a separate different saturation level (or solubility limit) is achieved
for each dye above which no more of that dye can be taken up by the ﬁbre. However,
most commercial dyeings are never carried out to equilibrium.
Apart from high temperature (high pressure) exhaust dyeing at 110–140 °C, dis-
perse dyes may also be exhaust dyed using carriers (e.g. ﬁbre plasticising agents that
decrease the ﬁbre Tg) at 100 °C.22,52,53 This method is not very popular except where
blend dyeing is practised and where high temperature dyeing, if used, would degrade
one of the ﬁbres. Odourless carriers are preferred, but there are problems with
carrier spotting, and carrier retention by the ﬁbres leads to fuming of the carrier
as it is volatilized off during post-heat setting treatments, while some carriers may
200 Handbook of technical textiles
potentally pose environmental pollution problems.22 Some 50% of disperse dye con-
sumption is used for navy and black shades, and some 70% of disperse dyes are
applied to polyester and polyester/cellulose blends by exhaust dyeing.54
Disperse dyes may also be applied by a pad-dry-thermoﬁx-wash-dry process in
a continuous open width fabric treatment. This utilises the sublimation properties
of disperse dyes, which vaporise directly from the solid state without prior melting.
Polyester can be dyed at 190–220 °C by such a process, originally called the Ther-
mosol process by DuPont.23 Sublimation of disperse dyes is also utilised in dry-heat
transfer printing,55 but conventional print application by printing and ﬁxing in
saturated or superheated steam is also practised, followed by washing off and
To minimise potential problems linked to the presence of disperse dyes on the
ﬁbre surface after dyeing (e.g. poor colour fastness to washing, rubbing and ther-
momigration), reduction clearing after dyeing with sodium hydroxide, sodium
dithionite (hydrosulphite) and a surfactant followed by hot washing is normally
practised, particularly with medium-heavy depths of colour.52 However, some
classes of disperse dyes (e.g. di-ester and thiophene azo dyes) are clearable by alkali
9.4.10 Pigment formulations
The range of chemical compounds used as pigments varies widely and includes both
inorganic pigments such as titanium dioxide, and the oxides of antimony, iron and
zinc, as well as carbon.57 Organic pigments may be based upon a very wide variety of
chemical structures, for example azo, anthraquinone, dioxazine, indanthrone, isoin-
dolinone, perylene, quinacridone, copper phthalocyanine, heterocyclic nickel com-
plexes and many others (see, for example, Table 9.4).58 The general considerations
relating to the manufacture of pigments and their application to technical textiles
are separately discussed in Section 9.3.2 (manufacture), Sections 9.5.1–9.5.3 (mass
pigmentation), Section 9.5.5 (coating) and Section 9.9.1 (printing). The ﬁnishing of
pigment formulations is technically complex and strict quality control is required to
ensure satisfactory application and performance of the pigment in practice.
9.5 Mass coloration of manufactured ﬁbres
9.5.1 Dyes and pigments for mass coloration
In mass coloration, dyes or pigments are incorporated into the polymer melt (in the
case of polyamide, polyester and polypropylene) or into the polymer solution (in
the case of viscose, secondary cellulose acetate, cellulose triacetate and acrylic or
modacrylic ﬁbres) during ﬁbre manufacture.6,13 The dyes that are being used pass
into a dissolved phase on incorporation into the polymer melt or solution, but pig-
ments remain as ﬁnely dispersed particles. In the main, mass pigmentation is much
more widely used for colouring manufactured ﬁbres (both synthetic and regener-
ated ﬁbres)6,13 except on wet-spun acrylic ﬁbres, where gel dyeing is used (see
Section 9.5.4).35,59 However, mass pigmentation can be used for dry-spun acrylic
polymers which are dissolved in a solvent (e.g. dimethyl formamide) and spun into
Technical criteria that are important for mass coloration include:13
Coloration of technical textiles 201
Table 9.4 High performance pigments for polypropylene ﬁbres
CI generic name CI number Chemical class
CI Pigment Yellow 93 20710 Azo condensation
Yellow 95 20034 Azo condensation
Yellow 109 56284 Isoindolinone
Yellow 110 56280 Isoindolinone
Yellow 155 Not known Azo condensation
Yellow 181 11777 Monoazo
Yellow 182 Not known Heterocyclic monoazo
Orange 61 11265 Isoindolinone
Red 122 73915 Quinacridone
Red 144 20735 Azo condensation
Red 149 71137 Perylene
Red 166 20730 Azo condensation
Red 177 65300 Anthraquinone
Red 202 Not known Quinacridone
Red 214 Not known Azo condensation
Red 242 20067 Azo condensation
Red 257 Not known Heterocyclic nickel complex
Violet 19 73900 Quinacridone
Violet 23 51319 Dioxazine
Violet 37 51345 Dioxazine
Blue 15:3 74160 Copper phthalocyanine
Blue 60 69800 Indanthrone
Green 7 74260 Copper phthalocyanine
CI denotes Colour Index. Source: see ref 58.
• pigment particle size and particle size distribution, both in the spinning mass and
in the ﬁlament
• pigment preparations
• solubility of the colorant in the spinning mass
• colour fastness properties
• ability to remain stable under the mass processing conditions of the polymer.
Fine pigment particles (<1 mm) are required because coarse particles would
interfere with the ﬁlterability of polymer solutions or melts and could impair the
tensile strength of ﬁbres, the diameter of which normally lies in the range 16–45 mm.
The pigments used must have good resistance to organic solvents and good heat
stability for use in ﬁbre manufacture.
Products suitable for the bath dyeing and mass coloration of manufactured ﬁbres
are illustrated in Table 9.5.13
9.5.2 Mass coloration methods
There are four main methods of incorporating colorants into manufactured ﬁbres,
which depend upon the speciﬁc ﬁbre production process.6,13 These are:
• batch process
• injection process
• chip blending
• chip dyeing.
202 Handbook of technical textiles
Table 9.5 Products for the bath dyeing and mass coloration of manufactured ﬁbres
Fibre Bath dyes Solvent dyes and pigments for mass coloration
Viscose Direct Aqueous pigment pastes
Acetate Disperse Acetone-soluble dyes
Pigment dispersions in acetate
Acrylic Disperse Pigment dispersions in polyacrylonitrile
Polyamide Disperse Aqueous dyes
Acid Polymer-soluble dyes
Polyester Disperse Polymer-soluble dyes
Pigment dispersions in polyester
Polypropylene Acid chelatable Pigment dispersions in various carriers
Source: see ref 13.
Pigment preparations or solvent dyes may be used in the batch method in which the
whole of the spinning mass is coloured, the colorant concentration being equal to that
in the coloured ﬁlament after extrusion. In the injection process, a coloured concen-
trate is continuously metered into the spinning mass which is then extruded. Chip
blending is suitable only for melt coloration,for example for polyamide,polyester and
polypropylene. Polymer chips are homogeneously mixed with the colour concentrate
prior to extrusion. Chip dyeing is a more specialised technique used with nylon 6.The
polymer chips are precoloured with polymer-soluble dyes and then melt spun.13
Mass pigmentation is widely used as the major coloration route for polypropy-
lene ﬁbres.1,6,13 The ﬂexibility of the smaller scale nature of polypropylene ﬁbre
manufacture compared with the large continuous polymerization/extrusion pro-
cesses for polyamide and polyester ﬁbres, the lower polymer melt temperature of
polypropylene and the difﬁculties in dyeing this hydrophobic, low linear density
ﬁbre in conventional dyeing equipment, ensure that mass pigmentation is the major
coloration route. Mass coloration of many other melt-spun ﬁbres is not economic
unless large ﬁbre weights per colour may be spun for a known end-use, because of
the high costs of cleaning out the production machinery to avoid subsequent colour
contamination problems. However, attempts continue to ﬁnd a satisfactory con-
ventional dyeing method for modiﬁed polypropylene ﬁbres using exhaust dyeing or
continuous dyeing techniques.1,60
9.5.3 Mass coloration and colour fastness properties
The colour fastness properties of manufactured ﬁbres produced by mass dyeing, and
particularly by mass pigmentation, are generally superior to those obtained on tech-
nical textiles by conventional dyeing and printing. Mass pigmentation is used where
high colour fastness to light and weathering is required, for example in tenting
fabrics, awnings, sun blinds, carpets, synthetic sports surfaces and so on, and where
the colour can be economically produced.
The organic pigments and a few inorganic pigments used for mass pigmentation
of polyester and polypropylene ﬁbres must exhibit:58
Coloration of technical textiles 203
• sufﬁcient thermal stability
• colour fastness to light, adequate for the intended end-use
• no migration (no blooming or contact bleed)
• compatibility with other additives, e.g. the UV stabilisers widely used in
polyoleﬁns, with no photodegradation effects on the polymer
• no adverse effect on the mechanical properties of the ﬁbres.
High performance organic pigments are used for brilliant colours and good overall
colour fastness performance on polypropylene ﬁbres (see Table 9.4).
Inorganic pigments such as titanium dioxide (rutile), zinc oxide, and antimony
oxide are used for white, and carbon (small particle size channel black) is used for
black, while some iron oxide browns are used for cost reasons. The tensile strength
of mass-pigmented polypropylene ﬁbres after 300 hours exposure in an Atlas
600 WRC accelerated light fastness testing equipment is markedly higher than
the uncoloured ﬁbre, demonstrating the protective effect of the presence of the
pigments against the deleterious effects of ultraviolet radiation on the ﬁbres.58
Colour retention in awning fabrics in outdoor applications is critical, and two
types of climatic conditions are most critical where pigments are incorporated
within acrylic and modacrylic technical textiles:61
• hot and dry (typically 38–49 °C, relative humidity <20%) with high average
• warm and humid (32–38 °C, relative humidity >70%) with average sunshine.
In hot and dry conditions, both the polymer and the pigment may degrade, whereas
in warm and humid conditions pigment degradation is more likely. However,
pigments that are degraded and fade under warm and humid conditions may often
be quite stable under hot dry conditions.
9.5.4 Gel dyeing of acrylic ﬁbres
For wet-spun acrylic ﬁbres, the manufacture of producer-dyed ﬁbres involves the
passage of acrylic tow in the gel state (i.e. never-dried state) through a bath con-
taining basic dyes.35,59 This is utilised in the Courtelle Neochrome process (formerly
Courtaulds, now Acordis) to produce dyed acrylic ﬁbres from a continuous ﬁbre
production line typically at a speed of 50 m min-1 with economic batch weights per
colour of 250–500 kg.
The liquid basic dyes are metered in at a rate appropriate to the acrylic tow
mass and speed, the recipe being based on a computerised colour match prediction
system allowing the selection of a very wide range of colours using a choice of the
technically best dyes (i.e. easiest to apply and highest colour fastness), or lowest
cost dyes, or least metameric dyes.62 As the freshly coagulated acrylic tow passes
through the dyebath, the basic dyes diffuse inside the gel-state acrylic tow in a
matter of seconds. The dyed tow is then drawn and steamed, crimped and cut to the
appropriate staple length for use in technical textiles, or may be used alternatively
in ﬁlament form.59
9.5.5 Pigments for technical coated fabrics
Many technical textiles are coated in order to provide the high performance speci-
ﬁcation demanded by the end-use. The many considerations governing the use of
204 Handbook of technical textiles
coloured organic pigments in coatings, and the range of pigments available, have
been reviewed by Lewis.63
9.6 Conventional dyeing and printing of technical textiles
9.6.1 Pretreatments prior to conventional coloration
Before ﬁbres, yarns or fabrics are to be dyed via batch exhaust or continuous
pad-ﬁxation methods, or printed by print-dry-steam-wash off-dry or pigment
print-dry-cure methods, it is important to remove any natural, added, or acquired
impurities from the ﬁbres in order that these impurities do not interfere with
coloration. Natural ﬁbres such as cotton, wool, silk and ﬂax (linen) ﬁbres contain
appreciable quantities of impurities naturally associated with the ﬁbres, which are
removed by scouring and by other treatments, for example degumming of silk to
remove sericin (gum) and carbonizing of wool to remove vegetable matter (e.g.
burrs, seeds etc.).64 Particularly important for cotton and ﬂax (linen) ﬁbres is the
efﬁcient removal of the natural waxes present mainly on the ﬁbre surface, in order
to impart hydrophilicity to the ﬁbres, thereby ensuring satisfactory wetting out,
with high levels of uniformity and reproducibility in subsequent dyeing or printing
Manufactured ﬁbres and ﬁlaments, that is, artiﬁcial ﬁbres from synthetic or
regenerated ﬁbres, are produced under carefully controlled conditions so that
water-soluble/emulsiﬁable spin ﬁnishes or ﬁbre lubricants are the main impurities,
and these are simply removed by scouring.64
For many woven or knitted technical fabrics, it may be necessary to singe the fabric
surface, by passage through a gas ﬂame or an infrared zone at open width, to remove
protruding surface ﬁbres. This gives a clear fabric surface and more uniform col-
oration, because a hairy fabric surface can impart a lighter coloured surface appear-
ance (termed frostiness) after dyeing or printing. Singeing may be integrated with
subsequent wet processes such as desizing.66
The warp yarns of most woven fabrics are generally sized with a ﬁlm-forming
polymer that adheres ﬁbres together with a more cohesive structure.67 Sizes are used
to increase yarn strength, decrease yarn hairiness and impart lubrication to staple
ﬁbre warp yarns in order to minimise the number of warp breaks during weaving.
In the weaving of synthetic continuous ﬁlament yarns, the size provides good inter-
ﬁlament binding to prevent ﬁlament snagging as well as providing yarn lubrication
and antistatic performance to decrease the build-up of electrostatic charges on the
yarns during high speed weaving. Yarns for knitting are not sized and a desizing
treatment is not therefore required.
All sizes, together with any other sizing components, for example waxes, soften-
ers and lubricants that may be hydrophobic, must be removed by appropriate desiz-
Coloration of technical textiles 205
ing treatments.68 Synthetic water-soluble sizes, (e.g. acrylates, polyvinyl alcohol) may
be simply removed by washing, whereas natural sizes, (e.g. starch, modiﬁed starch)
may require chemical degradation treatments, like oxidation, hydrolysis and so on.
If considered appropriate, desizing may be integrated with scouring, or with scour-
ing and bleaching to provide a shorter integrated treatment, while in large, verti-
cally integrated plants, undegraded sizes that are removed in desizing may be
recycled using ultraﬁltration and reused.
After every desizing treatment, all traces of size or degraded size are removed
by thorough washing followed by efﬁcient mechanical removal of liquid water (e.g.
hot mangling or vacuum extraction). This is followed by thermal drying on steam
heated cylinders (called cylinder or can drying) or by hot air drying on a stenter
(also known as a tenter, or frame (USA)).
Scouring is a critical treatment for natural cellulosic ﬁbres, for example cotton and
ﬂax (linen) and their blends with other ﬁbres, because all traces of hydrophobic
waxes (whether naturally occurring or applied during the manufacturing sequence)
must be effectively removed in order to achieve satisfactory wetting in all subsequent
dyeing, printing, ﬁnishing, coating, lamination and bonding operations.65 Scouring is
normally accomplished by hot alkaline treatment (e.g. sodium hydroxide) followed
by a thorough hot wash off. It is also important for the removal of fatty materials from
wool and any manufactured ﬁbres using hot detergent solutions.
Fibres must be uniformly white if pale colours or bright colours are required, and
hence natural ﬁbres such as cotton, silk, wool and linen must be chemically bleached
in order to achieve a satisfactory stable whiteness.8,64 Hydrogen peroxide under con-
trolled alkaline conditions is normally used in pad-steam-wash off, pad-batch-wash
off or immersion bleaching treatments, although other oxidising agents such as per-
acetic acid, cold alkaline sodium hypochlorite or sodium chlorite under acidic con-
ditions may also be used.
However, chlorine-based bleaching agents give a poor bleaching environment
and chlorine is retained by the ﬁbre, necessitating an antichlor aftertreatment with
a reducing agent (e.g. sodium sulphite) followed by washing to remove any resid-
ual odour in the fabric. Retained chlorine from chlorine-based bleaches or from
chlorinated water used for dyeing can give rise to shade changes when dyeing cotton
with reactive dyes. Regenerated cellulosic ﬁbres such as viscose, cuprammonium,
polynosic, modal, high wet modulus and lyocell ﬁbres are marketed by the ﬁbre pro-
ducers with a satisfactory whiteness for dyeing and printing.
9.6.6 Fluorescent brightening
If high whites are required, both natural and regenerated cellulose ﬁbres may be
chemically bleached and treated with a ﬂuorescent brightening agent.15,16 Fluores-
cent brightening agents are based upon diaminostilbene derivatives, triazoles,
aminocoumarins and many other organic compounds, and are absorbed by the ﬁbre.
206 Handbook of technical textiles
Fluorescent brightening agents are organic compounds that absorb the ultraviolet
radiation present in daylight and re-emit light in the blue–violet region of the visible
spectrum. During the absorption and re-emission processes, some energy is lost and
hence the light emitted is shifted to a longer wavelength. The effect is to add bright-
ness to the whiteness produced by chemical bleaching. Alternatively, blue tints may
be used, for example ultramarine.
Mercerization of cotton is a ﬁbre swelling/structural relaxation treatment that may
be carried out on yarns, but more usually on fabrics.69,70 Hank or warp merceriza-
tion of yarns often creates dyeability differences because of yarn tension variations
that pertain during mercerization. During mercerization in 22–27% caustic soda
solution, both mature and immature cotton ﬁbres swell so that the secondary wall
thickness is increased. The ﬁbre surface appearance and the internal structure of the
ﬁbre are modiﬁed. This improves the uniformity of fabric appearance after dyeing
and there is an apparent increase in colour depth after mercerization which has
been claimed to give cost savings of up to 30% on pale colours (1–2% dye owf, on
weight of fabric) and even 50–70% on heavy depths when using some reactive
dyes.71,72 Dead cotton ﬁbres (i.e. those with little or no secondary wall) are, however,
not improved after mercerization.
Woven fabric mercerization is normally carried out under tension on chain or
chainless fabric mercerizing ranges,70 whereas tubular fabric mercerizing ranges are
widely used for weft knitted cotton fabrics.73 Mercerization leads to a number of
changes in ﬁbre and fabric properties:69–73
• a more circular ﬁbre cross-section
• increased lustre
• increased tensile strength, a major factor for technical textile fabrics
• increased apparent colour depth after dyeing
• improved dyeability of immature cotton (greater uniformity of appearance)
• increase in ﬁbre moisture regain
• increase in water sorption
• improved dimensional stability.
After mercerization, the structure of native cotton ﬁbres, cellulose I, is converted
into cellulose II which is the stable ﬁbre form after drying.72 The sorptive capacity
of mercerized cotton is greater where the fabric is mercerized without tension
(slack mercerizing) to give stretch properties to the fabric. An increase in drying
temperature can also decrease the sorptive capacity, especially at temperatures
above 80 °C.74
9.6.8 Anhydrous liquid ammonia treatments
This form of cotton fabric pretreatment is much less common than mercerizing
and is most widely used in Japan.72,75 Impregnation in anhydrous liquid ammonia at
-38 °C in an enclosed machine followed by a swelling/relaxation stage, and removal
of the ammonia by thermal drying and steaming, converts the cellulose I crystalline
form back to either cellulose I or into cellulose III, depending upon the structural
collapse of the ﬁbre while the ﬁnal traces of ammonia are removed in the steamer.
Coloration of technical textiles 207
This ammonia-dry-steam process can be used to give better improvements in cotton
fabric properties than mercerization, although the increase in colour depth after
dyeing is usually somewhat lower than that achieved after mercerization. The high
capital cost of the machinery for anhydrous liquid ammonia treatment and ammonia
recovery, and environmental considerations, have limited the wider exploitation of
9.6.9 Heat setting
Synthetic thermoplastic ﬁbres, yarns and fabrics may be heat set, steam set or
hydro set in order to obtain satisfactory dimensional stability during subsequent
hot wet treatments.76 Fabrics may be preset prior to coloration or postset after
coloration.31 Hydrosetting in hot water is rarely carried out, but false twist textured
yarn can be steam set in an autoclave using a double vacuum-steam cycle to attain
satisfactory removal of air and hence uniformity of temperature in the treatment.
Steam setting avoids the slight ﬁbre yellowing that can occur in fabric form
through ﬁbre surface oxidation during hot air setting on a stenter, and the handle
Heat setting on modern stenters is often carried out by ﬁrst drying and then
heat setting in one passage through the stenter. The temperature and time of
heat setting must be carefully monitored and controlled to ensure that consis-
tent fabric properties are achieved. During heat setting, the segmental motion
of the chain molecules of the amorphous regions of the ﬁbre are generally
increased leading to structural relaxation within the ﬁbre structure. During cooling,
the temperature is decreased below the ﬁbre glass transition temperature (Tg)
and the new ﬁbre structure is stabilised. Because the polymer chain molecules
have vibrated and moved into new equilibrium positions at a high temperature
in heat setting, subsequent heat treatments at lower temperatures do not cause
the heat-set ﬁbres to relax and shrink, so that the fabric dimensional stability is
Presetting of fabric prior to dyeing alters the polymer chain molecular
arrangement within the ﬁbres, and hence can alter the rate of dye uptake during
dyeing.23,31,53 Process variations (e.g. temperature, time or tension differences)
during heat setting may thus give rise to dyeability variations that become appar-
ent after dyeing. Fabric postsetting after coloration can lead to the diffusion of dyes
such as disperse dyes to the ﬁbre surface and to sublimation, thermomigration and
blooming problems, all of which can alter the colour and markedly decrease the
colour fastness to washing and rubbing of technical textiles containing polyester
9.6.10 Quality control in pretreatment
In all the pretreatments given to fabrics, it is necessary to control the process care-
fully in order to minimise ﬁbre degradation and yellowing.8 Mechanical damage (i.e.
holes, poor dimensional stability and ﬁbre damage through overdrying) must also
be avoided. Fibre yellowing makes it very difﬁcult to dye pale bright colours while
any ﬁbre degradation may be subsequently increased during dyeing and printing
treatments and result in inferior physical properties (e.g. low tensile strength, tear
strength and abrasion resistance) or to poor colour fastness performance. Inade-
208 Handbook of technical textiles
quate pretreatment can lead to poor wettability, uneven coloration and inferior
adhesion of coatings in technical textiles.
9.7 Total colour management systems
9.7.1 Speciﬁcation of colours and colour communication
The time-honoured method of specifying colours involves sending physical stan-
dards (e.g. dyed or coloured patterns) to the dyehouse followed by dyeing samples
to match the colour in the laboratory.77 The samples are submitted to the colour
speciﬁer for acceptance or rejection. If they are not accepted by the colour speci-
ﬁer, this process must be repeated in order to obtain satisfactory colour matching
to the standard. The approved laboratory sample will then be used as the basis for
the initial dye recipe for bulk dyeings. A sample from bulk dyeing may then be
submitted to the speciﬁer for ﬁnal approval prior to delivery. Similar principles
apply to the production of laboratory strike-offs of each colour in a print for
approval by the colour speciﬁer prior to machine printing.
All this is a time-consuming procedure which has now been shortened consider-
ably in order to avoid colour changes through storage and handling of physical
samples and to achieve a quick response and provide just-in-time delivery to the
customer. The use of a colour speciﬁer program can dramatically decrease the cycle
time for approval. This involves the use of instrumental colour measurement for for-
mulation and quality control, accreditation procedures to enable self approval of
colours and colour speciﬁcation using reﬂectance data.77–79 In the most advanced
colour management systems it is now possible to visualise a colour on a colour
monitor so that colour communication between the colour speciﬁer and the dyer is
vastly simpliﬁed. A number of standardised colour speciﬁcation systems, for
example Pantone, Munsell Chip systems, can also be used.79
9.7.2 Colour measurement
Objective colour matching using a spectrophotometer for colour measurement
is superior to visual colour matching assessment because instrumental colour
measurement allows the colour to be speciﬁed in terms of reﬂectance data and the
precision of colour matching to the standard reﬂectance data can then be calculated
numerically in colour difference units (DE).80
Colour tolerancing systems can be used to provide better agreement between
visual assessment and the instrumentally measured colour difference, and colour
acceptability limits can be agreed in advance in order to facilitate decisions on
colour.80–82 Colour acceptability limits are numerical values at which the perceived
colour differences become unacceptable to the speciﬁer, that is, single number shade
passing systems. Instrumental shade sorting systems are widely used to separate
fabric lengths on fabric rolls into similar colours.83
The spectrophotometers currently in use may give different measured reﬂectance
values according to the instrument design. The geometry, wavelength scale,
bandwidth or light source may differ between different makes of spectropho-
tometer.77,80,81 The two most common geometries used for direction of illumination/
Coloration of technical textiles 209
direction of view are: diffuse /8° and 45°/0°. Readings given by these two geom-
etries are not compatible unless the ideal perfect diffuser is measured. Illumination
is provided either by a tungsten ﬁlament halogen cycle incandescent lamp or by a
pulsed xenon discharge lamp.
Tungsten ﬁlament lamps do not have signiﬁcant ultraviolet emission compared
with pulsed xenon discharge lamps. The measurement of samples containing ﬂuo-
rescent brightening agents or some ﬂuorescent materials is thus affected by inclu-
sion or exclusion of the ultraviolet component of the illumination.77
Spectrophotometers use either single-beam, double-beam or dual-beam optics.
The latter are now more widely used to compensate for the variability of the spec-
trum of pulsed xenon discharge lamps.77,84 The collection optics may gather light
across the sample image, focussing it on to the spectrophotometer aperture, or alter-
natively it is imaged at inﬁnity, gathering light along a narrow range of angles. This
latter method is claimed to provide a greater depth of ﬁeld and insensitivity to
sample surface imperfections. Considerable progress has been made by the manu-
facturers of spectrophotometers to ensure that the instruments give reliable, repeat-
able measurements, and the inter-instrument agreement (i.e. the colour difference
values for a set of colour standards measured with two or more instruments of the
same model) is now very low (typically 0.04 DE). Inter-instrument agreement and
precision of colour measurement are now very important for the colour measure-
ment of some technical fabrics where the colour matching has to be very close to
the standard, as in automotive fabrics where reproducibility to within 0.3 DE is
The spectrophotometers in use may utilise 16 data points at 20 nm intervals over
the 400–700 nm range, 31 data points from 400 to 700 at 10 nm intervals, or 40 data
points from 360 to 750 nm at 10 nm intervals.77 In addition, the bandwidth may be
20 nm or 10 nm or less. As a result, it is difﬁcult to convert measurements from one
format to the other. Although conversion is possible, the colour difference measured
at two different bandwidths on the same sample can be as high as 2.0 CIELAB units.
However, the largest aperture should be used for colour measurement because this
should provide more repeatable measurements.
Colour measurement of dyed textiles should be carried out on conditioned
samples because the colour may change with temperature and moisture content and
the colour change may exceed the pass/fail tolerance.77 The sample presentation
should also specify the number of fabric layers and the backing material to be used
because these factors also affect the perceived colour. Colour measurement of loose
ﬁbres generally gives rise to greater variations in measurement than on woven
fabrics so that it is advisable to use multiple measurements to improve the repeata-
bility. There are considerable differences in colour between cut and uncut pile yarn,
where measurements are made on the ﬁbre tips of a cut hank of yarn or on the side
of the yarn.80
Portable colour measurement systems utilise hand-held spectrophotometers with
data storage and extensive memory capacity for monitoring the colour batch-
to-batch and within batch (e.g. side-centre-side, and end-to-end colour variations
within a fabric roll).85 These are very convenient for quality control purposes both
within the laboraratory and in the production plant, but sophisticated on-line colour
measurement systems are also employed on continuous fabric dyeing ranges.86
A typical total colour control system is illustrated in Fig. 9.2.80
210 Handbook of technical textiles
Colorant and Colorant screening Substrate and colorant
material data and selection delivery testing
Prediction Recipe storage
of shades and retrieval
Application Colour correction Colorant and
process program chemical inventory
Pass Use of numerical
Batch sorting into those
that can be mixed
9.2 Total colour control (source: see ref 80, p. 45).
9.7.3 Laboratory matching
In the modern dyehouse, dyestuffs and chemicals are purchased to an agreed quality
standard.19,80 Dyestuffs for use in laboratory matching in many dyehouses are dis-
solved or dispersed in stock solutions above an automated laboratory dispensing
unit. The colour speciﬁer may supply a physical sample, the reﬂective curve of which
is measured on the spectrophotometer in the laboratory or reﬂectance data are sup-
plied directly to the laboratory. Computer match prediction is then carried out using
the appropriate database of the dyes used in the dyehouse on the substrate to be
dyed.80 If the substrate to be dyed in bulk has a different dyeability to that origi-
nally used to construct the database, adjustment of the recipe must be made. The
colorist in the laboratory must then select from the computer match prediction the
most appropriate recipe, taking into account such factors as recipe cost, the antici-
pated technical performance in bulk dyeing, colour fastness, metamerism, and the
closeness of the predicted colour match to the speciﬁed colour.
The appropriate dye recipe is then dispensed manually or on a laboratory dye
dispensing unit and a sample of the material is then dyed in an automated labora-
tory dyeing machine under conditions that will simulate those to be used in bulk
dyeing, for example the same pH, chemicals and auxiliaries, liquor ratio and tem-
perature–time relationship. The laboratory matching is given the same rinsing or
after-treatment that will be used in bulk dyeing, and is dried, conditioned, and the
colour measured on the spectrophotometer. If the colour is a commercial match to
the speciﬁed colour, then bulk dyeing is initiated. If the colour is outside the com-
Coloration of technical textiles 211
mercial colour tolerance owing to differences in substrate dyeability and so on, a
corrected recipe is predicted and the process repeated to obtain a commercial
colour match followed by bulk dyeing.80,81,87
Where there is close control over the colour strength of the dyestuffs and con-
sistent substrate dyeability, it is often possible to operate so-called ‘blind dyeing’ in
which the computed dye recipe in the laboratory is used immediately for bulk
dyeing.87 This shortens the time required, decreases dyehouse costs and offers quick
response and rapid delivery to customers. Where repeat dyeings of the same colour
are required, it is usually possible to input the reﬂectance data gained from bulk
dyeings in order to reﬁne the database and thereby achieve a greater level of
right-ﬁrst-time dyeings. Right-ﬁrst-time, right-on-time, right-every-time dyeing is the
goal of the dyer, because this is the lowest cost dyeing system that provides quick
response for customers.87
If a bulk dyeing proves to be off-shade and the original recipe requires a cor-
rection (i.e. an addition) that results in extending the dyeing time, the dyer suffers
a considerable ﬁnancial penalty. If the colour is too dark and the bulk dyeing must
be stripped and redyed, this imposes further cost penalties and often impairs the
quality, physical properties and surface appearance of the dyed material. In general,
the shorter the processing time under hot wet conditions in the dyebath, the lower
will be the ﬁbre degradation and hence the quality of the dyed material will be su-
perior, all important considerations for many technical textiles.
9.8 Dyeing machinery
Apart from mass coloration that has been discussed in Section 9.5, conventional
dyeing machinery is used for the dyeing of technical textile materials in the form of
all types of ﬁbres, tows, yarns (e.g. warp, hank, package), fabric, garments, carpets
and so on.13,88–91 Fabric may be dyed in rope form (i.e. as a strand) or at open width
(i.e. ﬂat), or circular weft knitted fabrics may be dyed in tubular form. Modern trends
are to dye in yarn or fabric form because this allows the decision on colour to be
made later in the manufacturing chain and the cost of dyeing is lower. Many tech-
nical fabrics are dyed at open width to avoid inserting creases into the fabric. Such
creases can be difﬁcult to remove in synthetic ﬁbre fabrics because of hydrosetting
occurring during dyeing.
9.8.1 Batch dyeing machinery for exhaust dyeing
In conventional exhaust dyeing, dye molecules are transported to the ﬁbre surface
where the substantivity of the dye for the ﬁbre ensures that adsorption takes place
to produce a higher surface concentration of dye.92 This promotes dye diffusion into
the ﬁbre, the rate of dye diffusion being dependent upon the dye concentration. Dye
molecules diffuse within the disordered regions of the ﬁbres, to provide adequate
ﬁbre penetration.21 Level dyeing is attained through the migration of dye, by des-
orption from inside the ﬁbre back into the dye liquor and thence adsorption and
diffusion in another part of the ﬁbre, this levelling process being aided by the rela-
tive motion of the dye liquor and the ﬁbre. After an appropriate time, a level, well-
penetrated dyeing is obtained. This process is facilitated if compatible dyes, that is,
dyes that diffuse at the same rate, are initially selected for use together with a
212 Handbook of technical textiles
9.3 Jig dyeing machine (source: see ref 89, p. 29).
selected levelling agent. Dye ﬁxation is ensured either through (i) electrostatic
attraction between the dye and dyesites inside the ﬁbre, (ii) by covalent bond for-
mation between the dye and the ﬁbre, (iii) by increasing the size of the dye or by
dye aggregation leading to mechanical entrapment, or (iv) by conversion of the
water-soluble dye into a water-insoluble form.
The three types of dyeing machinery for batch or exhaust dyeing are based on
machines in which:88,89,91
1 the material moves, but the liquor is stationery, e.g. jig and winch (beck)
machines for fabric dyeing
2 the liquor moves, but the material is stationery, e.g. hank or package dyeing of
yarns and beam dyeing of fabrics
3 both the liquor and the material move, e.g. jet, softﬂow and overﬂow jet dyeing
machines for fabrics.
In general, a lower liquor ratio decreases the water and energy consumption and
decreases the volume of waste water, decreasing efﬂuent treatment costs. It can also
facilitate a more rapid dyeing cycle and increase the dye exhaustion on the ﬁbre,
because the total dye liquor is circulated more rapidly.
In the jig (or jigger), fabric is dyed at open width by traversing fabric from one
roll through a dyebath and on to a second roll (see Fig. 9.3).89 When the second roll
is full, the rolls are stopped and the fabric motion is reversed, and the procedure
repeated as required. The dye liquor is added in portions to ensure satisfactory lev-
elness from end-to-end of the fabric. A hood prevents the release of steam and helps
to maintain the fabric temperature on the rolls where the majority of the dyeing
takes place. Most jigs operate at 98–100 °C (i.e. under atmospheric conditions) but
pressurised jigs operating at up to 140 °C are used for some technical fabrics, for
example polyester sailcloths. In the latter machine, the rolls and the dyebath are
enclosed in an autoclave (i.e. pressure vessel) which can be closed with a ring seal.
Jig dyeing operates at a liquor ratio of 3–5 : 1 and rinsing/washing off is more rapid
on modern twin bath jig designs in which a combination of water spray and vacuum
is used for removal of loose dyestuff.93
Jig dyeing is particularly suitable for technical fabrics that may be subjected to
creasing and hence are preferably dyed at open width. In addition it is preferred for
many technical fabrics that have a dense structure and where it is difﬁcult to pump
Coloration of technical textiles 213
9.4 Winch dyeing machine (source: see ref 89, p. 38).
9.5 Sectional diagram of a high temperature beam dyeing machine (source: see
ref 27, p. 117).
dye liquor through multiple fabric layers, as in beam dyeing (e.g. sailcloths, ﬁlter
The winch or beck dyeing machine may be used for dyeing in rope form, nor-
mally at temperatures of up to 98–100 °C (see Fig. 9.4).89 High temperature winches
have also been used in the past, but have now been replaced by high temperature
(i.e. pressurised) jet dyeing machines. The latter are less likely to give rise to fabric
creasing and have improved liquor interchange which aids the more rapid attain-
ment of level dyeing by promoting dye migration.
In beam dyeing, the fabric is wound at open width on to a perforated stainless
steel beam, and kept in place by the use of end plates (see Fig. 9.5).89 Dye liquor is
pumped through the multiple layers of fabric, usually from out to in, but in-to-out
ﬂow is also used. The fabric winding tension must be low to avoid stretching the
fabric, and to avoid high pressure being applied to the innermost fabric layers, other-
wise the fault known as watermarking or moiré may be observed. This is usually
seen as a shimmering surface pattern on dark colours, the pattern changing with the
orientation of the fabric relative to the observer. Too low a winding tension can,
however, lead to telescoping and movement of the fabric on the beam. It is normal
to wind a fent (or short sacriﬁcial fabric length) on to the beam ﬁrst to prevent per-
foration marks on the fabric layers next to the beam. These show as a pattern of
dark spots corresponding to the perforated holes in the beam and are often caused
214 Handbook of technical textiles
9.6 Softﬂow jet dyeing machine.
by poor dispersing or aggregation of disperse dyes. The liquor ratio in beam dyeing
is around 10 : 1 although this can be decreased by the use of spacers, and most beam
dyeing machines are pressurised machines capable of dyeing at temperatures of
130–140 °C. Beam dyeing is particularly effective for dyeing thin permeable fabrics
composed of synthetic ﬁlaments, e.g. nylon 6.6 and polyester fabrics.
Pressurised machines are generally used for dyeing technical textiles composed
of synthetic ﬁbre materials. Softﬂow jets provide a more gentle mechanical
action on the fabric rope, the main fabric transportation being carried out over a
winch reel followed by a softﬂow jet system (see Fig. 9.6).89,94 In some jet dyeing
machinery, the liquor ﬂow is split between two jets which exert a lower pressure
on the fabric. This is claimed to decrease linting (loss of ﬁbre) in staple ﬁbre
fabrics, and surface distortion. Garments are generally dyed in atmospheric
or pressurised rotary drum machines or in atmospheric overhead paddle dyeing
Aerodynamic fabric transport systems utilise a blower to aid the fabric circula-
tion through the jet dyeing machine. These enable liquor ratios as low as 1.3 : 1 to
be used on hydrophobic ﬁlament fabrics such as polyester, although higher liquor
ratios in the range 5–10 : 1 are used in conventional jets on hydrophilic cellulosic
9.8.2 Pad-batch dyeing
Both woven and knitted fabrics can be dyed using this method with the padding
(impregnation) stage being conducted under ambient or hot conditions.41,96 With
reactive dyes, fabric prepared for dyeing is usually padded under ambient condi-
tions and then wound up on a roll rotating on an A-frame. The dye concentration
and the pick up of dye liquor by the fabric must be controlled to ensure uniform
fabric coloration. The length of padded fabric on the roll may be covered with poly-
ethylene ﬁlm to prevent evaporation and is then rotated slowly (to avoid migration
of the dye liquor to the outer layers of the fabric roll) for an appropriate time to
achieve dye ﬁxation. The time required is dependent upon the depth of colour, the
reactivity of the reactive dye, the temperature and the alkalinity, but is generally in
the range 4–24 hours (often conveniently overnight). This is then followed by a thor-
ough hot wash off to remove the unﬁxed dyestuff and the alkali, and the fabric is
Coloration of technical textiles 215
9.8.3 Continuous dyeing machinery
Continuous dyeing can be carried out by dye impregnation, ﬁxation, washing off
and drying on ranges designed for handling woven fabrics at open width, and
there are also carpet and warp dyeing ranges.90 Continuous dyeing was originally
designed for efﬁcient and economical dyeing of long runs of fabric, and many
modiﬁcations have been made to facilitate more rapid turn around and less down-
time in between a greater number of shorter production runs per colour. Automatic
metering of liquid dyes to control the dye concentration in the dyebath and intelli-
gent padding systems are used to control the pick up of dye liquor by the fabric.
Thermoﬁxation (dry heat), superheated steam or saturated steam ﬁxation units in
which the temperature is monitored and controlled may be used to obtain dye
ﬁxation. Reproducible colour is obtained after washing off loose dyestuffs and
drying. Colour change during a production run is accomplished on-line within
minutes using automated wash down systems. Continuous colour monitoring on the
output dyed fabric on some ranges can be utilised to adjust the colour being dyed
on the input fabric. Either the whole width of the fabric may be continuously
monitored, or a traversing spectrophotometer measuring side-centre-side variations
may be employed.
For the continuous dyeing of woven polyester/cotton fabric, the polyester ﬁbres
are ﬁrst dyed with disperse dyes using a pad-dry-thermoﬁx treatment.90 The cotton
is then dyed using direct, reactive or vat dyes using a pad-steam process. The dyed
fabric is cleared of loose surface dyestuff by treatment on an open width washing
range and then dried over steam-heated cylinders and batched. A scray is used at
the fabric entry to the range to accumulate fabric so that the range continues to run
at 50–150 m min-1 while the next roll of fabric is sewn on to the fabric being dyed.
9.9.1 Printing styles
Printing leads to the production of a design or motif on a substrate by application
of a colorant or other reagent, usually in a paste or ink, in a predetermined pattern.
In printing, each colour is normally applied separately and a wide variety of print-
ing techniques is used. In direct printing, dyes are applied in a print thickener
containing auxiliaries and are diffused into the ﬁbres and ﬁxed in a steamer or high
temperature steamer.57 Surface dye and thickener are then thoroughly washed off
in a continuous open width washer, and the materials dried.
In pigment printing, water-insoluble pigments are applied with a heat-curable
binder system, followed by drying and curing, and the physical properties of the
pigment print depend greatly upon the adhesive properties of the print binder
system. Pigment printing is a simple, popular method particularly for printing
blended ﬁbre fabrics.7,57
Two other major styles of printing are employed, namely, discharge and resist
printing.97 In discharge printing, a dyed fabric is printed with a discharging agent
(a reducing agent) which decolorises the dye leaving a white motif against a dyed
ground. Alternatively, a dye resistant to discharging can simultaneously be applied
to give a second colour in the discharged area of the motif. In resist printing, the
resisting agent (which may act mechanically or chemically) is printed on to the
216 Handbook of technical textiles
undyed fabric. This prevents the ﬁxation of the ground colour which is then devel-
oped by dyeing, padding or overprinting. A white resist, or a coloured resist, can be
achieved if a selected dye or pigment is added to the resist paste and is then
9.9.2 The print image
The design image may be painted by hand on to transparent ﬁlm for photographic
development of diapositive images, or sophisticated CAD (computer-aided design)
systems are used in conjunction with a design input scanner. The design image is
then manipulated on screen, the colours are electronically separated and the digi-
tised design images for each colour transferred to an engraving system for transfer
on to a rotary or ﬂat screen, or for direct use in digital ink jet printing.98
9.9.3 Fabric printing machinery
Rotary screen printing is the dominant printing method now employed for 60–70%
of printed fabric production.99 The design motif for each colour is developed as open
mesh on the rotary screen by the use of ﬁlm, laser or black wax engraving systems.
Both lacquer screen and galvano screens are used. Each rotary screen secured in
end rings is ﬁxed in bearings and rotated in precise register and in a predetermined
sequence. A separate colour is supplied to each rotary screen and pushed by a
squeegee (e.g. a blade or a roller) through the open mesh of the screen on to the
fabric which is temporarily gummed on to a print table with a moving blanket
(apron).100 Machines capable of continuously printing up to 24–36 colours are avail-
able, although most designs involve less than eight colours, and rotary screen
printing on textile materials up to 5 m in width can be carried out, at speeds up to
80 m min-1, but typically at 40 m min-1.
Automatic or semiautomatic ﬂat screen (ﬂat bed) printing is used for many
designs where very precise images are required, using polyester, polypropylene or
polyamide monoﬁlament fabric as the screen material.100 In automated ﬂat screen
printing, the fabric is gummed to the print table and progressed forward intermit-
tently, one design repeat at a time, after the lowering, printing and lifting of the
screens, to print all the colours sequentially, using a squeegee system to force the
print paste into the fabric. The printing speed is lower than that normally obtained
in rotary-screen printing. Modern rotary and ﬂat screen printing machines may be
supplied with enough colour for each screen, with all the operations of weighing,
metering, dispersing and mixing of dyes and auxiliaries with stock thickener (suit-
ably diluted), or of pigments with binders and softeners controlled by a robotised
colour kitchen based upon a computed print recipe. The colours are supplied in
drums and supply pipes are used to furnish the colour for each screen in rotary
At the end of the print run, excess print paste is removed and stored, and this
may then be reused in a subsequent print run, or disposed of to landﬁll. Print
monitoring systems are available for monitoring and comparing the fabric print
with the electronically stored digitised design image. In the most sophisticated
machines, it is possible to use such monitoring systems for correction of faults on-
line, and many machines are designed for quick changeover of colours, for example
by screen and blanket washing and drying facilities on-line, and also for rapid
Coloration of technical textiles 217
changeover of screens at a design change.101 Automated setting up, monitoring,
control and correction systems and washing and drying on-line have all dramati-
cally improved the productivity and repeatability in rotary and ﬂat screen
The latest advance in textile printing is the introduction of digital ink jet print-
ing machines, capable of printing fabrics up to 2 m in width using acid, reactive or
disperse dye inksets.102–104 The fabric is normally pretreated and placed in the
machine in roll form, printed and then the dyes are ﬁxed, usually by steaming in a
separate machine, washed off and dried. Both piezoelectric and bubble jet printing
systems may be used, with any unused colour being diverted back to the ink
reservoir and recycled. Generally four, seven–eight, and up to 12 colours may be
printed; the greater the number of colours the greater the colour gamut that can
In general, digital ink jet printing systems are designed principally for use with
natural ﬁbres, (e.g. cellulosic, wool and silk fabrics) and also polyester fabrics.102–104
On some machines, the inkjets are periodically cleaned with solvent, automatically,
to avoid jet blockage, particularly with disperse dye systems. Such printing machines
may be run overnight without operator supervision, the design images being pre-
loaded, and design changeover being essentially instantaneous. Other systems are
already being used for printing ﬂags and banners and clearly have great potential
for printing short production runs of advanced technical textile fabrics.105 Ulti-
mately, some form of reprographic printing method may be developed and research
and development along these lines is continuing.106
Transfer printing may be carried out by sublimation transfer, melt transfer or
ﬁlm release methods.55 In sublimation (or dry heat) transfer printing, volatile
dyes (typically disperse dyes) are preprinted on to a paper substrate and are heated
in contact with the textile material, typically polyester fabric. The dyes sublime
and are transferred from the vapour phase into the fabric in this dry-heat transfer
printing method. This may be assisted by the application of a vacuum. Melt trans-
fer is principally used on garments whereby a waxy ink is printed on paper and a
hot iron applied to its reverse face to melt the wax on to the fabric surface. In the
ﬁlm release method, the print design is held in an ink layer which is transferred
completely to the textile from a release paper using heat and pressure. The design
is held on to the textile by the strong forces of adhesion between the ﬁlm and the
9.10 Colour fastness of technical textiles
The performance of a dyed or printed technical textile when exposed to various
agencies during end-use is normally assessed by appropriate colour fastness
testing.107,108 High standards of quality and performance in such tests are often
related to the higher cost of the dyes and pigments used which possess superior
colour fastness properties. There are national standards, for example British Stand-
ards (BS), European Standards (EN) and International Standards (ISO), but
within most countries now there is a move towards harmonisation of test methods
and performance standards, so that EN ISO standards will be used in the future. In
North America, there are ASTM (American Society for Testing and Materials) and
AATCC (American Association of Textile Chemists and Colorists) test methods. In
218 Handbook of technical textiles
addition, there are also test methods that have been devised by industry for use for
speciﬁc applications, for example automotive textiles.
Many colour fastness tests have been devised to simulate the likely end-use con-
ditions, and the Society of Dyers and Colourists in the UK and the AATCC in the
USA have been at the forefront of colour fastness testing developments. The colour
fastness test usually deﬁnes a standard test method to be followed, and gives the
method of assessment to be used, but the performance level which is satisfactory
for the end-use has to be agreed between the dyer or printer and the colour speci-
ﬁer. Companies often set their own in-house performance criteria for their ranges
of dyed or printed technical textiles, based upon their general working knowledge
and experience in the ﬁeld, through technical liaison with dye makers, through ﬁeld
testing under actual end-use conditions and by assessment of materials which are
the subject of complaints.
It is not possible to discuss the many colour fastness tests that are now in use
worldwide, but complete details are available in many other publications, which give
details of a wide range of standard tests.107,108 The major types of colour fastness test
relate to the colour fastness to wet treatments, (e.g. to washing), and to light and
weathering, to rubbing (crocking), atmospheric contaminants, and organic solvents,
(e.g. dry cleaning).
The colour fastness performance in standardised wash tests is rated by visual
assessment of the change in colour of the coloured material and the degree of stain-
ing on to adjacent materials in the wash liquor (e.g. a multiﬁbre fabric test strip,109
or speciﬁc adjacent fabrics), using ISO Grey Scales under standardised lighting con-
ditions against a neutral grey background in a viewing cabinet. The Grey Scale
ratings range from 5 (no change, i.e. excellent performance) through half point
ratings, for example 4–5, down to 1 (large change, i.e. poor performance). The colour
change may also be measured objectively using a spectrophotometer and the colour
difference converted into a Grey Scale rating.110
Colour fastness to light is normally assessed using a high intensity ﬁltered xenon
arc lamp to simulate natural daylight, sample strips being mounted, part covered,
on cards which can be individually rotated in a bank of holders that may be rotated
around the accelerated fading lamp, depending on the type of machine, in an atmos-
phere of controlled temperature and relative humidity. A set of blue wool standard
fabric strips that fade at known rates must also be used in each test. The set-up con-
ditions for speciﬁc test methods used for many types of technical textiles are pre-
programmed on modern light fastness testing machines.111
The degree of fade in British and European Standards is based upon visual
assessment of the degree of colour fade on the test sample compared with the
equivalent degree of fade on the blue wool samples.The light fastness rating changes
from 8 (highest) down to 1 (lowest). Because of difﬁculties with the supply of blue
wool standards, the Society of Dyers and Colourists is introducing a set of blue pig-
ment-printed light fastness standards that will replace the blue wool standards, but
in addition may also extend the light fastness rating range beyond 8 and below 1.112
Weathering may be conducted in ﬁeld trials, with samples exposed to sunlight either
covered or uncovered by glass, or alternatively by exposure for a standard number
of hours in an accelerated fading machine.
Colour fastness to rubbing (crocking) is assessed by rubbing a standard white
fabric against the dyed sample under a constant pressure for an agreed number of
strokes. The test may be conducted under wet or dry conditions, and the machine
Coloration of technical textiles 219
may be operated by hand, or in the latest machines performed automatically.113
Assessment of the degree of staining on the white fabric is assessed using the ISO
Grey Scale for staining. For pigment printed materials, the rub fastness is depen-
dent upon the properties of the adhesive binder used.
1. j shore, ‘Coloration of polypropylene’, Rev. Prog. Coloration, 1975 6 7–12.
2. c b stevens, in The Dyeing of Synthetic-polymer and Acetate Fibres, ed. D M Nunn, The Dyers
Company Publications Trust, Bradford, 1979, 1–75.
3. k-h ﬂuss, ‘Space dyeing – survey of methods’, Bayer Farben Revue, E1976 26 19–33.
4. j shore, Colorants and Auxiliaries, Organic Chemistry and Application Properties, Volume 1 –
Colorants, The Society of Dyers and Colourists, Bradford, 1990.
5. w saus, ‘SFD-Dry dyeing of polyester in CO2’, Textile Technol. Int., 1995 145–6, 148, 150.
6. p ackroyd, ‘The mass coloration of man-made ﬁbres’, Rev. Prog. Coloration, 1974 5 86–96.
7. v giesen and r eisenlohr, ‘Pigment printing’, Rev. Prog. Coloration, 1994 24 26–30.
8. w s hickman, in Cellulosics Dyeing, ed. J Shore, The Society of Dyers and Colourists, Bradford,
9. h zollinger, Colour Chemistry, Synthesis, Properties and Applications of Organic Dyes and
Pigments, VCH, New York, 1987.
10. i holme, ‘The provision, storage and handling of dyes and chemicals in dyeing and ﬁnishing plants’,
J. Soc. Dyers Colourists, 1978 94(9) 375–394.
11. g booth, The Manufacture of Organic Colorants and Intermediates, The Society of Dyers and
Colourists, Bradford, 1998.
12. j shore, Blends Dyeing, The Society of Dyers and Colourists, Bradford, 1998.
13. g clarke, A Practical Introduction to Fibre and Tow Coloration,The Society of Dyers and Colourists,
14. k mclaren, The Colour Science of Dyes and Pigments, 2nd edn, Adam Hilger, Bristol, 1986.
15. a k sarkar, Fluorescent Whitening Agents, Merrow, Watford, 1971.
16. r williamson, Fluorescent Brightening Agents, Elsevier, Amsterdam, 1980.
17. r anliker and g müller, ‘Fluorescent whitening agents’, in Environmental Quality and Safety, eds.
F Coulston and F Korte, Suppl Vol IV, Thieme, Stuttgart, 1975.
18. Colour Index International, 3rd edn, 4th revision, Books and CD-ROM Issue 3, Colour Index-
Pigments and Solvent Dyes, Book and CD-ROM, 1997.
19. i holme, The Provision, Storage and Handling of Dyes and Chemicals for Textile Dyeing, Printing
and Finishing, UNIDO Textile Monograph UF/GLO/78/115, Vienna, 1980.
20. d m nunn (ed), The Dyeing of Synthetic-polymer and Acetate Fibres, The Dyers Company Publica-
tions Trust, Bradford, 1979.
21. i holme, ‘Fibre physics and chemistry in relation to coloration’, Rev. Prog. Coloration, 1970 1 31–
22. a murray and k mortimer, ‘Carrier dyeing’, Rev. Prog. Coloration, 1971 2 67–72.
23. s m burkinshaw, Chemical Principles of Synthetic Fibre Dyeing, Blackie, London, 1995.
24. j e mcintyre and p n daniels (eds.), Textile Terms and Deﬁnitions, 10th edn, The Textile Institute,
25. j hilden, ‘The effect of ﬁbre properties on the dyeing of microﬁbres’, Int. Textile Bull., Dyeing/Print-
ing/Finishing, 1991 number (3), 19, 22, 24, 26.
26. p a dufﬁeld, in ‘Wool Dyeing’, ed. D M Lewis, The Society of Dyers and Colourists, Bradford, 1992,
27. w ingamells, Colour for Textiles – A User’s Handbook, The Society of Dyers and Colourists, Brad-
28. anon, ‘A revival of interest in low-temperature dyeing’, Wool Record, 1996 155(3618) 35.
29. a c welham, in ‘Wool Dyeing’, ed. D M Lewis, The Society of Dyers and Colourists, Bradford, 1992,
30. d m lewis, ‘Damage in wool dyeing’, Rev. Prog. Coloration, 1989 19 49–56.
31. p ginns and k silkstone, in The Dyeing of Synthetic-polymer and Acetate Fibres, ed. D M Nunn,
The Dyers Company Publications Trust, Bradford, 1979, 241–356.
32. l w c miles (ed.), Textile Printing, 2nd edn, The Society of Dyers and Colourists, Bradford, 1994.
33. t f cooke and h-d weigmann, ‘Stain blockers for nylon ﬁbres’, Rev. Prog. Coloration, 1990 20 10–18.
34. a c welham, ‘Advances in the afterchrome dyeing of wool’, J. Soc. Dyers Colourists, 1986 102(4)
35. i holme, ‘Dye–ﬁbre interrelations in acrylic ﬁbres’, Chimia, 1980 34 110–130.
220 Handbook of technical textiles
36. w beckmann, in The Dyeing of Synthetic-polymer and Acetate Fibres, ed. D M Nunn, The Dyers
Company Publications Trust, Bradford, 1979, 359–392.
37. j shore, in Cellulosics Dyeing, ed. J Shore, The Society of Dyers and Colourists, Bradford, 1995,
38. j shore, in Cellulosics Dyeing, ed. J Shore, The Society of Dyers and Colourists, Bradford, 1995,
39. t vickerstaff, The Physical Chemistry of Dyeing, 2nd edn, Oliver and Boyd, London, 1954.
40. j a hook and a c welham, ‘The use of reactant-ﬁxable dyes in the dyeing of cellulosic blends’, J.
Soc. Dyers Colourists, 1988 104(9) 329–337.
41. j shore, in Cellulosics Dyeing, ed. J Shore, The Society of Dyers and Colourists, Bradford, 1995,
42. d m lewis, in Wool Dyeing, ed. D M Lewis, The Society of Dyers and Colourists, Bradford, 1992,
43. m l gulrajani, ‘Dyeing of silk with reactive dyes’, Rev. Prog. Coloration, 1993 23 51–56.
44. p rys and h zollinger, in The Theory of Coloration of Textiles, 2nd edn, ed. A Johnson, The Society
of Dyers and Colourists, Bradford, 1989, 428–476.
45. m j bradbury, p s collishaw and s moorhouse, ‘Exploiting technology to gain competitive advan-
tage’, Int. Dyer, 1996 181(4) 13, 14, 17, 20, 22–23.
46. r schneider, ‘Minimization of water consumption in washing-off processes’, 18th IFATCC (Inter-
national Federation of Textile Chemists and Colorists) Congress, Copenhagen, Denmark, IFATCC,
47. b d waters, in Colour in Dyehouse Efﬂuent, ed. P Cooper, The Society of Dyers and Colourists,
Bradford, 1995, 22–30
48. c senior, in Cellulosics Dyeing, ed. J Shore, The Society of Dyers and Colourists, Bradford, 1995,
49. d a s phillips, m duncan, a graydon, g bevan, j lloyd, c harbon and j hoffmeister, ‘Testing colour
fading of cotton fabrics by activated oxygen bleach-containing detergents: an inter-laboratory trial’,
J. Soc. Dyers Colourists, 1997 113(10) 281–286.
50. f r latham, in Cellulosics Dyeing, ed. J Shore, The Society of Dyers and Colourists, Bradford, 1995,
51. t bechtold, ‘Electrochemistry in vat dyeing and sulphur dyeing – concepts and results’, 18th
IFATCC (International Federation of Textile Chemists and Colorists) Congress, Copenhagen,
Denmark, IFATCC, 1999, 42–46.
52. d blackburn, in The Dyeing of Synthetic-Polymer and Acetate Fibres, ed. D M Nunn, The Dyers
Company Publications Trust, Bradford, 1979, 77–130.
53. r broadhurst, in The Dyeing of Synthetic-Polymer and Acetate Fibres, ed. D M Nunn, The Dyers
Company Publications Trust, Bradford, 1979, 131–240.
54. a t leaver, ‘Novel approaches in disperse dye design to meet changing customer needs’, American
Association of Textile Chemists and Colorists 1999 International Conference, Charlotte, USA,
AATCC, 1999, 367–374.
55. i d rattee, in Textile Printing, 2nd edn, ed. L W C Miles, The Society of Dyers and Colourists, Brad-
ford, 1994, 58–98.
56. p w leadbetter and a t leaver, ‘Recent advances in disperse dye development. Introducing a new
generation of high fastness disperse dyes’, 15th IFATCC (International Federation of Textile
Chemists and Colorists) Congress, Lucerne, Switzerland, IFATCC, 1990.
57. h gutjahr and r r koch, in Textile Printing, 2nd edn, ed. L W C Miles, The Society of Dyers and
Colourists, Bradford, 1994, 139–195.
58. b kaul, c ripke and m sandri, ‘Technical aspects of the mass-dyeing of polyoleﬁn ﬁbres with organic
pigments’, Chem. Fibres Int., 1996 46(4) 126–129.
59. h emsermann and r foppe, in Acrylic Fiber Technology and Applications, ed. J C Masson, Marcel
Dekker, New York, 1995, 285–312.
60. l ruys and f vandekerckhove, ‘Breakthrough in dyeable polypropylene’, Int. Dyer, 1998 183(8)
61. a lulay, in Acrylic Fiber Technology and Applications, ed. J C Masson, Marcel Dekker, New York,
62. i holme, ‘Dispensing system enables continuous quick response’, Int. Dyer, 1991 176(1) 10–11.
63. p a lewis, ‘Coloured organic pigments for coating fabrics’, J. Coated Fabrics, 1994 23(3) 166–201.
64. e r trotman, Textile Scouring and Bleaching, Grifﬁn, London, 1968.
65. i holme, i a panti, b d patel and h xin, ‘Chemical pretreatment of cotton fabrics for higher quality
and performance’, West-European Textiles Tomorrow, International Symposium, University of
Ghent, Belgium, 1990, 35–59.
66. h driver, ‘Fabric singeing – the vital ﬁrst step’, Textile Technol. Int., 1993, 178–180.
67. i holme, ‘Sizing for high speed weaving’, Textile Horizons, 1985 5(6) 42, 44.
68. i holme, ‘Chemical pretreatment – current technology and innovations’, Textile Horizons Int., 1993
Coloration of technical textiles 221
69. j t marsh, Mercerising, Chapman and Hall, London, 1951.
70. r freytag and j-j donzé, in Handbook of Fiber Science and Technology: Volume 1. Chemical
Processing of Fibers and Fabrics, Fundamentals and Preparation Part A, eds. M Lewin and S B Sello,
Marcel Dekker, New York, 1983, 93–165.
71. p f greenwood, ‘Piece mercerizing: a modern process for knitted cottons’, Textile Inst. Ind., 1976
72. i holme, in The Dyeing of Cellulosic Fibres, ed. C Preston, The Dyers Company Publications Trust,
Bradford, 1986, 106–141.
73. g euscher, ‘Medium knit mercerizing’, Textile Asia, 1982 13(9) 57–60, 62.
74. i gailey, ‘Causes of unlevel dyeing of cotton cellulose. The inﬂuence of mercerizing and bleaching
processes on the ﬁne structure of cellulose’, J. Soc. Dyers Colourists, 1951 67 357–361.
75. c v stevens and l g roldan (-gonzalez), in Handbook of Fiber Science and Technology: Volume
1. Chemical Processing of Fibers and Fabrics, Fundamentals and Preparation Part A, eds. M Lewin
and S B Sello, Marcel Dekker, New York, 1983, 167–203.
76. j w s hearle and l w c miles, The Setting of Fibres and Fabrics, Merrow, Watford, 1971.
77. k c lau, ‘Dynamic response to colour speciﬁcations’, J. Soc. Dyers Colourists, 1995 111(5) 142–
78. c sargeant, ‘Colour range management’, J. Soc. Dyers Colourists, 1995 111(9) 272–274.
79. c sargeant, ‘Colour visualisation and communication – a personal view’, Rev. Prog. Coloration,
1999 29 65–70.
80. j park, Instrumental Colour Formulation – A Practical Guide, The Society of Dyers and Colourists,
81. r mcdonald (ed.), Colour Physics for Industry, 2nd edn, The Society of Dyers and Colourists,
82. X-Rite, A Guide to Understanding Color Tolerancing, Grandville, Michigan, USA, X-Rite Inc, 1994.
83. y s w li, c w m yuen, k w yeung and k m sin, ‘Instrumental shade sorting in the last three decades’,
J. Soc. Dyers Colourists, 1998 114 203–209.
84. d battle, in Colour Physics for Industry, 2nd edn, ed. R McDonald, The Society of Dyers and
Colourists, Bradford, 1997, 57–80.
85. d s reininger, ‘Textile applications for hand-held colour measuring instruments’, Textile Chem.
Colorist, 1997 29(2) 13–17.
86. k van wursch, ‘On-line colorimetry in continuous dyeing’, J. Soc. Dyers Colourists, 1995 111(5)
87. b glover, p s collishaw and r f hyde,‘Creating wealth from textile coloration’, 15th IFATCC (Inter-
national Federation of Textile Chemists and Colorists) Congress, Lucerne, Switzerland, IFATCC,
88. j park, A Practical Introduction to Yarn Dyeing, The Society of Dyers and Colourists, Bradford,
89. d h wyles, in Engineering in Textile Coloration, ed. C Duckworth, The Dyers Company Publica-
tions Trust, Bradford, 1983, 1–137.
90. j park and s s smith, A Practical Introduction to the Continuous Dyeing of Woven Fabrics, Roaches
(Engineering), Upperhulme, Leek, UK, 1990.
91. g w madaras, g j parish and j shore, Batchwise Dyeing of Woven Cellulosic Fabrics, The Society of
Dyers and Colourists, Bradford, 1993.
92. r mcgregor and r h peters, ‘Effect of rate of ﬂow on dyeing, I – diffusional boundary layer in
dyeing’, J. Soc. Dyers Colourists, 1965 81(9) 393–400.
93. e henningsen, ‘Serious alternative to continuous dyeing’, Textile Month, 1998 February 19–20.
94. m white, ‘Developments in jet dyeing’, Rev. Prog. Coloration, 1998 28 80–94.
95. j a bone, p s collishaw and t d kelly, ‘Garment dyeing’, Rev. Prog. Coloration, 1998 18 37–46.
96. m r fox and h h sumner, in The Dyeing of Cellulosic Fibres, ed. C Preston, The Dyers Company
Publications Trust, Bradford, 1986, 142–195.
97. c berry and j g ferguson, in Textile Printing, 2nd edn, ed. L W C Miles, The Society of Dyers and
Colourists, Bradford, 1994, 196–239.
98. i holme, ‘Quick response printing’, African Textiles, 1997/98 Dec/Jan 20, 30.
99. h a ellis, ‘Printing techniques – the choice’, Textile Horizons, 1985 5(4) 37–38, 40.
100. c j hawkyard, in Textile Printing, 2nd edn, ed. L W C Miles, The Society of Dyers and Colourists,
Bradford, 1994, 18–57.
101. i holme, ‘Right ﬁrst time’, African Textiles, 1998 August/September 39–40.
102. w c tincher, q hu and x li, ‘Ink jet systems for printing fabrics’, Textile Chem. Colorist, 1998 30(5)
103. b siegel, s ervine and k siemensmeyer, ‘Ink jet: the future of textile printing’, 18th IFATCC
(International Federation of Textile Chemists and Colorists) Congress, Copenhagen, Denmark,
1999, IFATCC, 144–148.
104. t l dawson, ‘Jet Printing’, Rev. Prog. Coloration, 1992 22 22–31.
105. anon, ‘Digital printing points the way’, Textile Horizons, 1997 16(8) 25–26.
222 Handbook of technical textiles
106. w w carr, f l cook, w r lanigan, m e sikorski and w c tincher, ‘Printing textile fabrics with
xerography’, Textile. Chem. Colorist, 1991 23(5) 33–41.
107. Methods of Test for Colour Fastness of Textiles and Leather (BS 1006:1990. ISO 105).
108. AATCC Technical Manual 1999, Vol 74, Research Triangle Park, North Carolina, USA, American
Association of Textile Chemists and Colorists, 1998.
109. w beal, ‘New multiﬁbre from the Society’, J. Soc. Dyers Colourists, 1987 103(5/6) 177.
110. k j smith, in Colour Physics for Industry, 2nd edn, ed. R McDonald, The Society of Dyers and
Colourists, Bradford, 1997, 121–208.
111. i holme, ‘Colour fastness testing’, Textile Horizons, 1998 18(6) 12–13.
112. i holme, ‘Dyed materials: getting the colour right’, ATA J., 1998 9(1) 70–73.
113. p j smith, ‘Colour fastness testing methods and equipment’, Rev. Prog. Coloration, 1994 24 31–40.
Heat and ﬂame protection
Department of Textile Technology, Indian Institute of Technology, Hauz Khas,
New Delhi – 110016, India
With industrialisation, the safety of human beings has become an important issue.
A growing segment of the industrial textiles industry has therefore been involved
in a number of new developments in ﬁbres, fabrics, protective clothing.1–10 Major
challenges to coatings and fabrication technology for production in the ﬂame-
retardant textile industry have been to produce environmentally friendly, non-toxic
ﬂame-retardant systems that complement the comfort properties of textiles.11–14 The
1990s, therefore, saw some major innovations in the development of heat-resistant
ﬁbres and ﬂame-protective clothing for ﬁreﬁghters, foundry workers, military,
aviation and space personnel, and for other industrial workers who are exposed to
For heat and ﬂame protection, requirements range from clothing for situations
in which the wearer may be subjected to occasional exposure to a moderate level
of radiant heat as part of his/her normal working day, to clothing for prolonged
protection, where the wearer is subject to severe radiant and convective heat, to
direct ﬂame, for example the ﬁreﬁghter’s suit. In the process of accomplishing ﬂame
protection, however, the garment may be so thermally insulative and water vapour
impermeable that the wearer may begin to suffer discomfort and heat stress. Body
temperature may rise and the wearer may become wet with sweat. Attempts have
therefore been made to develop thermal and ﬂame protective garments which can
be worn without any discomfort.
In this chapter, various factors affecting the ﬂammability, development of
new inherently heat-resistant ﬁbres, and the ﬂame-retardant ﬁnishes for both
natural and man-made ﬁbre fabrics along with the relevant test methods are
224 Handbook of technical textiles
10.2 What constitutes ﬂammability?
Ease of ignition, rate of burning and heat release rate are the important properties
of textile materials which determine the extent of ﬁre hazard. The other factors that
inﬂuence the thermal protection level include melting and shrinkage characteristics
of synthetic ﬁbre fabrics, and emission of smoke and toxic gases during burning. So,
while selecting and designing ﬂame protective clothing, the following points should
be kept in mind:
• the thermal or burning behaviour of textile ﬁbres
• the inﬂuence of fabric structure and garment shape on the burning behaviour
• selection of non-toxic, smoke-free ﬂame-retardant additives or ﬁnishes
• design of the protective garment, depending on its usage, with comfort
• the intensity of the ignition source
• the oxygen supply.
10.3 Thermal behaviour of ﬁbres
The effect of heat on a textile material can produce physical as well as chemical
change.8,15,16 In thermoplastic ﬁbres, the physical changes occur at the second order
transition (Tg), and melting temperature (Tm), while the chemical changes take place
at pyrolysis temperatures (Tp) at which thermal degradation occurs. Textile com-
bustion is a complex process that involves heating, decomposition leading to gasiﬁ-
cation (fuel generation), ignition and ﬂame propagation.
A self-sustaining ﬂame requires a fuel source and a means of gasifying the fuel,
after which it must be mixed with oxygen and heat. When a ﬁbre is subjected to
heat, it pyrolyses at Tp (Fig. 10.1) and volatile liquids and gases, which are com-
bustible, act as the fuels for further combustion. After pyrolysis, if the temperature
is equal to or greater than combustion temperature Tc, ﬂammable volatile liquids
burn in the presence of oxygen to give products such as carbon dioxide and water.
When a textile is ignited, heat from an external source raises its temperature until
it degrades. The rate of this initial rise in temperature depends on the speciﬁc heat
combustion CO2 + H2O + Non-flammable
Fibre Oxygen gases
Char + Flammable volatiles + Non-flammable
and gases gases
10.1 Combustion of ﬁbres.
Heat and ﬂame protection 225
of the ﬁbre, its thermal conductivity17 and also the latent heat of fusion (for melting
ﬁbres) and the heat of pyrolysis.
Frank-Kamenetzky18 demonstrated the inﬂuence of the nature of a reactive
(ﬂammable) material and its environment. The heat generation and heat loss was
plotted as a function of temperature (Fig. 10.2). The plot shows that the loss of heat
is approximately proportional to the difference in temperature between the com-
bustion zone and the environment, and can be represented by an approximately
straight line. The equilibrium between the heat generation and the heat loss is real-
ized at the points of intersection of I and II (Fig. 10.2(a)). Point A represents the
ambient temperature, point C represents the stationary temperature and both are
stable while B is unstable. To the left of B, the heat loss exceeds the heat genera-
tion, while to the right of B this is just the reverse. Therefore, the temperature cor-
responding to B is the ignition temperature. During a ﬁre accident, the material must
be heated to such an extent that it reaches the ignition temperature. The tempera-
ture at B is also considered to be the self-extinguishing temperature; at lower tem-
peratures heat loss exceeds heat generation. Figure 10.2(b) shows three materials
with different degrees of ﬂammability but in the same environment. The ﬁrst (Ia) is
highly ﬂammable, the second (Ib) moderately ﬂammable while the third (Ic) is ﬂame
resistant under these conditions. Figure 10.2(c), on the other hand, represents a
material in different environments. An increased heat loss may be caused by a
higher rate of air ﬂow, less insulation and so on. From the above, it is thus evident
that the ﬂammable material may be barely ﬂammable or even non-ﬂammable under
Heat Heat Ia Ib Ic
(a) Temperature Temperature (b)
10.2 Schematic Stability diagram of Combustion. (a) Flame stability diagram, (b) three
degrees of ﬂammability, (c) four different surroundings.
226 Handbook of technical textiles
In protective clothing, it is desirable to have low propensity for ignition from a
ﬂaming source or, if the item ignites, a slow ﬁre spread with low heat output would
be ideal. In general, thermoplastic-ﬁbre fabrics19,20 such as nylon, polyester ﬁbre, and
polypropylene ﬁbres fulﬁl these requirements because they shrink away from ﬂame
and, if they burn, they do so with a small slowly spreading ﬂame and ablate. For pro-
tective clothing, however, there are additional requirements, such as protection
against heat by providing insulation, as well as high dimensional stability of the
fabrics, so that, upon exposure to the heat ﬂuxes that are expected during the course
of the wearer’s work, they will neither shrink nor melt, and if they then decompose,
form char. The above mentioned requirements cannot be met by thermoplastic
ﬁbres and so recourse must be made to one of the so-called high-performance ﬁbres
such as aramid ﬁbre (e.g. Nomex, DuPont), ﬂame-retardant cotton or wool, partially
oxidised acrylic ﬁbres, and so on. It may also be noted that the aramid ﬁbres, in spite
of their high oxygen index and high thermal stability, have not been found suitable
for preventing skin burns in molten-metal splashes because of their high thermal
From the foregoing discussion, it may be noted that the mode of decomposition
and the nature of the decomposition products (solid, liquid, and gaseous products)
depend on the chemical nature of the ﬁbre, and also on the type of ﬁnishes or
coatings applied to the fabrics. If such decomposition products are of a ﬂammable
nature, the presence of atmospheric oxygen gives rise to ignition, with or without
ﬂames. When the heat evolved is higher than that required for thermal decom-
position, it can spread the ignition to cause the total destruction of the material
In addition to the ﬁbre characteristics and fabric ﬁnish, several garment charac-
teristics also inﬂuence thermal protection. For a given fabric thickness, the lower the
density, the greater the thermal resistance. This applies to ﬁbres such as cotton, wool,
and so on, which produce an insulating char on heating. Hence, thicker fabrics
made from cotton, wool and other non-melting ﬁbres give good thermal protection,
whereas the thicker thermoplastic-ﬁbre fabrics produce more severe burns.
Flame retardance of materials is normally expressed as oxygen index:16
(OI) = (OI)m + f (FR) (1)
where (OI)m is the oxygen index of the virgin material, and f(FR) is the function of
the ﬂame retardant. Thermal properties of textile ﬁbres including OI values are
given in Table 10.1.
Miller et al.21 have also studied the extinguishability of fabrics by determining the
burning rate as a function of the environmental oxygen concentration. They quoted
the intrinsic oxygen index, (OI)o, values at extrapolated zero burning rates for
cotton, wool, modacrylic, and aramid ﬁbre for top ignition of vertically oriented
samples, and for bottom ignition of both vertically oriented and 45°-inclined
samples. Intrinsic oxygen index values were, however, lower than normal limiting
oxygen index (LOI) values, for example, (OI)o for top-ignited cotton is 13 whereas
the normal LOI is 18.
In another study, Van Krevelen16 has established a good correlation between
the chemical composition and the LOI value of the polymers. According to him, the
composition parameter (CP) describing the combined effect of hydrogen and
halogen content should be less than one for ﬂame retardant materials. Figure 10.4
shows the relationship between CP and LOI for some textile materials
Heat and ﬂame protection 227
Heat + Light
CO2 CO2 H2O
Liquid condensates, tars
10.3 Combustion as a feedback mechanism.
CP = (H C) - 0.65(F C) - 1.1(Cl C) - x(Br C)
13 13 13
where (H/C), (F/C) and (Cl/C) are the atomic ratios of the respective elements in
the polymer composition, and coefﬁcient x is probably 1.6, but is still uncertain
owing to the lack of sufﬁcient data. Although there is some data scatter, as shown
in Fig. 10.4, there is a correlation between the LOI and CP.
• if CP ≥ 1 then LOI ª 17.5
• if CP £ 1 then LOI ª 42.5 to 60.